#------------------------------------------------------------------------------
#$Date: 2018-11-16 15:31:04 +0200 (Fri, 16 Nov 2018) $
#$Revision: 212008 $
#$URL: file:///home/coder/svn-repositories/cod/cif/2/10/35/2103503.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2103503
loop_
_publ_author_name
'Pavlovska, A.'
'Werner, S.'
'Maximov, B.'
'Mill, B.'
_publ_section_title
;
 Pressure-induced phase transitions of piezoelectric single crystals
 from the langasite family: La₃Nb~0.5~Ga~5.5~O₁₄ and
 La₃Ta~0.5~Ga~5.5~O₁₄
;
_journal_issue                   6
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              939
_journal_page_last               947
_journal_paper_doi               10.1107/S0108768102010273
_journal_volume                  58
_journal_year                    2002
_chemical_formula_sum            'Ga11 La6 O28 Ta'
_chemical_formula_weight         2229.33
_space_group_IT_number           5
_symmetry_space_group_name_Hall  'A 2y'
_symmetry_space_group_name_H-M   'A 1 2 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            1
_cell_length_a                   5.024
_cell_length_b                   7.980
_cell_length_c                   13.823
_cell_measurement_temperature    293(2)
_cell_volume                     554.2
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_pressure         11.57E+6
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.516
_diffrn_measured_fraction_theta_max 0.516
_diffrn_radiation_source         synchrotron
_diffrn_radiation_wavelength     0.56000
_diffrn_reflns_av_R_equivalents  0.0528
_diffrn_reflns_av_sigmaI/netI    0.0483
_diffrn_reflns_limit_h_max       6
_diffrn_reflns_limit_h_min       -6
_diffrn_reflns_limit_k_max       7
_diffrn_reflns_limit_k_min       -6
_diffrn_reflns_limit_l_max       18
_diffrn_reflns_limit_l_min       -19
_diffrn_reflns_number            840
_diffrn_reflns_theta_full        23.01
_diffrn_reflns_theta_max         23.01
_diffrn_reflns_theta_min         3.19
_exptl_absorpt_coefficient_mu    15.538
_exptl_crystal_density_diffrn    6.680
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             980
_refine_diff_density_max         1.679
_refine_diff_density_min         -1.807
_refine_diff_density_rms         0.418
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   -0.04(10)
_refine_ls_extinction_coef       0.0061(13)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.230
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     75
_refine_ls_number_reflns         667
_refine_ls_number_restraints     1
_refine_ls_restrained_S_all      1.229
_refine_ls_R_factor_all          0.0486
_refine_ls_R_factor_gt           0.0486
_refine_ls_shift/su_max          0.083
_refine_ls_shift/su_mean         0.018
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.1000P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1357
_refine_ls_wR_factor_ref         0.1357
_reflns_number_gt                667
_reflns_number_total             667
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            sn0021-11.57d3a2.cif
_cod_data_source_block           11.57d3a2
_cod_depositor_comments
;
The _diffrn_ambient_pressure was taken from the original data block
header, after comparison with the paper text and supplementary
material.

When more than one structure was present in the sn0021.cif file for a
given pressure, the structure with the minimal _refine_ls_R_factor_all
value was taken as the best one, and all others marked with the
'_cod_suboptimal_structure yes' tag.

Changing (with the help of Perl) all _diffrn_radiation_source values in
the files that were reportedly colected on the HASYLAB D3 beamline
(Hamburg) from 'fine-focus sealed tube' to synchrotron.

The command was:

perl -i -ne \
    "s/'fine-focus sealed tube'/synchrotron/; \
    print unless /_diffrn_radiation_type|_diffrn_radiation_monochromator/" \
    *d3*.cif \
    11.57split.cif \
    21.85split.cif \
    22.85split.cif

Saulius Gra\<zulis
;
_cod_database_code               2103503
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z'
'x, y+1/2, z+1/2'
'-x, y+1/2, -z+1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
La1 La -0.0016(6) 0.7834(3) 0.2182(3) 0.0207(10) Uani 1 1 d .
La2 La 0.0000 0.4339(5) 0.0000 0.0191(15) Uani 1 2 d S
Ga1 Ga 0.0000 -0.0016(9) 0.0000 0.0257(11) Uani 0.50 2 d SP
Ta Ta 0.0000 -0.0016(9) 0.0000 0.0257(11) Uani 0.50 2 d SP
Ga2 Ga 0.4799(4) 0.4993(11) 0.1669(8) 0.0186(9) Uani 1 1 d .
Ga3 Ga -0.5000 0.7627(12) 0.0000 0.023(3) Uani 1 2 d S
Ga4 Ga 0.4964(14) 0.6183(10) 0.3848(6) 0.0169(12) Uani 1 1 d .
O1 O 0.164(3) 0.013(6) 0.334(4) 0.011(4) Uiso 1 1 d .
O2 O 0.286(7) 0.640(6) 0.089(4) 0.022(9) Uiso 1 1 d .
O3 O 0.298(5) 0.057(4) 0.776(3) 0.005(6) Uiso 1 1 d .
O4 O 0.379(9) 0.282(7) 0.182(5) 0.061(12) Uiso 1 1 d .
O5 O 0.254(8) 0.857(7) 0.920(4) 0.025(10) Uiso 1 1 d .
O6 O 0.206(5) 0.986(3) 0.1197(19) 0.007(4) Uiso 1 1 d .
O7 O 0.255(10) 0.179(8) 0.978(4) 0.036(13) Uiso 1 1 d .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
La La -0.9400 1.6200 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ta Ta -0.9400 4.4000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ga Ga 0.2490 1.0600 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0028 0.0036 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O6 La1 O5 66.4(11) . 2_556
O6 La1 O3 114.6(8) . 3_554
O5 La1 O3 139.9(14) 2_556 3_554
O6 La1 O4 134.5(16) . 4
O5 La1 O4 92.4(17) 2_556 4
O3 La1 O4 107.4(15) 3_554 4
O6 La1 O1 74.1(13) . 1_565
O5 La1 O1 119.8(17) 2_556 1_565
O3 La1 O1 97.1(12) 3_554 1_565
O4 La1 O1 84.2(15) 4 1_565
O6 La1 O1 126.2(15) . 4
O5 La1 O1 78.6(18) 2_556 4
O3 La1 O1 69.5(12) 3_554 4
O4 La1 O1 84.2(16) 4 4
O1 La1 O1 158.6(11) 1_565 4
O6 La1 O2 69.7(12) . .
O5 La1 O2 81.3(15) 2_556 .
O3 La1 O2 63.9(7) 3_554 .
O4 La1 O2 149.7(19) 4 .
O1 La1 O2 124.6(10) 1_565 .
O1 La1 O2 65.5(13) 4 .
O6 La1 O3 72.6(9) . 2_566
O5 La1 O3 61.2(14) 2_556 2_566
O3 La1 O3 158.8(5) 3_554 2_566
O4 La1 O3 61.9(14) 4 2_566
O1 La1 O3 64.8(11) 1_565 2_566
O1 La1 O3 123.8(10) 4 2_566
O2 La1 O3 134.9(7) . 2_566
O6 La1 Ga2 103.8(7) . 4
O5 La1 Ga2 82.6(12) 2_556 4
O3 La1 Ga2 130.9(8) 3_554 4
O4 La1 Ga2 31.2(14) 4 4
O1 La1 Ga2 64.6(5) 1_565 4
O1 La1 Ga2 111.0(7) 4 4
O2 La1 Ga2 163.9(10) . 4
O3 La1 Ga2 32.7(7) 2_566 4
O6 La1 Ga2 91.2(6) . .
O5 La1 Ga2 112.3(12) 2_556 .
O3 La1 Ga2 31.6(8) 3_554 .
O4 La1 Ga2 134.3(14) 4 .
O1 La1 Ga2 112.1(6) 1_565 .
O1 La1 Ga2 65.3(5) 4 .
O2 La1 Ga2 32.4(11) . .
O3 La1 Ga2 163.8(7) 2_566 .
Ga2 La1 Ga2 162.4(2) 4 .
O6 La1 Ta 32.7(6) . 1_565
O5 La1 Ta 34.5(12) 2_556 1_565
O3 La1 Ta 129.6(8) 3_554 1_565
O4 La1 Ta 121.0(14) 4 1_565
O1 La1 Ta 100.7(12) 1_565 1_565
O1 La1 Ta 100.6(13) 4 1_565
O2 La1 Ta 67.2(11) . 1_565
O3 La1 Ta 67.7(8) 2_566 1_565
Ga2 La1 Ta 99.2(2) 4 1_565
Ga2 La1 Ta 98.5(2) . 1_565
O6 La1 Ga1 32.7(6) . 1_565
O5 La1 Ga1 34.5(12) 2_556 1_565
O3 La1 Ga1 129.6(8) 3_554 1_565
O4 La1 Ga1 121.0(14) 4 1_565
O1 La1 Ga1 100.7(12) 1_565 1_565
O1 La1 Ga1 100.6(13) 4 1_565
O2 La1 Ga1 67.2(11) . 1_565
O3 La1 Ga1 67.7(8) 2_566 1_565
Ga2 La1 Ga1 99.2(2) 4 1_565
Ga2 La1 Ga1 98.5(2) . 1_565
Ta La1 Ga1 0.0(2) 1_565 1_565
O7 La2 O7 66(2) 2_556 1_554
O7 La2 O1 85.6(16) 2_556 4
O7 La2 O1 119.8(17) 1_554 4
O7 La2 O1 119.8(17) 2_556 3_554
O7 La2 O1 85.6(16) 1_554 3_554
O1 La2 O1 151(2) 4 3_554
O7 La2 O2 142.5(17) 2_556 .
O7 La2 O2 108.0(17) 1_554 .
O1 La2 O2 64.9(12) 4 .
O1 La2 O2 95.4(13) 3_554 .
O7 La2 O2 108.0(17) 2_556 2
O7 La2 O2 142.5(17) 1_554 2
O1 La2 O2 95.4(13) 4 2
O1 La2 O2 64.9(12) 3_554 2
O2 La2 O2 98(2) . 2
O7 La2 O4 59.7(18) 2_556 2
O7 La2 O4 84.5(17) 1_554 2
O1 La2 O4 125.8(11) 4 2
O1 La2 O4 66.1(13) 3_554 2
O2 La2 O4 157.3(15) . 2
O2 La2 O4 63.1(14) 2 2
O7 La2 O4 84.5(17) 2_556 .
O7 La2 O4 59.7(18) 1_554 .
O1 La2 O4 66.1(13) 4 .
O1 La2 O4 125.8(11) 3_554 .
O2 La2 O4 63.1(14) . .
O2 La2 O4 157.3(15) 2 .
O4 La2 O4 138.1(19) 2 .
O7 La2 Ga2 115.0(14) 2_556 .
O7 La2 Ga2 80.6(14) 1_554 .
O1 La2 Ga2 64.6(5) 4 .
O1 La2 Ga2 110.5(7) 3_554 .
O2 La2 Ga2 32.3(11) . .
O2 La2 Ga2 129.9(11) 2 .
O4 La2 Ga2 165.0(10) 2 .
O4 La2 Ga2 31.2(9) . .
O7 La2 Ga2 80.6(14) 2_556 2
O7 La2 Ga2 115.0(14) 1_554 2
O1 La2 Ga2 110.5(7) 4 2
O1 La2 Ga2 64.6(5) 3_554 2
O2 La2 Ga2 129.9(11) . 2
O2 La2 Ga2 32.3(11) 2 2
O4 La2 Ga2 31.2(9) 2 2
O4 La2 Ga2 165.0(10) . 2
Ga2 La2 Ga2 162.2(4) . 2
O7 La2 Ga1 33.0(12) 2_556 .
O7 La2 Ga1 33.0(12) 1_554 .
O1 La2 Ga1 104.5(12) 4 .
O1 La2 Ga1 104.5(12) 3_554 .
O2 La2 Ga1 131.1(11) . .
O2 La2 Ga1 131.1(11) 2 .
O4 La2 Ga1 69.0(10) 2 .
O4 La2 Ga1 69.0(10) . .
Ga2 La2 Ga1 98.90(18) . .
Ga2 La2 Ga1 98.90(18) 2 .
O7 La2 Ta 33.0(12) 2_556 .
O7 La2 Ta 33.0(12) 1_554 .
O1 La2 Ta 104.5(12) 4 .
O1 La2 Ta 104.5(12) 3_554 .
O2 La2 Ta 131.1(11) . .
O2 La2 Ta 131.1(11) 2 .
O4 La2 Ta 69.0(10) 2 .
O4 La2 Ta 69.0(10) . .
Ga2 La2 Ta 98.90(18) . .
Ga2 La2 Ta 98.90(18) 2 .
Ga1 La2 Ta 0.0 . .
O5 Ga1 O5 113(3) 2_546 1_544
O5 Ga1 O6 95.7(16) 2_546 2_545
O5 Ga1 O6 81.1(15) 1_544 2_545
O5 Ga1 O6 81.1(15) 2_546 1_545
O5 Ga1 O6 95.7(16) 1_544 1_545
O6 Ga1 O6 174.2(16) 2_545 1_545
O5 Ga1 O7 155.1(14) 2_546 1_554
O5 Ga1 O7 85.0(19) 1_544 1_554
O6 Ga1 O7 104.7(19) 2_545 1_554
O6 Ga1 O7 79.6(19) 1_545 1_554
O5 Ga1 O7 85.0(19) 2_546 2_556
O5 Ga1 O7 155.1(14) 1_544 2_556
O6 Ga1 O7 79.6(19) 2_545 2_556
O6 Ga1 O7 104.7(19) 1_545 2_556
O7 Ga1 O7 85(3) 1_554 2_556
O5 Ga1 O4 111.6(14) 2_546 2
O5 Ga1 O4 106.2(18) 1_544 2
O6 Ga1 O4 38.8(12) 2_545 2
O6 Ga1 O4 146.9(12) 1_545 2
O7 Ga1 O4 78(2) 1_554 2
O7 Ga1 O4 49(2) 2_556 2
O5 Ga1 O4 106.2(18) 2_546 .
O5 Ga1 O4 111.6(14) 1_544 .
O6 Ga1 O4 146.9(12) 2_545 .
O6 Ga1 O4 38.8(12) 1_545 .
O7 Ga1 O4 49(2) 1_554 .
O7 Ga1 O4 78(2) 2_556 .
O4 Ga1 O4 108.7(18) 2 .
O5 Ga1 O2 57.9(16) 2_546 2_545
O5 Ga1 O2 66.7(15) 1_544 2_545
O6 Ga1 O2 55.4(11) 2_545 2_545
O6 Ga1 O2 118.9(12) 1_545 2_545
O7 Ga1 O2 146.7(18) 1_554 2_545
O7 Ga1 O2 113.4(19) 2_556 2_545
O4 Ga1 O2 92.8(11) 2 2_545
O4 Ga1 O2 157.5(13) . 2_545
O5 Ga1 O2 66.7(15) 2_546 1_545
O5 Ga1 O2 57.9(16) 1_544 1_545
O6 Ga1 O2 118.9(12) 2_545 1_545
O6 Ga1 O2 55.4(11) 1_545 1_545
O7 Ga1 O2 113.4(19) 1_554 1_545
O7 Ga1 O2 146.7(18) 2_556 1_545
O4 Ga1 O2 157.5(13) 2 1_545
O4 Ga1 O2 92.8(11) . 1_545
O2 Ga1 O2 66.9(15) 2_545 1_545
O5 Ga1 La1 101.5(15) 2_546 2_545
O5 Ga1 La1 41.5(14) 1_544 2_545
O6 Ga1 La1 40.6(8) 2_545 2_545
O6 Ga1 La1 135.2(8) 1_545 2_545
O7 Ga1 La1 103.2(17) 1_554 2_545
O7 Ga1 La1 120.1(18) 2_556 2_545
O4 Ga1 La1 74.1(10) 2 2_545
O4 Ga1 La1 148.3(8) . 2_545
O2 Ga1 La1 43.7(8) 2_545 2_545
O2 Ga1 La1 84.1(9) 1_545 2_545
O5 Ga1 La1 41.5(14) 2_546 1_545
O5 Ga1 La1 101.5(15) 1_544 1_545
O6 Ga1 La1 135.2(8) 2_545 1_545
O6 Ga1 La1 40.6(8) 1_545 1_545
O7 Ga1 La1 120.1(18) 1_554 1_545
O7 Ga1 La1 103.2(17) 2_556 1_545
O4 Ga1 La1 148.3(8) 2 1_545
O4 Ga1 La1 74.1(10) . 1_545
O2 Ga1 La1 84.1(9) 2_545 1_545
O2 Ga1 La1 43.7(8) 1_545 1_545
La1 Ga1 La1 120.7(2) 2_545 1_545
O5 Ta O5 113(3) 2_546 1_544
O5 Ta O6 95.7(16) 2_546 2_545
O5 Ta O6 81.1(15) 1_544 2_545
O5 Ta O6 81.1(15) 2_546 1_545
O5 Ta O6 95.7(16) 1_544 1_545
O6 Ta O6 174.2(16) 2_545 1_545
O5 Ta O7 155.1(14) 2_546 1_554
O5 Ta O7 85.0(19) 1_544 1_554
O6 Ta O7 104.7(19) 2_545 1_554
O6 Ta O7 79.6(19) 1_545 1_554
O5 Ta O7 85.0(19) 2_546 2_556
O5 Ta O7 155.1(14) 1_544 2_556
O6 Ta O7 79.6(19) 2_545 2_556
O6 Ta O7 104.7(19) 1_545 2_556
O7 Ta O7 85(3) 1_554 2_556
O5 Ta Ga4 162.5(14) 2_546 3_544
O5 Ta Ga4 52.3(14) 1_544 3_544
O6 Ta Ga4 90.4(7) 2_545 3_544
O6 Ta Ga4 91.3(7) 1_545 3_544
O7 Ta Ga4 33.6(17) 1_554 3_544
O7 Ta Ga4 112.2(17) 2_556 3_544
O5 Ta Ga4 52.3(14) 2_546 4_545
O5 Ta Ga4 162.5(14) 1_544 4_545
O6 Ta Ga4 91.3(7) 2_545 4_545
O6 Ta Ga4 90.4(7) 1_545 4_545
O7 Ta Ga4 112.2(17) 1_554 4_545
O7 Ta Ga4 33.6(17) 2_556 4_545
Ga4 Ta Ga4 144.2(4) 3_544 4_545
O5 Ta Ga3 33.3(14) 2_546 1_545
O5 Ta Ga3 99.8(14) 1_544 1_545
O6 Ta Ga3 62.9(7) 2_545 1_545
O6 Ta Ga3 113.2(8) 1_545 1_545
O7 Ta Ga3 165.4(18) 1_554 1_545
O7 Ta Ga3 85.3(17) 2_556 1_545
Ga4 Ta Ga3 145.7(2) 3_544 1_545
Ga4 Ta Ga3 62.77(14) 4_545 1_545
O5 Ta Ga3 99.8(14) 2_546 1_645
O5 Ta Ga3 33.3(14) 1_544 1_645
O6 Ta Ga3 113.2(8) 2_545 1_645
O6 Ta Ga3 62.9(7) 1_545 1_645
O7 Ta Ga3 85.3(17) 1_554 1_645
O7 Ta Ga3 165.4(18) 2_556 1_645
Ga4 Ta Ga3 62.77(14) 3_544 1_645
Ga4 Ta Ga3 145.7(2) 4_545 1_645
Ga3 Ta Ga3 106.3(4) 1_545 1_645
O5 Ta Ga4 113.6(14) 2_546 4_645
O5 Ta Ga4 86.5(14) 1_544 4_645
O6 Ta Ga4 150.7(8) 2_545 4_645
O6 Ta Ga4 32.7(8) 1_545 4_645
O7 Ta Ga4 47.5(18) 1_554 4_645
O7 Ta Ga4 103.0(18) 2_556 4_645
Ga4 Ta Ga4 61.3(3) 3_544 4_645
Ga4 Ta Ga4 107.0(2) 4_545 4_645
Ga3 Ta Ga4 145.88(19) 1_545 4_645
Ga3 Ta Ga4 62.45(13) 1_645 4_645
O5 Ta Ga4 86.5(14) 2_546 3_444
O5 Ta Ga4 113.6(14) 1_544 3_444
O6 Ta Ga4 32.7(8) 2_545 3_444
O6 Ta Ga4 150.7(8) 1_545 3_444
O7 Ta Ga4 103.0(18) 1_554 3_444
O7 Ta Ga4 47.5(18) 2_556 3_444
Ga4 Ta Ga4 107.0(2) 3_544 3_444
Ga4 Ta Ga4 61.3(3) 4_545 3_444
Ga3 Ta Ga4 62.45(13) 1_545 3_444
Ga3 Ta Ga4 145.88(19) 1_645 3_444
Ga4 Ta Ga4 144.5(4) 4_645 3_444
O1 Ga2 O3 119(2) 4_655 3_554
O1 Ga2 O2 119(2) 4_655 .
O3 Ga2 O2 93.8(19) 3_554 .
O1 Ga2 O4 110(2) 4_655 .
O3 Ga2 O4 90(2) 3_554 .
O2 Ga2 O4 120(2) . .
O1 Ga2 O1 175(3) 4_655 4
O3 Ga2 O1 59.5(14) 3_554 4
O2 Ga2 O1 56.5(15) . 4
O4 Ga2 O1 75.7(18) . 4
O1 Ga2 La1 138.4(17) 4_655 4_545
O3 Ga2 La1 51.5(10) 3_554 4_545
O2 Ga2 La1 102.3(12) . 4_545
O4 Ga2 La1 41.9(17) . 4_545
O1 Ga2 La1 45.8(9) 4 4_545
O1 Ga2 La2 136.0(18) 4_655 .
O3 Ga2 La2 104.2(9) 3_554 .
O2 Ga2 La2 46.7(15) . .
O4 Ga2 La2 74.5(18) . .
O1 Ga2 La2 44.8(10) 4 .
La1 Ga2 La2 74.51(14) 4_545 .
O1 Ga2 La1 132.3(17) 4_655 .
O3 Ga2 La1 45.6(11) 3_554 .
O2 Ga2 La1 48.4(14) . .
O4 Ga2 La1 114.4(15) . .
O1 Ga2 La1 42.7(9) 4 .
La1 Ga2 La1 74.55(11) 4_545 .
La2 Ga2 La1 74.74(16) . .
O1 Ga2 La2 42.8(18) 4_655 1_655
O3 Ga2 La2 162.0(10) 3_554 1_655
O2 Ga2 La2 95.7(13) . 1_655
O4 Ga2 La2 98.2(17) . 1_655
O1 Ga2 La2 138.1(10) 4 1_655
La1 Ga2 La2 139.8(3) 4_545 1_655
La2 Ga2 La2 93.4(3) . 1_655
La1 Ga2 La2 139.9(3) . 1_655
O1 Ga2 La1 44.6(17) 4_655 4_645
O3 Ga2 La1 97.1(11) 3_554 4_645
O2 Ga2 La1 163.8(12) . 4_645
O4 Ga2 La1 71.8(16) . 4_645
O1 Ga2 La1 139.7(10) 4 4_645
La1 Ga2 La1 93.9(2) 4_545 4_645
La2 Ga2 La1 139.9(3) . 4_645
La1 Ga2 La1 139.9(4) . 4_645
La2 Ga2 La1 70.76(13) 1_655 4_645
O1 Ga2 La1 39.1(17) 4_655 1_655
O3 Ga2 La1 92.5(10) 3_554 1_655
O2 Ga2 La1 96.7(14) . 1_655
O4 Ga2 La1 142.7(16) . 1_655
O1 Ga2 La1 135.8(9) 4 1_655
La1 Ga2 La1 139.8(3) 4_545 1_655
La2 Ga2 La1 139.8(3) . 1_655
La1 Ga2 La1 93.2(2) . 1_655
La2 Ga2 La1 71.28(13) 1_655 1_655
La1 Ga2 La1 70.94(10) 4_645 1_655
O1 Ga2 O4 74.6(19) 4_655 4_655
O3 Ga2 O4 52.1(13) 3_554 4_655
O2 Ga2 O4 94.0(19) . 4_655
O4 Ga2 O4 131.9(14) . 4_655
O1 Ga2 O4 101.7(13) 4 4_655
La1 Ga2 O4 102.5(10) 4_545 4_655
La2 Ga2 O4 136.3(9) . 4_655
La1 Ga2 O4 62.9(9) . 4_655
La2 Ga2 O4 111.8(9) 1_655 4_655
La1 Ga2 O4 83.4(10) 4_645 4_655
La1 Ga2 O4 40.6(9) 1_655 4_655
O2 Ga3 O2 118(3) 2 1_455
O2 Ga3 O5 102.7(19) 2 2_556
O2 Ga3 O5 102(2) 1_455 2_556
O2 Ga3 O5 102(2) 2 1_454
O2 Ga3 O5 102.7(19) 1_455 1_454
O5 Ga3 O5 131(4) 2_556 1_454
O2 Ga3 Ta 81.7(13) 2 1_565
O2 Ga3 Ta 139.6(14) 1_455 1_565
O5 Ga3 Ta 37.6(19) 2_556 1_565
O5 Ga3 Ta 107.2(16) 1_454 1_565
O2 Ga3 Ta 139.6(14) 2 1_465
O2 Ga3 Ta 81.7(13) 1_455 1_465
O5 Ga3 Ta 107.2(16) 2_556 1_465
O5 Ga3 Ta 37.6(19) 1_454 1_465
Ta Ga3 Ta 106.3(4) 1_565 1_465
O2 Ga3 O1 63.5(13) 2 3_454
O2 Ga3 O1 81.8(16) 1_455 3_454
O5 Ga3 O1 165.3(15) 2_556 3_454
O5 Ga3 O1 60(2) 1_454 3_454
Ta Ga3 O1 137.0(7) 1_565 3_454
Ta Ga3 O1 87.4(6) 1_465 3_454
O2 Ga3 O1 81.8(16) 2 4
O2 Ga3 O1 63.5(13) 1_455 4
O5 Ga3 O1 60(2) 2_556 4
O5 Ga3 O1 165.3(15) 1_454 4
Ta Ga3 O1 87.4(6) 1_565 4
Ta Ga3 O1 137.0(7) 1_465 4
O1 Ga3 O1 110.1(17) 3_454 4
O2 Ga3 O2 102.8(17) 2 2_455
O2 Ga3 O2 62.7(18) 1_455 2_455
O5 Ga3 O2 154.3(16) 2_556 2_455
O5 Ga3 O2 44.7(17) 1_454 2_455
Ta Ga3 O2 151.9(7) 1_565 2_455
Ta Ga3 O2 52.7(7) 1_465 2_455
O1 Ga3 O2 39.3(8) 3_454 2_455
O1 Ga3 O2 120.7(9) 4 2_455
O2 Ga3 O2 62.7(18) 2 .
O2 Ga3 O2 102.8(17) 1_455 .
O5 Ga3 O2 44.7(17) 2_556 .
O5 Ga3 O2 154.3(16) 1_454 .
Ta Ga3 O2 52.7(7) 1_565 .
Ta Ga3 O2 151.9(7) 1_465 .
O1 Ga3 O2 120.7(9) 3_454 .
O1 Ga3 O2 39.3(8) 4 .
O2 Ga3 O2 153.4(13) 2_455 .
O2 Ga3 O4 31.7(14) 2 2
O2 Ga3 O4 90.0(17) 1_455 2
O5 Ga3 O4 125.7(16) 2_556 2
O5 Ga3 O4 96(2) 1_454 2
Ta Ga3 O4 113.0(6) 1_565 2
Ta Ga3 O4 127.0(6) 1_465 2
O1 Ga3 O4 39.6(8) 3_454 2
O1 Ga3 O4 79.7(11) 4 2
O2 Ga3 O4 77.0(9) 2_455 2
O2 Ga3 O4 81.0(9) . 2
O2 Ga3 O4 90.0(17) 2 1_455
O2 Ga3 O4 31.7(14) 1_455 1_455
O5 Ga3 O4 96(2) 2_556 1_455
O5 Ga3 O4 125.7(16) 1_454 1_455
Ta Ga3 O4 127.0(6) 1_565 1_455
Ta Ga3 O4 113.0(6) 1_465 1_455
O1 Ga3 O4 79.7(11) 3_454 1_455
O1 Ga3 O4 39.6(8) 4 1_455
O2 Ga3 O4 81.0(9) 2_455 1_455
O2 Ga3 O4 77.0(9) . 1_455
O4 Ga3 O4 68.1(15) 2 1_455
O4 Ga4 O7 115(3) 4_655 3_554
O4 Ga4 O6 97.1(18) 4_655 4_645
O7 Ga4 O6 136(2) 3_554 4_645
O4 Ga4 O3 88(2) 4_655 3_554
O7 Ga4 O3 106(2) 3_554 3_554
O6 Ga4 O3 104.8(13) 4_645 3_554
O4 Ga4 Ta 143.3(17) 4_655 3
O7 Ga4 Ta 36.1(19) 3_554 3
O6 Ga4 Ta 119.6(9) 4_645 3
O3 Ga4 Ta 84.5(10) 3_554 3
O4 Ga4 Ta 102.2(16) 4_655 3_655
O7 Ga4 Ta 104.9(19) 3_554 3_655
O6 Ga4 Ta 35.3(8) 4_645 3_655
O3 Ga4 Ta 139.2(10) 3_554 3_655
Ta Ga4 Ta 107.0(2) 3 3_655
O4 Ga4 O1 53.4(18) 4_655 1_565
O7 Ga4 O1 67(2) 3_554 1_565
O6 Ga4 O1 150.3(10) 4_645 1_565
O3 Ga4 O1 80.0(12) 3_554 1_565
Ta Ga4 O1 89.9(6) 3 1_565
Ta Ga4 O1 137.2(7) 3_655 1_565
O4 Ga4 O1 63(2) 4_655 4_655
O7 Ga4 O1 166.6(19) 3_554 4_655
O6 Ga4 O1 56.3(11) 4_645 4_655
O3 Ga4 O1 60.8(9) 3_554 4_655
Ta Ga4 O1 138.1(7) 3 4_655
Ta Ga4 O1 88.4(6) 3_655 4_655
O1 Ga4 O1 105.0(8) 1_565 4_655
O4 Ga4 O4 109(3) 4_655 3
O7 Ga4 O4 33.6(18) 3_554 3
O6 Ga4 O4 108.4(12) 4_645 3
O3 Ga4 O4 140.0(11) 3_554 3
Ta Ga4 O4 60.0(7) 3 3
Ta Ga4 O4 73.9(7) 3_655 3
O1 Ga4 O4 82.0(11) 1_565 3
O1 Ga4 O4 159.1(9) 4_655 3
O4 Ga4 O2 133(2) 4_655 4_645
O7 Ga4 O2 112(2) 3_554 4_645
O6 Ga4 O2 39.4(9) 4_645 4_645
O3 Ga4 O2 88.2(11) 3_554 4_645
Ta Ga4 O2 83.0(6) 3 4_645
Ta Ga4 O2 56.0(6) 3_655 4_645
O1 Ga4 O2 166.8(9) 1_565 4_645
O1 Ga4 O2 73.8(10) 4_655 4_645
O4 Ga4 O2 103.8(11) 3 4_645
O4 Ga4 O2 63(2) 4_655 .
O7 Ga4 O2 120(2) 3_554 .
O6 Ga4 O2 101.3(10) 4_645 .
O3 Ga4 O2 25.8(9) 3_554 .
Ta Ga4 O2 107.9(5) 3 .
Ta Ga4 O2 134.8(6) 3_655 .
O1 Ga4 O2 70.2(11) 1_565 .
O1 Ga4 O2 46.4(7) 4_655 .
O4 Ga4 O2 150.1(10) 3 .
O2 Ga4 O2 101.4(11) 4_645 .
O4 Ga4 O2 39(2) 4_655 4_655
O7 Ga4 O2 82(2) 3_554 4_655
O6 Ga4 O2 110.6(9) 4_645 4_655
O3 Ga4 O2 117.2(15) 3_554 4_655
Ta Ga4 O2 117.1(6) 3 4_655
Ta Ga4 O2 92.7(6) 3_655 4_655
O1 Ga4 O2 45.4(7) 1_565 4_655
O1 Ga4 O2 100.2(10) 4_655 4_655
O4 Ga4 O2 70.4(10) 3 4_655
O2 Ga4 O2 147.7(10) 4_645 4_655
O2 Ga4 O2 96.1(10) . 4_655
Ga2 O1 La1 106(2) 4_645 1_545
Ga2 O1 La2 108(2) 4_645 3_545
La1 O1 La2 106.4(16) 1_545 3_545
Ga2 O1 La1 113(2) 4_645 4_545
La1 O1 La1 110.1(18) 1_545 4_545
La2 O1 La1 112.6(17) 3_545 4_545
Ga2 O1 O3 147(3) 4_645 2_556
La1 O1 O3 58.9(11) 1_545 2_556
La2 O1 O3 104.7(10) 3_545 2_556
La1 O1 O3 56.4(11) 4_545 2_556
Ga2 O1 O2 149(3) 4_645 4_545
La1 O1 O2 104.1(12) 1_545 4_545
La2 O1 O2 57.2(14) 3_545 4_545
La1 O1 O2 60.0(13) 4_545 4_545
O3 O1 O2 58.2(11) 2_556 4_545
Ga2 O1 O4 142(3) 4_645 4_545
La1 O1 O4 45.0(13) 1_545 4_545
La2 O1 O4 69.6(14) 3_545 4_545
La1 O1 O4 101.5(11) 4_545 4_545
O3 O1 O4 49.2(11) 2_556 4_545
O2 O1 O4 62.9(15) 4_545 4_545
Ga2 O1 O7 80(2) 4_645 3_544
La1 O1 O7 81.2(16) 1_545 3_544
La2 O1 O7 45.9(12) 3_545 3_544
La1 O1 O7 159(2) 4_545 3_544
O3 O1 O7 122.3(16) 2_556 3_544
O2 O1 O7 100.2(18) 4_545 3_544
O4 O1 O7 73.1(16) 4_545 3_544
Ga2 O1 O6 85.4(18) 4_645 1_545
La1 O1 O6 49.7(11) 1_545 1_545
La2 O1 O6 155.8(18) 3_545 1_545
La1 O1 O6 78.1(16) 4_545 1_545
O3 O1 O6 61.9(14) 2_556 1_545
O2 O1 O6 118.9(18) 4_545 1_545
O4 O1 O6 87.3(17) 4_545 1_545
O7 O1 O6 122(2) 3_544 1_545
Ga2 O1 O3 30.6(11) 4_645 2_656
La1 O1 O3 93.3(16) 1_545 2_656
La2 O1 O3 138.9(16) 3_545 2_656
La1 O1 O3 92.8(16) 4_545 2_656
O3 O1 O3 116(2) 2_556 2_656
O2 O1 O3 151(2) 4_545 2_656
O4 O1 O3 138(2) 4_545 2_656
O7 O1 O3 105.0(15) 3_544 2_656
O6 O1 O3 57.5(12) 1_545 2_656
Ga2 O1 O4 35.4(12) 4_645 4_645
La1 O1 O4 76.1(19) 1_545 4_645
La2 O1 O4 100(2) 3_545 4_645
La1 O1 O4 142.9(19) 4_545 4_645
O3 O1 O4 133(3) 2_556 4_645
O2 O1 O4 156(3) 4_545 4_645
O4 O1 O4 107(2) 4_545 4_645
O7 O1 O4 56.2(17) 3_544 4_645
O6 O1 O4 79.9(18) 1_545 4_645
O3 O1 O4 50.1(11) 2_656 4_645
Ga2 O1 O2 30.8(12) 4_645 4_645
La1 O1 O2 136.8(15) 1_545 4_645
La2 O1 O2 93.3(18) 3_545 4_645
La1 O1 O2 96.3(16) 4_545 4_645
O3 O1 O2 151(2) 2_556 4_645
O2 O1 O2 119(3) 4_545 4_645
O4 O1 O2 159(2) 4_545 4_645
O7 O1 O2 86.2(17) 3_544 4_645
O6 O1 O2 107.5(14) 1_545 4_645
O3 O1 O2 50.6(9) 2_656 4_645
O4 O1 O2 62.7(13) 4_645 4_645
Ga2 O1 O5 84.7(17) 4_645 3_544
La1 O1 O5 160(2) 1_545 3_544
La2 O1 O5 85.2(18) 3_545 3_544
La1 O1 O5 50.0(13) 4_545 3_544
O3 O1 O5 103.0(17) 2_556 3_544
O2 O1 O5 68.1(17) 4_545 3_544
O4 O1 O5 131.0(18) 4_545 3_544
O7 O1 O5 118(2) 3_544 3_544
O6 O1 O5 117(2) 1_545 3_544
O3 O1 O5 87.8(15) 2_656 3_544
O4 O1 O5 118.6(18) 4_645 3_544
O2 O1 O5 56.0(13) 4_645 3_544
Ga2 O1 Ga2 175(3) 4_645 4_545
La1 O1 Ga2 69.6(6) 1_545 4_545
La2 O1 Ga2 70.6(7) 3_545 4_545
La1 O1 Ga2 72.1(6) 4_545 4_545
O3 O1 Ga2 34.2(6) 2_556 4_545
O2 O1 Ga2 34.6(10) 4_545 4_545
O4 O1 Ga2 32.3(10) 4_545 4_545
O7 O1 Ga2 96.4(12) 3_544 4_545
O6 O1 Ga2 93.8(12) 1_545 4_545
O3 O1 Ga2 150(2) 2_656 4_545
O4 O1 Ga2 139(2) 4_645 4_545
O2 O1 Ga2 153(2) 4_645 4_545
O5 O1 Ga2 100.4(13) 3_544 4_545
Ga2 O1 Ga4 59.3(13) 4_645 1_545
La1 O1 Ga4 69.6(11) 1_545 1_545
La2 O1 Ga4 75.9(13) 3_545 1_545
La1 O1 Ga4 170.7(15) 4_545 1_545
O3 O1 Ga4 126.5(17) 2_556 1_545
O2 O1 Ga4 129.3(19) 4_545 1_545
O4 O1 Ga4 84.8(15) 4_545 1_545
O7 O1 Ga4 30.1(10) 3_544 1_545
O6 O1 Ga4 95.6(14) 1_545 1_545
O3 O1 Ga4 78.0(9) 2_656 1_545
O4 O1 Ga4 27.9(12) 4_645 1_545
O2 O1 Ga4 79.0(11) 4_645 1_545
O5 O1 Ga4 129.8(15) 3_544 1_545
Ga2 O1 Ga4 115.5(13) 4_545 1_545
Ga2 O1 Ga3 63.5(13) 4_645 3_645
La1 O1 Ga3 167.5(14) 1_545 3_645
La2 O1 Ga3 72.5(13) 3_545 3_645
La1 O1 Ga3 81.3(13) 4_545 3_645
O3 O1 Ga3 133.7(17) 2_556 3_645
O2 O1 Ga3 85.9(18) 4_545 3_645
O4 O1 Ga3 140(2) 4_545 3_645
O7 O1 Ga3 89.7(16) 3_544 3_645
O6 O1 Ga3 131.6(13) 1_545 3_645
O3 O1 Ga3 80.6(10) 2_656 3_645
O4 O1 Ga3 91.7(14) 4_645 3_645
O2 O1 Ga3 32.9(10) 4_645 3_645
O5 O1 Ga3 31.6(10) 3_544 3_645
Ga2 O1 Ga3 120.4(14) 4_545 3_645
Ga4 O1 Ga3 98.3(10) 1_545 3_645
Ga2 O1 Ga4 62.2(14) 4_645 4_645
La1 O1 Ga4 78.3(13) 1_545 4_645
La2 O1 Ga4 170.5(10) 3_545 4_645
La1 O1 Ga4 72.5(13) 4_545 4_645
O3 O1 Ga4 84.8(16) 2_556 4_645
O2 O1 Ga4 130(2) 4_545 4_645
O4 O1 Ga4 118.1(19) 4_545 4_645
O7 O1 Ga4 128.6(15) 3_544 4_645
O6 O1 Ga4 30.8(7) 1_545 4_645
O3 O1 Ga4 31.6(8) 2_656 4_645
O4 O1 Ga4 73.2(14) 4_645 4_645
O2 O1 Ga4 78.0(11) 4_645 4_645
O5 O1 Ga4 92.8(15) 3_544 4_645
Ga2 O1 Ga4 118.9(14) 4_545 4_645
Ga4 O1 Ga4 98.5(10) 1_545 4_645
Ga3 O1 Ga4 101.1(9) 3_645 4_645
Ga2 O1 O4 72.5(17) 4_645 .
La1 O1 O4 101(2) 1_545 .
La2 O1 O4 151(2) 3_545 .
La1 O1 O4 47.0(13) 4_545 .
O3 O1 O4 80.9(18) 2_556 .
O2 O1 O4 107(2) 4_545 .
O4 O1 O4 127.8(16) 4_545 .
O7 O1 O4 151.4(17) 3_544 .
O6 O1 O4 51.0(15) 1_545 .
O3 O1 O4 46.5(13) 2_656 .
O4 O1 O4 96.2(12) 4_645 .
O2 O1 O4 73.0(14) 4_645 .
O5 O1 O4 66.3(18) 3_544 .
Ga2 O1 O4 111.1(16) 4_545 .
Ga4 O1 O4 123.8(15) 1_545 .
Ga3 O1 O4 83.3(15) 3_645 .
Ga4 O1 O4 28.8(11) 4_645 .
Ga2 O1 O3 76.3(16) 4_645 3_544
La1 O1 O3 40.6(9) 1_545 3_544
La2 O1 O3 90.5(15) 3_545 3_544
La1 O1 O3 149(2) 4_545 3_544
O3 O1 O3 98.8(14) 2_556 3_544
O2 O1 O3 126.4(17) 4_545 3_544
O4 O1 O3 66.2(14) 4_545 3_544
O7 O1 O3 48.6(13) 3_544 3_544
O6 O1 O3 73.0(13) 1_545 3_544
O3 O1 O3 81.4(10) 2_656 3_544
O4 O1 O3 41.1(15) 4_645 3_544
O2 O1 O3 103.1(13) 4_645 3_544
O5 O1 O3 158.2(13) 3_544 3_544
Ga2 O1 O3 98.3(10) 4_545 3_544
Ga4 O1 O3 29.1(7) 1_545 3_544
Ga3 O1 O3 127.1(11) 3_645 3_544
Ga4 O1 O3 87.9(12) 4_645 3_544
O4 O1 O3 116.7(19) . 3_544
Ga2 O1 O2 81.8(17) 4_645 3_545
La1 O1 O2 147(2) 1_545 3_545
La2 O1 O2 42.1(10) 3_545 3_545
La1 O1 O2 95.3(17) 4_545 3_545
O3 O1 O2 128.1(17) 2_556 3_545
O2 O1 O2 70.0(19) 4_545 3_545
O4 O1 O2 110.6(19) 4_545 3_545
O7 O1 O2 68.3(16) 3_544 3_545
O6 O1 O2 162.0(14) 1_545 3_545
O3 O1 O2 106.7(14) 2_656 3_545
O4 O1 O2 96.5(18) 4_645 3_545
O2 O1 O2 56.1(15) 4_645 3_545
O5 O1 O2 49.8(15) 3_544 3_545
Ga2 O1 O2 100.1(13) 4_545 3_545
Ga4 O1 O2 88.7(13) 1_545 3_545
Ga3 O1 O2 30.4(8) 3_645 3_545
Ga4 O1 O2 131.2(12) 4_645 3_545
O4 O1 O2 112.5(19) . 3_545
O3 O1 O2 115.7(17) 3_544 3_545
Ga2 O1 O7 117(2) 4_645 4_546
La1 O1 O7 77.0(13) 1_545 4_546
La2 O1 O7 29.4(10) 3_545 4_546
La1 O1 O7 124.8(12) 4_545 4_546
O3 O1 O7 89.9(12) 2_556 4_546
O2 O1 O7 65.2(16) 4_545 4_546
O4 O1 O7 44.4(15) 4_545 4_546
O7 O1 O7 38.0(14) 3_544 4_546
O6 O1 O7 126.5(17) 1_545 4_546
O3 O1 O7 142.3(15) 2_656 4_546
O4 O1 O7 92.3(17) 4_645 4_546
O2 O1 O7 115.3(19) 4_645 4_546
O5 O1 O7 113(2) 3_544 4_546
Ga2 O1 O7 59.2(10) 4_545 4_546
Ga4 O1 O7 64.4(10) 1_545 4_546
Ga3 O1 O7 101.2(16) 3_645 4_546
Ga4 O1 O7 153.7(18) 4_645 4_546
O4 O1 O7 170.3(12) . 4_546
O3 O1 O7 67.5(11) 3_544 4_546
O2 O1 O7 71.0(15) 3_545 4_546
Ga2 O1 O5 118(2) 4_645 2_546
La1 O1 O5 28.7(10) 1_545 2_546
La2 O1 O5 121.0(12) 3_545 2_546
La1 O1 O5 81.4(14) 4_545 2_546
O3 O1 O5 35.2(11) 2_556 2_546
O2 O1 O5 91.4(14) 4_545 2_546
O4 O1 O5 51.4(15) 4_545 2_546
O7 O1 O5 108.9(19) 3_544 2_546
O6 O1 O5 36.6(9) 1_545 2_546
O3 O1 O5 93.4(16) 2_656 2_546
O4 O1 O5 98(2) 4_645 2_546
O2 O1 O5 143.9(17) 4_645 2_546
O5 O1 O5 131.3(18) 3_544 2_546
Ga2 O1 O5 59.8(9) 4_545 2_546
Ga4 O1 O5 97.7(15) 1_545 2_546
Ga3 O1 O5 161.3(18) 3_645 2_546
Ga4 O1 O5 66.9(11) 4_645 2_546
O4 O1 O5 79.8(16) . 2_546
O3 O1 O5 68.6(12) 3_544 2_546
O2 O1 O5 159.8(12) 3_545 2_546
O7 O1 O5 94.4(15) 4_546 2_546
Ga2 O1 O6 119(2) 4_645 4_545
La1 O1 O6 125.8(11) 1_545 4_545
La2 O1 O6 86.6(12) 3_545 4_545
La1 O1 O6 26.5(8) 4_545 4_545
O3 O1 O6 67.0(11) 2_556 4_545
O2 O1 O6 40.6(12) 4_545 4_545
O4 O1 O6 98.3(12) 4_545 4_545
O7 O1 O6 132.3(17) 3_544 4_545
O6 O1 O6 104.2(15) 1_545 4_545
O3 O1 O6 110.7(15) 2_656 4_545
O4 O1 O6 154.7(17) 4_645 4_545
O2 O1 O6 92.7(15) 4_645 4_545
O5 O1 O6 37.0(9) 3_544 4_545
Ga2 O1 O6 66.0(7) 4_545 4_545
Ga4 O1 O6 160.0(16) 1_545 4_545
Ga3 O1 O6 66.7(9) 3_645 4_545
Ga4 O1 O6 97.4(12) 4_645 4_545
O4 O1 O6 69.5(15) . 4_545
O3 O1 O6 164.1(7) 3_544 4_545
O2 O1 O6 71.7(11) 3_545 4_545
O7 O1 O6 104.2(12) 4_546 4_545
O5 O1 O6 99.6(12) 2_546 4_545
Ga2 O1 O2 79.8(17) 4_645 1_545
La1 O1 O2 27.7(7) 1_545 1_545
La2 O1 O2 124.0(17) 3_545 1_545
La1 O1 O2 114.1(18) 4_545 1_545
O3 O1 O2 77.8(13) 2_556 1_545
O2 O1 O2 130.9(14) 4_545 1_545
O4 O1 O2 72.3(16) 4_545 1_545
O7 O1 O2 84.6(15) 3_544 1_545
O6 O1 O2 37.1(10) 1_545 1_545
O3 O1 O2 66.1(11) 2_656 1_545
O4 O1 O2 55.4(17) 4_645 1_545
O2 O1 O2 110.3(12) 4_645 1_545
O5 O1 O2 150.1(17) 3_544 1_545
Ga2 O1 O2 96.3(11) 4_545 1_545
Ga4 O1 O2 61.1(10) 1_545 1_545
Ga3 O1 O2 143.2(8) 3_645 1_545
Ga4 O1 O2 57.3(9) 4_645 1_545
O4 O1 O2 84.6(17) . 1_545
O3 O1 O2 36.0(7) 3_544 1_545
O2 O1 O2 149.5(16) 3_545 1_545
O7 O1 O2 96.4(14) 4_546 1_545
O5 O1 O2 42.7(9) 2_546 1_545
O6 O1 O2 138.7(14) 4_545 1_545
Ga2 O1 O3 84.7(15) 4_645 3_554
La1 O1 O3 129.1(17) 1_545 3_554
La2 O1 O3 117.1(16) 3_545 3_554
La1 O1 O3 29.5(7) 4_545 3_554
O3 O1 O3 84.7(14) 2_556 3_554
O2 O1 O3 80.3(15) 4_545 3_554
O4 O1 O3 131.0(14) 4_545 3_554
O7 O1 O3 148.9(17) 3_544 3_554
O6 O1 O3 83.2(13) 1_545 3_554
O3 O1 O3 71.0(10) 2_656 3_554
O4 O1 O3 118.4(12) 4_645 3_554
O2 O1 O3 67.3(11) 4_645 3_554
O5 O1 O3 33.5(12) 3_544 3_554
Ga2 O1 O3 100.6(11) 4_545 3_554
Ga4 O1 O3 143.9(5) 1_545 3_554
Ga3 O1 O3 59.2(8) 3_645 3_554
Ga4 O1 O3 63.1(8) 4_645 3_554
O4 O1 O3 34.5(13) . 3_554
O3 O1 O3 150.5(14) 3_544 3_554
O2 O1 O3 83.1(10) 3_545 3_554
O7 O1 O3 142.1(15) 4_546 3_554
O5 O1 O3 102.1(14) 2_546 3_554
O6 O1 O3 39.7(7) 4_545 3_554
O2 O1 O3 118.8(14) 1_545 3_554
Ga2 O1 Ga4 133(2) 4_645 1_445
La1 O1 Ga4 51.6(6) 1_545 1_445
La2 O1 Ga4 57.1(7) 3_545 1_445
La1 O1 Ga4 114.0(5) 4_545 1_445
O3 O1 Ga4 64.4(9) 2_556 1_445
O2 O1 Ga4 65.9(11) 4_545 1_445
O4 O1 Ga4 15.5(11) 4_545 1_445
O7 O1 Ga4 58.1(10) 3_544 1_445
O6 O1 Ga4 98.9(12) 1_545 1_445
O3 O1 Ga4 140.7(16) 2_656 1_445
O4 O1 Ga4 98.6(17) 4_645 1_445
O2 O1 Ga4 143.4(18) 4_645 1_445
O5 O1 Ga4 131.4(14) 3_544 1_445
Ga2 O1 Ga4 42.1(5) 4_545 1_445
Ga4 O1 Ga4 73.5(8) 1_545 1_445
Ga3 O1 Ga4 129.6(14) 3_645 1_445
Ga4 O1 Ga4 129.2(13) 4_645 1_445
O4 O1 Ga4 143.1(16) . 1_445
O3 O1 Ga4 60.6(7) 3_544 1_445
O2 O1 Ga4 99.2(12) 3_545 1_445
O7 O1 Ga4 29.7(8) 4_546 1_445
O5 O1 Ga4 64.8(10) 2_546 1_445
O6 O1 Ga4 105.2(5) 4_545 1_445
O2 O1 Ga4 76.5(9) 1_545 1_445
O3 O1 Ga4 142.5(7) 3_554 1_445
Ga2 O1 Ga4 137(2) 4_645 4_545
La1 O1 Ga4 59.0(8) 1_545 4_545
La2 O1 Ga4 114.3(4) 3_545 4_545
La1 O1 Ga4 52.7(8) 4_545 4_545
O3 O1 Ga4 9.7(8) 2_556 4_545
O2 O1 Ga4 65.5(13) 4_545 4_545
O4 O1 Ga4 57.2(11) 4_545 4_545
O7 O1 Ga4 129.7(13) 3_544 4_545
O6 O1 Ga4 53.7(8) 1_545 4_545
O3 O1 Ga4 106.8(16) 2_656 4_545
O4 O1 Ga4 129(2) 4_645 4_545
O2 O1 Ga4 143.9(17) 4_645 4_545
O5 O1 Ga4 101.7(13) 3_544 4_545
Ga2 O1 Ga4 43.8(5) 4_545 4_545
Ga4 O1 Ga4 128.5(13) 1_545 4_545
Ga3 O1 Ga4 133.2(13) 3_645 4_545
Ga4 O1 Ga4 75.2(10) 4_645 4_545
O4 O1 Ga4 71.8(13) . 4_545
O3 O1 Ga4 99.6(11) 3_544 4_545
O2 O1 Ga4 134.2(11) 3_545 4_545
O7 O1 Ga4 99.2(9) 4_546 4_545
O5 O1 Ga4 32.1(7) 2_546 4_545
O6 O1 Ga4 67.6(7) 4_545 4_545
O2 O1 Ga4 74.1(9) 1_545 4_545
O3 O1 Ga4 79.2(9) 3_554 4_545
Ga4 O1 Ga4 72.6(4) 1_445 4_545
Ga2 O1 Ga3 140(2) 4_645 3_545
La1 O1 Ga3 113.1(4) 1_545 3_545
La2 O1 Ga3 53.5(7) 3_545 3_545
La1 O1 Ga3 60.5(8) 4_545 3_545
O3 O1 Ga3 66.9(9) 2_556 3_545
O2 O1 Ga3 9.3(11) 4_545 3_545
O4 O1 Ga3 70.7(12) 4_545 3_545
O7 O1 Ga3 98.5(13) 3_544 3_545
O6 O1 Ga3 126.3(11) 1_545 3_545
O3 O1 Ga3 147.0(16) 2_656 3_545
O4 O1 Ga3 153(2) 4_645 3_545
O2 O1 Ga3 109.5(16) 4_645 3_545
O5 O1 Ga3 60.6(11) 3_544 3_545
Ga2 O1 Ga3 43.8(5) 4_545 3_545
Ga4 O1 Ga3 128.5(13) 1_545 3_545
Ga3 O1 Ga3 76.7(9) 3_645 3_545
Ga4 O1 Ga3 132.9(13) 4_645 3_545
O4 O1 Ga3 106.7(16) . 3_545
O3 O1 Ga3 131.5(10) 3_544 3_545
O2 O1 Ga3 61.2(9) 3_545 3_545
O7 O1 Ga3 66.5(10) 4_546 3_545
O5 O1 Ga3 100.6(7) 2_546 3_545
O6 O1 Ga3 37.7(5) 4_545 3_545
O2 O1 Ga3 140.1(8) 1_545 3_545
O3 O1 Ga3 76.9(9) 3_554 3_545
Ga4 O1 Ga3 71.9(4) 1_445 3_545
Ga4 O1 Ga3 73.7(4) 4_545 3_545
Ga2 O1 O4 77.2(18) 4_645 3_545
La1 O1 O4 112.7(16) 1_545 3_545
La2 O1 O4 31.4(8) 3_545 3_545
La1 O1 O4 131(2) 4_545 3_545
O3 O1 O4 135.2(14) 2_556 3_545
O2 O1 O4 86.5(18) 4_545 3_545
O4 O1 O4 92.0(17) 4_545 3_545
O7 O1 O4 32.0(13) 3_544 3_545
O6 O1 O4 150.4(16) 1_545 3_545
O3 O1 O4 107.8(12) 2_656 3_545
O4 O1 O4 72.0(19) 4_645 3_545
O2 O1 O4 67.6(14) 4_645 3_545
O5 O1 O4 85.7(17) 3_544 3_545
Ga2 O1 O4 101.3(12) 4_545 3_545
Ga4 O1 O4 54.9(9) 1_545 3_545
Ga3 O1 O4 59.8(11) 3_645 3_545
Ga4 O1 O4 139.3(8) 4_645 3_545
O4 O1 O4 140.0(17) . 3_545
O3 O1 O4 79.7(12) 3_544 3_545
O2 O1 O4 36.4(11) 3_545 3_545
O7 O1 O4 47.7(11) 4_546 3_545
O5 O1 O4 138.6(16) 2_546 3_545
O6 O1 O4 105.1(13) 4_545 3_545
O2 O1 O4 115.1(13) 1_545 3_545
O3 O1 O4 118.2(13) 3_554 3_545
Ga4 O1 O4 76.8(9) 1_445 3_545
Ga4 O1 O4 144.9(9) 4_545 3_545
Ga3 O1 O4 80.8(11) 3_545 3_545
Ga2 O1 Ta 97.0(18) 4_645 3_545
La1 O1 Ta 68.3(11) 1_545 3_545
La2 O1 Ta 44.8(8) 3_545 3_545
La1 O1 Ta 148.5(9) 4_545 3_545
O3 O1 Ta 103.0(11) 2_556 3_545
O2 O1 Ta 89.3(15) 4_545 3_545
O4 O1 Ta 53.8(12) 4_545 3_545
O7 O1 Ta 19.3(9) 3_544 3_545
O6 O1 Ta 115.4(15) 1_545 3_545
O3 O1 Ta 118.6(12) 2_656 3_545
O4 O1 Ta 68.5(15) 4_645 3_545
O2 O1 Ta 105.4(15) 4_645 3_545
O5 O1 Ta 128.0(18) 3_544 3_545
Ga2 O1 Ta 78.5(8) 4_545 3_545
Ga4 O1 Ta 40.6(5) 1_545 3_545
Ga3 O1 Ta 104.9(12) 3_645 3_545
Ga4 O1 Ta 133.8(13) 4_645 3_545
O4 O1 Ta 162.5(18) . 3_545
O3 O1 Ta 46.0(7) 3_544 3_545
O2 O1 Ta 78.9(12) 3_545 3_545
O7 O1 Ta 24.1(7) 4_546 3_545
O5 O1 Ta 93.5(12) 2_546 3_545
O6 O1 Ta 127.9(10) 4_545 3_545
O2 O1 Ta 79.6(10) 1_545 3_545
O3 O1 Ta 161.4(14) 3_554 3_545
Ga4 O1 Ta 38.8(4) 1_445 3_545
Ga4 O1 Ta 110.6(7) 4_545 3_545
Ga3 O1 Ta 90.4(8) 3_545 3_545
O4 O1 Ta 45.2(7) 3_545 3_545
Ga2 O1 Ga1 97.0(18) 4_645 3_545
La1 O1 Ga1 68.3(11) 1_545 3_545
La2 O1 Ga1 44.8(8) 3_545 3_545
La1 O1 Ga1 148.5(9) 4_545 3_545
O3 O1 Ga1 103.0(11) 2_556 3_545
O2 O1 Ga1 89.3(15) 4_545 3_545
O4 O1 Ga1 53.8(12) 4_545 3_545
O7 O1 Ga1 19.3(9) 3_544 3_545
O6 O1 Ga1 115.4(15) 1_545 3_545
O3 O1 Ga1 118.6(12) 2_656 3_545
O4 O1 Ga1 68.5(15) 4_645 3_545
O2 O1 Ga1 105.4(15) 4_645 3_545
O5 O1 Ga1 128.0(18) 3_544 3_545
Ga2 O1 Ga1 78.5(8) 4_545 3_545
Ga4 O1 Ga1 40.6(5) 1_545 3_545
Ga3 O1 Ga1 104.9(12) 3_645 3_545
Ga4 O1 Ga1 133.8(13) 4_645 3_545
O4 O1 Ga1 162.5(18) . 3_545
O3 O1 Ga1 46.0(7) 3_544 3_545
O2 O1 Ga1 78.9(12) 3_545 3_545
O7 O1 Ga1 24.1(7) 4_546 3_545
O5 O1 Ga1 93.5(12) 2_546 3_545
O6 O1 Ga1 127.9(10) 4_545 3_545
O2 O1 Ga1 79.6(10) 1_545 3_545
O3 O1 Ga1 161.4(14) 3_554 3_545
Ga4 O1 Ga1 38.8(4) 1_445 3_545
Ga4 O1 Ga1 110.6(7) 4_545 3_545
Ga3 O1 Ga1 90.4(8) 3_545 3_545
O4 O1 Ga1 45.2(7) 3_545 3_545
Ta O1 Ga1 0.00(9) 3_545 3_545
Ga2 O1 Ga1 99.7(19) 4_645 .
La1 O1 Ga1 46.7(9) 1_545 .
La2 O1 Ga1 146.4(10) 3_545 .
La1 O1 Ga1 70.8(13) 4_545 .
O3 O1 Ga1 47.4(11) 2_556 .
O2 O1 Ga1 104.7(16) 4_545 .
O4 O1 Ga1 77.0(14) 4_545 .
O7 O1 Ga1 126.1(17) 3_544 .
O6 O1 Ga1 14.5(5) 1_545 .
O3 O1 Ga1 71.2(13) 2_656 .
O4 O1 Ga1 92.7(18) 4_645 .
O2 O1 Ga1 120.0(15) 4_645 .
O5 O1 Ga1 115.9(17) 3_544 .
Ga2 O1 Ga1 79.7(9) 4_545 .
Ga4 O1 Ga1 104.5(12) 1_545 .
Ga3 O1 Ga1 138.6(13) 3_645 .
Ga4 O1 Ga1 42.0(6) 4_645 .
O4 O1 Ga1 55.3(14) . .
O3 O1 Ga1 78.5(11) 3_544 .
O2 O1 Ga1 165.6(16) 3_545 .
O7 O1 Ga1 119.8(13) 4_546 .
O5 O1 Ga1 25.6(8) 2_546 .
O6 O1 Ga1 95.4(10) 4_545 .
O2 O1 Ga1 43.5(8) 1_545 .
O3 O1 Ga1 82.8(10) 3_554 .
Ga4 O1 Ga1 90.3(8) 1_445 .
Ga4 O1 Ga1 39.3(4) 4_545 .
Ga3 O1 Ga1 112.5(7) 3_545 .
O4 O1 Ga1 158.0(14) 3_545 .
Ta O1 Ga1 115.0(10) 3_545 .
Ga1 O1 Ga1 115.0(10) 3_545 .
Ga2 O1 Ta 99.7(19) 4_645 .
La1 O1 Ta 46.7(9) 1_545 .
La2 O1 Ta 146.4(10) 3_545 .
La1 O1 Ta 70.8(13) 4_545 .
O3 O1 Ta 47.4(11) 2_556 .
O2 O1 Ta 104.7(16) 4_545 .
O4 O1 Ta 77.0(14) 4_545 .
O7 O1 Ta 126.1(17) 3_544 .
O6 O1 Ta 14.5(5) 1_545 .
O3 O1 Ta 71.2(13) 2_656 .
O4 O1 Ta 92.7(18) 4_645 .
O2 O1 Ta 120.0(15) 4_645 .
O5 O1 Ta 115.9(17) 3_544 .
Ga2 O1 Ta 79.7(9) 4_545 .
Ga4 O1 Ta 104.5(12) 1_545 .
Ga3 O1 Ta 138.6(13) 3_645 .
Ga4 O1 Ta 42.0(6) 4_645 .
O4 O1 Ta 55.3(14) . .
O3 O1 Ta 78.5(11) 3_544 .
O2 O1 Ta 165.6(16) 3_545 .
O7 O1 Ta 119.8(13) 4_546 .
O5 O1 Ta 25.6(8) 2_546 .
O6 O1 Ta 95.4(10) 4_545 .
O2 O1 Ta 43.5(8) 1_545 .
O3 O1 Ta 82.8(10) 3_554 .
Ga4 O1 Ta 90.3(8) 1_445 .
Ga4 O1 Ta 39.3(4) 4_545 .
Ga3 O1 Ta 112.5(7) 3_545 .
O4 O1 Ta 158.0(14) 3_545 .
Ta O1 Ta 115.0(10) 3_545 .
Ga1 O1 Ta 115.0(10) 3_545 .
Ga1 O1 Ta 0.00(17) . .
Ga2 O1 Ta 103.5(18) 4_645 3
La1 O1 Ta 149.0(8) 1_545 3
La2 O1 Ta 72.3(12) 3_545 3
La1 O1 Ta 48.1(10) 4_545 3
O3 O1 Ta 91.0(12) 2_556 3
O2 O1 Ta 48.1(13) 4_545 3
O4 O1 Ta 110.9(14) 4_545 3
O7 O1 Ta 113.4(17) 3_544 3
O6 O1 Ta 125.0(15) 1_545 3
O3 O1 Ta 107.8(13) 2_656 3
O4 O1 Ta 134.8(17) 4_645 3
O2 O1 Ta 73.3(13) 4_645 3
O5 O1 Ta 20.2(9) 3_544 3
Ga2 O1 Ta 81.4(8) 4_545 3
Ga4 O1 Ta 135.9(14) 1_545 3
Ga3 O1 Ta 43.2(6) 3_645 3
Ga4 O1 Ta 108.2(12) 4_645 3
O4 O1 Ta 79.7(15) . 3
O3 O1 Ta 162.0(16) 3_544 3
O2 O1 Ta 47.4(9) 3_545 3
O7 O1 Ta 97.6(14) 4_546 3
O5 O1 Ta 124.8(11) 2_546 3
O6 O1 Ta 25.2(4) 4_545 3
O2 O1 Ta 162.0(14) 1_545 3
O3 O1 Ta 45.1(7) 3_554 3
Ga4 O1 Ta 111.5(7) 1_445 3
Ga4 O1 Ta 92.6(7) 4_545 3
Ga3 O1 Ta 40.4(4) 3_545 3
O4 O1 Ta 82.7(12) 3_545 3
Ta O1 Ta 117.0(11) 3_545 3
Ga1 O1 Ta 117.0(11) 3_545 3
Ga1 O1 Ta 118.9(11) . 3
Ta O1 Ta 118.9(11) . 3
Ga2 O1 Ga1 103.5(18) 4_645 3
La1 O1 Ga1 149.0(8) 1_545 3
La2 O1 Ga1 72.3(12) 3_545 3
La1 O1 Ga1 48.1(10) 4_545 3
O3 O1 Ga1 91.0(12) 2_556 3
O2 O1 Ga1 48.1(13) 4_545 3
O4 O1 Ga1 110.9(14) 4_545 3
O7 O1 Ga1 113.4(17) 3_544 3
O6 O1 Ga1 125.0(15) 1_545 3
O3 O1 Ga1 107.8(13) 2_656 3
O4 O1 Ga1 134.8(17) 4_645 3
O2 O1 Ga1 73.3(13) 4_645 3
O5 O1 Ga1 20.2(9) 3_544 3
Ga2 O1 Ga1 81.4(8) 4_545 3
Ga4 O1 Ga1 135.9(14) 1_545 3
Ga3 O1 Ga1 43.2(6) 3_645 3
Ga4 O1 Ga1 108.2(12) 4_645 3
O4 O1 Ga1 79.7(15) . 3
O3 O1 Ga1 162.0(16) 3_544 3
O2 O1 Ga1 47.4(9) 3_545 3
O7 O1 Ga1 97.6(14) 4_546 3
O5 O1 Ga1 124.8(11) 2_546 3
O6 O1 Ga1 25.2(4) 4_545 3
O2 O1 Ga1 162.0(14) 1_545 3
O3 O1 Ga1 45.1(7) 3_554 3
Ga4 O1 Ga1 111.5(7) 1_445 3
Ga4 O1 Ga1 92.6(7) 4_545 3
Ga3 O1 Ga1 40.4(4) 3_545 3
O4 O1 Ga1 82.7(12) 3_545 3
Ta O1 Ga1 117.0(11) 3_545 3
Ga1 O1 Ga1 117.0(11) 3_545 3
Ga1 O1 Ga1 118.9(11) . 3
Ta O1 Ga1 118.9(11) . 3
Ta O1 Ga1 0.00(9) 3 3
Ga2 O1 O5 50.5(15) 4_645 2_646
La1 O1 O5 63.4(11) 1_545 2_646
La2 O1 O5 144.2(17) 3_545 2_646
La1 O1 O5 102.9(16) 4_545 2_646
O3 O1 O5 98.3(17) 2_556 2_646
O2 O1 O5 156(2) 4_545 2_646
O4 O1 O5 108.4(19) 4_545 2_646
O7 O1 O5 98.5(17) 3_544 2_646
O6 O1 O5 36.8(8) 1_545 2_646
O3 O1 O5 29.9(10) 2_656 2_646
O4 O1 O5 45.6(15) 4_645 2_646
O2 O1 O5 78.1(11) 4_645 2_646
O5 O1 O5 116.0(14) 3_544 2_646
Ga2 O1 O5 127.4(15) 4_545 2_646
Ga4 O1 O5 68.4(11) 1_545 2_646
Ga3 O1 O5 109.9(7) 3_645 2_646
Ga4 O1 O5 30.6(8) 4_645 2_646
O4 O1 O5 58.7(14) . 2_646
O3 O1 O5 58.8(11) 3_544 2_646
O2 O1 O5 132.2(10) 3_545 2_646
O7 O1 O5 126.3(18) 4_546 2_646
O5 O1 O5 67.6(11) 2_546 2_646
O6 O1 O5 127.9(15) 4_545 2_646
O2 O1 O5 36.2(8) 1_545 2_646
O3 O1 O5 91.7(11) 3_554 2_646
Ga4 O1 O5 112.3(13) 1_445 2_646
Ga4 O1 O5 90.4(11) 4_545 2_646
Ga3 O1 O5 161.8(14) 3_545 2_646
O4 O1 O5 117.3(12) 3_545 2_646
Ta O1 O5 103.7(12) 3_545 2_646
Ga1 O1 O5 103.7(12) 3_545 2_646
Ga1 O1 O5 51.2(8) . 2_646
Ta O1 O5 51.2(8) . 2_646
Ta O1 O5 134.8(12) 3 2_646
Ga1 O1 O5 134.8(12) 3 2_646
Ga2 O1 O6 110.2(19) 4_645 4_535
La1 O1 O6 46.4(8) 1_545 4_535
La2 O1 O6 61.0(10) 3_545 4_535
La1 O1 O6 135.6(7) 4_545 4_535
O3 O1 O6 81.7(11) 2_556 4_535
O2 O1 O6 87.1(13) 4_545 4_535
O4 O1 O6 34.1(11) 4_545 4_535
O7 O1 O6 41.8(11) 3_544 4_535
O6 O1 O6 95.8(14) 1_545 4_535
O3 O1 O6 121.1(14) 2_656 4_535
O4 O1 O6 76.0(16) 4_645 4_535
O2 O1 O6 126.8(16) 4_645 4_535
O5 O1 O6 145.7(18) 3_544 4_535
Ga2 O1 O6 64.5(7) 4_545 4_535
Ga4 O1 O6 51.1(7) 1_545 4_535
Ga3 O1 O6 128.4(15) 3_645 4_535
Ga4 O1 O6 121.5(14) 4_645 4_535
O4 O1 O6 147(2) . 4_535
O3 O1 O6 39.6(6) 3_544 4_535
O2 O1 O6 100.5(14) 3_545 4_535
O7 O1 O6 32.3(9) 4_546 4_535
O5 O1 O6 69.7(10) 2_546 4_535
O6 O1 O6 127.4(8) 4_545 4_535
O2 O1 O6 64.2(9) 1_545 4_535
O3 O1 O6 165.0(7) 3_554 4_535
Ga4 O1 O6 22.7(4) 1_445 4_535
Ga4 O1 O6 88.1(7) 4_545 4_535
Ga3 O1 O6 91.9(7) 3_545 4_535
O4 O1 O6 68.8(10) 3_545 4_535
Ta O1 O6 23.9(4) 3_545 4_535
Ga1 O1 O6 23.9(4) 3_545 4_535
Ga1 O1 O6 92.5(9) . 4_535
Ta O1 O6 92.5(9) . 4_535
Ta O1 O6 128.6(10) 3 4_535
Ga1 O1 O6 128.6(10) 3 4_535
O5 O1 O6 96.5(12) 2_646 4_535
Ga2 O1 La1 27.4(12) 4_645 1_645
La1 O1 La1 78.8(10) 1_545 1_645
La2 O1 La1 119.2(13) 3_545 1_645
La1 O1 La1 122.1(13) 4_545 1_645
O3 O1 La1 125.9(18) 2_556 1_645
O2 O1 La1 176(2) 4_545 1_645
O4 O1 La1 118.8(18) 4_545 1_645
O7 O1 La1 77.2(12) 3_544 1_645
O6 O1 La1 65.3(8) 1_545 1_645
O3 O1 La1 29.8(7) 2_656 1_645
O4 O1 La1 21.0(11) 4_645 1_645
O2 O1 La1 58.1(9) 4_645 1_645
O5 O1 La1 110.1(9) 3_544 1_645
Ga2 O1 La1 148.3(15) 4_545 1_645
Ga4 O1 La1 48.6(4) 1_545 1_645
Ga3 O1 La1 90.8(3) 3_645 1_645
Ga4 O1 La1 52.9(4) 4_645 1_645
O4 O1 La1 75.3(12) . 1_645
O3 O1 La1 54.1(6) 3_544 1_645
O2 O1 La1 105.8(8) 3_545 1_645
O7 O1 La1 113.0(12) 4_546 1_645
O5 O1 La1 92.5(12) 2_546 1_645
O6 O1 La1 139.8(10) 4_545 1_645
O2 O1 La1 52.5(7) 1_545 1_645
O3 O1 La1 100.3(7) 3_554 1_645
Ga4 O1 La1 114.7(10) 1_445 1_645
Ga4 O1 La1 118.7(12) 4_545 1_645
Ga3 O1 La1 166.9(11) 3_545 1_645
O4 O1 La1 89.5(8) 3_545 1_645
Ta O1 La1 89.0(8) 3_545 1_645
Ga1 O1 La1 89.0(8) 3_545 1_645
Ga1 O1 La1 79.5(8) . 1_645
Ta O1 La1 79.5(8) . 1_645
Ta O1 La1 129.9(7) 3 1_645
Ga1 O1 La1 129.9(7) 3 1_645
O5 O1 La1 28.6(7) 2_646 1_645
O6 O1 La1 92.9(9) 4_535 1_645
Ga2 O1 La2 29.1(12) 4_645 3_645
La1 O1 La2 118.9(12) 1_545 3_645
La2 O1 La2 79.5(10) 3_545 3_645
La1 O1 La2 123.5(12) 4_545 3_645
O3 O1 La2 175.6(18) 2_556 3_645
O2 O1 La2 126(2) 4_545 3_645
O4 O1 La2 132.7(17) 4_545 3_645
O7 O1 La2 59.7(11) 3_544 3_645
O6 O1 La2 113.7(8) 1_545 3_645
O3 O1 La2 59.5(8) 2_656 3_645
O4 O1 La2 43.7(13) 4_645 3_645
O2 O1 La2 27.4(10) 4_645 3_645
O5 O1 La2 78.5(10) 3_544 3_645
Ga2 O1 La2 150.0(16) 4_545 3_645
Ga4 O1 La2 52.7(4) 1_545 3_645
Ga3 O1 La2 48.6(4) 3_645 3_645
Ga4 O1 La2 91.0(3) 4_645 3_645
O4 O1 La2 96.1(10) . 3_645
O3 O1 La2 79.6(8) 3_544 3_645
O2 O1 La2 56.0(7) 3_545 3_645
O7 O1 La2 93.3(12) 4_546 3_645
O5 O1 La2 141.2(13) 2_546 3_645
O6 O1 La2 115.1(11) 4_545 3_645
O2 O1 La2 98.7(8) 1_545 3_645
O3 O1 La2 94.7(7) 3_554 3_645
Ga4 O1 La2 117.8(11) 1_445 3_645
Ga4 O1 La2 166.2(11) 4_545 3_645
Ga3 O1 La2 117.3(11) 3_545 3_645
O4 O1 La2 48.8(7) 3_545 3_645
Ta O1 La2 79.0(7) 3_545 3_645
Ga1 O1 La2 79.0(7) 3_545 3_645
Ga1 O1 La2 128.2(8) . 3_645
Ta O1 La2 128.2(8) . 3_645
Ta O1 La2 91.6(8) 3 3_645
Ga1 O1 La2 91.6(8) 3 3_645
O5 O1 La2 77.3(7) 2_646 3_645
O6 O1 La2 99.4(10) 4_535 3_645
La1 O1 La2 49.8(2) 1_645 3_645
Ga2 O1 O7 116(2) 4_645 2_556
La1 O1 O7 61.0(13) 1_545 2_556
La2 O1 O7 135.9(7) 3_545 2_556
La1 O1 O7 50.4(11) 4_545 2_556
O3 O1 O7 31.3(10) 2_556 2_556
O2 O1 O7 83.7(14) 4_545 2_556
O4 O1 O7 75.0(14) 4_545 2_556
O7 O1 O7 141.6(19) 3_544 2_556
O6 O1 O7 35.7(10) 1_545 2_556
O3 O1 O7 85.2(16) 2_656 2_556
O4 O1 O7 116(2) 4_645 2_556
O2 O1 O7 125.7(17) 4_645 2_556
O5 O1 O7 99.4(15) 3_544 2_556
Ga2 O1 O7 65.4(8) 4_545 2_556
Ga4 O1 O7 126.4(16) 1_545 2_556
Ga3 O1 O7 128.7(15) 3_645 2_556
Ga4 O1 O7 53.6(10) 4_645 2_556
O4 O1 O7 52.8(15) . 2_556
O3 O1 O7 98.6(14) 3_544 2_556
O2 O1 O7 144.9(15) 3_545 2_556
O7 O1 O7 119.0(14) 4_546 2_556
O5 O1 O7 32.7(8) 2_546 2_556
O6 O1 O7 73.1(10) 4_545 2_556
O2 O1 O7 65.6(12) 1_545 2_556
O3 O1 O7 69.5(11) 3_554 2_556
Ga4 O1 O7 90.4(9) 1_445 2_556
Ga4 O1 O7 21.6(6) 4_545 2_556
Ga3 O1 O7 90.6(7) 3_545 2_556
O4 O1 O7 166.3(10) 3_545 2_556
Ta O1 O7 124.9(12) 3_545 2_556
Ga1 O1 O7 124.9(12) 3_545 2_556
Ga1 O1 O7 23.1(8) . 2_556
Ta O1 O7 23.1(8) . 2_556
Ta O1 O7 97.7(10) 3 2_556
Ga1 O1 O7 97.7(10) 3 2_556
O5 O1 O7 71.9(13) 2_646 2_556
O6 O1 O7 101.1(11) 4_535 2_556
La1 O1 O7 100.5(12) 1_645 2_556
La2 O1 O7 144.6(11) 3_645 2_556
Ga2 O1 La1 31.6(11) 4_645 4_645
La1 O1 La1 120.9(13) 1_545 4_645
La2 O1 La1 122.5(13) 3_545 4_645
La1 O1 La1 81.4(10) 4_545 4_645
O3 O1 La1 126.4(17) 2_556 4_645
O2 O1 La1 128.8(18) 4_545 4_645
O4 O1 La1 166(2) 4_545 4_645
O7 O1 La1 109.0(11) 3_544 4_645
O6 O1 La1 79.6(9) 1_545 4_645
O3 O1 La1 27.6(8) 2_656 4_645
O4 O1 La1 65.5(10) 4_645 4_645
O2 O1 La1 29.4(10) 4_645 4_645
O5 O1 La1 61.3(10) 3_544 4_645
Ga2 O1 La1 153.4(15) 4_545 4_645
Ga4 O1 La1 90.9(4) 1_545 4_645
Ga3 O1 La1 54.1(4) 3_645 4_645
Ga4 O1 La1 49.2(4) 4_645 4_645
O4 O1 La1 45.5(10) . 4_645
O3 O1 La1 104.2(7) 3_544 4_645
O2 O1 La1 82.8(9) 3_545 4_645
O7 O1 La1 143.6(13) 4_546 4_645
O5 O1 La1 116.1(13) 2_546 4_645
O6 O1 La1 90.4(9) 4_545 4_645
O2 O1 La1 93.7(9) 1_545 4_645
O3 O1 La1 53.3(5) 3_554 4_645
Ga4 O1 La1 164.1(11) 1_445 4_645
Ga4 O1 La1 117.2(11) 4_545 4_645
Ga3 O1 La1 121.8(11) 3_545 4_645
O4 O1 La1 96.6(9) 3_545 4_645
Ta O1 La1 127.7(7) 3_545 4_645
Ga1 O1 La1 127.7(7) 3_545 4_645
Ga1 O1 La1 91.0(8) . 4_645
Ta O1 La1 91.0(8) . 4_645
Ta O1 La1 81.5(7) 3 4_645
Ga1 O1 La1 81.5(7) 3 4_645
O5 O1 La1 57.6(6) 2_646 4_645
O6 O1 La1 141.4(9) 4_535 4_645
La1 O1 La1 50.2(2) 1_645 4_645
La2 O1 La1 50.6(2) 3_645 4_645
O7 O1 La1 97.0(12) 2_556 4_645
Ga2 O1 O7 49.6(14) 4_645 4_646
La1 O1 O7 98.0(15) 1_545 4_646
La2 O1 O7 63.8(12) 3_545 4_646
La1 O1 O7 151.0(18) 4_545 4_646
O3 O1 O7 151.8(18) 2_556 4_646
O2 O1 O7 121(2) 4_545 4_646
O4 O1 O7 103.4(17) 4_545 4_646
O7 O1 O7 31.0(14) 3_544 4_646
O6 O1 O7 117.5(13) 1_545 4_646
O3 O1 O7 78.2(10) 2_656 4_646
O4 O1 O7 37.8(16) 4_645 4_646
O2 O1 O7 56.6(13) 4_645 4_646
O5 O1 O7 101.6(16) 3_544 4_646
Ga2 O1 O7 126.8(16) 4_545 4_646
Ga4 O1 O7 28.6(8) 1_545 4_646
Ga3 O1 O7 70.1(11) 3_645 4_646
Ga4 O1 O7 107.6(8) 4_645 4_646
O4 O1 O7 122.1(11) . 4_646
O3 O1 O7 57.7(11) 3_544 4_646
O2 O1 O7 62.0(13) 3_545 4_646
O7 O1 O7 67.6(11) 4_546 4_646
O5 O1 O7 126.2(19) 2_546 4_646
O6 O1 O7 133.3(16) 4_545 4_646
O2 O1 O7 87.6(12) 1_545 4_646
O3 O1 O7 123.6(11) 3_554 4_646
Ga4 O1 O7 88.8(12) 1_445 4_646
Ga4 O1 O7 156.3(15) 4_545 4_646
Ga3 O1 O7 115.1(15) 3_545 4_646
O4 O1 O7 34.3(10) 3_545 4_646
Ta O1 O7 50.0(9) 3_545 4_646
Ga1 O1 O7 50.0(9) 3_545 4_646
Ga1 O1 O7 129.5(13) . 4_646
Ta O1 O7 129.5(13) . 4_646
Ta O1 O7 108.1(14) 3 4_646
Ga1 O1 O7 108.1(14) 3 4_646
O5 O1 O7 83.0(11) 2_646 4_646
O6 O1 O7 70.2(11) 4_535 4_646
La1 O1 O7 55.6(7) 1_645 4_646
La2 O1 O7 29.3(8) 3_645 4_646
O7 O1 O7 152.5(18) 2_556 4_646
La1 O1 O7 78.1(7) 4_645 4_646
Ga2 O1 O6 53.9(13) 4_645 4_645
La1 O1 O6 146.0(15) 1_545 4_645
La2 O1 O6 106.3(14) 3_545 4_645
La1 O1 O6 64.8(10) 4_545 4_645
O3 O1 O6 120.3(16) 2_556 4_645
O2 O1 O6 101.3(16) 4_545 4_645
O4 O1 O6 163.7(17) 4_545 4_645
O7 O1 O6 116.0(14) 3_544 4_645
O6 O1 O6 97.9(12) 1_545 4_645
O3 O1 O6 55.0(9) 2_656 4_645
O4 O1 O6 89.3(12) 4_645 4_645
O2 O1 O6 31.5(10) 4_645 4_645
O5 O1 O6 33.4(9) 3_544 4_645
Ga2 O1 O6 131.5(13) 4_545 4_645
Ga4 O1 O6 109.9(6) 1_545 4_645
Ga3 O1 O6 33.9(5) 3_645 4_645
Ga4 O1 O6 68.1(7) 4_645 4_645
O4 O1 O6 50.0(12) . 4_645
O3 O1 O6 130.1(6) 3_544 4_645
O2 O1 O6 64.2(10) 3_545 4_645
O7 O1 O6 135.1(16) 4_546 4_645
O5 O1 O6 129.8(15) 2_546 4_645
O6 O1 O6 65.5(8) 4_545 4_645
O2 O1 O6 120.5(10) 1_545 4_645
O3 O1 O6 35.7(6) 3_554 4_645
Ga4 O1 O6 162.4(13) 1_445 4_645
Ga4 O1 O6 114.1(11) 4_545 4_645
Ga3 O1 O6 94.0(10) 3_545 4_645
O4 O1 O6 90.9(10) 3_545 4_645
Ta O1 O6 134.5(10) 3_545 4_645
Ga1 O1 O6 134.5(10) 3_545 4_645
Ga1 O1 O6 105.0(10) . 4_645
Ta O1 O6 105.0(10) . 4_645
Ta O1 O6 53.6(6) 3 4_645
Ga1 O1 O6 53.6(6) 3 4_645
O5 O1 O6 84.4(8) 2_646 4_645
O6 O1 O6 157.7(12) 4_535 4_645
La1 O1 O6 77.2(4) 1_645 4_645
La2 O1 O6 58.9(4) 3_645 4_645
O7 O1 O6 100.3(12) 2_556 4_645
La1 O1 O6 27.9(4) 4_645 4_645
O7 O1 O6 87.9(9) 4_646 4_645
Ga2 O1 Ga2 71.2(16) 4_645 3_545
La1 O1 Ga2 132.6(17) 1_545 3_545
La2 O1 Ga2 40.5(7) 3_545 3_545
La1 O1 Ga2 114.2(16) 4_545 3_545
O3 O1 Ga2 141.8(14) 2_556 3_545
O2 O1 Ga2 84.6(18) 4_545 3_545
O4 O1 Ga2 108.7(17) 4_545 3_545
O7 O1 Ga2 51.4(13) 3_544 3_545
O6 O1 Ga2 156.2(7) 1_545 3_545
O3 O1 Ga2 100.3(11) 2_656 3_545
O4 O1 Ga2 78.6(16) 4_645 3_545
O2 O1 Ga2 52.9(12) 4_645 3_545
O5 O1 Ga2 66.4(13) 3_544 3_545
Ga2 O1 Ga2 109.1(12) 4_545 3_545
Ga4 O1 Ga2 69.3(8) 1_545 3_545
Ga3 O1 Ga2 39.7(6) 3_645 3_545
Ga4 O1 Ga2 130.5(5) 4_645 3_545
O4 O1 Ga2 121.7(15) . 3_545
O3 O1 Ga2 96.9(11) 3_544 3_545
O2 O1 Ga2 19.4(8) 3_545 3_545
O7 O1 Ga2 64.6(11) 4_546 3_545
O5 O1 Ga2 158.4(14) 2_546 3_545
O6 O1 Ga2 91.1(10) 4_545 3_545
O2 O1 Ga2 130.2(11) 1_545 3_545
O3 O1 Ga2 98.2(10) 3_554 3_545
Ga4 O1 Ga2 94.4(9) 1_445 3_545
Ga4 O1 Ga2 150.0(9) 4_545 3_545
Ga3 O1 Ga2 76.7(8) 3_545 3_545
O4 O1 Ga2 20.2(7) 3_545 3_545
Ta O1 Ga2 65.3(7) 3_545 3_545
Ga1 O1 Ga2 65.3(7) 3_545 3_545
Ga1 O1 Ga2 170.7(6) . 3_545
Ta O1 Ga2 170.7(6) . 3_545
Ta O1 Ga2 66.6(7) 3 3_545
Ga1 O1 Ga2 66.6(7) 3 3_545
O5 O1 Ga2 119.5(8) 2_646 3_545
O6 O1 Ga2 88.8(10) 4_535 3_545
La1 O1 Ga2 91.2(5) 1_645 3_545
La2 O1 Ga2 42.6(4) 3_645 3_545
O7 O1 Ga2 164.2(13) 2_556 3_545
La1 O1 Ga2 82.2(5) 4_645 3_545
O7 O1 Ga2 42.8(9) 4_646 3_545
O6 O1 Ga2 71.8(7) 4_645 3_545
Ga2 O1 Ga2 73.5(15) 4_645 .
La1 O1 Ga2 112.7(16) 1_545 .
La2 O1 Ga2 138.6(17) 3_545 .
La1 O1 Ga2 40.9(7) 4_545 .
O3 O1 Ga2 85.0(14) 2_556 .
O2 O1 Ga2 99.5(16) 4_545 .
O4 O1 Ga2 134.0(15) 4_545 .
O7 O1 Ga2 152.1(11) 3_544 .
O6 O1 Ga2 63.6(10) 1_545 .
O3 O1 Ga2 52.3(9) 2_656 .
O4 O1 Ga2 102.2(13) 4_645 .
O2 O1 Ga2 67.0(12) 4_645 .
O5 O1 Ga2 53.5(12) 3_544 .
Ga2 O1 Ga2 111.0(12) 4_545 .
Ga4 O1 Ga2 130.1(6) 1_545 .
Ga3 O1 Ga2 72.1(8) 3_645 .
Ga4 O1 Ga2 40.8(6) 4_645 .
O4 O1 Ga2 12.8(11) . .
O3 O1 Ga2 128.2(12) 3_544 .
O2 O1 Ga2 100.4(12) 3_545 .
O7 O1 Ga2 164.0(14) 4_546 .
O5 O1 Ga2 90.2(13) 2_546 .
O6 O1 Ga2 59.9(8) 4_545 .
O2 O1 Ga2 97.3(11) 1_545 .
O3 O1 Ga2 22.4(4) 3_554 .
Ga4 O1 Ga2 149.4(9) 1_445 .
Ga4 O1 Ga2 76.9(8) 4_545 .
Ga3 O1 Ga2 97.6(9) 3_545 .
O4 O1 Ga2 131.0(11) 3_545 .
Ta O1 Ga2 170.4(5) 3_545 .
Ga1 O1 Ga2 170.4(5) 3_545 .
Ga1 O1 Ga2 66.7(7) . .
Ta O1 Ga2 66.7(7) . .
Ta O1 Ga2 67.4(7) 3 .
Ga1 O1 Ga2 67.4(7) 3 .
O5 O1 Ga2 69.6(9) 2_646 .
O6 O1 Ga2 159.1(14) 4_535 .
La1 O1 Ga2 82.0(5) 1_645 .
La2 O1 Ga2 92.7(5) 3_645 .
O7 O1 Ga2 60.5(10) 2_556 .
La1 O1 Ga2 43.1(4) 4_645 .
O7 O1 Ga2 121.1(8) 4_646 .
O6 O1 Ga2 40.1(5) 4_645 .
Ga2 O1 Ga2 111.4(9) 3_545 .
Ga2 O1 Ga2 68.2(15) 4_645 1_545
La1 O1 Ga2 39.3(6) 1_545 1_545
La2 O1 Ga2 108.7(15) 3_545 1_545
La1 O1 Ga2 135.1(18) 4_545 1_545
O3 O1 Ga2 96.7(15) 2_556 1_545
O2 O1 Ga2 139.7(15) 4_545 1_545
O4 O1 Ga2 76.8(15) 4_545 1_545
O7 O1 Ga2 65.0(13) 3_544 1_545
O6 O1 Ga2 57.0(10) 1_545 1_545
O3 O1 Ga2 65.7(10) 2_656 1_545
O4 O1 Ga2 37.0(15) 4_645 1_545
O2 O1 Ga2 98.3(11) 4_645 1_545
O5 O1 Ga2 152.2(9) 3_544 1_545
Ga2 O1 Ga2 106.9(11) 4_545 1_545
Ga4 O1 Ga2 39.4(5) 1_545 1_545
Ga3 O1 Ga2 128.6(6) 3_645 1_545
Ga4 O1 Ga2 69.4(8) 4_645 1_545
O4 O1 Ga2 98.2(16) . 1_545
O3 O1 Ga2 18.5(6) 3_544 1_545
O2 O1 Ga2 127.8(12) 3_545 1_545
O7 O1 Ga2 85.7(11) 4_546 1_545
O5 O1 Ga2 62.3(10) 2_546 1_545
O6 O1 Ga2 160.4(14) 4_545 1_545
O2 O1 Ga2 21.7(6) 1_545 1_545
O3 O1 Ga2 132.2(10) 3_554 1_545
Ga4 O1 Ga2 75.1(7) 1_445 1_545
Ga4 O1 Ga2 94.4(9) 4_545 1_545
Ga3 O1 Ga2 146.9(8) 3_545 1_545
O4 O1 Ga2 94.0(10) 3_545 1_545
Ta O1 Ga2 64.5(6) 3_545 1_545
Ga1 O1 Ga2 64.5(6) 3_545 1_545
Ga1 O1 Ga2 65.1(7) . 1_545
Ta O1 Ga2 65.1(7) . 1_545
Ta O1 Ga2 171.6(5) 3 1_545
Ga1 O1 Ga2 171.6(5) 3 1_545
O5 O1 Ga2 40.7(8) 2_646 1_545
O6 O1 Ga2 56.3(6) 4_535 1_545
La1 O1 Ga2 42.1(4) 1_645 1_545
La2 O1 Ga2 80.5(5) 3_645 1_545
O7 O1 Ga2 87.3(12) 2_556 1_545
La1 O1 Ga2 91.2(5) 4_645 1_545
O7 O1 Ga2 66.0(9) 4_646 1_545
O6 O1 Ga2 119.0(5) 4_645 1_545
Ga2 O1 Ga2 108.4(9) 3_545 1_545
Ga2 O1 Ga2 109.9(9) . 1_545
Ga2 O1 O5 118(2) 4_645 4_546
La1 O1 O5 134.4(7) 1_545 4_546
La2 O1 O5 50.3(11) 3_545 4_546
La1 O1 O5 63.7(13) 4_545 4_546
O3 O1 O5 87.2(12) 2_556 4_546
O2 O1 O5 31.4(13) 4_545 4_546
O4 O1 O5 90.3(15) 4_545 4_546
O7 O1 O5 95.2(14) 3_544 4_546
O6 O1 O5 140.4(16) 1_545 4_546
O3 O1 O5 130.7(15) 2_656 4_546
O4 O1 O5 138(2) 4_645 4_546
O2 O1 O5 87.6(16) 4_645 4_546
O5 O1 O5 43.5(14) 3_544 4_546
Ga2 O1 O5 65.7(9) 4_545 4_546
Ga4 O1 O5 123.6(15) 1_545 4_546
Ga3 O1 O5 54.7(8) 3_645 4_546
Ga4 O1 O5 131.8(15) 4_645 4_546
O4 O1 O5 103.0(19) . 4_546
O3 O1 O5 140.3(15) 3_544 4_546
O2 O1 O5 41.6(9) 3_545 4_546
O7 O1 O5 73.3(11) 4_546 4_546
O5 O1 O5 121.9(11) 2_546 4_546
O6 O1 O5 37.1(9) 4_545 4_546
O2 O1 O5 162.0(9) 1_545 4_546
O3 O1 O5 68.9(11) 3_554 4_546
Ga4 O1 O5 88.0(8) 1_445 4_546
Ga4 O1 O5 92.6(9) 4_545 4_546
Ga3 O1 O5 22.1(5) 3_545 4_546
O4 O1 O5 69.2(11) 3_545 4_546
Ta O1 O5 94.3(11) 3_545 4_546
Ga1 O1 O5 94.3(11) 3_545 4_546
Ga1 O1 O5 128.9(11) . 4_546
Ta O1 O5 128.9(11) . 4_546
Ta O1 O5 24.6(7) 3 4_546
Ga1 O1 O5 24.6(7) 3 4_546
O5 O1 O5 159.4(16) 2_646 4_546
O6 O1 O5 104.0(11) 4_535 4_546
La1 O1 O5 145.0(10) 1_645 4_546
La2 O1 O5 96.7(10) 3_645 4_546
O7 O1 O5 105.9(12) 2_556 4_546
La1 O1 O5 103.3(11) 4_645 4_546
O7 O1 O5 101.5(14) 4_646 4_546
O6 O1 O5 75.8(10) 4_645 4_546
Ga2 O1 O5 59.4(9) 3_545 4_546
Ga2 O1 O5 91.3(12) . 4_546
Ga2 O1 O5 158.7(14) 1_545 4_546
Ga2 O1 O1 110(2) 4_645 2_556
La1 O1 O1 118.4(8) 1_545 2_556
La2 O1 O1 14.5(12) 3_545 2_556
La1 O1 O1 99.5(11) 4_545 2_556
O3 O1 O1 103.3(10) 2_556 2_556
O2 O1 O1 49.0(14) 4_545 2_556
O4 O1 O1 77.5(14) 4_545 2_556
O7 O1 O1 59.1(13) 3_544 2_556
O6 O1 O1 163.9(9) 1_545 2_556
O3 O1 O1 138.6(16) 2_656 2_556
O4 O1 O1 109.4(19) 4_645 2_556
O2 O1 O1 88.6(17) 4_645 2_556
O5 O1 O1 71.3(14) 3_544 2_556
Ga2 O1 O1 70.5(6) 4_545 2_556
Ga4 O1 O1 88.4(11) 1_545 2_556
Ga3 O1 O1 62.7(10) 3_645 2_556
Ga4 O1 O1 163.3(9) 4_645 2_556
O4 O1 O1 137.1(16) . 2_556
O3 O1 O1 105.0(10) 3_544 2_556
O2 O1 O1 33.2(9) 3_545 2_556
O7 O1 O1 42.4(11) 4_546 2_556
O5 O1 O1 127.4(8) 2_546 2_556
O6 O1 O1 73.2(7) 4_545 2_556
O2 O1 O1 138.3(8) 1_545 2_556
O3 O1 O1 102.7(8) 3_554 2_556
Ga4 O1 O1 67.3(5) 1_445 2_556
Ga4 O1 O1 112.2(4) 4_545 2_556
Ga3 O1 O1 43.2(4) 3_545 2_556
O4 O1 O1 37.7(9) 3_545 2_556
Ta O1 O1 59.3(6) 3_545 2_556
Ga1 O1 O1 59.3(6) 3_545 2_556
Ga1 O1 O1 150.1(6) . 2_556
Ta O1 O1 150.1(6) . 2_556
Ta O1 O1 57.8(7) 3 2_556
Ga1 O1 O1 57.8(7) 3 2_556
O5 O1 O1 155.0(12) 2_646 2_556
O6 O1 O1 74.6(6) 4_535 2_556
La1 O1 O1 127.0(11) 1_645 2_556
La2 O1 O1 81.1(10) 3_645 2_556
O7 O1 O1 132.3(7) 2_556 2_556
La1 O1 O1 116.0(11) 4_645 2_556
O7 O1 O1 72.0(12) 4_646 2_556
O6 O1 O1 95.3(10) 4_645 2_556
Ga2 O1 O1 38.7(7) 3_545 2_556
Ga2 O1 O1 124.4(7) . 2_556
Ga2 O1 O1 123.0(7) 1_545 2_556
O5 O1 O1 36.3(9) 4_546 2_556
Ga2 O1 O1 106.5(18) 4_645 4_545
La1 O1 O1 10.4(7) 1_545 4_545
La2 O1 O1 96.7(12) 3_545 4_545
La1 O1 O1 118.3(18) 4_545 4_545
O3 O1 O1 64.3(14) 2_556 4_545
O2 O1 O1 102.3(13) 4_545 4_545
O4 O1 O1 40.1(13) 4_545 4_545
O7 O1 O1 71.4(12) 3_544 4_545
O6 O1 O1 59.7(15) 1_545 4_545
O3 O1 O1 98.8(16) 2_656 4_545
O4 O1 O1 73.6(15) 4_645 4_545
O2 O1 O1 136.2(12) 4_645 4_545
O5 O1 O1 167.2(12) 3_544 4_545
Ga2 O1 O1 68.6(9) 4_545 4_545
Ga4 O1 O1 62.6(4) 1_545 4_545
Ga3 O1 O1 160.4(15) 3_645 4_545
Ga4 O1 O1 87.3(16) 4_645 4_545
O4 O1 O1 111(2) . 4_545
O3 O1 O1 34.6(5) 3_544 4_545
O2 O1 O1 136.5(17) 3_545 4_545
O7 O1 O1 67.3(10) 4_546 4_545
O5 O1 O1 37.8(13) 2_546 4_545
O6 O1 O1 130.3(9) 4_545 4_545
O2 O1 O1 32.9(8) 1_545 4_545
O3 O1 O1 139.3(17) 3_554 4_545
Ga4 O1 O1 43.8(5) 1_445 4_545
Ga4 O1 O1 66.0(11) 4_545 4_545
Ga3 O1 O1 110.6(6) 3_545 4_545
O4 O1 O1 102.5(12) 3_545 4_545
Ta O1 O1 57.9(6) 3_545 4_545
Ga1 O1 O1 57.9(6) 3_545 4_545
Ga1 O1 O1 57.0(12) . 4_545
Ta O1 O1 57.0(12) . 4_545
Ta O1 O1 150.0(5) 3 4_545
Ga1 O1 O1 150.0(5) 3 4_545
O5 O1 O1 69.1(13) 2_646 4_545
O6 O1 O1 36.2(6) 4_535 4_545
La1 O1 O1 80.0(8) 1_645 4_545
La2 O1 O1 114.2(7) 3_645 4_545
O7 O1 O1 70.5(15) 2_556 4_545
La1 O1 O1 126.3(13) 4_645 4_545
O7 O1 O1 90.5(10) 4_646 4_545
O6 O1 O1 153.5(15) 4_645 4_545
Ga2 O1 O1 122.5(13) 3_545 4_545
Ga2 O1 O1 123.0(18) . 4_545
Ga2 O1 O1 38.3(4) 1_545 4_545
O5 O1 O1 130.3(10) 4_546 4_545
O1 O1 O1 109.4(9) 2_556 4_545
Ga2 O1 O1 112.5(19) 4_645 4
La1 O1 O1 100.3(19) 1_545 4
La2 O1 O1 121.7(15) 3_545 4
La1 O1 O1 11.0(4) 4_545 4
O3 O1 O1 50.4(14) 2_556 4
O2 O1 O1 66.4(13) 4_545 4
O4 O1 O1 98.4(14) 4_545 4
O7 O1 O1 166.5(15) 3_544 4
O6 O1 O1 67.2(16) 1_545 4
O3 O1 O1 88.3(15) 2_656 4
O4 O1 O1 137(2) 4_645 4
O2 O1 O1 101.2(12) 4_645 4
O5 O1 O1 59.8(10) 3_544 4
Ga2 O1 O1 72.0(9) 4_545 4
Ga4 O1 O1 162.2(19) 1_545 4
Ga3 O1 O1 90.5(8) 3_645 4
Ga4 O1 O1 64.5(12) 4_645 4
O4 O1 O1 41.8(11) . 4
O3 O1 O1 138.0(19) 3_544 4
O2 O1 O1 106.3(14) 3_545 4
O7 O1 O1 129.0(10) 4_546 4
O5 O1 O1 71.6(15) 2_546 4
O6 O1 O1 37.1(6) 4_545 4
O2 O1 O1 103.1(17) 1_545 4
O3 O1 O1 34.3(4) 3_554 4
Ga4 O1 O1 112.4(7) 1_445 4
Ga4 O1 O1 45.0(9) 4_545 4
Ga3 O1 O1 68.4(7) 3_545 4
O4 O1 O1 141.8(17) 3_545 4
Ta O1 O1 150.4(5) 3_545 4
Ga1 O1 O1 150.4(5) 3_545 4
Ga1 O1 O1 59.8(13) . 4
Ta O1 O1 59.8(13) . 4
Ta O1 O1 59.2(6) 3 4
Ga1 O1 O1 59.2(6) 3 4
O5 O1 O1 94.1(16) 2_646 4
O6 O1 O1 132.0(9) 4_535 4
La1 O1 O1 116.3(13) 1_645 4
La2 O1 O1 128.6(6) 3_645 4
O7 O1 O1 39.8(11) 2_556 4
La1 O1 O1 81.8(6) 4_645 4
O7 O1 O1 157.8(11) 4_646 4
O6 O1 O1 69.9(5) 4_645 4
Ga2 O1 O1 125.1(13) 3_545 4
Ga2 O1 O1 39.0(4) . 4
Ga2 O1 O1 124.1(17) 1_545 4
O5 O1 O1 74.0(11) 4_546 4
O1 O1 O1 109.4(9) 2_556 4
O1 O1 O1 109.1(18) 4_545 4
Ga2 O1 O1 176.5(16) 4_645 1_455
La1 O1 O1 71.1(5) 1_545 1_455
La2 O1 O1 70.9(5) 3_545 1_455
La1 O1 O1 70.3(5) 4_545 1_455
O3 O1 O1 33.8(12) 2_556 1_455
O2 O1 O1 33.2(14) 4_545 1_455
O4 O1 O1 34.2(13) 4_545 1_455
O7 O1 O1 97.8(9) 3_544 1_455
O6 O1 O1 94.1(5) 1_545 1_455
O3 O1 O1 150.1(12) 2_656 1_455
O4 O1 O1 141.1(14) 4_645 1_455
O2 O1 O1 151.9(12) 4_645 1_455
O5 O1 O1 98.6(8) 3_544 1_455
Ga2 O1 O1 1.9(9) 4_545 1_455
Ga4 O1 O1 117.4(4) 1_545 1_455
Ga3 O1 O1 119.0(5) 3_645 1_455
Ga4 O1 O1 118.6(5) 4_645 1_455
O4 O1 O1 109.8(10) . 1_455
O3 O1 O1 100.2(4) 3_544 1_455
O2 O1 O1 99.5(6) 3_545 1_455
O7 O1 O1 60.5(8) 4_546 1_455
O5 O1 O1 60.6(7) 2_546 1_455
O6 O1 O1 64.1(5) 4_545 1_455
O2 O1 O1 97.7(5) 1_545 1_455
O3 O1 O1 98.7(4) 3_554 1_455
Ga4 O1 O1 43.9(5) 1_445 1_455
Ga4 O1 O1 43.4(5) 4_545 1_455
Ga3 O1 O1 42.4(5) 3_545 1_455
O4 O1 O1 101.8(6) 3_545 1_455
Ta O1 O1 80.1(2) 3_545 1_455
Ga1 O1 O1 80.1(2) 3_545 1_455
Ga1 O1 O1 79.9(2) . 1_455
Ta O1 O1 79.9(2) . 1_455
Ta O1 O1 79.6(2) 3 1_455
Ga1 O1 O1 79.6(2) 3 1_455
O5 O1 O1 128.2(7) 2_646 1_455
O6 O1 O1 66.4(4) 4_535 1_455
La1 O1 O1 149.9(5) 1_645 1_455
La2 O1 O1 150.4(6) 3_645 1_455
O7 O1 O1 65.0(7) 2_556 1_455
La1 O1 O1 151.6(6) 4_645 1_455
O7 O1 O1 128.1(8) 4_646 1_455
O6 O1 O1 129.6(5) 4_645 1_455
Ga2 O1 O1 109.0(3) 3_545 1_455
Ga2 O1 O1 109.4(3) . 1_455
Ga2 O1 O1 108.7(2) 1_545 1_455
O5 O1 O1 64.4(6) 4_546 1_455
O1 O1 O1 70.3(5) 2_556 1_455
O1 O1 O1 70.4(4) 4_545 1_455
O1 O1 O1 70.4(4) 4 1_455
Ga2 O1 O1 3.5(16) 4_645 1_655
La1 O1 O1 108.9(5) 1_545 1_655
La2 O1 O1 109.1(5) 3_545 1_655
La1 O1 O1 109.7(5) 4_545 1_655
O3 O1 O1 146.2(12) 2_556 1_655
O2 O1 O1 146.8(14) 4_545 1_655
O4 O1 O1 145.8(13) 4_545 1_655
O7 O1 O1 82.2(9) 3_544 1_655
O6 O1 O1 85.9(5) 1_545 1_655
O3 O1 O1 29.9(12) 2_656 1_655
O4 O1 O1 38.9(14) 4_645 1_655
O2 O1 O1 28.1(12) 4_645 1_655
O5 O1 O1 81.4(8) 3_544 1_655
Ga2 O1 O1 178.1(9) 4_545 1_655
Ga4 O1 O1 62.6(4) 1_545 1_655
Ga3 O1 O1 61.0(5) 3_645 1_655
Ga4 O1 O1 61.4(5) 4_645 1_655
O4 O1 O1 70.2(10) . 1_655
O3 O1 O1 79.8(4) 3_544 1_655
O2 O1 O1 80.5(6) 3_545 1_655
O7 O1 O1 119.5(8) 4_546 1_655
O5 O1 O1 119.4(7) 2_546 1_655
O6 O1 O1 115.9(5) 4_545 1_655
O2 O1 O1 82.3(5) 1_545 1_655
O3 O1 O1 81.3(4) 3_554 1_655
Ga4 O1 O1 136.1(5) 1_445 1_655
Ga4 O1 O1 136.6(5) 4_545 1_655
Ga3 O1 O1 137.6(5) 3_545 1_655
O4 O1 O1 78.2(6) 3_545 1_655
Ta O1 O1 99.9(2) 3_545 1_655
Ga1 O1 O1 99.9(2) 3_545 1_655
Ga1 O1 O1 100.1(2) . 1_655
Ta O1 O1 100.1(2) . 1_655
Ta O1 O1 100.4(2) 3 1_655
Ga1 O1 O1 100.4(2) 3 1_655
O5 O1 O1 51.8(7) 2_646 1_655
O6 O1 O1 113.6(4) 4_535 1_655
La1 O1 O1 30.1(5) 1_645 1_655
La2 O1 O1 29.6(6) 3_645 1_655
O7 O1 O1 115.0(7) 2_556 1_655
La1 O1 O1 28.4(6) 4_645 1_655
O7 O1 O1 51.9(8) 4_646 1_655
O6 O1 O1 50.4(5) 4_645 1_655
Ga2 O1 O1 71.0(3) 3_545 1_655
Ga2 O1 O1 70.6(3) . 1_655
Ga2 O1 O1 71.3(2) 1_545 1_655
O5 O1 O1 115.6(6) 4_546 1_655
O1 O1 O1 109.7(5) 2_556 1_655
O1 O1 O1 109.6(4) 4_545 1_655
O1 O1 O1 109.6(4) 4 1_655
O1 O1 O1 180(3) 1_455 1_655
Ga2 O1 Ga4 69.2(16) 4_645 2_646
La1 O1 Ga4 97.9(14) 1_545 2_646
La2 O1 Ga4 44.4(8) 3_545 2_646
La1 O1 Ga4 149.2(18) 4_545 2_646
O3 O1 Ga4 137.8(14) 2_556 2_646
O2 O1 Ga4 101.6(18) 4_545 2_646
O4 O1 Ga4 89.0(14) 4_545 2_646
O7 O1 Ga4 17.6(11) 3_544 2_646
O6 O1 Ga4 131.7(14) 1_545 2_646
O3 O1 Ga4 98.3(10) 2_656 2_646
O4 O1 Ga4 55.4(15) 4_645 2_646
O2 O1 Ga4 69.9(12) 4_645 2_646
O5 O1 Ga4 101.6(15) 3_544 2_646
Ga2 O1 Ga4 107.7(12) 4_545 2_646
Ga4 O1 Ga4 36.2(5) 1_545 2_646
Ga3 O1 Ga4 72.4(8) 3_645 2_646
Ga4 O1 Ga4 127.5(7) 4_645 2_646
O4 O1 Ga4 140.8(10) . 2_646
O3 O1 Ga4 61.7(9) 3_544 2_646
O2 O1 Ga4 54.0(9) 3_545 2_646
O7 O1 Ga4 48.7(9) 4_546 2_646
O5 O1 Ga4 126.1(14) 2_546 2_646
O6 O1 Ga4 123.9(12) 4_545 2_646
O2 O1 Ga4 96.6(10) 1_545 2_646
O3 O1 Ga4 131.5(10) 3_554 2_646
Ga4 O1 Ga4 73.6(7) 1_445 2_646
Ga4 O1 Ga4 146.2(9) 4_545 2_646
Ga3 O1 Ga4 97.3(10) 3_545 2_646
O4 O1 Ga4 18.8(6) 3_545 2_646
Ta O1 Ga4 35.9(4) 3_545 2_646
Ga1 O1 Ga4 35.9(4) 3_545 2_646
Ga1 O1 Ga4 140.0(11) . 2_646
Ta O1 Ga4 140.0(11) . 2_646
Ta O1 Ga4 101.1(10) 3 2_646
Ga1 O1 Ga4 101.1(10) 3 2_646
O5 O1 Ga4 100.9(10) 2_646 2_646
O6 O1 Ga4 59.2(7) 4_535 2_646
La1 O1 Ga4 74.8(5) 1_645 2_646
La2 O1 Ga4 44.9(4) 3_645 2_646
O7 O1 Ga4 158.8(14) 2_556 2_646
La1 O1 Ga4 95.4(5) 4_645 2_646
O7 O1 Ga4 20.1(7) 4_646 2_646
O6 O1 Ga4 98.7(7) 4_645 2_646
Ga2 O1 Ga4 35.5(4) 3_545 2_646
Ga2 O1 Ga4 136.9(6) . 2_646
Ga2 O1 Ga4 75.3(7) 1_545 2_646
O5 O1 Ga4 87.7(11) 4_546 2_646
O1 O1 Ga4 54.3(7) 2_556 2_646
O1 O1 Ga4 88.3(8) 4_545 2_646
O1 O1 Ga4 160.3(16) 4 2_646
O1 O1 Ga4 108.8(2) 1_455 2_646
O1 O1 Ga4 71.2(2) 1_655 2_646
Ga2 O1 Ga3 69.8(16) 4_645 1_645
La1 O1 Ga3 45.1(8) 1_545 1_645
La2 O1 Ga3 143.4(16) 3_545 1_645
La1 O1 Ga3 100.7(15) 4_545 1_645
O3 O1 Ga3 80.8(14) 2_556 1_645
O2 O1 Ga3 138.9(17) 4_545 1_645
O4 O1 Ga3 89.7(16) 4_545 1_645
O7 O1 Ga3 100.1(15) 3_544 1_645
O6 O1 Ga3 23.7(7) 1_545 1_645
O3 O1 Ga3 49.0(10) 2_656 1_645
O4 O1 Ga3 56.8(16) 4_645 1_645
O2 O1 Ga3 98.0(12) 4_645 1_645
O5 O1 Ga3 129.6(15) 3_544 1_645
Ga2 O1 Ga3 107.7(12) 4_545 1_645
Ga4 O1 Ga3 72.3(8) 1_545 1_645
Ga3 O1 Ga3 129.5(6) 3_645 1_645
Ga4 O1 Ga3 36.9(5) 4_645 1_645
O4 O1 Ga3 64.8(15) . 1_645
O3 O1 Ga3 53.0(8) 3_544 1_645
O2 O1 Ga3 151.0(8) 3_545 1_645
O7 O1 Ga3 116.8(14) 4_546 1_645
O5 O1 Ga3 48.1(8) 2_546 1_645
O6 O1 Ga3 127.2(13) 4_545 1_645
O2 O1 Ga3 20.5(6) 1_545 1_645
O3 O1 Ga3 99.4(10) 3_554 1_645
Ga4 O1 Ga3 96.1(9) 1_445 1_645
Ga4 O1 Ga3 74.0(8) 4_545 1_645
Ga3 O1 Ga3 147.6(9) 3_545 1_645
O4 O1 Ga3 126.8(11) 3_545 1_645
Ta O1 Ga3 98.6(9) 3_545 1_645
Ga1 O1 Ga3 98.6(9) 3_545 1_645
Ga1 O1 Ga3 36.0(4) . 1_645
Ta O1 Ga3 36.0(4) . 1_645
Ta O1 Ga3 144.4(12) 3 1_645
Ga1 O1 Ga3 144.4(12) 3 1_645
O5 O1 Ga3 19.9(6) 2_646 1_645
O6 O1 Ga3 84.7(9) 4_535 1_645
La1 O1 Ga3 45.2(4) 1_645 1_645
La2 O1 Ga3 95.0(5) 3_645 1_645
O7 O1 Ga3 58.8(10) 2_556 1_645
La1 O1 Ga3 76.1(6) 4_645 1_645
O7 O1 Ga3 94.0(10) 4_646 1_645
O6 O1 Ga3 101.3(7) 4_645 1_645
Ga2 O1 Ga3 135.2(6) 3_545 1_645
Ga2 O1 Ga3 77.3(7) . 1_645
Ga2 O1 Ga3 35.2(4) 1_545 1_645
O5 O1 Ga3 164.0(13) 4_546 1_645
O1 O1 Ga3 157.9(6) 2_556 1_645
O1 O1 Ga3 52.4(10) 4_545 1_645
O1 O1 Ga3 90.2(15) 4 1_645
O1 O1 Ga3 108.6(2) 1_455 1_645
O1 O1 Ga3 71.4(2) 1_655 1_645
Ga4 O1 Ga3 108.2(8) 2_646 1_645
Ga2 O1 Ga4 74.6(15) 4_645 .
La1 O1 Ga4 149.1(18) 1_545 .
La2 O1 Ga4 102.4(14) 3_545 .
La1 O1 Ga4 46.7(8) 4_545 .
O3 O1 Ga4 103.1(14) 2_556 .
O2 O1 Ga4 82.2(15) 4_545 .
O4 O1 Ga4 143.1(15) 4_545 .
O7 O1 Ga4 128.1(16) 3_544 .
O6 O1 Ga4 100.4(13) 1_545 .
O3 O1 Ga4 71.4(10) 2_656 .
O4 O1 Ga4 110.0(13) 4_645 .
O2 O1 Ga4 50.5(11) 4_645 .
O5 O1 Ga4 18.0(10) 3_544 .
Ga2 O1 Ga4 110.8(11) 4_545 .
Ga4 O1 Ga4 129.5(7) 1_545 .
Ga3 O1 Ga4 38.4(5) 3_645 .
Ga4 O1 Ga4 75.0(8) 4_645 .
O4 O1 Ga4 49.4(13) . .
O3 O1 Ga4 150.6(6) 3_544 .
O2 O1 Ga4 64.0(10) 3_545 .
O7 O1 Ga4 131.2(16) 4_546 .
O5 O1 Ga4 122.9(14) 2_546 .
O6 O1 Ga4 44.8(6) 4_545 .
O2 O1 Ga4 132.1(11) 1_545 .
O3 O1 Ga4 20.9(5) 3_554 .
Ga4 O1 Ga4 147.8(9) 1_445 .
Ga4 O1 Ga4 98.8(9) 4_545 .
Ga3 O1 Ga4 75.9(8) 3_545 .
O4 O1 Ga4 97.8(11) 3_545 .
Ta O1 Ga4 142.6(12) 3_545 .
Ga1 O1 Ga4 142.6(12) 3_545 .
Ga1 O1 Ga4 102.4(10) . .
Ta O1 Ga4 102.4(10) . .
Ta O1 Ga4 36.6(4) 3 .
Ga1 O1 Ga4 36.6(4) 3 .
O5 O1 Ga4 98.5(9) 2_646 .
O6 O1 Ga4 163.4(13) 4_535 .
La1 O1 Ga4 96.8(5) 1_645 .
La2 O1 Ga4 77.0(5) 3_645 .
O7 O1 Ga4 90.4(11) 2_556 .
La1 O1 Ga4 46.6(4) 4_645 .
O7 O1 Ga4 104.6(11) 4_646 .
O6 O1 Ga4 20.7(4) 4_645 .
Ga2 O1 Ga4 77.6(7) 3_545 .
Ga2 O1 Ga4 36.8(4) . .
Ga2 O1 Ga4 137.2(6) 1_545 .
O5 O1 Ga4 60.9(9) 4_546 .
O1 O1 Ga4 88.9(7) 2_556 .
O1 O1 Ga4 159.4(17) 4_545 .
O1 O1 Ga4 53.9(3) 4 .
O1 O1 Ga4 108.9(3) 1_455 .
O1 O1 Ga4 71.1(3) 1_655 .
Ga4 O1 Ga4 110.6(8) 2_646 .
Ga3 O1 Ga4 111.6(8) 1_645 .
Ga2 O1 O4 145(2) 4_645 1_455
La1 O1 O4 77.8(11) 1_545 1_455
La2 O1 O4 103.5(9) 3_545 1_455
La1 O1 O4 38.6(7) 4_545 1_455
O3 O1 O4 19.2(10) 2_556 1_455
O2 O1 O4 48.6(14) 4_545 1_455
O4 O1 O4 63.6(7) 4_545 1_455
O7 O1 O4 134.7(12) 3_544 1_455
O6 O1 O4 70.6(11) 1_545 1_455
O3 O1 O4 115.9(17) 2_656 1_455
O4 O1 O4 149(2) 4_645 1_455
O2 O1 O4 134.9(18) 4_645 1_455
O5 O1 O4 83.8(13) 3_544 1_455
Ga2 O1 O4 38.6(9) 4_545 1_455
Ga4 O1 O4 145.5(14) 1_545 1_455
Ga3 O1 O4 114.7(14) 3_645 1_455
Ga4 O1 O4 85.5(12) 4_645 1_455
O4 O1 O4 72.5(14) . 1_455
O3 O1 O4 118.0(13) 3_544 1_455
O2 O1 O4 114.4(14) 3_545 1_455
O7 O1 O4 97.8(10) 4_546 1_455
O5 O1 O4 52.3(10) 2_546 1_455
O6 O1 O4 48.1(9) 4_545 1_455
O2 O1 O4 94.4(12) 1_545 1_455
O3 O1 O4 67.8(10) 3_554 1_455
Ga4 O1 O4 77.5(7) 1_445 1_455
Ga4 O1 O4 20.3(7) 4_545 1_455
Ga3 O1 O4 55.6(8) 3_545 1_455
O4 O1 O4 134.5(14) 3_545 1_455
Ta O1 O4 116.0(8) 3_545 1_455
Ga1 O1 O4 116.0(8) 3_545 1_455
Ga1 O1 O4 57.0(9) . 1_455
Ta O1 O4 57.0(9) . 1_455
Ta O1 O4 72.7(9) 3 1_455
Ga1 O1 O4 72.7(9) 3 1_455
O5 O1 O4 107.0(14) 2_646 1_455
O6 O1 O4 97.6(9) 4_535 1_455
La1 O1 O4 135.5(14) 1_645 1_455
La2 O1 O4 161.8(14) 3_645 1_455
O7 O1 O4 35.1(9) 2_556 1_455
La1 O1 O4 116.2(12) 4_645 1_455
O7 O1 O4 165.3(14) 4_646 1_455
O6 O1 O4 103.4(12) 4_645 1_455
Ga2 O1 O4 131.9(12) 3_545 1_455
Ga2 O1 O4 73.1(10) . 1_455
Ga2 O1 O4 114.6(13) 1_545 1_455
O5 O1 O4 72.9(11) 4_546 1_455
O1 O1 O4 97.4(8) 2_556 1_455
O1 O1 O4 83.5(12) 4_545 1_455
O1 O1 O4 34.9(9) 4 1_455
O1 O1 O4 37.3(8) 1_455 1_455
O1 O1 O4 142.7(8) 1_655 1_455
Ga4 O1 O4 145.7(10) 2_646 1_455
Ga3 O1 O4 92.8(11) 1_645 1_455
Ga4 O1 O4 84.8(10) . 1_455
Ga2 O1 O1 54.0(12) 4_645 2_656
La1 O1 O1 133.8(10) 1_545 2_656
La2 O1 O1 57.2(11) 3_545 2_656
La1 O1 O1 116.0(12) 4_545 2_656
O3 O1 O1 158.3(18) 2_556 2_656
O2 O1 O1 100(2) 4_545 2_656
O4 O1 O1 122.9(17) 4_545 2_656
O7 O1 O1 56.0(13) 3_544 2_656
O6 O1 O1 139.4(9) 1_545 2_656
O3 O1 O1 83.0(8) 2_656 2_656
O4 O1 O1 66.4(14) 4_645 2_656
O2 O1 O1 37.1(10) 4_645 2_656
O5 O1 O1 66.0(12) 3_544 2_656
Ga2 O1 O1 126.4(17) 4_545 2_656
Ga4 O1 O1 64.6(7) 1_545 2_656
Ga3 O1 O1 34.9(8) 3_645 2_656
Ga4 O1 O1 113.5(4) 4_645 2_656
O4 O1 O1 109.2(11) . 2_656
O3 O1 O1 93.7(7) 3_544 2_656
O2 O1 O1 30.5(8) 3_545 2_656
O7 O1 O1 78.5(13) 4_546 2_656
O5 O1 O1 162.3(10) 2_546 2_656
O6 O1 O1 97.9(10) 4_545 2_656
O2 O1 O1 121.4(7) 1_545 2_656
O3 O1 O1 93.2(6) 3_554 2_656
Ga4 O1 O1 107.7(11) 1_445 2_656
Ga4 O1 O1 164.5(11) 4_545 2_656
Ga3 O1 O1 91.5(12) 3_545 2_656
O4 O1 O1 30.9(9) 3_545 2_656
Ta O1 O1 73.4(8) 3_545 2_656
Ga1 O1 O1 73.4(8) 3_545 2_656
Ga1 O1 O1 153.8(9) . 2_656
Ta O1 O1 153.8(9) . 2_656
Ta O1 O1 72.7(8) 3 2_656
Ga1 O1 O1 72.7(8) 3 2_656
O5 O1 O1 103.4(7) 2_646 2_656
O6 O1 O1 97.2(9) 4_535 2_656
La1 O1 O1 75.7(3) 1_645 2_656
La2 O1 O1 26.0(2) 3_645 2_656
O7 O1 O1 161.5(10) 2_556 2_656
La1 O1 O1 66.4(3) 4_645 2_656
O7 O1 O1 36.1(10) 4_646 2_656
O6 O1 O1 61.2(5) 4_645 2_656
Ga2 O1 O1 17.3(5) 3_545 2_656
Ga2 O1 O1 101.1(3) . 2_656
Ga2 O1 O1 100.7(3) 1_545 2_656
O5 O1 O1 72.0(11) 4_546 2_656
O1 O1 O1 56.0(11) 2_556 2_656
O1 O1 O1 125.4(9) 4_545 2_656
O1 O1 O1 125.4(9) 4 2_656
O1 O1 O1 126.3(7) 1_455 2_656
O1 O1 O1 53.7(7) 1_655 2_656
Ga4 O1 O1 38.4(6) 2_646 2_656
Ga3 O1 O1 120.8(5) 1_645 2_656
Ga4 O1 O1 72.4(4) . 2_656
O4 O1 O1 144.3(13) 1_455 2_656
Ga2 O1 O1 56.7(16) 4_645 4_655
La1 O1 O1 116(2) 1_545 4_655
La2 O1 O1 137.4(17) 3_545 4_655
La1 O1 O1 57.0(6) 4_545 4_655
O3 O1 O1 100.6(17) 2_556 4_655
O2 O1 O1 113.1(14) 4_545 4_655
O4 O1 O1 148(2) 4_545 4_655
O7 O1 O1 135.5(12) 3_544 4_655
O6 O1 O1 66.8(14) 1_545 4_655
O3 O1 O1 38.1(11) 2_656 4_655
O4 O1 O1 86.9(14) 4_645 4_655
O2 O1 O1 52.5(10) 4_645 4_655
O5 O1 O1 55.9(10) 3_544 4_655
Ga2 O1 O1 127.8(12) 4_545 4_655
Ga4 O1 O1 114.3(6) 1_545 4_655
Ga3 O1 O1 65.2(6) 3_645 4_655
Ga4 O1 O1 37.9(9) 4_645 4_655
O4 O1 O1 20.6(10) . 4_655
O3 O1 O1 118.7(11) 3_544 4_655
O2 O1 O1 95.5(12) 3_545 4_655
O7 O1 O1 166.3(19) 4_546 4_655
O5 O1 O1 99.2(16) 2_546 4_655
O6 O1 O1 72.6(5) 4_545 4_655
O2 O1 O1 94.3(14) 1_545 4_655
O3 O1 O1 32.8(4) 3_554 4_655
Ga4 O1 O1 163.6(16) 1_445 4_655
Ga4 O1 O1 91.9(12) 4_545 4_655
Ga3 O1 O1 109.5(7) 3_545 4_655
O4 O1 O1 119.5(12) 3_545 4_655
Ta O1 O1 153.7(5) 3_545 4_655
Ga1 O1 O1 153.7(5) 3_545 4_655
Ga1 O1 O1 73.9(12) . 4_655
Ta O1 O1 73.9(12) . 4_655
Ta O1 O1 73.7(4) 3 4_655
Ga1 O1 O1 73.7(4) 3 4_655
O5 O1 O1 61.2(11) 2_646 4_655
O6 O1 O1 157.7(13) 4_535 4_655
La1 O1 O1 67.6(7) 1_645 4_655
La2 O1 O1 76.7(6) 3_645 4_655
O7 O1 O1 73.3(13) 2_556 4_655
La1 O1 O1 26.5(4) 4_645 4_655
O7 O1 O1 104.5(9) 4_646 4_655
O6 O1 O1 31.3(5) 4_645 4_655
Ga2 O1 O1 101.9(10) 3_545 4_655
Ga2 O1 O1 16.8(3) . 4_655
Ga2 O1 O1 101.5(10) 1_545 4_655
O5 O1 O1 98.3(10) 4_546 4_655
O1 O1 O1 125.5(12) 2_556 4_655
O1 O1 O1 125(2) 4_545 4_655
O1 O1 O1 55.9(6) 4 4_655
O1 O1 O1 126.2(4) 1_455 4_655
O1 O1 O1 53.8(4) 1_655 4_655
Ga4 O1 O1 121.5(8) 2_646 4_655
Ga3 O1 O1 73.9(11) 1_645 4_655
Ga4 O1 O1 37.9(3) . 4_655
O4 O1 O1 89.8(11) 1_455 4_655
O1 O1 O1 88.7(5) 2_656 4_655
Ga2 O1 O1 50.6(15) 4_645 4_645
La1 O1 O1 56.1(8) 1_545 4_645
La2 O1 O1 112.8(13) 3_545 4_645
La1 O1 O1 135(2) 4_545 4_645
O3 O1 O1 111.0(19) 2_556 4_645
O2 O1 O1 156.6(13) 4_545 4_645
O4 O1 O1 94.1(14) 4_545 4_645
O7 O1 O1 66.8(11) 3_544 4_645
O6 O1 O1 60.3(13) 1_545 4_645
O3 O1 O1 50.9(12) 2_656 4_645
O4 O1 O1 22.3(13) 4_645 4_645
O2 O1 O1 81.0(11) 4_645 4_645
O5 O1 O1 134.8(9) 3_544 4_645
Ga2 O1 O1 124.5(11) 4_545 4_645
Ga4 O1 O1 37.1(2) 1_545 4_645
Ga3 O1 O1 112.4(8) 3_645 4_645
Ga4 O1 O1 62.6(12) 4_645 4_645
O4 O1 O1 90.3(18) . 4_645
O3 O1 O1 30.5(4) 3_544 4_645
O2 O1 O1 118.5(13) 3_545 4_645
O7 O1 O1 95.9(9) 4_546 4_645
O5 O1 O1 75.8(13) 2_546 4_645
O6 O1 O1 159.8(14) 4_545 4_645
O2 O1 O1 33.1(8) 1_545 4_645
O3 O1 O1 121.1(10) 3_554 4_645
Ga4 O1 O1 90.8(5) 1_445 4_645
Ga4 O1 O1 106.9(14) 4_545 4_645
Ga3 O1 O1 161.9(9) 3_545 4_645
O4 O1 O1 90.3(10) 3_545 4_645
Ta O1 O1 72.3(4) 3_545 4_645
Ga1 O1 O1 72.3(4) 3_545 4_645
Ga1 O1 O1 71.8(12) . 4_645
Ta O1 O1 71.8(12) . 4_645
Ta O1 O1 154.1(6) 3 4_645
Ga1 O1 O1 154.1(6) 3 4_645
O5 O1 O1 32.0(11) 2_646 4_645
O6 O1 O1 70.2(4) 4_535 4_645
La1 O1 O1 24.7(6) 1_645 4_645
La2 O1 O1 65.6(6) 3_645 4_645
O7 O1 O1 94.9(16) 2_556 4_645
La1 O1 O1 74.6(7) 4_645 4_645
O7 O1 O1 57.7(8) 4_646 4_645
O6 O1 O1 101.9(6) 4_645 4_645
Ga2 O1 O1 100.0(10) 3_545 4_645
Ga2 O1 O1 100.1(11) . 4_645
Ga2 O1 O1 17.6(3) 1_545 4_645
O5 O1 O1 159.2(17) 4_546 4_645
O1 O1 O1 125.5(12) 2_556 4_645
O1 O1 O1 55.9(6) 4_545 4_645
O1 O1 O1 125(2) 4 4_645
O1 O1 O1 126.2(4) 1_455 4_645
O1 O1 O1 53.8(4) 1_655 4_645
Ga4 O1 O1 72.0(7) 2_646 4_645
Ga3 O1 O1 36.6(8) 1_645 4_645
Ga4 O1 O1 121.2(5) . 4_645
O4 O1 O1 127.0(17) 1_455 4_645
O1 O1 O1 88.7(5) 2_656 4_645
O1 O1 O1 88.5(9) 4_655 4_645
Ga2 O1 O2 141(2) 4_645 3_445
La1 O1 O2 105.0(8) 1_545 3_445
La2 O1 O2 39.9(7) 3_545 3_445
La1 O1 O2 76.4(10) 4_545 3_445
O3 O1 O2 70.9(12) 2_556 3_445
O2 O1 O2 17.4(14) 4_545 3_445
O4 O1 O2 60.3(14) 4_545 3_445
O7 O1 O2 83.1(12) 3_544 3_445
O6 O1 O2 132.8(9) 1_545 3_445
O3 O1 O2 161.0(17) 2_656 3_445
O4 O1 O2 139.0(19) 4_645 3_445
O2 O1 O2 114.3(15) 4_645 3_445
O5 O1 O2 73.3(12) 3_544 3_445
Ga2 O1 O2 40.5(8) 4_545 3_445
Ga4 O1 O2 112.8(12) 1_545 3_445
Ga3 O1 O2 82.3(9) 3_645 3_445
Ga4 O1 O2 147.8(12) 4_645 3_445
O4 O1 O2 123.0(17) . 3_445
O3 O1 O2 115.9(12) 3_544 3_445
O2 O1 O2 59.7(8) 3_545 3_445
O7 O1 O2 50.1(10) 4_546 3_445
O5 O1 O2 100.3(8) 2_546 3_445
O6 O1 O2 54.1(7) 4_545 3_445
O2 O1 O2 132.6(11) 1_545 3_445
O3 O1 O2 93.1(9) 3_554 3_445
Ga4 O1 O2 58.2(6) 1_445 3_445
Ga4 O1 O2 79.3(6) 4_545 3_445
Ga3 O1 O2 16.5(5) 3_545 3_445
O4 O1 O2 70.0(9) 3_545 3_445
Ta O1 O2 74.0(7) 3_545 3_445
Ga1 O1 O2 74.0(7) 3_545 3_445
Ga1 O1 O2 118.3(6) . 3_445
Ta O1 O2 118.3(6) . 3_445
Ta O1 O2 53.4(6) 3 3_445
Ga1 O1 O2 53.4(6) 3 3_445
O5 O1 O2 167.7(11) 2_646 3_445
O6 O1 O2 76.5(8) 4_535 3_445
La1 O1 O2 159.2(12) 1_645 3_445
La2 O1 O2 113.5(11) 3_645 3_445
O7 O1 O2 99.2(8) 2_556 3_445
La1 O1 O2 133.5(11) 4_645 3_445
O7 O1 O2 103.7(13) 4_646 3_445
O6 O1 O2 106.0(10) 4_645 3_445
Ga2 O1 O2 71.0(7) 3_545 3_445
Ga2 O1 O2 114.1(10) . 3_445
Ga2 O1 O2 132.6(9) 1_545 3_445
O5 O1 O2 30.3(7) 4_546 3_445
O1 O1 O2 33.1(5) 2_556 3_445
O1 O1 O2 100.1(9) 4_545 3_445
O1 O1 O2 83.5(9) 4 3_445
O1 O1 O2 39.7(6) 1_455 3_445
O1 O1 O2 140.3(6) 1_655 3_445
Ga4 O1 O2 84.3(8) 2_646 3_445
Ga3 O1 O2 147.8(8) 1_645 3_445
Ga4 O1 O2 90.0(9) . 3_445
O4 O1 O2 64.6(9) 1_455 3_445
O1 O1 O2 87.7(11) 2_656 3_445
O1 O1 O2 125.4(8) 4_655 3_445
O1 O1 O2 145.7(9) 4_645 3_445
Ga2 O1 La1 94.4(17) 4_645 4_535
La1 O1 La1 34.8(8) 1_545 4_535
La2 O1 La1 79.6(12) 3_545 4_535
La1 O1 La1 142.7(13) 4_545 4_535
O3 O1 La1 86.7(12) 2_556 4_535
O2 O1 La1 107.6(13) 4_545 4_535
O4 O1 La1 47.9(12) 4_545 4_535
O7 O1 La1 46.5(12) 3_544 4_535
O6 O1 La1 79.5(12) 1_545 4_535
O3 O1 La1 99.8(12) 2_656 4_535
O4 O1 La1 59.0(15) 4_645 4_535
O2 O1 La1 118.8(13) 4_645 4_535
O5 O1 La1 163.7(18) 3_544 4_535
Ga2 O1 La1 80.2(8) 4_545 4_535
Ga4 O1 La1 40.1(5) 1_545 4_535
Ga3 O1 La1 135.2(12) 3_645 4_535
Ga4 O1 La1 101.2(11) 4_645 4_535
O4 O1 La1 129.0(18) . 4_535
O3 O1 La1 18.9(4) 3_544 4_535
O2 O1 La1 113.9(13) 3_545 4_535
O7 O1 La1 52.7(10) 4_546 4_535
O5 O1 La1 63.1(11) 2_546 4_535
O6 O1 La1 146.1(5) 4_545 4_535
O2 O1 La1 44.4(7) 1_545 4_535
O3 O1 La1 162.7(13) 3_554 4_535
Ga4 O1 La1 41.8(4) 1_445 4_535
Ga4 O1 La1 90.0(7) 4_545 4_535
Ga3 O1 La1 113.2(7) 3_545 4_535
O4 O1 La1 78.2(9) 3_545 4_535
Ta O1 La1 35.9(4) 3_545 4_535
Ga1 O1 La1 35.9(4) 3_545 4_535
Ga1 O1 La1 80.3(7) . 4_535
Ta O1 La1 80.3(7) . 4_535
Ta O1 La1 150.2(10) 3 4_535
Ga1 O1 La1 150.2(10) 3 4_535
O5 O1 La1 74.8(10) 2_646 4_535
O6 O1 La1 21.8(4) 4_535 4_535
La1 O1 La1 73.0(6) 1_645 4_535
La2 O1 La1 92.8(7) 3_645 4_535
O7 O1 La1 95.7(11) 2_556 4_535
La1 O1 La1 123.1(7) 4_645 4_535
O7 O1 La1 66.3(10) 4_646 4_535
O6 O1 La1 148.3(6) 4_645 4_535
Ga2 O1 La1 97.9(9) 3_545 4_535
Ga2 O1 La1 141.7(11) . 4_535
Ga2 O1 La1 34.5(3) 1_545 4_535
O5 O1 La1 125.6(11) 4_546 4_535
O1 O1 La1 93.9(4) 2_556 4_535
O1 O1 La1 25.3(5) 4_545 4_535
O1 O1 La1 134.2(13) 4 4_535
O1 O1 La1 82.09(16) 1_455 4_535
O1 O1 La1 97.91(16) 1_655 4_535
Ga4 O1 La1 63.1(6) 2_646 4_535
Ga3 O1 La1 64.4(6) 1_645 4_535
Ga4 O1 La1 168.9(4) . 4_535
O4 O1 La1 105.4(10) 1_455 4_535
O1 O1 La1 100.3(5) 2_656 4_535
O1 O1 La1 135.9(11) 4_655 4_535
O1 O1 La1 49.17(8) 4_645 4_535
O2 O1 La1 98.2(7) 3_445 4_535
Ga2 O1 La1 99.8(18) 4_645 3_545
La1 O1 La1 142.1(12) 1_545 3_545
La2 O1 La1 37.9(9) 3_545 3_545
La1 O1 La1 83.8(13) 4_545 3_545
O3 O1 La1 109.4(12) 2_556 3_545
O2 O1 La1 51.4(15) 4_545 3_545
O4 O1 La1 98.7(15) 4_545 3_545
O7 O1 La1 76.7(14) 3_544 3_545
O6 O1 La1 161.7(15) 1_545 3_545
O3 O1 La1 121.9(13) 2_656 3_545
O4 O1 La1 114.3(18) 4_645 3_545
O2 O1 La1 72.1(13) 4_645 3_545
O5 O1 La1 47.3(13) 3_544 3_545
Ga2 O1 La1 82.6(9) 4_545 3_545
Ga4 O1 La1 102.1(11) 1_545 3_545
Ga3 O1 La1 41.5(6) 3_645 3_545
Ga4 O1 La1 139.2(11) 4_645 3_545
O4 O1 La1 113.6(17) . 3_545
O3 O1 La1 125.2(13) 3_544 3_545
O2 O1 La1 18.7(6) 3_545 3_545
O7 O1 La1 66.6(12) 4_546 3_545
O5 O1 La1 142.3(8) 2_546 3_545
O6 O1 La1 57.9(7) 4_545 3_545
O2 O1 La1 161.0(13) 1_545 3_545
O3 O1 La1 79.9(9) 3_554 3_545
Ga4 O1 La1 90.5(7) 1_445 3_545
Ga4 O1 La1 115.7(7) 4_545 3_545
Ga3 O1 La1 42.5(5) 3_545 3_545
O4 O1 La1 47.2(8) 3_545 3_545
Ta O1 La1 81.6(8) 3_545 3_545
Ga1 O1 La1 81.6(8) 3_545 3_545
Ga1 O1 La1 152.4(9) . 3_545
Ta O1 La1 152.4(9) . 3_545
Ta O1 La1 36.8(4) 3 3_545
Ga1 O1 La1 36.8(4) 3 3_545
O5 O1 La1 150.0(8) 2_646 3_545
O6 O1 La1 98.8(9) 4_535 3_545
La1 O1 La1 124.5(7) 1_645 3_545
La2 O1 La1 74.8(7) 3_645 3_545
O7 O1 La1 129.4(10) 2_556 3_545
La1 O1 La1 95.5(8) 4_645 3_545
O7 O1 La1 78.1(11) 4_646 3_545
O6 O1 La1 71.9(7) 4_645 3_545
Ga2 O1 La1 35.7(4) 3_545 3_545
Ga2 O1 La1 100.8(9) . 3_545
Ga2 O1 La1 141.2(11) 1_545 3_545
O5 O1 La1 23.6(7) 4_546 3_545
O1 O1 La1 24.3(5) 2_556 3_545
O1 O1 La1 133.5(13) 4_545 3_545
O1 O1 La1 94.7(10) 4 3_545
O1 O1 La1 81.75(15) 1_455 3_545
O1 O1 La1 98.25(15) 1_655 3_545
Ga4 O1 La1 66.0(6) 2_646 3_545
Ga3 O1 La1 169.6(4) 1_645 3_545
Ga4 O1 La1 64.7(6) . 3_545
O4 O1 La1 96.4(10) 1_455 3_545
O1 O1 La1 49.1(8) 2_656 3_545
O1 O1 La1 101.3(9) 4_655 3_545
O1 O1 La1 135.7(13) 4_645 3_545
O2 O1 La1 42.3(5) 3_445 3_545
La1 O1 La1 117.2(9) 4_535 3_545
Ga2 O1 La2 100.0(18) 4_645 .
La1 O1 La2 82.7(13) 1_545 .
La2 O1 La2 146.0(11) 3_545 .
La1 O1 La2 36.3(9) 4_545 .
O3 O1 La2 51.3(11) 2_556 .
O2 O1 La2 88.8(15) 4_545 .
O4 O1 La2 98.8(13) 4_545 .
O7 O1 La2 163.1(17) 3_544 .
O6 O1 La2 42.0(9) 1_545 .
O3 O1 La2 70.7(12) 2_656 .
O4 O1 La2 114.5(17) 4_645 .
O2 O1 La2 102.2(14) 4_645 .
O5 O1 La2 79.0(14) 3_544 .
Ga2 O1 La2 82.8(9) 4_545 .
Ga4 O1 La2 136.6(12) 1_545 .
Ga3 O1 La2 105.3(11) 3_645 .
Ga4 O1 La2 41.8(6) 4_645 .
O4 O1 La2 29.6(10) . .
O3 O1 La2 114.6(12) 3_544 .
O2 O1 La2 128.5(14) 3_545 .
O7 O1 La2 141.2(9) 4_546 .
O5 O1 La2 56.1(10) 2_546 .
O6 O1 La2 62.8(8) 4_545 .
O2 O1 La2 78.7(10) 1_545 .
O3 O1 La2 46.5(7) 3_554 .
Ga4 O1 La2 114.4(7) 1_445 .
Ga4 O1 La2 42.2(5) 4_545 .
Ga3 O1 La2 92.6(7) 3_545 .
O4 O1 La2 164.7(13) 3_545 .
Ta O1 La2 149.4(9) 3_545 .
Ga1 O1 La2 149.4(9) 3_545 .
Ga1 O1 La2 37.1(4) . .
Ta O1 La2 37.1(4) . .
Ta O1 La2 83.3(8) 3 .
Ga1 O1 La2 83.3(8) 3 .
O5 O1 La2 69.4(10) 2_646 .
O6 O1 La2 125.5(9) 4_535 .
La1 O1 La2 94.6(8) 1_645 .
La2 O1 La2 125.5(7) 3_645 .
O7 O1 La2 24.7(8) 2_556 .
La1 O1 La2 75.1(7) 4_645 .
O7 O1 La2 148.9(9) 4_646 .
O6 O1 La2 75.6(7) 4_645 .
Ga2 O1 La2 144.7(10) 3_545 .
Ga2 O1 La2 35.8(4) . .
Ga2 O1 La2 98.9(9) 1_545 .
O5 O1 La2 99.8(11) 4_546 .
O1 O1 La2 134.8(4) 2_556 .
O1 O1 La2 92.8(14) 4_545 .
O1 O1 La2 25.8(9) 4 .
O1 O1 La2 81.79(15) 1_455 .
O1 O1 La2 98.21(15) 1_655 .
Ga4 O1 La2 169.0(5) 2_646 .
Ga3 O1 La2 64.5(6) 1_645 .
Ga4 O1 La2 67.1(6) . .
O4 O1 La2 45.2(8) 1_455 .
O1 O1 La2 136.8(4) 2_656 .
O1 O1 La2 49.8(7) 4_655 .
O1 O1 La2 99.6(13) 4_645 .
O2 O1 La2 106.2(7) 3_445 .
La1 O1 La2 117.1(9) 4_535 .
La1 O1 La2 119.8(9) 3_545 .
Ga2 O1 O2 87.0(17) 4_645 .
La1 O1 O2 105.9(15) 1_545 .
La2 O1 O2 138.4(15) 3_545 .
La1 O1 O2 29.8(7) 4_545 .
O3 O1 O2 71.3(12) 2_556 .
O2 O1 O2 89.8(17) 4_545 .
O4 O1 O2 120.4(14) 4_545 .
O7 O1 O2 166.1(11) 3_544 .
O6 O1 O2 59.8(11) 1_545 .
O3 O1 O2 63.2(10) 2_656 .
O4 O1 O2 113.2(15) 4_645 .
O2 O1 O2 80.5(15) 4_645 .
O5 O1 O2 57.2(14) 3_544 .
Ga2 O1 O2 97.3(10) 4_545 .
Ga4 O1 O2 140.9(9) 1_545 .
Ga3 O1 O2 81.2(10) 3_645 .
Ga4 O1 O2 44.4(8) 4_645 .
O4 O1 O2 17.2(11) . .
O3 O1 O2 131.0(13) 3_544 .
O2 O1 O2 106.7(14) 3_545 .
O7 O1 O2 154.4(9) 4_546 .
O5 O1 O2 80.3(12) 2_546 .
O6 O1 O2 53.0(8) 4_545 .
O2 O1 O2 96.3(12) 1_545 .
O3 O1 O2 23.6(7) 3_554 .
Ga4 O1 O2 135.6(8) 1_445 .
Ga4 O1 O2 63.4(7) 4_545 .
Ga3 O1 O2 89.7(8) 3_545 .
O4 O1 O2 141.0(12) 3_545 .
Ta O1 O2 173.7(10) 3_545 .
Ga1 O1 O2 173.7(10) 3_545 .
Ga1 O1 O2 59.3(8) . .
Ta O1 O2 59.3(8) . .
Ta O1 O2 66.5(8) 3 .
Ga1 O1 O2 66.5(8) 3 .
O5 O1 O2 75.0(11) 2_646 .
O6 O1 O2 149.8(11) 4_535 .
La1 O1 O2 92.3(8) 1_645 .
La2 O1 O2 106.6(7) 3_645 .
O7 O1 O2 48.7(10) 2_556 .
La1 O1 O2 57.1(6) 4_645 .
O7 O1 O2 135.1(9) 4_646 .
O6 O1 O2 51.8(7) 4_645 .
Ga2 O1 O2 120.8(9) 3_545 .
Ga2 O1 O2 14.0(4) . .
Ga2 O1 O2 112.9(10) 1_545 .
O5 O1 O2 88.2(11) 4_546 .
O1 O1 O2 124.0(6) 2_556 .
O1 O1 O2 116.2(16) 4_545 .
O1 O1 O2 25.7(5) 4 .
O1 O1 O2 95.8(4) 1_455 .
O1 O1 O2 84.2(4) 1_655 .
Ga4 O1 O2 150.3(7) 2_646 .
Ga3 O1 O2 78.1(8) 1_645 .
Ga4 O1 O2 43.3(6) . .
O4 O1 O2 59.2(9) 1_455 .
O1 O1 O2 112.9(5) 2_656 .
O1 O1 O2 30.6(5) 4_655 .
O1 O1 O2 106.9(12) 4_645 .
O2 O1 O2 105.9(9) 3_445 .
La1 O1 O2 139.2(10) 4_535 .
La1 O1 O2 102.7(9) 3_545 .
La2 O1 O2 24.3(5) . .
Ga2 O1 O2 132(2) 4_645 1_445
La1 O1 O2 26.3(5) 1_545 1_445
La2 O1 O2 98.2(9) 3_545 1_445
La1 O1 O2 91.5(10) 4_545 1_445
O3 O1 O2 35.6(9) 2_556 1_445
O2 O1 O2 78.8(12) 4_545 1_445
O4 O1 O2 28.6(13) 4_545 1_445
O7 O1 O2 92.3(13) 3_544 1_445
O6 O1 O2 58.8(9) 1_545 1_445
O3 O1 O2 113.5(15) 2_656 1_445
O4 O1 O2 102.1(19) 4_645 1_445
O2 O1 O2 162.4(15) 4_645 1_445
O5 O1 O2 138.0(11) 3_544 1_445
Ga2 O1 O2 44.2(7) 4_545 1_445
Ga4 O1 O2 91.0(10) 1_545 1_445
Ga3 O1 O2 164.6(9) 3_645 1_445
Ga4 O1 O2 89.5(10) 4_645 1_445
O4 O1 O2 101.7(15) . 1_445
O3 O1 O2 63.7(7) 3_544 1_445
O2 O1 O2 138.8(12) 3_545 1_445
O7 O1 O2 71.9(11) 4_546 1_445
O5 O1 O2 22.9(8) 2_546 1_445
O6 O1 O2 101.2(7) 4_545 1_445
O2 O1 O2 52.1(6) 1_545 1_445
O3 O1 O2 117.9(11) 3_554 1_445
Ga4 O1 O2 42.1(6) 1_445 1_445
Ga4 O1 O2 39.0(6) 4_545 1_445
Ga3 O1 O2 88.0(5) 3_545 1_445
O4 O1 O2 118.0(10) 3_545 1_445
Ta O1 O2 74.5(7) 3_545 1_445
Ga1 O1 O2 74.5(7) 3_545 1_445
Ga1 O1 O2 48.5(5) . 1_445
Ta O1 O2 48.5(5) . 1_445
Ta O1 O2 122.9(6) 3 1_445
Ga1 O1 O2 122.9(6) 3 1_445
O5 O1 O2 84.9(10) 2_646 1_445
O6 O1 O2 50.7(7) 4_535 1_445
La1 O1 O2 104.5(9) 1_645 1_445
La2 O1 O2 143.3(11) 3_645 1_445
O7 O1 O2 50.6(9) 2_556 1_445
La1 O1 O2 138.4(11) 4_645 1_445
O7 O1 O2 117.5(13) 4_646 1_445
O6 O1 O2 150.9(12) 4_645 1_445
Ga2 O1 O2 136.4(10) 3_545 1_445
Ga2 O1 O2 110.9(10) . 1_445
Ga2 O1 O2 65.5(7) 1_545 1_445
O5 O1 O2 110.0(7) 4_546 1_445
O1 O1 O2 105.6(6) 2_556 1_445
O1 O1 O2 29.2(7) 4_545 1_445
O1 O1 O2 84.0(10) 4 1_445
O1 O1 O2 45.6(5) 1_455 1_445
O1 O1 O2 134.4(5) 1_655 1_445
Ga4 O1 O2 109.9(9) 2_646 1_445
Ga3 O1 O2 65.0(6) 1_645 1_445
Ga4 O1 O2 137.9(9) . 1_445
O4 O1 O2 54.6(9) 1_455 1_445
O1 O1 O2 147.9(8) 2_656 1_445
O1 O1 O2 121.7(14) 4_655 1_445
O1 O1 O2 82.3(9) 4_645 1_445
O2 O1 O2 82.8(5) 3_445 1_445
La1 O1 O2 51.3(6) 4_535 1_445
La1 O1 O2 124.6(6) 3_545 1_445
La2 O1 O2 75.2(7) . 1_445
O2 O1 O2 99.2(9) . 1_445
Ga2 O1 O4 126(2) 4_645 3_445
La1 O1 O4 93.6(10) 1_545 3_445
La2 O1 O4 19.0(5) 3_545 3_445
La1 O1 O4 105.6(12) 4_545 3_445
O3 O1 O4 86.2(11) 2_556 3_445
O2 O1 O4 45.8(14) 4_545 3_445
O4 O1 O4 52.3(16) 4_545 3_445
O7 O1 O4 54.4(9) 3_544 3_445
O6 O1 O4 139.6(11) 1_545 3_445
O3 O1 O4 156.7(15) 2_656 3_445
O4 O1 O4 110.6(18) 4_645 3_445
O2 O1 O4 111.9(17) 4_645 3_445
O5 O1 O4 93.2(15) 3_544 3_445
Ga2 O1 O4 52.1(9) 4_545 3_445
Ga4 O1 O4 83.6(10) 1_545 3_445
Ga3 O1 O4 88.1(11) 3_645 3_445
Ga4 O1 O4 170.1(11) 4_645 3_445
O4 O1 O4 152(2) . 3_445
O3 O1 O4 89.5(10) 3_544 3_445
O2 O1 O4 58.3(10) 3_545 3_445
O7 O1 O4 22.0(10) 4_546 3_445
O5 O1 O4 103.2(10) 2_546 3_445
O6 O1 O4 82.7(9) 4_545 3_445
O2 O1 O4 116.7(12) 1_545 3_445
O3 O1 O4 120.0(12) 3_554 3_445
Ga4 O1 O4 42.1(6) 1_445 3_445
Ga4 O1 O4 95.8(6) 4_545 3_445
Ga3 O1 O4 45.5(7) 3_545 3_445
O4 O1 O4 49.2(7) 3_545 3_445
Ta O1 O4 45.1(6) 3_545 3_445
Ga1 O1 O4 45.1(6) 3_545 3_445
Ga1 O1 O4 128.1(7) . 3_445
Ta O1 O4 128.1(7) . 3_445
Ta O1 O4 76.0(9) 3 3_445
Ga1 O1 O4 76.0(9) 3 3_445
O5 O1 O4 148.3(15) 2_646 3_445
O6 O1 O4 52.9(7) 4_535 3_445
La1 O1 O4 131.5(11) 1_645 3_445
La2 O1 O4 97.9(10) 3_645 3_445
O7 O1 O4 117.5(7) 2_556 3_445
La1 O1 O4 140.7(12) 4_645 3_445
O7 O1 O4 78.9(12) 4_646 3_445
O6 O1 O4 120.4(12) 4_645 3_445
Ga2 O1 O4 59.3(7) 3_545 3_445
Ga2 O1 O4 142.1(12) . 3_445
Ga2 O1 O4 107.7(10) 1_545 3_445
O5 O1 O4 51.5(9) 4_546 3_445
O1 O1 O4 25.4(6) 2_556 3_445
O1 O1 O4 85.1(10) 4_545 3_445
O1 O1 O4 112.2(11) 4 3_445
O1 O1 O4 52.6(6) 1_455 3_445
O1 O1 O4 127.4(6) 1_655 3_445
Ga4 O1 O4 58.7(7) 2_646 3_445
Ga3 O1 O4 137.1(10) 1_645 3_445
Ga4 O1 O4 111.1(11) . 3_445
O4 O1 O4 87.3(8) 1_455 3_445
O1 O1 O4 76.2(11) 2_656 3_445
O1 O1 O4 149.0(13) 4_655 3_445
O1 O1 O4 117.5(9) 4_645 3_445
O2 O1 O4 29.2(7) 3_445 3_445
La1 O1 O4 74.2(7) 4_535 3_445
La1 O1 O4 48.5(7) 3_545 3_445
La2 O1 O4 132.2(7) . 3_445
O2 O1 O4 135.1(10) . 3_445
O2 O1 O4 80.8(7) 1_445 3_445
Ga2 O1 O4 76.7(17) 4_645 1_545
La1 O1 O4 35.6(8) 1_545 1_545
La2 O1 O4 97.3(15) 3_545 1_545
La1 O1 O4 141.9(18) 4_545 1_545
O3 O1 O4 94.5(14) 2_556 1_545
O2 O1 O4 128.7(15) 4_545 1_545
O4 O1 O4 66.5(17) 4_545 1_545
O7 O1 O4 55.9(15) 3_544 1_545
O6 O1 O4 65.8(12) 1_545 1_545
O3 O1 O4 78.0(11) 2_656 1_545
O4 O1 O4 42.5(17) 4_645 1_545
O2 O1 O4 105.2(13) 4_645 1_545
O5 O1 O4 161.2(8) 3_544 1_545
Ga2 O1 O4 98.0(11) 4_545 1_545
Ga4 O1 O4 35.1(8) 1_545 1_545
Ga3 O1 O4 131.9(10) 3_645 1_545
Ga4 O1 O4 81.6(10) 4_645 1_545
O4 O1 O4 110.4(19) . 1_545
O3 O1 O4 7.3(9) 3_544 1_545
O2 O1 O4 122.7(14) 3_545 1_545
O7 O1 O4 73.1(12) 4_546 1_545
O5 O1 O4 62.7(11) 2_546 1_545
O6 O1 O4 161.4(10) 4_545 1_545
O2 O1 O4 28.7(9) 1_545 1_545
O3 O1 O4 144.7(11) 3_554 1_545
Ga4 O1 O4 63.0(8) 1_445 1_545
Ga4 O1 O4 94.3(9) 4_545 1_545
Ga3 O1 O4 134.9(9) 3_545 1_545
O4 O1 O4 86.9(11) 3_545 1_545
Ta O1 O4 52.6(8) 3_545 1_545
Ga1 O1 O4 52.6(8) 3_545 1_545
Ga1 O1 O4 71.3(9) . 1_545
Ta O1 O4 71.3(9) . 1_545
Ta O1 O4 169.2(13) 3 1_545
Ga1 O1 O4 169.2(13) 3 1_545
O5 O1 O4 53.4(10) 2_646 1_545
O6 O1 O4 43.6(8) 4_535 1_545
La1 O1 O4 52.5(7) 1_645 1_545
La2 O1 O4 83.6(8) 3_645 1_545
O7 O1 O4 91.8(13) 2_556 1_545
La1 O1 O4 102.5(7) 4_645 1_545
O7 O1 O4 63.6(11) 4_646 1_545
O6 O1 O4 129.7(7) 4_645 1_545
Ga2 O1 O4 103.8(10) 3_545 1_545
Ga2 O1 O4 122.3(10) . 1_545
Ga2 O1 O4 12.8(6) 1_545 1_545
O5 O1 O4 146.4(13) 4_546 1_545
O1 O1 O4 111.8(8) 2_556 1_545
O1 O1 O4 31.2(4) 4_545 1_545
O1 O1 O4 131.0(17) 4 1_545
O1 O1 O4 99.9(5) 1_455 1_545
O1 O1 O4 80.1(5) 1_655 1_545
Ga4 O1 O4 68.7(8) 2_646 1_545
Ga3 O1 O4 46.1(7) 1_645 1_545
Ga4 O1 O4 149.1(7) . 1_545
O4 O1 O4 113.5(13) 1_455 1_545
O1 O1 O4 99.6(6) 2_656 1_545
O1 O1 O4 114.3(11) 4_655 1_545
O1 O1 O4 28.0(5) 4_645 1_545
O2 O1 O4 120.0(10) 3_445 1_545
La1 O1 O4 21.8(5) 4_535 1_545
La1 O1 O4 132.4(11) 3_545 1_545
La2 O1 O4 107.4(10) . 1_545
O2 O1 O4 124.1(11) . 1_545
O2 O1 O4 60.3(7) 1_445 1_545
O4 O1 O4 95.1(10) 3_445 1_545
Ga2 O1 La2 157(2) 4_645 3_445
La1 O1 La2 81.7(5) 1_545 3_445
La2 O1 La2 48.8(3) 3_545 3_445
La1 O1 La2 83.4(5) 4_545 3_445
O3 O1 La2 56.0(9) 2_556 3_445
O2 O1 La2 28.1(11) 4_545 3_445
O4 O1 La2 37.1(12) 4_545 3_445
O7 O1 La2 80.3(10) 3_544 3_445
O6 O1 La2 114.9(8) 1_545 3_445
O3 O1 La2 172.2(16) 2_656 3_445
O4 O1 La2 133.3(17) 4_645 3_445
O2 O1 La2 136.4(17) 4_645 3_445
O5 O1 La2 94.9(11) 3_544 3_445
Ga2 O1 La2 21.9(5) 4_545 3_445
Ga4 O1 La2 105.6(9) 1_545 3_445
Ga3 O1 La2 105.4(10) 3_645 3_445
Ga4 O1 La2 140.7(9) 4_645 3_445
O4 O1 La2 128.3(13) . 3_445
O3 O1 La2 98.3(7) 3_544 3_445
O2 O1 La2 80.5(9) 3_545 3_445
O7 O1 La2 42.3(8) 4_546 3_445
O5 O1 La2 79.3(7) 2_546 3_445
O6 O1 La2 68.2(5) 4_545 3_445
O2 O1 La2 109.3(8) 1_545 3_445
O3 O1 La2 107.6(8) 3_554 3_445
Ga4 O1 La2 37.8(2) 1_445 3_445
Ga4 O1 La2 65.56(18) 4_545 3_445
Ga3 O1 La2 34.4(2) 3_545 3_445
O4 O1 La2 79.7(8) 3_545 3_445
Ta O1 La2 65.1(4) 3_545 3_445
Ga1 O1 La2 65.1(4) 3_545 3_445
Ga1 O1 La2 101.1(4) . 3_445
Ta O1 La2 101.1(4) . 3_445
Ta O1 La2 74.7(5) 3 3_445
Ga1 O1 La2 74.7(5) 3 3_445
O5 O1 La2 144.7(11) 2_646 3_445
O6 O1 La2 59.2(4) 4_535 3_445
La1 O1 La2 152.0(10) 1_645 3_445
La2 O1 La2 128.2(10) 3_645 3_445
O7 O1 La2 87.1(6) 2_556 3_445
La1 O1 La2 156.1(11) 4_645 3_445
O7 O1 La2 108.3(12) 4_646 3_445
O6 O1 La2 128.2(10) 4_645 3_445
Ga2 O1 La2 87.4(7) 3_545 3_445
Ga2 O1 La2 124.3(7) . 3_445
Ga2 O1 La2 112.5(7) 1_545 3_445
O5 O1 La2 53.2(6) 4_546 3_445
O1 O1 La2 49.1(3) 2_556 3_445
O1 O1 La2 77.2(6) 4_545 3_445
O1 O1 La2 86.7(6) 4 3_445
O1 O1 La2 22.2(5) 1_455 3_445
O1 O1 La2 157.8(5) 1_655 3_445
Ga4 O1 La2 88.4(7) 2_646 3_445
Ga3 O1 La2 125.0(7) 1_645 3_445
Ga4 O1 La2 110.1(7) . 3_445
O4 O1 La2 57.3(7) 1_455 3_445
O1 O1 La2 104.8(11) 2_656 3_445
O1 O1 La2 139.8(5) 4_655 3_445
O1 O1 La2 128.7(5) 4_645 3_445
O2 O1 La2 23.4(5) 3_445 3_445
La1 O1 La2 79.5(4) 4_535 3_445
La1 O1 La2 64.6(4) 3_545 3_445
La2 O1 La2 102.6(4) . 3_445
O2 O1 La2 112.3(6) . 3_445
O2 O1 La2 60.0(5) 1_445 3_445
O4 O1 La2 30.6(5) 3_445 3_445
O4 O1 La2 100.8(7) 1_545 3_445
Ga2 O1 La1 155(2) 4_645 1_445
La1 O1 La1 48.6(2) 1_545 1_445
La2 O1 La1 81.7(5) 3_545 1_445
La1 O1 La1 82.6(5) 4_545 1_445
O3 O1 La1 29.8(8) 2_556 1_445
O2 O1 La1 55.6(11) 4_545 1_445
O4 O1 La1 19.6(10) 4_545 1_445
O7 O1 La1 92.7(11) 3_544 1_445
O6 O1 La1 78.2(8) 1_545 1_445
O3 O1 La1 135.3(16) 2_656 1_445
O4 O1 La1 121.3(18) 4_645 1_445
O2 O1 La1 174.0(17) 4_645 1_445
O5 O1 La1 119.9(9) 3_544 1_445
Ga2 O1 La1 21.0(5) 4_545 1_445
Ga4 O1 La1 102.9(9) 1_545 1_445
Ga3 O1 La1 141.3(9) 3_645 1_445
Ga4 O1 La1 107.3(10) 4_645 1_445
O4 O1 La1 110.0(14) . 1_445
O3 O1 La1 80.4(7) 3_544 1_445
O2 O1 La1 118.0(9) 3_545 1_445
O7 O1 La1 61.2(8) 4_546 1_445
O5 O1 La1 41.9(7) 2_546 1_445
O6 O1 La1 83.7(4) 4_545 1_445
O2 O1 La1 75.4(7) 1_545 1_445
O3 O1 La1 112.0(8) 3_554 1_445
Ga4 O1 La1 34.6(2) 1_445 1_445
Ga4 O1 La1 38.3(2) 4_545 1_445
Ga3 O1 La1 64.75(18) 3_545 1_445
O4 O1 La1 108.6(8) 3_545 1_445
Ta O1 La1 73.4(4) 3_545 1_445
Ga1 O1 La1 73.4(4) 3_545 1_445
Ga1 O1 La1 65.3(4) . 1_445
Ta O1 La1 65.3(4) . 1_445
Ta O1 La1 101.8(4) 3 1_445
Ga1 O1 La1 101.8(4) 3 1_445
O5 O1 La1 108.0(10) 2_646 1_445
O6 O1 La1 53.3(4) 4_535 1_445
La1 O1 La1 127.3(10) 1_645 1_445
La2 O1 La1 152.3(11) 3_645 1_445
O7 O1 La1 57.9(7) 2_556 1_445
La1 O1 La1 154.9(11) 4_645 1_445
O7 O1 La1 123.1(12) 4_646 1_445
O6 O1 La1 147.2(9) 4_645 1_445
Ga2 O1 La1 122.2(8) 3_545 1_445
Ga2 O1 La1 114.8(8) . 1_445
Ga2 O1 La1 86.5(6) 1_545 1_445
O5 O1 La1 86.6(6) 4_546 1_445
O1 O1 La1 85.7(3) 2_556 1_445
O1 O1 La1 48.3(5) 4_545 1_445
O1 O1 La1 78.8(7) 4 1_445
O1 O1 La1 22.5(5) 1_455 1_445
O1 O1 La1 157.5(5) 1_655 1_445
Ga4 O1 La1 108.1(7) 2_646 1_445
Ga3 O1 La1 88.1(7) 1_645 1_445
Ga4 O1 La1 127.2(7) . 1_445
O4 O1 La1 44.3(7) 1_455 1_445
O1 O1 La1 138.6(11) 2_656 1_445
O1 O1 La1 130.2(12) 4_655 1_445
O1 O1 La1 104.0(8) 4_645 1_445
O2 O1 La1 59.7(5) 3_445 1_445
La1 O1 La1 63.8(4) 4_535 1_445
La1 O1 La1 101.9(4) 3_545 1_445
La2 O1 La1 80.5(5) . 1_445
O2 O1 La1 101.0(7) . 1_445
O2 O1 La1 23.4(4) 1_445 1_445
O4 O1 La1 62.9(5) 3_445 1_445
O4 O1 La1 78.9(7) 1_545 1_445
La2 O1 La1 37.58(11) 3_445 1_445
Ga2 O1 La1 162(2) 4_645 4_445
La1 O1 La1 82.7(5) 1_545 4_445
La2 O1 La1 83.5(5) 3_545 4_445
La1 O1 La1 49.0(3) 4_545 4_445
O3 O1 La1 28.5(9) 2_556 4_445
O2 O1 La1 30.2(12) 4_545 4_445
O4 O1 La1 54.1(10) 4_545 4_445
O7 O1 La1 117.9(10) 3_544 4_445
O6 O1 La1 88.7(8) 1_545 4_445
O3 O1 La1 135.6(15) 2_656 4_445
O4 O1 La1 158.6(19) 4_645 4_445
O2 O1 La1 138.6(15) 4_645 4_445
O5 O1 La1 82.6(10) 3_544 4_445
Ga2 O1 La1 23.1(5) 4_545 4_445
Ga4 O1 La1 138.5(8) 1_545 4_445
Ga3 O1 La1 109.3(9) 3_645 4_445
Ga4 O1 La1 105.5(10) 4_645 4_445
O4 O1 La1 90.5(13) . 4_445
O3 O1 La1 118.2(7) 3_544 4_445
O2 O1 La1 99.7(10) 3_545 4_445
O7 O1 La1 79.9(8) 4_546 4_445
O5 O1 La1 63.2(7) 2_546 4_445
O6 O1 La1 46.0(4) 4_545 4_445
O2 O1 La1 105.4(8) 1_545 4_445
O3 O1 La1 77.6(7) 3_554 4_445
Ga4 O1 La1 65.1(2) 1_445 4_445
Ga4 O1 La1 35.28(19) 4_545 4_445
Ga3 O1 La1 38.5(2) 3_545 4_445
O4 O1 La1 114.6(9) 3_545 4_445
Ta O1 La1 101.0(4) 3_545 4_445
Ga1 O1 La1 101.0(4) 3_545 4_445
Ga1 O1 La1 74.5(5) . 4_445
Ta O1 La1 74.5(5) . 4_445
Ta O1 La1 66.3(4) 3 4_445
Ga1 O1 La1 66.3(4) 3 4_445
O5 O1 La1 125.6(11) 2_646 4_445
O6 O1 La1 87.4(4) 4_535 4_445
La1 O1 La1 154.0(11) 1_645 4_445
La2 O1 La1 155.5(11) 3_645 4_445
O7 O1 La1 54.2(6) 2_556 4_445
La1 O1 La1 130.4(10) 4_645 4_445
O7 O1 La1 146.3(12) 4_646 4_445
O6 O1 La1 110.3(9) 4_645 4_445
Ga2 O1 La1 114.8(8) 3_545 4_445
Ga2 O1 La1 88.6(7) . 4_445
Ga2 O1 La1 122.0(7) 1_545 4_445
O5 O1 La1 58.8(6) 4_546 4_445
O1 O1 La1 78.1(3) 2_556 4_445
O1 O1 La1 85.0(6) 4_545 4_445
O1 O1 La1 49.6(5) 4 4_445
O1 O1 La1 21.3(4) 1_455 4_445
O1 O1 La1 158.7(4) 1_655 4_445
Ga4 O1 La1 126.1(7) 2_646 4_445
Ga3 O1 La1 109.1(8) 1_645 4_445
Ga4 O1 La1 89.7(7) . 4_445
O4 O1 La1 20.1(7) 1_455 4_445
O1 O1 La1 130.1(11) 2_656 4_445
O1 O1 La1 105.3(7) 4_655 4_445
O1 O1 La1 138.1(11) 4_645 4_445
O2 O1 La1 45.0(5) 3_445 4_445
La1 O1 La1 101.3(4) 4_535 4_445
La1 O1 La1 81.0(5) 3_545 4_445
La2 O1 La1 64.8(4) . 4_445
O2 O1 La1 75.3(6) . 4_445
O2 O1 La1 56.6(4) 1_445 4_445
O4 O1 La1 67.4(6) 3_445 4_445
O4 O1 La1 116.2(7) 1_545 4_445
La2 O1 La1 38.11(12) 3_445 4_445
La1 O1 La1 37.82(10) 1_445 4_445
Ga2 O1 O4 28.6(14) 4_645 1_655
La1 O1 O4 108.9(12) 1_545 1_655
La2 O1 O4 130.7(11) 3_545 1_655
La1 O1 O4 85.9(10) 4_545 1_655
O3 O1 O4 122.6(17) 2_556 1_655
O2 O1 O4 139.0(18) 4_545 1_655
O4 O1 O4 153.9(18) 4_545 1_655
O7 O1 O4 108.1(13) 3_544 1_655
O6 O1 O4 69.6(9) 1_545 1_655
O3 O1 O4 15.7(9) 2_656 1_655
O4 O1 O4 58.4(8) 4_645 1_655
O2 O1 O4 37.9(12) 4_645 1_655
O5 O1 O4 72.6(11) 3_544 1_655
Ga2 O1 O4 155.1(15) 4_545 1_655
Ga4 O1 O4 85.5(7) 1_545 1_655
Ga3 O1 O4 65.6(6) 3_645 1_655
Ga4 O1 O4 40.2(6) 4_645 1_655
O4 O1 O4 44.0(7) . 1_655
O3 O1 O4 94.5(9) 3_544 1_655
O2 O1 O4 93.3(10) 3_545 1_655
O7 O1 O4 145.7(11) 4_546 1_655
O5 O1 O4 106.2(12) 2_546 1_655
O6 O1 O4 99.1(10) 4_545 1_655
O2 O1 O4 81.8(9) 1_545 1_655
O3 O1 O4 60.2(6) 3_554 1_655
Ga4 O1 O4 155.1(12) 1_445 1_655
Ga4 O1 O4 113.0(11) 4_545 1_655
Ga3 O1 O4 132.9(11) 3_545 1_655
O4 O1 O4 102.0(9) 3_545 1_655
Ta O1 O4 125.0(8) 3_545 1_655
Ga1 O1 O4 125.0(8) 3_545 1_655
Ga1 O1 O4 82.1(8) . 1_655
Ta O1 O4 82.1(8) . 1_655
Ta O1 O4 92.8(8) 3 1_655
Ga1 O1 O4 92.8(8) 3 1_655
O5 O1 O4 45.6(7) 2_646 1_655
O6 O1 O4 133.5(10) 4_535 1_655
La1 O1 O4 40.7(5) 1_645 1_655
La2 O1 O4 53.7(6) 3_645 1_655
O7 O1 O4 91.7(12) 2_556 1_655
La1 O1 O4 12.0(5) 4_645 1_655
O7 O1 O4 78.1(8) 4_646 1_655
O6 O1 O4 39.5(6) 4_645 1_655
Ga2 O1 O4 90.3(6) 3_545 1_655
Ga2 O1 O4 45.4(5) . 1_655
Ga2 O1 O4 80.3(7) 1_545 1_655
O5 O1 O4 115.2(11) 4_546 1_655
O1 O1 O4 126.3(11) 2_556 1_655
O1 O1 O4 114.4(13) 4_545 1_655
O1 O1 O4 84.2(8) 4 1_655
O1 O1 O4 153.8(7) 1_455 1_655
O1 O1 O4 26.2(7) 1_655 1_655
Ga4 O1 O4 97.2(6) 2_646 1_655
Ga3 O1 O4 64.2(6) 1_645 1_655
Ga4 O1 O4 57.0(6) . 1_655
O4 O1 O4 116.6(14) 1_455 1_655
O1 O1 O4 73.5(7) 2_656 1_655
O1 O1 O4 28.9(7) 4_655 1_655
O1 O1 O4 64.3(8) 4_645 1_655
O2 O1 O4 145.4(12) 3_445 1_655
La1 O1 O4 113.4(8) 4_535 1_655
La1 O1 O4 107.1(8) 3_545 1_655
La2 O1 O4 72.4(7) . 1_655
O2 O1 O4 58.5(7) . 1_655
O2 O1 O4 127.7(11) 1_445 1_655
O4 O1 O4 149.7(13) 3_445 1_655
O4 O1 O4 92.1(9) 1_545 1_655
La2 O1 O4 167.1(11) 3_445 1_655
La1 O1 O4 147.4(11) 1_445 1_655
La1 O1 O4 133.8(10) 4_445 1_655
Ga2 O1 O4 117.4(19) 4_645 4
La1 O1 O4 120.0(12) 1_545 4
La2 O1 O4 97.3(12) 3_545 4
La1 O1 O4 15.7(10) 4_545 4
O3 O1 O4 62.1(11) 2_556 4
O2 O1 O4 47.9(13) 4_545 4
O4 O1 O4 99.9(12) 4_545 4
O7 O1 O4 143.0(16) 3_544 4
O6 O1 O4 93.6(13) 1_545 4
O3 O1 O4 103.5(14) 2_656 4
O4 O1 O4 152.0(18) 4_645 4
O2 O1 O4 94.2(15) 4_645 4
O5 O1 O4 41.0(9) 3_544 4
Ga2 O1 O4 68.0(8) 4_545 4
Ga4 O1 O4 169.9(14) 1_545 4
Ga3 O1 O4 72.3(10) 3_645 4
Ga4 O1 O4 87.2(11) 4_645 4
O4 O1 O4 60.0(16) . 4
O3 O1 O4 160.6(11) 3_544 4
O2 O1 O4 81.3(12) 3_545 4
O7 O1 O4 112.9(11) 4_546 4
O5 O1 O4 92.3(11) 2_546 4
O6 O1 O4 10.8(7) 4_545 4
O2 O1 O4 128.9(12) 1_545 4
O3 O1 O4 33.6(7) 3_554 4
Ga4 O1 O4 109.3(5) 1_445 4
Ga4 O1 O4 61.0(7) 4_545 4
Ga3 O1 O4 46.7(6) 3_545 4
O4 O1 O4 115.6(12) 3_545 4
Ta O1 O4 137.0(8) 3_545 4
Ga1 O1 O4 137.0(8) 3_545 4
Ga1 O1 O4 85.4(9) . 4
Ta O1 O4 85.4(9) . 4
Ta O1 O4 34.0(7) 3 4
Ga1 O1 O4 34.0(7) 3 4
O5 O1 O4 117.8(13) 2_646 4
O6 O1 O4 132.0(6) 4_535 4
La1 O1 O4 133.3(10) 1_645 4
La2 O1 O4 119.2(10) 3_645 4
O7 O1 O4 63.7(10) 2_556 4
La1 O1 O4 86.6(9) 4_645 4
O7 O1 O4 141.5(15) 4_646 4
O6 O1 O4 64.4(8) 4_645 4
Ga2 O1 O4 100.6(10) 3_545 4
Ga2 O1 O4 51.5(7) . 4
Ga2 O1 O4 150.3(12) 1_545 4
O5 O1 O4 47.9(10) 4_546 4
O1 O1 O4 83.9(6) 2_556 4
O1 O1 O4 126.3(10) 4_545 4
O1 O1 O4 26.4(9) 4 4
O1 O1 O4 66.1(5) 1_455 4
O1 O1 O4 113.9(5) 1_655 4
Ga4 O1 O4 134.3(11) 2_646 4
Ga3 O1 O4 116.4(11) 1_645 4
Ga4 O1 O4 44.0(6) . 4
O4 O1 O4 42.9(9) 1_455 4
O1 O1 O4 105.5(8) 2_656 4
O1 O1 O4 65.7(5) 4_655 4
O1 O1 O4 149.8(14) 4_645 4
O2 O1 O4 63.0(7) 3_445 4
La1 O1 O4 146.9(6) 4_535 4
La1 O1 O4 68.4(8) 3_545 4
La2 O1 O4 52.0(7) . 4
O2 O1 O4 43.1(7) . 4
O2 O1 O4 97.4(7) 1_445 4
O4 O1 O4 92.1(8) 3_445 4
O4 O1 O4 154.9(8) 1_545 4
La2 O1 O4 74.2(5) 3_445 4
La1 O1 O4 83.2(5) 1_445 4
La1 O1 O4 45.9(5) 4_445 4
O4 O1 O4 93.8(10) 1_655 4
Ga2 O1 O2 34.4(15) 4_645 3_645
La1 O1 O2 134.8(11) 1_545 3_645
La2 O1 O2 80.4(9) 3_545 3_645
La1 O1 O2 107.7(12) 4_545 3_645
O3 O1 O2 164.1(17) 2_556 3_645
O2 O1 O2 115.9(18) 4_545 3_645
O4 O1 O2 144.3(17) 4_545 3_645
O7 O1 O2 72.2(12) 3_544 3_645
O6 O1 O2 118.2(8) 1_545 3_645
O3 O1 O2 60.7(11) 2_656 3_645
O4 O1 O2 58.7(14) 4_645 3_645
O2 O1 O2 14.6(12) 4_645 3_645
O5 O1 O2 62.1(10) 3_544 3_645
Ga2 O1 O2 147.6(14) 4_545 3_645
Ga4 O1 O2 69.1(6) 1_545 3_645
Ga3 O1 O2 32.9(5) 3_645 3_645
Ga4 O1 O2 90.4(6) 4_645 3_645
O4 O1 O2 87.6(12) . 3_645
O3 O1 O2 96.1(8) 3_544 3_645
O2 O1 O2 47.5(5) 3_545 3_645
O7 O1 O2 100.8(12) 4_546 3_645
O5 O1 O2 152.4(11) 2_546 3_645
O6 O1 O2 98.8(9) 4_545 3_645
O2 O1 O2 112.1(8) 1_545 3_645
O3 O1 O2 79.7(6) 3_554 3_645
Ga4 O1 O2 128.8(11) 1_445 3_645
Ga4 O1 O2 158.2(11) 4_545 3_645
Ga3 O1 O2 106.6(10) 3_545 3_645
O4 O1 O2 53.3(8) 3_545 3_645
Ta O1 O2 91.3(8) 3_545 3_645
Ga1 O1 O2 91.3(8) 3_545 3_645
Ga1 O1 O2 131.8(7) . 3_645
Ta O1 O2 131.8(7) . 3_645
Ta O1 O2 76.1(7) 3 3_645
Ga1 O1 O2 76.1(7) 3 3_645
O5 O1 O2 84.8(7) 2_646 3_645
O6 O1 O2 113.6(10) 4_535 3_645
La1 O1 O2 60.3(5) 1_645 3_645
La2 O1 O2 16.5(5) 3_645 3_645
O7 O1 O2 140.2(11) 2_556 3_645
La1 O1 O2 43.4(5) 4_645 3_645
O7 O1 O2 43.9(9) 4_646 3_645
O6 O1 O2 44.2(6) 4_645 3_645
Ga2 O1 O2 40.1(4) 3_545 3_645
Ga2 O1 O2 81.5(6) . 3_645
Ga2 O1 O2 95.7(5) 1_545 3_645
O5 O1 O2 84.8(9) 4_546 3_645
O1 O1 O2 77.8(9) 2_556 3_645
O1 O1 O2 130.7(7) 4_545 3_645
O1 O1 O2 114.0(7) 4 3_645
O1 O1 O2 146.9(5) 1_455 3_645
O1 O1 O2 33.1(5) 1_655 3_645
Ga4 O1 O2 55.5(5) 2_646 3_645
Ga3 O1 O2 104.2(5) 1_645 3_645
Ga4 O1 O2 61.0(6) . 3_645
O4 O1 O2 145.4(13) 1_455 3_645
O1 O1 O2 23.3(5) 2_656 3_645
O1 O1 O2 67.2(8) 4_655 3_645
O1 O1 O2 79.8(7) 4_645 3_645
O2 O1 O2 107.2(10) 3_445 3_645
La1 O1 O2 109.1(7) 4_535 3_645
La1 O1 O2 65.4(6) 3_545 3_645
La2 O1 O2 116.8(7) . 3_645
O2 O1 O2 94.8(7) . 3_645
O2 O1 O2 159.9(11) 1_445 3_645
O4 O1 O2 99.4(9) 3_445 3_645
O4 O1 O2 99.8(8) 1_545 3_645
La2 O1 O2 126.9(9) 3_445 3_645
La1 O1 O2 161.8(10) 1_445 3_645
La1 O1 O2 142.1(9) 4_445 3_645
O4 O1 O2 50.3(7) 1_655 3_645
O4 O1 O2 102.7(9) 4 3_645
Ga2 O1 O4 73.0(15) 4_645 4_655
La1 O1 O4 139.5(17) 1_545 4_655
La2 O1 O4 112.3(15) 3_545 4_655
La1 O1 O4 43.3(8) 4_545 4_655
O3 O1 O4 99.0(14) 2_556 4_655
O2 O1 O4 87.4(15) 4_545 4_655
O4 O1 O4 144.1(16) 4_545 4_655
O7 O1 O4 135.6(15) 3_544 4_655
O6 O1 O4 90.5(13) 1_545 4_655
O3 O1 O4 64.9(11) 2_656 4_655
O4 O1 O4 108.0(13) 4_645 4_655
O2 O1 O4 53.1(12) 4_645 4_655
O5 O1 O4 27.4(12) 3_544 4_655
Ga2 O1 O4 112.4(12) 4_545 4_655
Ga4 O1 O4 131.0(6) 1_545 4_655
Ga3 O1 O4 46.9(8) 3_645 4_655
Ga4 O1 O4 65.4(9) 4_645 4_655
O4 O1 O4 39.5(17) . 4_655
O3 O1 O4 146.1(9) 3_544 4_655
O2 O1 O4 73.7(12) 3_545 4_655
O7 O1 O4 140.9(16) 4_546 4_655
O5 O1 O4 114.6(14) 2_546 4_655
O6 O1 O4 47.8(7) 4_545 4_655
O2 O1 O4 122.7(12) 1_545 4_655
O3 O1 O4 14.3(6) 3_554 4_655
Ga4 O1 O4 153.0(9) 1_445 4_655
Ga4 O1 O4 93.4(9) 4_545 4_655
Ga3 O1 O4 82.1(9) 3_545 4_655
O4 O1 O4 106.6(11) 3_545 4_655
Ta O1 O4 151.8(12) 3_545 4_655
Ga1 O1 O4 151.8(12) 3_545 4_655
Ga1 O1 O4 93.0(10) . 4_655
Ta O1 O4 93.0(10) . 4_655
Ta O1 O4 44.6(7) 3 4_655
Ga1 O1 O4 44.6(7) 3 4_655
O5 O1 O4 90.2(11) 2_646 4_655
O6 O1 O4 173.1(13) 4_535 4_655
La1 O1 O4 92.3(7) 1_645 4_655
La2 O1 O4 80.4(7) 3_645 4_655
O7 O1 O4 82.5(11) 2_556 4_655
La1 O1 O4 42.7(6) 4_645 4_655
O7 O1 O4 109.2(11) 4_646 4_655
O6 O1 O4 21.5(6) 4_645 4_655
Ga2 O1 O4 86.5(9) 3_545 4_655
Ga2 O1 O4 26.9(7) . 4_655
Ga2 O1 O4 130.2(8) 1_545 4_655
O5 O1 O4 69.2(11) 4_546 4_655
O1 O1 O4 98.6(9) 2_556 4_655
O1 O1 O4 149.8(17) 4_545 4_655
O1 O1 O4 48.6(6) 4 4_655
O1 O1 O4 110.5(4) 1_455 4_655
O1 O1 O4 69.5(4) 1_655 4_655
Ga4 O1 O4 118.0(9) 2_646 4_655
Ga3 O1 O4 102.2(9) 1_645 4_655
Ga4 O1 O4 9.9(6) . 4_655
O4 O1 O4 81.9(12) 1_455 4_655
O1 O1 O4 79.6(6) 2_656 4_655
O1 O1 O4 29.1(6) 4_655 4_655
O1 O1 O4 115.6(8) 4_645 4_655
O2 O1 O4 97.1(10) 3_445 4_655
La1 O1 O4 164.6(8) 4_535 4_655
La1 O1 O4 74.5(8) 3_545 4_655
La2 O1 O4 58.5(7) . 4_655
O2 O1 O4 34.4(7) . 4_655
O2 O1 O4 132.0(10) 1_445 4_655
O4 O1 O4 120.2(12) 3_445 4_655
O4 O1 O4 142.8(6) 1_545 4_655
La2 O1 O4 115.5(8) 3_445 4_655
La1 O1 O4 125.9(8) 1_445 4_655
La1 O1 O4 90.0(7) 4_445 4_655
O4 O1 O4 51.7(7) 1_655 4_655
O4 O1 O4 44.4(5) 4 4_655
O2 O1 O4 65.3(7) 3_645 4_655
Ga2 O1 O2 107.2(19) 4_645 2_545
La1 O1 O2 20.7(9) 1_545 2_545
La2 O1 O2 123.6(11) 3_545 2_545
La1 O1 O2 91.3(14) 4_545 2_545
O3 O1 O2 47.6(11) 2_556 2_545
O2 O1 O2 102.9(14) 4_545 2_545
O4 O1 O2 55.6(14) 4_545 2_545
O7 O1 O2 101.8(15) 3_544 2_545
O6 O1 O2 32.3(8) 1_545 2_545
O3 O1 O2 85.5(14) 2_656 2_545
O4 O1 O2 85.6(18) 4_645 2_545
O2 O1 O2 135.6(15) 4_645 2_545
O5 O1 O2 140.3(16) 3_544 2_545
Ga2 O1 O2 70.0(9) 4_545 2_545
Ga4 O1 O2 86.6(10) 1_545 2_545
Ga3 O1 O2 163.8(12) 3_645 2_545
Ga4 O1 O2 62.9(8) 4_645 2_545
O4 O1 O2 81.2(16) . 2_545
O3 O1 O2 57.8(7) 3_544 2_545
O2 O1 O2 165.7(12) 3_545 2_545
O7 O1 O2 94.9(11) 4_546 2_545
O5 O1 O2 12.4(8) 2_546 2_545
O6 O1 O2 111.4(9) 4_545 2_545
O2 O1 O2 30.2(7) 1_545 2_545
O3 O1 O2 108.4(11) 3_554 2_545
Ga4 O1 O2 66.6(6) 1_445 2_545
Ga4 O1 O2 44.3(6) 4_545 2_545
Ga3 O1 O2 112.2(5) 3_545 2_545
O4 O1 O2 133.4(12) 3_545 2_545
Ta O1 O2 88.9(8) 3_545 2_545
Ga1 O1 O2 88.9(8) 3_545 2_545
Ga1 O1 O2 26.2(5) . 2_545
Ta O1 O2 26.2(5) . 2_545
Ta O1 O2 136.7(9) 3 2_545
Ga1 O1 O2 136.7(9) 3 2_545
O5 O1 O2 57.6(8) 2_646 2_545
O6 O1 O2 66.3(7) 4_535 2_545
La1 O1 O2 80.9(8) 1_645 2_545
La2 O1 O2 128.9(8) 3_645 2_545
O7 O1 O2 41.1(10) 2_556 2_545
La1 O1 O2 110.7(9) 4_645 2_545
O7 O1 O2 115.0(12) 4_646 2_545
O6 O1 O2 130.0(11) 4_645 2_545
Ga2 O1 O2 153.2(10) 3_545 2_545
Ga2 O1 O2 92.9(9) . 2_545
Ga2 O1 O2 50.1(6) 1_545 2_545
O5 O1 O2 133.9(7) 4_546 2_545
O1 O1 O2 133.1(5) 2_556 2_545
O1 O1 O2 31.0(10) 4_545 2_545
O1 O1 O2 80.9(13) 4 2_545
O1 O1 O2 71.0(3) 1_455 2_545
O1 O1 O2 109.0(3) 1_655 2_545
Ga4 O1 O2 118.0(9) 2_646 2_545
Ga3 O1 O2 37.8(4) 1_645 2_545
Ga4 O1 O2 128.5(10) . 2_545
O4 O1 O2 64.6(10) 1_455 2_545
O1 O1 O2 150.7(5) 2_656 2_545
O1 O1 O2 98.7(13) 4_655 2_545
O1 O1 O2 63.4(9) 4_645 2_545
O2 O1 O2 110.1(6) 3_445 2_545
La1 O1 O2 55.3(6) 4_535 2_545
La1 O1 O2 152.3(3) 3_545 2_545
La2 O1 O2 61.9(7) . 2_545
O2 O1 O2 85.2(7) . 2_545
O2 O1 O2 28.0(7) 1_445 2_545
O4 O1 O2 107.8(7) 3_445 2_545
O4 O1 O2 51.5(7) 1_545 2_545
La2 O1 O2 87.8(4) 3_445 2_545
La1 O1 O2 50.4(4) 1_445 2_545
La1 O1 O2 75.4(5) 4_445 2_545
O4 O1 O2 99.7(9) 1_655 2_545
O4 O1 O2 103.4(9) 4 2_545
O2 O1 O2 141.2(7) 3_645 2_545
O4 O1 O2 119.2(10) 4_655 2_545
Ga2 O1 O2 65.3(16) 4_645 2_645
La1 O1 O2 46.9(8) 1_545 2_645
La2 O1 O2 140.4(15) 3_545 2_645
La1 O1 O2 105.1(16) 4_545 2_645
O3 O1 O2 86.0(15) 2_556 2_645
O2 O1 O2 144.0(19) 4_545 2_645
O4 O1 O2 91.9(17) 4_545 2_645
O7 O1 O2 95.9(14) 3_544 2_645
O6 O1 O2 29.0(8) 1_545 2_645
O3 O1 O2 46.4(10) 2_656 2_645
O4 O1 O2 51.3(16) 4_645 2_645
O2 O1 O2 94.2(11) 4_645 2_645
O5 O1 O2 130.2(14) 3_544 2_645
Ga2 O1 O2 111.9(12) 4_545 2_645
Ga4 O1 O2 67.6(8) 1_545 2_645
Ga3 O1 O2 126.4(5) 3_645 2_645
Ga4 O1 O2 38.5(7) 4_645 2_645
O4 O1 O2 67.1(15) . 2_645
O3 O1 O2 49.9(7) 3_544 2_645
O2 O1 O2 145.9(7) 3_545 2_645
O7 O1 O2 115.5(13) 4_546 2_645
O5 O1 O2 52.8(9) 2_546 2_645
O6 O1 O2 131.7(12) 4_545 2_645
O2 O1 O2 20.4(6) 1_545 2_645
O3 O1 O2 101.6(10) 3_554 2_645
Ga4 O1 O2 97.0(9) 1_445 2_645
Ga4 O1 O2 79.4(9) 4_545 2_645
Ga3 O1 O2 152.9(9) 3_545 2_645
O4 O1 O2 121.6(10) 3_545 2_645
Ta O1 O2 95.9(8) 3_545 2_645
Ga1 O1 O2 95.9(8) 3_545 2_645
Ga1 O1 O2 41.4(6) . 2_645
Ta O1 O2 41.4(6) . 2_645
Ta O1 O2 146.7(10) 3 2_645
Ga1 O1 O2 146.7(10) 3 2_645
O5 O1 O2 16.6(7) 2_646 2_645
O6 O1 O2 83.7(8) 4_535 2_645
La1 O1 O2 40.1(5) 1_645 2_645
La2 O1 O2 89.9(5) 3_645 2_645
O7 O1 O2 64.2(10) 2_556 2_645
La1 O1 O2 73.9(6) 4_645 2_645
O7 O1 O2 88.6(9) 4_646 2_645
O6 O1 O2 100.2(7) 4_645 2_645
Ga2 O1 O2 129.8(6) 3_545 2_645
Ga2 O1 O2 79.3(8) . 2_645
Ga2 O1 O2 31.7(5) 1_545 2_645
O5 O1 O2 168.8(13) 4_546 2_645
O1 O1 O2 154.7(6) 2_556 2_645
O1 O1 O2 53.3(10) 4_545 2_645
O1 O1 O2 94.8(15) 4 2_645
O1 O1 O2 112.9(4) 1_455 2_645
O1 O1 O2 67.1(4) 1_655 2_645
Ga4 O1 O2 103.3(7) 2_646 2_645
Ga3 O1 O2 5.5(4) 1_645 2_645
Ga4 O1 O2 112.2(8) . 2_645
O4 O1 O2 98.3(12) 1_455 2_645
O1 O1 O2 115.6(5) 2_656 2_645
O1 O1 O2 74.3(10) 4_655 2_645
O1 O1 O2 31.4(9) 4_645 2_645
O2 O1 O2 151.3(8) 3_445 2_645
La1 O1 O2 62.8(6) 4_535 2_645
La1 O1 O2 164.6(6) 3_545 2_645
La2 O1 O2 69.0(7) . 2_645
O2 O1 O2 81.2(6) . 2_645
O2 O1 O2 68.5(8) 1_445 2_645
O4 O1 O2 136.6(10) 3_445 2_645
O4 O1 O2 43.3(7) 1_545 2_645
La2 O1 O2 128.1(7) 3_445 2_645
La1 O1 O2 91.8(7) 1_445 2_645
La1 O1 O2 114.4(8) 4_445 2_645
O4 O1 O2 62.0(7) 1_655 2_645
O4 O1 O2 120.9(10) 4 2_645
O2 O1 O2 99.7(6) 3_645 2_645
O4 O1 O2 103.2(9) 4_655 2_645
O2 O1 O2 41.9(5) 2_545 2_645
Ga2 O1 O2 36.2(15) 4_645 1_645
La1 O1 O2 70.6(8) 1_545 1_645
La2 O1 O2 125.4(12) 3_545 1_645
La1 O1 O2 119.5(13) 4_545 1_645
O3 O1 O2 116.5(15) 2_556 1_645
O2 O1 O2 174.4(16) 4_545 1_645
O4 O1 O2 112.6(17) 4_545 1_645
O7 O1 O2 81.1(11) 3_544 1_645
O6 O1 O2 56.4(8) 1_545 1_645
O3 O1 O2 30.8(8) 2_656 1_645
O4 O1 O2 25.9(14) 4_645 1_645
O2 O1 O2 66.7(11) 4_645 1_645
O5 O1 O2 116.3(10) 3_544 1_645
Ga2 O1 O2 139.9(13) 4_545 1_645
Ga4 O1 O2 51.3(6) 1_545 1_645
Ga3 O1 O2 99.6(5) 3_645 1_645
Ga4 O1 O2 47.7(6) 4_645 1_645
O4 O1 O2 72.9(13) . 1_645
O3 O1 O2 50.7(6) 3_544 1_645
O2 O1 O2 115.4(9) 3_545 1_645
O7 O1 O2 114.4(11) 4_546 1_645
O5 O1 O2 83.0(10) 2_546 1_645
O6 O1 O2 141.1(10) 4_545 1_645
O2 O1 O2 43.6(4) 1_545 1_645
O3 O1 O2 101.5(8) 3_554 1_645
Ga4 O1 O2 110.8(9) 1_445 1_645
Ga4 O1 O2 109.5(9) 4_545 1_645
Ga3 O1 O2 176.3(9) 3_545 1_645
O4 O1 O2 97.2(9) 3_545 1_645
Ta O1 O2 90.3(7) 3_545 1_645
Ga1 O1 O2 90.3(7) 3_545 1_645
Ga1 O1 O2 70.4(6) . 1_645
Ta O1 O2 70.4(6) . 1_645
Ta O1 O2 136.4(7) 3 1_645
Ga1 O1 O2 136.4(7) 3 1_645
O5 O1 O2 20.2(8) 2_646 1_645
O6 O1 O2 90.3(8) 4_535 1_645
La1 O1 O2 9.6(5) 1_645 1_645
La2 O1 O2 59.3(5) 3_645 1_645
O7 O1 O2 91.9(10) 2_556 1_645
La1 O1 O2 55.1(5) 4_645 1_645
O7 O1 O2 62.9(9) 4_646 1_645
O6 O1 O2 82.9(6) 4_645 1_645
Ga2 O1 O2 100.4(5) 3_545 1_645
Ga2 O1 O2 81.3(6) . 1_645
Ga2 O1 O2 36.1(4) 1_545 1_645
O5 O1 O2 154.2(9) 4_546 1_645
O1 O1 O2 134.8(9) 2_556 1_645
O1 O1 O2 72.8(8) 4_545 1_645
O1 O1 O2 112.1(13) 4 1_645
O1 O1 O2 141.3(5) 1_455 1_645
O1 O1 O2 38.7(5) 1_655 1_645
Ga4 O1 O2 81.2(6) 2_646 1_645
Ga3 O1 O2 35.7(4) 1_645 1_645
Ga4 O1 O2 101.4(5) . 1_645
O4 O1 O2 127.0(12) 1_455 1_645
O1 O1 O2 85.2(5) 2_656 1_645
O1 O1 O2 68.7(7) 4_655 1_645
O1 O1 O2 20.1(6) 4_645 1_645
O2 O1 O2 164.1(12) 3_445 1_645
La1 O1 O2 69.2(6) 4_535 1_645
La1 O1 O2 134.1(6) 3_545 1_645
La2 O1 O2 88.6(7) . 1_645
O2 O1 O2 90.0(7) . 1_645
O2 O1 O2 95.7(9) 1_445 1_645
O4 O1 O2 134.9(10) 3_445 1_645
O4 O1 O2 47.7(7) 1_545 1_645
La2 O1 O2 148.5(9) 3_445 1_645
La1 O1 O2 118.9(8) 1_445 1_645
La1 O1 O2 144.7(9) 4_445 1_645
O4 O1 O2 44.3(6) 1_655 1_645
O4 O1 O2 132.7(9) 4 1_645
O2 O1 O2 69.7(4) 3_645 1_645
O4 O1 O2 95.5(7) 4_655 1_645
O2 O1 O2 71.5(7) 2_545 1_645
O2 O1 O2 30.5(7) 2_645 1_645
Ga2 O1 O2 104.4(18) 4_645 4_535
La1 O1 O2 47.1(10) 1_545 4_535
La2 O1 O2 62.1(10) 3_545 4_535
La1 O1 O2 141.3(7) 4_545 4_535
O3 O1 O2 86.7(10) 2_556 4_535
O2 O1 O2 92.3(13) 4_545 4_535
O4 O1 O2 39.8(12) 4_545 4_535
O7 O1 O2 37.8(12) 3_544 4_535
O6 O1 O2 95.6(13) 1_545 4_535
O3 O1 O2 116.1(12) 2_656 4_535
O4 O1 O2 70.2(15) 4_645 4_535
O2 O1 O2 121.6(15) 4_645 4_535
O5 O1 O2 147.3(17) 3_544 4_535
Ga2 O1 O2 70.3(8) 4_545 4_535
Ga4 O1 O2 45.3(6) 1_545 4_535
Ga3 O1 O2 126.3(13) 3_645 4_535
Ga4 O1 O2 119.3(12) 4_645 4_535
O4 O1 O2 146.4(19) . 4_535
O3 O1 O2 34.9(7) 3_544 4_535
O2 O1 O2 99.8(12) 3_545 4_535
O7 O1 O2 34.5(9) 4_546 4_535
O5 O1 O2 72.3(12) 2_546 4_535
O6 O1 O2 132.8(6) 4_545 4_535
O2 O1 O2 62.2(11) 1_545 4_535
O3 O1 O2 170.8(7) 3_554 4_535
Ga4 O1 O2 28.5(4) 1_445 4_535
Ga4 O1 O2 92.7(7) 4_545 4_535
Ga3 O1 O2 96.7(7) 3_545 4_535
O4 O1 O2 66.5(9) 3_545 4_535
Ta O1 O2 21.4(4) 3_545 4_535
Ga1 O1 O2 21.4(4) 3_545 4_535
Ga1 O1 O2 93.8(9) . 4_535
Ta O1 O2 93.8(9) . 4_535
Ta O1 O2 132.0(9) 3 4_535
Ga1 O1 O2 132.0(9) 3 4_535
O5 O1 O2 92.8(12) 2_646 4_535
O6 O1 O2 5.9(4) 4_535 4_535
La1 O1 O2 87.5(8) 1_645 4_535
La2 O1 O2 94.2(8) 3_645 4_535
O7 O1 O2 104.3(11) 2_556 4_535
La1 O1 O2 135.6(7) 4_645 4_535
O7 O1 O2 65.1(10) 4_646 4_535
O6 O1 O2 153.0(9) 4_645 4_535
Ga2 O1 O2 86.6(8) 3_545 4_535
Ga2 O1 O2 159.1(12) . 4_535
Ga2 O1 O2 52.2(6) 1_545 4_535
O5 O1 O2 107.4(10) 4_546 4_535
O1 O1 O2 76.2(5) 2_556 4_535
O1 O1 O2 36.8(8) 4_545 4_535
O1 O1 O2 137.1(8) 4 4_535
O1 O1 O2 72.2(3) 1_455 4_535
O1 O1 O2 107.8(3) 1_655 4_535
Ga4 O1 O2 55.3(6) 2_646 4_535
Ga3 O1 O2 82.5(8) 1_645 4_535
Ga4 O1 O2 163.8(12) . 4_535
O4 O1 O2 103.1(9) 1_455 4_535
O1 O1 O2 93.7(7) 2_656 4_535
O1 O1 O2 153.6(9) 4_655 4_535
O1 O1 O2 65.3(4) 4_645 4_535
O2 O1 O2 81.0(6) 3_445 4_535
La1 O1 O2 18.2(4) 4_535 4_535
La1 O1 O2 100.0(8) 3_545 4_535
La2 O1 O2 128.4(9) . 4_535
O2 O1 O2 152.5(9) . 4_535
O2 O1 O2 54.6(8) 1_445 4_535
O4 O1 O2 56.0(7) 3_445 4_535
O4 O1 O2 39.5(7) 1_545 4_535
La2 O1 O2 64.6(4) 3_445 4_535
La1 O1 O2 58.8(4) 1_445 4_535
La1 O1 O2 93.2(4) 4_445 4_535
O4 O1 O2 128.0(9) 1_655 4_535
O4 O1 O2 137.8(5) 4 4_535
O2 O1 O2 108.8(8) 3_645 4_535
O4 O1 O2 173.1(11) 4_655 4_535
O2 O1 O2 67.6(6) 2_545 4_535
O2 O1 O2 81.0(7) 2_645 4_535
O2 O1 O2 85.3(8) 1_645 4_535
Ga2 O1 O4 39.3(16) 4_645 3_645
La1 O1 O4 117.2(12) 1_545 3_645
La2 O1 O4 69.0(9) 3_545 3_645
La1 O1 O4 130.0(13) 4_545 3_645
O3 O1 O4 172.0(16) 2_556 3_645
O2 O1 O4 119.1(19) 4_545 3_645
O4 O1 O4 122.9(16) 4_545 3_645
O7 O1 O4 49.8(11) 3_544 3_645
O6 O1 O4 121.9(9) 1_545 3_645
O3 O1 O4 69.9(10) 2_656 3_645
O4 O1 O4 46.1(17) 4_645 3_645
O2 O1 O4 36.3(12) 4_645 3_645
O5 O1 O4 81.8(12) 3_544 3_645
Ga2 O1 O4 139.2(13) 4_545 3_645
Ga4 O1 O4 48.1(6) 1_545 3_645
Ga3 O1 O4 50.4(7) 3_645 3_645
Ga4 O1 O4 101.5(5) 4_645 3_645
O4 O1 O4 107.0(11) . 3_645
O3 O1 O4 76.7(8) 3_544 3_645
O2 O1 O4 50.6(8) 3_545 3_645
O7 O1 O4 82.3(11) 4_546 3_645
O5 O1 O4 143.4(13) 2_546 3_645
O6 O1 O4 116.5(11) 4_545 3_645
O2 O1 O4 101.3(9) 1_545 3_645
O3 O1 O4 102.5(8) 3_554 3_645
Ga4 O1 O4 107.6(9) 1_445 3_645
Ga4 O1 O4 175.2(11) 4_545 3_645
Ga3 O1 O4 111.0(10) 3_545 3_645
O4 O1 O4 38.0(4) 3_545 3_645
Ta O1 O4 69.1(6) 3_545 3_645
Ga1 O1 O4 69.1(6) 3_545 3_645
Ga1 O1 O4 136.2(7) . 3_645
Ta O1 O4 136.2(7) . 3_645
Ta O1 O4 91.7(8) 3 3_645
Ga1 O1 O4 91.7(8) 3 3_645
O5 O1 O4 85.1(9) 2_646 3_645
O6 O1 O4 90.8(9) 4_535 3_645
La1 O1 O4 56.7(5) 1_645 3_645
La2 O1 O4 11.1(5) 3_645 3_645
O7 O1 O4 155.1(10) 2_556 3_645
La1 O1 O4 61.5(6) 4_645 3_645
O7 O1 O4 21.2(8) 4_646 3_645
O6 O1 O4 67.1(6) 4_645 3_645
Ga2 O1 O4 34.5(5) 3_545 3_645
Ga2 O1 O4 102.9(6) . 3_645
Ga2 O1 O4 81.1(6) 1_545 3_645
O5 O1 O4 92.2(10) 4_546 3_645
O1 O1 O4 71.9(9) 2_556 3_645
O1 O1 O4 110.7(8) 4_545 3_645
O1 O1 O4 136.8(8) 4 3_645
O1 O1 O4 139.8(5) 1_455 3_645
O1 O1 O4 40.2(5) 1_655 3_645
Ga4 O1 O4 34.2(4) 2_646 3_645
Ga3 O1 O4 101.2(6) 1_645 3_645
Ga4 O1 O4 83.4(7) . 3_645
O4 O1 O4 164.3(16) 1_455 3_645
O1 O1 O4 20.3(5) 2_656 3_645
O1 O1 O4 87.3(8) 4_655 3_645
O1 O1 O4 68.4(8) 4_645 3_645
O2 O1 O4 104.9(9) 3_445 3_645
La1 O1 O4 87.2(7) 4_535 3_645
La1 O1 O4 69.1(7) 3_545 3_645
La2 O1 O4 136.5(6) . 3_645
O2 O1 O4 116.7(7) . 3_645
O2 O1 O4 138.5(10) 1_445 3_645
O4 O1 O4 87.2(9) 3_445 3_645
O4 O1 O4 81.7(8) 1_545 3_645
La2 O1 O4 117.7(9) 3_445 3_645
La1 O1 O4 142.2(9) 1_445 3_645
La1 O1 O4 149.3(10) 4_445 3_645
O4 O1 O4 64.7(5) 1_655 3_645
O4 O1 O4 122.7(10) 4 3_645
O2 O1 O4 22.9(6) 3_645 3_645
O4 O1 O4 88.2(7) 4_655 3_645
O2 O1 O4 131.1(9) 2_545 3_645
O2 O1 O4 95.8(6) 2_645 3_645
O2 O1 O4 65.9(6) 1_645 3_645
O2 O1 O4 85.9(7) 4_535 3_645
Ga2 O1 O4 111(2) 4_645 2
La1 O1 O4 61.5(12) 1_545 2
La2 O1 O4 140.8(6) 3_545 2
La1 O1 O4 51.3(11) 4_545 2
O3 O1 O4 36.2(12) 2_556 2
O2 O1 O4 88.2(16) 4_545 2
O4 O1 O4 78.9(13) 4_545 2
O7 O1 O4 142.7(16) 3_544 2
O6 O1 O4 31.8(8) 1_545 2
O3 O1 O4 80.3(13) 2_656 2
O4 O1 O4 112(2) 4_645 2
O2 O1 O4 121.5(15) 4_645 2
O5 O1 O4 99.2(14) 3_544 2
Ga2 O1 O4 70.3(9) 4_545 2
Ga4 O1 O4 124.6(13) 1_545 2
Ga3 O1 O4 127.3(12) 3_645 2
Ga4 O1 O4 48.7(7) 4_645 2
O4 O1 O4 49.0(13) . 2
O3 O1 O4 97.6(12) 3_544 2
O2 O1 O4 146.6(14) 3_545 2
O7 O1 O4 123.1(12) 4_546 2
O5 O1 O4 34.1(10) 2_546 2
O6 O1 O4 75.3(9) 4_545 2
O2 O1 O4 63.5(10) 1_545 2
O3 O1 O4 68.1(8) 3_554 2
Ga4 O1 O4 94.1(8) 1_445 2
Ga4 O1 O4 26.5(5) 4_545 2
Ga3 O1 O4 94.8(7) 3_545 2
O4 O1 O4 170.8(7) 3_545 2
Ta O1 O4 127.3(9) 3_545 2
Ga1 O1 O4 127.3(9) 3_545 2
Ga1 O1 O4 20.2(5) . 2
Ta O1 O4 20.2(5) . 2
Ta O1 O4 99.2(9) 3 2
Ga1 O1 O4 99.2(9) 3 2
O5 O1 O4 67.5(10) 2_646 2
O6 O1 O4 103.4(9) 4_535 2
La1 O1 O4 95.9(9) 1_645 2
La2 O1 O4 139.7(8) 3_645 2
O7 O1 O4 4.9(7) 2_556 2
La1 O1 O4 92.6(8) 4_645 2
O7 O1 O4 149.2(13) 4_646 2
O6 O1 O4 97.5(9) 4_645 2
Ga2 O1 O4 165.4(11) 3_545 2
Ga2 O1 O4 57.4(6) . 2
Ga2 O1 O4 85.2(9) 1_545 2
O5 O1 O4 109.2(11) 4_546 2
O1 O1 O4 136.9(6) 2_556 2
O1 O1 O4 71.4(13) 4_545 2
O1 O1 O4 40.4(11) 4 2
O1 O1 O4 69.9(4) 1_455 2
O1 O1 O4 110.1(4) 1_655 2
Ga4 O1 O4 159.0(11) 2_646 2
Ga3 O1 O4 55.2(7) 1_645 2
Ga4 O1 O4 88.9(8) . 2
O4 O1 O4 39.6(11) 1_455 2
O1 O1 O4 158.1(6) 2_656 2
O1 O1 O4 69.5(10) 4_655 2
O1 O1 O4 91.6(14) 4_645 2
O2 O1 O4 103.9(7) 3_445 2
La1 O1 O4 96.3(9) 4_535 2
La1 O1 O4 132.4(8) 3_545 2
La2 O1 O4 22.1(4) . 2
O2 O1 O4 46.4(6) . 2
O2 O1 O4 53.5(7) 1_445 2
O4 O1 O4 122.4(6) 3_445 2
O4 O1 O4 90.6(8) 1_545 2
La2 O1 O4 92.1(5) 3_445 2
La1 O1 O4 62.2(5) 1_445 2
La1 O1 O4 58.9(5) 4_445 2
O4 O1 O4 86.9(8) 1_655 2
O4 O1 O4 65.4(6) 4 2
O2 O1 O4 135.9(8) 3_645 2
O4 O1 O4 80.6(8) 4_655 2
O2 O1 O4 41.1(7) 2_545 2
O2 O1 O4 60.6(7) 2_645 2
O2 O1 O4 87.6(8) 1_645 2
O2 O1 O4 106.3(9) 4_535 2
O4 O1 O4 150.1(5) 3_645 2
Ga3 O2 Ga2 113.1(17) 1_655 .
Ga3 O2 La2 110(2) 1_655 .
Ga2 O2 La2 101(2) . .
Ga3 O2 O6 71.0(16) 1_655 .
Ga2 O2 O6 126(2) . .
La2 O2 O6 129.5(17) . .
Ga3 O2 La1 123(2) 1_655 .
Ga2 O2 La1 99(2) . .
La2 O2 La1 108.1(13) . .
O6 O2 La1 51.7(10) . .
Ga3 O2 O3 138(2) 1_655 3_554
Ga2 O2 O3 42.8(14) . 3_554
La2 O2 O3 108.8(19) . 3_554
O6 O2 O3 95.8(12) . 3_554
La1 O2 O3 56.6(9) . 3_554
Ga3 O2 O5 37.7(12) 1_655 1_554
Ga2 O2 O5 150(2) . 1_554
La2 O2 O5 88.1(19) . 1_554
O6 O2 O5 62.0(15) . 1_554
La1 O2 O5 105.2(18) . 1_554
O3 O2 O5 158(2) 3_554 1_554
Ga3 O2 O1 157(2) 1_655 4
Ga2 O2 O1 89(2) . 4
La2 O2 O1 57.8(14) . 4
O6 O2 O1 100.9(16) . 4
La1 O2 O1 54.5(13) . 4
O3 O2 O1 62.6(18) 3_554 4
O5 O2 O1 119.7(19) 1_554 4
Ga3 O2 O5 38.0(15) 1_655 2_656
Ga2 O2 O5 88.1(16) . 2_656
La2 O2 O5 146(2) . 2_656
O6 O2 O5 62.2(15) . 2_656
La1 O2 O5 102.3(19) . 2_656
O3 O2 O5 99.9(18) 3_554 2_656
O5 O2 O5 70(2) 1_554 2_656
O1 O2 O5 156(3) 4 2_656
Ga3 O2 O4 130.0(19) 1_655 .
Ga2 O2 O4 29.7(13) . .
La2 O2 O4 72.1(16) . .
O6 O2 O4 147(2) . .
La1 O2 O4 101.5(19) . .
O3 O2 O4 51.5(17) 3_554 .
O5 O2 O4 151(3) 1_554 .
O1 O2 O4 67.8(17) 4 .
O5 O2 O4 116.0(18) 2_656 .
Ga3 O2 O2 30.9(14) 1_655 2_655
Ga2 O2 O2 95.3(15) . 2_655
La2 O2 O2 90.6(17) . 2_655
O6 O2 O2 102.0(10) . 2_655
La1 O2 O2 153.5(11) . 2_655
O3 O2 O2 135(2) 3_554 2_655
O5 O2 O2 55.5(16) 1_554 2_655
O1 O2 O2 148(2) 4 2_655
O5 O2 O2 56.0(14) 2_656 2_655
O4 O2 O2 102.1(13) . 2_655
Ga3 O2 O1 83.6(14) 1_655 4_655
Ga2 O2 O1 29.9(11) . 4_655
La2 O2 O1 117.4(18) . 4_655
O6 O2 O1 112.9(17) . 4_655
La1 O2 O1 114(2) . 4_655
O3 O2 O1 64.4(17) 3_554 4_655
O5 O2 O1 121.1(17) 1_554 4_655
O1 O2 O1 119(3) 4 4_655
O5 O2 O1 60.2(15) 2_656 4_655
O4 O2 O1 55.8(14) . 4_655
O2 O2 O1 71.1(14) 2_655 4_655
Ga3 O2 O5 100(2) 1_655 2_556
Ga2 O2 O5 143(2) . 2_556
La2 O2 O5 81.5(13) . 2_556
O6 O2 O5 50.2(11) . 2_556
La1 O2 O5 46.6(12) . 2_556
O3 O2 O5 101.0(17) 3_554 2_556
O5 O2 O5 67(2) 1_554 2_556
O1 O2 O5 60.8(16) 4 2_556
O5 O2 O5 110(2) 2_656 2_556
O4 O2 O5 128.7(19) . 2_556
O2 O2 O5 122(2) 2_655 2_556
O1 O2 O5 158(2) 4_655 2_556
Ga3 O2 Ta 65.0(13) 1_655 1_565
Ga2 O2 Ta 160(2) . 1_565
La2 O2 Ta 97.6(13) . 1_565
O6 O2 Ta 34.8(8) . 1_565
La1 O2 Ta 69.1(10) . 1_565
O3 O2 Ta 124.4(13) 3_554 1_565
O5 O2 Ta 36.2(12) 1_554 1_565
O1 O2 Ta 96.0(14) 4 1_565
O5 O2 Ta 79.6(16) 2_656 1_565
O4 O2 Ta 163.7(15) . 1_565
O2 O2 Ta 90.4(13) 2_655 1_565
O1 O2 Ta 139.7(16) 4_655 1_565
O5 O2 Ta 35.4(11) 2_556 1_565
Ga3 O2 Ga1 65.0(13) 1_655 1_565
Ga2 O2 Ga1 160(2) . 1_565
La2 O2 Ga1 97.6(13) . 1_565
O6 O2 Ga1 34.8(8) . 1_565
La1 O2 Ga1 69.1(10) . 1_565
O3 O2 Ga1 124.4(13) 3_554 1_565
O5 O2 Ga1 36.2(12) 1_554 1_565
O1 O2 Ga1 96.0(14) 4 1_565
O5 O2 Ga1 79.6(16) 2_656 1_565
O4 O2 Ga1 163.7(15) . 1_565
O2 O2 Ga1 90.4(13) 2_655 1_565
O1 O2 Ga1 139.7(16) 4_655 1_565
O5 O2 Ga1 35.4(11) 2_556 1_565
Ta O2 Ga1 0.00(13) 1_565 1_565
Ga3 O2 O1 67.8(15) 1_655 3_554
Ga2 O2 O1 119(2) . 3_554
La2 O2 O1 42.5(10) . 3_554
O6 O2 O1 112.8(17) . 3_554
La1 O2 O1 133.6(14) . 3_554
O3 O2 O1 148.6(18) 3_554 3_554
O5 O2 O1 52.7(18) 1_554 3_554
O1 O2 O1 98(2) 4 3_554
O5 O2 O1 104.8(17) 2_656 3_554
O4 O2 O1 99.5(18) . 3_554
O2 O2 O1 52.9(13) 2_655 3_554
O1 O2 O1 112.4(17) 4_655 3_554
O5 O2 O1 88.4(15) 2_556 3_554
Ta O2 O1 79.6(12) 1_565 3_554
Ga1 O2 O1 79.6(12) 1_565 3_554
Ga3 O2 O2 91(2) 1_655 2
Ga2 O2 O2 141.7(14) . 2
La2 O2 O2 41.1(11) . 2
O6 O2 O2 89.5(10) . 2
La1 O2 O2 91.4(12) . 2
O3 O2 O2 130(2) 3_554 2
O5 O2 O2 55.8(15) 1_554 2
O1 O2 O2 67.8(14) 4 2
O5 O2 O2 125.5(19) 2_656 2
O4 O2 O2 112.2(12) . 2
O2 O2 O2 91(2) 2_655 2
O1 O2 O2 153.2(19) 4_655 2
O5 O2 O2 48.3(12) 2_556 2
Ta O2 O2 56.6(8) 1_565 2
Ga1 O2 O2 56.6(8) 1_565 2
O1 O2 O2 42.2(11) 3_554 2
Ga3 O2 Ga2 52.5(12) 1_655 2_655
Ga2 O2 Ga2 101.3(17) . 2_655
La2 O2 Ga2 62.5(10) . 2_655
O6 O2 Ga2 117.6(16) . 2_655
La1 O2 Ga2 158.7(16) . 2_655
O3 O2 Ga2 143.2(17) 3_554 2_655
O5 O2 Ga2 57.4(16) 1_554 2_655
O1 O2 Ga2 120.4(19) 4 2_655
O5 O2 Ga2 83.8(15) 2_656 2_655
O4 O2 Ga2 93.8(16) . 2_655
O2 O2 Ga2 28.1(10) 2_655 2_655
O1 O2 Ga2 87.1(13) 4_655 2_655
O5 O2 Ga2 112.1(16) 2_556 2_655
Ta O2 Ga2 92.5(12) 1_565 2_655
Ga1 O2 Ga2 92.5(12) 1_565 2_655
O1 O2 Ga2 27.1(4) 3_554 2_655
O2 O2 Ga2 68.9(13) 2 2_655
Ga3 O2 Ga4 54.0(12) 1_655 4_655
Ga2 O2 Ga4 112.7(17) . 4_655
La2 O2 Ga4 146.2(17) . 4_655
O6 O2 Ga4 24.3(6) . 4_655
La1 O2 Ga4 70.4(11) . 4_655
O3 O2 Ga4 98.3(11) 3_554 4_655
O5 O2 Ga4 61.2(15) 1_554 4_655
O1 O2 Ga4 123.6(17) 4 4_655
O5 O2 Ga4 37.9(12) 2_656 4_655
O4 O2 Ga4 141.7(17) . 4_655
O2 O2 Ga4 83.6(6) 2_655 4_655
O1 O2 Ga4 92.1(13) 4_655 4_655
O5 O2 Ga4 73.7(13) 2_556 4_655
Ta O2 Ga4 49.4(7) 1_565 4_655
Ga1 O2 Ga4 49.4(7) 1_565 4_655
O1 O2 Ga4 113.2(14) 3_554 4_655
O2 O2 Ga4 105.6(7) 2 4_655
Ga2 O2 Ga4 106.1(11) 2_655 4_655
Ga3 O2 O7 104.4(18) 1_655 1_554
Ga2 O2 O7 71.4(18) . 1_554
La2 O2 O7 35.3(10) . 1_554
O6 O2 O7 162.8(18) . 1_554
La1 O2 O7 131.0(15) . 1_554
O3 O2 O7 98.2(17) 3_554 1_554
O5 O2 O7 103.9(18) 1_554 1_554
O1 O2 O7 76.9(18) 4 1_554
O5 O2 O7 124.6(17) 2_656 1_554
O4 O2 O7 48.0(16) . 1_554
O2 O2 O7 74.8(10) 2_655 1_554
O1 O2 O7 82.3(15) 4_655 1_554
O5 O2 O7 116.7(15) 2_556 1_554
Ta O2 O7 128.1(15) 1_565 1_554
Ga1 O2 O7 128.1(15) 1_565 1_554
O1 O2 O7 51.6(12) 3_554 1_554
O2 O2 O7 73.8(11) 2 1_554
Ga2 O2 O7 52.9(9) 2_655 1_554
Ga4 O2 O7 158.3(13) 4_655 1_554
Ga3 O2 La2 61.5(10) 1_655 1_655
Ga2 O2 La2 58.0(10) . 1_655
La2 O2 La2 95.2(13) . 1_655
O6 O2 La2 123.9(13) . 1_655
La1 O2 La2 150.7(16) . 1_655
O3 O2 La2 99.7(15) 3_554 1_655
O5 O2 La2 92.7(15) 1_554 1_655
O1 O2 La2 134.0(18) 4 1_655
O5 O2 La2 62.1(11) 2_656 1_655
O4 O2 La2 68.5(12) . 1_655
O2 O2 La2 37.3(8) 2_655 1_655
O1 O2 La2 37.5(10) 4_655 1_655
O5 O2 La2 159.1(18) 2_556 1_655
Ta O2 La2 126.1(12) 1_565 1_655
Ga1 O2 La2 126.1(12) 1_565 1_655
O1 O2 La2 75.7(9) 3_554 1_655
O2 O2 La2 117.9(17) 2 1_655
Ga2 O2 La2 49.7(5) 2_655 1_655
Ga4 O2 La2 99.8(8) 4_655 1_655
O7 O2 La2 63.4(10) 1_554 1_655
Ga3 O2 La1 69.5(11) 1_655 1_655
Ga2 O2 La1 57.2(10) . 1_655
La2 O2 La1 152.1(15) . 1_655
O6 O2 La1 77.7(11) . 1_655
La1 O2 La1 93.6(13) . 1_655
O3 O2 La1 68.4(11) 3_554 1_655
O5 O2 La1 103.2(15) 1_554 1_655
O1 O2 La1 131(2) 4 1_655
O5 O2 La1 33.5(12) 2_656 1_655
O4 O2 La1 86.8(13) . 1_655
O2 O2 La1 75.9(12) 2_655 1_655
O1 O2 La1 35.2(10) 4_655 1_655
O5 O2 La1 126.4(16) 2_556 1_655
Ta O2 La1 106.6(12) 1_565 1_655
Ga1 O2 La1 106.6(12) 1_565 1_655
O1 O2 La1 128.6(11) 3_554 1_655
O2 O2 La1 158.9(14) 2 1_655
Ga2 O2 La1 102.1(8) 2_655 1_655
Ga4 O2 La1 57.4(6) 4_655 1_655
O7 O2 La1 116.8(12) 1_554 1_655
La2 O2 La1 59.4(5) 1_655 1_655
Ga3 O2 La1 163.9(18) 1_655 4_545
Ga2 O2 La1 52.1(11) . 4_545
La2 O2 La1 70.6(10) . 4_545
O6 O2 La1 121.6(14) . 4_545
La1 O2 La1 70.4(10) . 4_545
O3 O2 La1 38.3(10) 3_554 4_545
O5 O2 La1 154.7(16) 1_554 4_545
O1 O2 La1 36.8(12) 4 4_545
O5 O2 La1 135.4(17) 2_656 4_545
O4 O2 La1 34.0(11) . 4_545
O2 O2 La1 135.2(7) 2_655 4_545
O1 O2 La1 82.0(14) 4_655 4_545
O5 O2 La1 96.0(13) 2_556 4_545
Ta O2 La1 131.1(10) 1_565 4_545
Ga1 O2 La1 131.1(10) 1_565 4_545
O1 O2 La1 111.4(13) 3_554 4_545
O2 O2 La1 99.0(9) 2 4_545
Ga2 O2 La1 119.3(12) 2_655 4_545
Ga4 O2 La1 133.7(13) 4_655 4_545
O7 O2 La1 66.5(11) 1_554 4_545
La2 O2 La1 102.5(10) 1_655 4_545
La1 O2 La1 102.0(10) 1_655 4_545
Ga3 O2 Ga4 120.2(16) 1_655 .
Ga2 O2 Ga4 43.4(12) . .
La2 O2 Ga4 126.1(16) . .
O6 O2 Ga4 85.9(13) . .
La1 O2 Ga4 59.0(10) . .
O3 O2 Ga4 17.7(7) 3_554 .
O5 O2 Ga4 144(2) 1_554 .
O1 O2 Ga4 79.0(17) 4 .
O5 O2 Ga4 82.3(15) 2_656 .
O4 O2 Ga4 62.1(14) . .
O2 O2 Ga4 124.2(17) 2_655 .
O1 O2 Ga4 55.6(13) 4_655 .
O5 O2 Ga4 105.6(15) 2_556 .
Ta O2 Ga4 119.1(13) 1_565 .
Ga1 O2 Ga4 119.1(13) 1_565 .
O1 O2 Ga4 161.2(15) 3_554 .
O2 O2 Ga4 144.9(16) 2 .
Ga2 O2 Ga4 142.3(11) 2_655 .
Ga4 O2 Ga4 83.2(9) 4_655 .
O7 O2 Ga4 110.0(14) 1_554 .
La2 O2 Ga4 93.1(8) 1_655 .
La1 O2 Ga4 51.7(5) 1_655 .
La1 O2 Ga4 55.7(7) 4_545 .
Ga3 O2 Ga3 102.8(16) 1_655 .
Ga2 O2 Ga3 143.4(18) . .
La2 O2 Ga3 58.5(7) . .
O6 O2 Ga3 71.8(9) . .
La1 O2 Ga3 64.9(8) . .
O3 O2 Ga3 111.0(14) 3_554 .
O5 O2 Ga3 65.2(11) 1_554 .
O1 O2 Ga3 54.8(12) 4 .
O5 O2 Ga3 126.4(18) 2_656 .
O4 O2 Ga3 117.5(14) . .
O2 O2 Ga3 113.3(19) 2_655 .
O1 O2 Ga3 173.3(17) 4_655 .
O5 O2 Ga3 23.5(10) 2_556 .
Ta O2 Ga3 46.8(5) 1_565 .
Ga1 O2 Ga3 46.8(5) 1_565 .
O1 O2 Ga3 68.7(8) 3_554 .
O2 O2 Ga3 26.6(7) 2 .
Ga2 O2 Ga3 94.9(10) 2_655 .
Ga4 O2 Ga3 93.5(10) 4_655 .
O7 O2 Ga3 93.8(11) 1_554 .
La2 O2 Ga3 144.4(13) 1_655 .
La1 O2 Ga3 149.4(13) 1_655 .
La1 O2 Ga3 91.4(7) 4_545 .
Ga4 O2 Ga3 121.4(10) . .
Ga3 O2 Ga4 114.0(16) 1_655 4_645
Ga2 O2 Ga4 39.4(12) . 4_645
La2 O2 Ga4 63.5(10) . 4_645
O6 O2 Ga4 164.9(17) . 4_645
La1 O2 Ga4 120.8(15) . 4_645
O3 O2 Ga4 70.8(13) 3_554 4_645
O5 O2 Ga4 131(2) 1_554 4_645
O1 O2 Ga4 79.4(14) 4 4_645
O5 O2 Ga4 112.2(14) 2_656 4_645
O4 O2 Ga4 19.9(11) . 4_645
O2 O2 Ga4 84.1(5) 2_655 4_645
O1 O2 Ga4 55.6(11) 4_655 4_645
O5 O2 Ga4 137.3(15) 2_556 4_645
Ta O2 Ga4 160.1(14) 1_565 4_645
Ga1 O2 Ga4 160.1(14) 1_565 4_645
O1 O2 Ga4 81.9(12) 3_554 4_645
O2 O2 Ga4 104.3(6) 2 4_645
Ga2 O2 Ga4 73.8(8) 2_655 4_645
Ga4 O2 Ga4 147.7(10) 4_655 4_645
O7 O2 Ga4 32.1(10) 1_554 4_645
La2 O2 Ga4 54.7(6) 1_655 4_645
La1 O2 Ga4 90.6(8) 1_655 4_645
La1 O2 Ga4 51.1(6) 4_545 4_645
Ga4 O2 Ga4 79.3(9) . 4_645
Ga3 O2 Ga4 118.8(10) . 4_645
Ga3 O2 O7 89.9(16) 1_655 2_656
Ga2 O2 O7 48.7(14) . 2_656
La2 O2 O7 69.6(13) . 2_656
O6 O2 O7 156.3(15) . 2_656
La1 O2 O7 143.7(19) . 2_656
O3 O2 O7 89.0(16) 3_554 2_656
O5 O2 O7 110.8(19) 1_554 2_656
O1 O2 O7 101.9(18) 4 2_656
O5 O2 O7 94.1(12) 2_656 2_656
O4 O2 O7 42.4(13) . 2_656
O2 O2 O7 60.1(9) 2_655 2_656
O1 O2 O7 49.0(13) 4_655 2_656
O5 O2 O7 151.1(19) 2_556 2_656
Ta O2 O7 146.6(16) 1_565 2_656
Ga1 O2 O7 146.6(16) 1_565 2_656
O1 O2 O7 70.3(13) 3_554 2_656
O2 O2 O7 105.1(14) 2 2_656
Ga2 O2 O7 54.2(10) 2_655 2_656
Ga4 O2 O7 132.0(12) 4_655 2_656
O7 O2 O7 34.5(15) 1_554 2_656
La2 O2 O7 32.6(8) 1_655 2_656
La1 O2 O7 82.5(10) 1_655 2_656
La1 O2 O7 75.2(11) 4_545 2_656
Ga4 O2 O7 92.1(12) . 2_656
Ga3 O2 O7 127.8(14) . 2_656
Ga4 O2 O7 24.1(8) 4_645 2_656
Ga3 O2 O3 67.2(14) 1_655 2_666
Ga2 O2 O3 87.7(16) . 2_666
La2 O2 O3 171.2(17) . 2_666
O6 O2 O3 41.9(8) . 2_666
La1 O2 O3 68.3(10) . 2_666
O3 O2 O3 76.3(10) 3_554 2_666
O5 O2 O3 85.2(17) 1_554 2_666
O1 O2 O3 121.3(19) 4 2_666
O5 O2 O3 34.5(12) 2_656 2_666
O4 O2 O3 116.2(18) . 2_666
O2 O2 O3 90.3(8) 2_655 2_666
O1 O2 O3 71.1(13) 4_655 2_666
O5 O2 O3 90.6(13) 2_556 2_666
Ta O2 O3 73.6(10) 1_565 2_666
Ga1 O2 O3 73.6(10) 1_565 2_666
O1 O2 O3 134.1(17) 3_554 2_666
O2 O2 O3 130.2(8) 2 2_666
Ga2 O2 O3 117.8(12) 2_655 2_666
Ga4 O2 O3 25.5(5) 4_655 2_666
O7 O2 O3 152.7(11) 1_554 2_666
La2 O2 O3 90.8(7) 1_655 2_666
La1 O2 O3 36.1(6) 1_655 2_666
La1 O2 O3 114.4(14) 4_545 2_666
Ga4 O2 O3 59.7(9) . 2_666
Ga3 O2 O3 113.3(10) . 2_666
Ga4 O2 O3 125.3(11) 4_645 2_666
O7 O2 O3 118.2(11) 2_656 2_666
Ga3 O2 O4 97.7(17) 1_655 4_655
Ga2 O2 O4 56.8(16) . 4_655
La2 O2 O4 150.1(19) . 4_655
O6 O2 O4 68.9(14) . 4_655
La1 O2 O4 62.0(13) . 4_655
O3 O2 O4 41.4(11) 3_554 4_655
O5 O2 O4 121(2) 1_554 4_655
O1 O2 O4 99(2) 4 4_655
O5 O2 O4 59.8(16) 2_656 4_655
O4 O2 O4 82.1(14) . 4_655
O2 O2 O4 109.7(17) 2_655 4_655
O1 O2 O4 54.2(15) 4_655 4_655
O5 O2 O4 104.3(17) 2_556 4_655
Ta O2 O4 103.7(15) 1_565 4_655
Ga1 O2 O4 103.7(15) 1_565 4_655
O1 O2 O4 162.5(14) 3_554 4_655
O2 O2 O4 152.5(16) 2 4_655
Ga2 O2 O4 135.7(12) 2_655 4_655
Ga4 O2 O4 60.7(11) 4_655 4_655
O7 O2 O4 128.2(18) 1_554 4_655
La2 O2 O4 88.9(11) 1_655 4_655
La1 O2 O4 33.9(9) 1_655 4_655
La1 O2 O4 79.6(12) 4_545 4_655
Ga4 O2 O4 24.0(9) . 4_655
Ga3 O2 O4 126.2(14) . 4_655
Ga4 O2 O4 96.1(13) 4_645 4_655
O7 O2 O4 101.1(15) 2_656 4_655
O3 O2 O4 36.1(10) 2_666 4_655
Ga3 O2 Ga2 145.3(18) 1_655 1_455
Ga2 O2 Ga2 101.0(16) . 1_455
La2 O2 Ga2 54.3(7) . 1_455
O6 O2 Ga2 94.8(10) . 1_455
La1 O2 Ga2 54.3(7) . 1_455
O3 O2 Ga2 73.5(12) 3_554 1_455
O5 O2 Ga2 107.6(13) 1_554 1_455
O1 O2 Ga2 12.2(11) 4 1_455
O5 O2 Ga2 155.8(18) 2_656 1_455
O4 O2 Ga2 78.6(13) . 1_455
O2 O2 Ga2 143.4(19) 2_655 1_455
O1 O2 Ga2 130.8(17) 4_655 1_455
O5 O2 Ga2 50.5(11) 2_556 1_455
Ta O2 Ga2 85.1(7) 1_565 1_455
Ga1 O2 Ga2 85.1(7) 1_565 1_455
O1 O2 Ga2 90.7(9) 3_554 1_455
O2 O2 Ga2 56.8(9) 2 1_455
Ga2 O2 Ga2 115.7(11) 2_655 1_455
Ga4 O2 Ga2 118.8(10) 4_655 1_455
O7 O2 Ga2 79.7(10) 1_554 1_455
La2 O2 Ga2 141.3(13) 1_655 1_455
La1 O2 Ga2 140.1(12) 1_655 1_455
La1 O2 Ga2 48.9(5) 4_545 1_455
Ga4 O2 Ga2 89.0(9) . 1_455
Ga3 O2 Ga2 42.6(4) . 1_455
Ga4 O2 Ga2 88.0(8) 4_645 1_455
O7 O2 Ga2 108.8(13) 2_656 1_455
O3 O2 Ga2 122.7(10) 2_666 1_455
O4 O2 Ga2 106.6(13) 4_655 1_455
Ga3 O2 O6 4.7(9) 1_655 2_655
Ga2 O2 O6 115.3(13) . 2_655
La2 O2 O6 113.2(15) . 2_655
O6 O2 O6 66.3(12) . 2_655
La1 O2 O6 117.9(15) . 2_655
O3 O2 O6 136.2(14) 3_554 2_655
O5 O2 O6 36.4(10) 1_554 2_655
O1 O2 O6 155.8(18) 4 2_655
O5 O2 O6 36.3(13) 2_656 2_655
O4 O2 O6 133.9(14) . 2_655
O2 O2 O6 35.7(7) 2_655 2_655
O1 O2 O6 85.5(12) 4_655 2_655
O5 O2 O6 96.7(15) 2_556 2_655
Ta O2 O6 61.4(8) 1_565 2_655
Ga1 O2 O6 61.4(8) 1_565 2_655
O1 O2 O6 70.8(10) 3_554 2_655
O2 O2 O6 90.8(13) 2 2_655
Ga2 O2 O6 56.8(7) 2_655 2_655
Ga4 O2 O6 49.5(6) 4_655 2_655
O7 O2 O6 109.0(12) 1_554 2_655
La2 O2 O6 65.4(6) 1_655 2_655
La1 O2 O6 68.8(6) 1_655 2_655
La1 O2 O6 167.2(10) 4_545 2_655
Ga4 O2 O6 118.5(10) . 2_655
Ga3 O2 O6 101.0(10) . 2_655
Ga4 O2 O6 118.5(9) 4_645 2_655
O7 O2 O6 94.4(11) 2_656 2_655
O3 O2 O6 63.7(9) 2_666 2_655
O4 O2 O6 95.5(11) 4_655 2_655
Ga2 O2 O6 143.6(11) 1_455 2_655
Ga3 O2 O7 127(2) 1_655 2_556
Ga2 O2 O7 86.7(17) . 2_556
La2 O2 O7 18.4(9) . 2_556
O6 O2 O7 136.0(14) . 2_556
La1 O2 O7 99.3(13) . 2_556
O3 O2 O7 90.5(15) 3_554 2_556
O5 O2 O7 106.2(19) 1_554 2_556
O1 O2 O7 45.1(13) 4 2_556
O5 O2 O7 158(2) 2_656 2_556
O4 O2 O7 57.1(14) . 2_556
O2 O2 O7 103.6(15) 2_655 2_556
O1 O2 O7 109.0(16) 4_655 2_556
O5 O2 O7 85.8(13) 2_556 2_556
Ta O2 O7 110.1(12) 1_565 2_556
Ga1 O2 O7 110.1(12) 1_565 2_556
O1 O2 O7 60.1(12) 3_554 2_556
O2 O2 O7 55.2(9) 2 2_556
Ga2 O2 O7 76.6(11) 2_655 2_556
Ga4 O2 O7 158.9(13) 4_655 2_556
O7 O2 O7 34.3(13) 1_554 2_556
La2 O2 O7 97.6(12) 1_655 2_556
La1 O2 O7 143.4(14) 1_655 2_556
La1 O2 O7 52.2(9) 4_545 2_556
Ga4 O2 O7 107.7(13) . 2_556
Ga3 O2 O7 65.4(9) . 2_556
Ga4 O2 O7 53.5(9) 4_645 2_556
O7 O2 O7 66.9(12) 2_656 2_556
O3 O2 O7 165.4(17) 2_666 2_556
O4 O2 O7 131.7(16) 4_655 2_556
Ga2 O2 O7 45.7(8) 1_455 2_556
O6 O2 O7 130.8(14) 2_655 2_556
Ga3 O2 O1 102.7(18) 1_655 1_565
Ga2 O2 O1 91.9(18) . 1_565
La2 O2 O1 135.8(13) . 1_565
O6 O2 O1 39.5(10) . 1_565
La1 O2 O1 27.7(6) . 1_565
O3 O2 O1 56.3(10) 3_554 1_565
O5 O2 O1 101.5(18) 1_554 1_565
O1 O2 O1 80.6(13) 4 1_565
O5 O2 O1 75.4(15) 2_656 1_565
O4 O2 O1 107.8(18) . 1_565
O2 O2 O1 130.4(11) 2_655 1_565
O1 O2 O1 94.3(13) 4_655 1_565
O5 O2 O1 64.1(13) 2_556 1_565
Ta O2 O1 70.4(10) 1_565 1_565
Ga1 O2 O1 70.4(10) 1_565 1_565
O1 O2 O1 149.5(16) 3_554 1_565
O2 O2 O1 112.4(11) 2 1_565
Ga2 O2 O1 154.9(14) 2_655 1_565
Ga4 O2 O1 48.9(8) 4_655 1_565
O7 O2 O1 152.1(16) 1_554 1_565
La2 O2 O1 126.7(10) 1_655 1_565
La1 O2 O1 67.4(7) 1_655 1_565
La1 O2 O1 85.6(11) 4_545 1_565
Ga4 O2 O1 48.7(8) . 1_565
Ga3 O2 O1 86.5(8) . 1_565
Ga4 O2 O1 127.0(13) 4_645 1_565
O7 O2 O1 140.1(15) 2_656 1_565
O3 O2 O1 41.0(6) 2_666 1_565
O4 O2 O1 40.2(10) 4_655 1_565
Ga2 O2 O1 81.9(8) 1_455 1_565
O6 O2 O1 98.3(11) 2_655 1_565
O7 O2 O1 125.8(12) 2_556 1_565
Ga3 O2 La1 57.0(12) 1_655 2
Ga2 O2 La1 149(2) . 2
La2 O2 La1 62.4(10) . 2
O6 O2 La1 81.6(12) . 2
La1 O2 La1 110.9(12) . 2
O3 O2 La1 163.3(15) 3_554 2
O5 O2 La1 25.8(12) 1_554 2
O1 O2 La1 101.5(16) 4 2
O5 O2 La1 93.5(16) 2_656 2
O4 O2 La1 130.0(17) . 2
O2 O2 La1 60.9(14) 2_655 2
O1 O2 La1 131.8(15) 4_655 2
O5 O2 La1 64.7(13) 2_556 2
Ta O2 La1 48.4(6) 1_565 2
Ga1 O2 La1 48.4(6) 1_565 2
O1 O2 La1 31.4(8) 3_554 2
O2 O2 La1 33.8(9) 2 2
Ga2 O2 La1 48.0(6) 2_655 2
Ga4 O2 La1 86.1(9) 4_655 2
O7 O2 La1 82.2(11) 1_554 2
La2 O2 La1 95.4(9) 1_655 2
La1 O2 La1 126.4(10) 1_655 2
La1 O2 La1 130.8(10) 4_545 2
Ga4 O2 La1 167.4(12) . 2
Ga3 O2 La1 52.5(5) . 2
Ga4 O2 La1 113.2(11) 4_645 2
O7 O2 La1 100.0(13) 2_656 2
O3 O2 La1 110.8(13) 2_666 2
O4 O2 La1 146.8(15) 4_655 2
Ga2 O2 La1 90.3(7) 1_455 2
O6 O2 La1 57.6(6) 2_655 2
O7 O2 La1 80.4(11) 2_556 2
O1 O2 La1 118.7(11) 1_565 2
Ga3 O2 O6 66.4(13) 1_655 2
Ga2 O2 O6 178(2) . 2
La2 O2 O6 77.5(11) . 2
O6 O2 O6 56.2(11) . 2
La1 O2 O6 82.5(11) . 2
O3 O2 O6 138.8(14) 3_554 2
O5 O2 O6 29.4(9) 1_554 2
O1 O2 O6 91.4(14) 4 2
O5 O2 O6 92.5(16) 2_656 2
O4 O2 O6 149.1(16) . 2
O2 O2 O6 83.5(15) 2_655 2
O1 O2 O6 149.9(16) 4_655 2
O5 O2 O6 38.4(12) 2_556 2
Ta O2 O6 21.4(5) 1_565 2
Ga1 O2 O6 21.4(5) 1_565 2
O1 O2 O6 59.5(10) 3_554 2
O2 O2 O6 36.9(7) 2 2
Ga2 O2 O6 76.8(9) 2_655 2
Ga4 O2 O6 68.8(8) 4_655 2
O7 O2 O6 106.7(13) 1_554 2
La2 O2 O6 120.6(11) 1_655 2
La1 O2 O6 123.8(11) 1_655 2
La1 O2 O6 128.0(9) 4_545 2
Ga4 O2 O6 138.6(12) . 2
Ga3 O2 O6 36.7(5) . 2
Ga4 O2 O6 138.8(12) 4_645 2
O7 O2 O6 129.3(15) 2_656 2
O3 O2 O6 93.9(11) 2_666 2
O4 O2 O6 125.1(14) 4_655 2
Ga2 O2 O6 79.3(7) 1_455 2
O6 O2 O6 64.4(7) 2_655 2
O7 O2 O6 92.0(11) 2_556 2
O1 O2 O6 90.1(10) 1_565 2
La1 O2 O6 29.3(4) 2 2
Ga3 O2 Ga2 90.5(15) 1_655 4_655
Ga2 O2 Ga2 79.2(15) . 4_655
La2 O2 Ga2 156.8(14) . 4_655
O6 O2 Ga2 46.6(9) . 4_655
La1 O2 Ga2 49.7(8) . 4_655
O3 O2 Ga2 55.7(7) 3_554 4_655
O5 O2 Ga2 103.4(18) 1_554 4_655
O1 O2 Ga2 99.0(17) 4 4_655
O5 O2 Ga2 56.7(13) 2_656 4_655
O4 O2 Ga2 103.0(16) . 4_655
O2 O2 Ga2 112.6(12) 2_655 4_655
O1 O2 Ga2 74.0(13) 4_655 4_655
O5 O2 Ga2 84.7(14) 2_556 4_655
Ta O2 Ga2 81.4(10) 1_565 4_655
Ga1 O2 Ga2 81.4(10) 1_565 4_655
O1 O2 Ga2 155.7(15) 3_554 4_655
O2 O2 Ga2 132.4(9) 2 4_655
Ga2 O2 Ga2 140.6(10) 2_655 4_655
Ga4 O2 Ga2 42.6(5) 4_655 4_655
O7 O2 Ga2 150.4(15) 1_554 4_655
La2 O2 Ga2 104.2(8) 1_655 4_655
La1 O2 Ga2 44.8(5) 1_655 4_655
La1 O2 Ga2 92.5(10) 4_545 4_655
Ga4 O2 Ga2 41.3(5) . 4_655
Ga3 O2 Ga2 107.9(9) . 4_655
Ga4 O2 Ga2 118.4(11) 4_645 4_655
O7 O2 Ga2 122.5(13) 2_656 4_655
O3 O2 Ga2 23.3(5) 2_666 4_655
O4 O2 Ga2 22.5(9) 4_655 4_655
Ga2 O2 Ga2 102.6(9) 1_455 4_655
O6 O2 Ga2 86.9(8) 2_655 4_655
O7 O2 Ga2 142.0(13) 2_556 4_655
O1 O2 Ga2 22.6(3) 1_565 4_655
La1 O2 Ga2 127.0(11) 2 4_655
O6 O2 Ga2 102.7(10) 2 4_655
Ga3 O2 O4 67.7(15) 1_655 2_655
Ga2 O2 O4 85.0(16) . 2_655
La2 O2 O4 56.7(10) . 2_655
O6 O2 O4 136.0(16) . 2_655
La1 O2 O4 164.9(14) . 2_655
O3 O2 O4 125.1(16) 3_554 2_655
O5 O2 O4 76.0(17) 1_554 2_655
O1 O2 O4 111.4(18) 4 2_655
O5 O2 O4 92.3(15) 2_656 2_655
O4 O2 O4 75.0(19) . 2_655
O2 O2 O4 38.3(9) 2_655 2_655
O1 O2 O4 77.0(14) 4_655 2_655
O5 O2 O4 124.2(16) 2_556 2_655
Ta O2 O4 110.5(13) 1_565 2_655
Ga1 O2 O4 110.5(13) 1_565 2_655
O1 O2 O4 35.9(9) 3_554 2_655
O2 O2 O4 76.7(13) 2 2_655
Ga2 O2 O4 18.8(7) 2_655 2_655
Ga4 O2 O4 121.5(11) 4_655 2_655
O7 O2 O4 36.8(10) 1_554 2_655
La2 O2 O4 42.1(7) 1_655 2_655
La1 O2 O4 100.9(9) 1_655 2_655
La1 O2 O4 101.8(11) 4_545 2_655
Ga4 O2 O4 128.1(12) . 2_655
Ga3 O2 O4 103.2(11) . 2_655
Ga4 O2 O4 55.1(8) 4_645 2_655
O7 O2 O4 36.5(11) 2_656 2_655
O3 O2 O4 126.6(10) 2_666 2_655
O4 O2 O4 130.6(15) 4_655 2_655
Ga2 O2 O4 110.7(10) 1_455 2_655
O6 O2 O4 72.3(9) 2_655 2_655
O7 O2 O4 66.3(10) 2_556 2_655
O1 O2 O4 167.4(11) 1_565 2_655
La1 O2 O4 63.7(9) 2 2_655
O6 O2 O4 93.1(11) 2 2_655
Ga2 O2 O4 145.3(9) 4_655 2_655
Ga3 O2 Ga1 25.4(9) 1_655 1_665
Ga2 O2 Ga1 96.8(12) . 1_665
La2 O2 Ga1 134.6(15) . 1_665
O6 O2 Ga1 63.7(9) . 1_665
La1 O2 Ga1 109.7(14) . 1_665
O3 O2 Ga1 112.5(13) 3_554 1_665
O5 O2 Ga1 58.4(11) 1_554 1_665
O1 O2 Ga1 164.0(18) 4 1_665
O5 O2 Ga1 12.7(12) 2_656 1_665
O4 O2 Ga1 122.4(12) . 1_665
O2 O2 Ga1 46.2(7) 2_655 1_665
O1 O2 Ga1 67.5(10) 4_655 1_665
O5 O2 Ga1 107.6(15) 2_556 1_665
Ta O2 Ga1 73.9(8) 1_565 1_665
Ga1 O2 Ga1 73.9(8) 1_565 1_665
O1 O2 Ga1 92.5(11) 3_554 1_665
O2 O2 Ga1 114.0(14) 2 1_665
Ga2 O2 Ga1 73.2(7) 2_655 1_665
Ga4 O2 Ga1 40.5(4) 4_655 1_665
O7 O2 Ga1 119.0(11) 1_554 1_665
La2 O2 Ga1 60.5(5) 1_655 1_665
La1 O2 Ga1 45.2(4) 1_655 1_665
La1 O2 Ga1 146.9(11) 4_545 1_665
Ga4 O2 Ga1 94.9(8) . 1_665
Ga3 O2 Ga1 119.3(11) . 1_665
Ga4 O2 Ga1 114.2(8) 4_645 1_665
O7 O2 Ga1 93.0(10) 2_656 1_665
O3 O2 Ga1 44.6(7) 2_666 1_665
O4 O2 Ga1 72.4(10) 4_655 1_665
Ga2 O2 Ga1 157.7(12) 1_455 1_665
O6 O2 Ga1 23.8(4) 2_655 1_665
O7 O2 Ga1 149.7(14) 2_556 1_665
O1 O2 Ga1 84.3(9) 1_565 1_665
La1 O2 Ga1 81.2(8) 2 1_665
O6 O2 Ga1 83.4(8) 2 1_665
Ga2 O2 Ga1 67.7(6) 4_655 1_665
O4 O2 Ga1 84.0(9) 2_655 1_665
Ga3 O2 Ta 25.4(9) 1_655 1_665
Ga2 O2 Ta 96.8(12) . 1_665
La2 O2 Ta 134.6(15) . 1_665
O6 O2 Ta 63.7(9) . 1_665
La1 O2 Ta 109.7(14) . 1_665
O3 O2 Ta 112.5(13) 3_554 1_665
O5 O2 Ta 58.4(11) 1_554 1_665
O1 O2 Ta 164.0(18) 4 1_665
O5 O2 Ta 12.7(12) 2_656 1_665
O4 O2 Ta 122.4(12) . 1_665
O2 O2 Ta 46.2(7) 2_655 1_665
O1 O2 Ta 67.5(10) 4_655 1_665
O5 O2 Ta 107.6(15) 2_556 1_665
Ta O2 Ta 73.9(8) 1_565 1_665
Ga1 O2 Ta 73.9(8) 1_565 1_665
O1 O2 Ta 92.5(11) 3_554 1_665
O2 O2 Ta 114.0(14) 2 1_665
Ga2 O2 Ta 73.2(7) 2_655 1_665
Ga4 O2 Ta 40.5(4) 4_655 1_665
O7 O2 Ta 119.0(11) 1_554 1_665
La2 O2 Ta 60.5(5) 1_655 1_665
La1 O2 Ta 45.2(4) 1_655 1_665
La1 O2 Ta 146.9(11) 4_545 1_665
Ga4 O2 Ta 94.9(8) . 1_665
Ga3 O2 Ta 119.3(11) . 1_665
Ga4 O2 Ta 114.2(8) 4_645 1_665
O7 O2 Ta 93.0(10) 2_656 1_665
O3 O2 Ta 44.6(7) 2_666 1_665
O4 O2 Ta 72.4(10) 4_655 1_665
Ga2 O2 Ta 157.7(12) 1_455 1_665
O6 O2 Ta 23.8(4) 2_655 1_665
O7 O2 Ta 149.7(14) 2_556 1_665
O1 O2 Ta 84.3(9) 1_565 1_665
La1 O2 Ta 81.2(8) 2 1_665
O6 O2 Ta 83.4(8) 2 1_665
Ga2 O2 Ta 67.7(6) 4_655 1_665
O4 O2 Ta 84.0(9) 2_655 1_665
Ga1 O2 Ta 0.00(14) 1_665 1_665
Ga3 O2 O7 47.1(13) 1_655 1_564
Ga2 O2 O7 142.2(18) . 1_564
La2 O2 O7 115.8(16) . 1_564
O6 O2 O7 28.9(11) . 1_564
La1 O2 O7 78.2(13) . 1_564
O3 O2 O7 124.0(13) 3_554 1_564
O5 O2 O7 33.8(15) 1_554 1_564
O1 O2 O7 117.3(16) 4 1_564
O5 O2 O7 56.6(13) 2_656 1_564
O4 O2 O7 171.9(17) . 1_564
O2 O2 O7 76.7(9) 2_655 1_564
O1 O2 O7 116.7(15) 4_655 1_564
O5 O2 O7 56.8(13) 2_556 1_564
Ta O2 O7 23.1(8) 1_565 1_564
Ga1 O2 O7 23.1(8) 1_565 1_564
O1 O2 O7 86.2(14) 3_554 1_564
O2 O2 O7 75.9(10) 2 1_564
Ga2 O2 O7 88.8(11) 2_655 1_564
Ga4 O2 O7 30.5(8) 4_655 1_564
O7 O2 O7 137.7(18) 1_554 1_564
La2 O2 O7 107.8(10) 1_655 1_564
La1 O2 O7 85.1(10) 1_655 1_564
La1 O2 O7 148.1(12) 4_545 1_564
Ga4 O2 O7 111.8(12) . 1_564
Ga3 O2 O7 69.8(10) . 1_564
Ga4 O2 O7 160.8(12) 4_645 1_564
O7 O2 O7 136.7(10) 2_656 1_564
O3 O2 O7 56.0(11) 2_666 1_564
O4 O2 O7 90.7(13) 4_655 1_564
Ga2 O2 O7 107.2(10) 1_455 1_564
O6 O2 O7 42.7(7) 2_655 1_564
O7 O2 O7 131.0(10) 2_556 1_564
O1 O2 O7 68.2(11) 1_565 1_564
La1 O2 O7 56.6(9) 2 1_564
O6 O2 O7 39.0(9) 2 1_564
Ga2 O2 O7 70.5(10) 4_655 1_564
O4 O2 O7 107.4(13) 2_655 1_564
Ga1 O2 O7 51.1(8) 1_665 1_564
Ta O2 O7 51.1(8) 1_665 1_564
Ga3 O2 Ga4 25.8(10) 1_655 3_554
Ga2 O2 Ga4 134.8(15) . 3_554
La2 O2 Ga4 110.9(14) . 3_554
O6 O2 Ga4 49.5(9) . 3_554
La1 O2 Ga4 100.2(13) . 3_554
O3 O2 Ga4 138.8(13) 3_554 3_554
O5 O2 Ga4 23.0(11) 1_554 3_554
O1 O2 Ga4 135.1(16) 4 3_554
O5 O2 Ga4 48.0(13) 2_656 3_554
O4 O2 Ga4 155.7(14) . 3_554
O2 O2 Ga4 54.6(7) 2_655 3_554
O1 O2 Ga4 105.1(12) 4_655 3_554
O5 O2 Ga4 74.9(13) 2_556 3_554
Ta O2 Ga4 39.5(5) 1_565 3_554
Ga1 O2 Ga4 39.5(5) 1_565 3_554
O1 O2 Ga4 72.6(11) 3_554 3_554
O2 O2 Ga4 77.8(10) 2 3_554
Ga2 O2 Ga4 68.5(8) 2_655 3_554
Ga4 O2 Ga4 40.7(5) 4_655 3_554
O7 O2 Ga4 120.7(12) 1_554 3_554
La2 O2 Ga4 87.2(7) 1_655 3_554
La1 O2 Ga4 81.2(7) 1_655 3_554
La1 O2 Ga4 170.1(10) 4_545 3_554
Ga4 O2 Ga4 122.6(11) . 3_554
Ga3 O2 Ga4 81.6(8) . 3_554
Ga4 O2 Ga4 138.6(10) 4_645 3_554
O7 O2 Ga4 114.6(12) 2_656 3_554
O3 O2 Ga4 62.9(9) 2_666 3_554
O4 O2 Ga4 98.9(12) 4_655 3_554
Ga2 O2 Ga4 123.4(9) 1_455 3_554
O6 O2 Ga4 21.9(4) 2_655 3_554
O7 O2 Ga4 129.1(13) 2_556 3_554
O1 O2 Ga4 87.0(10) 1_565 3_554
La1 O2 Ga4 48.7(5) 2 3_554
O6 O2 Ga4 45.3(5) 2 3_554
Ga2 O2 Ga4 83.1(8) 4_655 3_554
O4 O2 Ga4 86.6(10) 2_655 3_554
Ga1 O2 Ga4 38.1(4) 1_665 3_554
Ta O2 Ga4 38.1(4) 1_665 3_554
O7 O2 Ga4 22.2(7) 1_564 3_554
Ga3 O2 O3 103.9(18) 1_655 2_566
Ga2 O2 O3 121(2) . 2_566
La2 O2 O3 107.2(10) . 2_566
O6 O2 O3 34.8(7) . 2_566
La1 O2 O3 22.9(5) . 2_566
O3 O2 O3 79.0(10) 3_554 2_566
O5 O2 O3 82.3(15) 1_554 2_566
O1 O2 O3 66.1(14) 4 2_566
O5 O2 O3 95.2(15) 2_656 2_566
O4 O2 O3 123.6(18) . 2_566
O2 O2 O3 134.0(11) 2_655 2_566
O1 O2 O3 128.9(17) 4_655 2_566
O5 O2 O3 29.5(11) 2_556 2_566
Ta O2 O3 46.2(7) 1_565 2_566
Ga1 O2 O3 46.2(7) 1_565 2_566
O1 O2 O3 117.2(13) 3_554 2_566
O2 O2 O3 77.8(7) 2 2_566
Ga2 O2 O3 137.5(15) 2_655 2_566
Ga4 O2 O3 58.0(6) 4_655 2_566
O7 O2 O3 139.7(9) 1_554 2_566
La2 O2 O3 156.9(9) 1_655 2_566
La1 O2 O3 99.6(8) 1_655 2_566
La1 O2 O3 90.8(10) 4_545 2_566
Ga4 O2 O3 78.7(9) . 2_566
Ga3 O2 O3 52.2(6) . 2_566
Ga4 O2 O3 141.9(13) 4_645 2_566
O7 O2 O3 165.9(17) 2_656 2_566
O3 O2 O3 66.3(5) 2_666 2_566
O4 O2 O3 74.8(12) 4_655 2_566
Ga2 O2 O3 60.9(6) 1_455 2_566
O6 O2 O3 99.3(11) 2_655 2_566
O7 O2 O3 105.5(9) 2_556 2_566
O1 O2 O3 34.6(6) 1_565 2_566
La1 O2 O3 89.9(10) 2 2_566
O6 O2 O3 60.8(9) 2 2_566
Ga2 O2 O3 55.8(6) 4_655 2_566
O4 O2 O3 153.0(14) 2_655 2_566
Ga1 O2 O3 98.4(9) 1_665 2_566
Ta O2 O3 98.4(9) 1_665 2_566
O7 O2 O3 57.3(10) 1_564 2_566
Ga4 O2 O3 79.4(9) 3_554 2_566
Ga3 O2 O6 111.3(14) 1_655 4_645
Ga2 O2 O6 24.8(11) . 4_645
La2 O2 O6 122.2(15) . 4_645
O6 O2 O6 101.1(13) . 4_645
La1 O2 O6 80.3(12) . 4_645
O3 O2 O6 30.0(9) 3_554 4_645
O5 O2 O6 146.4(16) 1_554 4_645
O1 O2 O6 90.8(17) 4 4_645
O5 O2 O6 76.7(14) 2_656 4_645
O4 O2 O6 50.6(12) . 4_645
O2 O2 O6 105.9(15) 2_655 4_645
O1 O2 O6 35.2(12) 4_655 4_645
O5 O2 O6 127.0(16) 2_556 4_645
Ta O2 O6 135.9(13) 1_565 4_645
Ga1 O2 O6 135.9(13) 1_565 4_645
O1 O2 O6 142.4(13) 3_554 4_645
O2 O2 O6 157.7(13) 2 4_645
Ga2 O2 O6 120.9(10) 2_655 4_645
Ga4 O2 O6 91.2(9) 4_655 4_645
O7 O2 O6 95.9(13) 1_554 4_645
La2 O2 O6 72.2(7) 1_655 4_645
La1 O2 O6 43.2(5) 1_655 4_645
La1 O2 O6 58.8(7) 4_545 4_645
Ga4 O2 O6 21.4(4) . 4_645
Ga3 O2 O6 140.8(11) . 4_645
Ga4 O2 O6 63.8(7) 4_645 4_645
O7 O2 O6 72.2(11) 2_656 4_645
O3 O2 O6 65.8(9) 2_666 4_645
O4 O2 O6 32.3(10) 4_655 4_645
Ga2 O2 O6 102.4(10) 1_455 4_645
O6 O2 O6 111.4(8) 2_655 4_645
O7 O2 O6 105.5(12) 2_556 4_645
O1 O2 O6 67.9(9) 1_565 4_645
La1 O2 O6 166.7(9) 2 4_645
O6 O2 O6 157.2(13) 2 4_645
Ga2 O2 O6 54.6(6) 4_655 4_645
O4 O2 O6 107.2(11) 2_655 4_645
Ga1 O2 O6 88.3(7) 1_665 4_645
Ta O2 O6 88.3(7) 1_665 4_645
O7 O2 O6 121.8(12) 1_564 4_645
Ga4 O2 O6 123.9(9) 3_554 4_645
O3 O2 O6 99.8(11) 2_566 4_645
Ga3 O2 O4 135(2) 1_655 4
Ga2 O2 O4 97.3(17) . 4
La2 O2 O4 94.6(12) . 4
O6 O2 O4 64.2(11) . 4
La1 O2 O4 14.5(9) . 4
O3 O2 O4 55.2(11) 3_554 4
O5 O2 O4 110.7(16) 1_554 4
O1 O2 O4 40.1(15) 4 4
O5 O2 O4 116.6(18) 2_656 4
O4 O2 O4 92.7(14) . 4
O2 O2 O4 165.2(11) 2_655 4
O1 O2 O4 118.1(18) 4_655 4
O5 O2 O4 45.8(13) 2_556 4
Ta O2 O4 75.2(10) 1_565 4
Ga1 O2 O4 75.2(10) 1_565 4
O1 O2 O4 125.6(12) 3_554 4
O2 O2 O4 84.2(13) 2 4
Ga2 O2 O4 152.8(12) 2_655 4
Ga4 O2 O4 84.4(10) 4_655 4
O7 O2 O4 116.7(12) 1_554 4
La2 O2 O4 154.8(14) 1_655 4
La1 O2 O4 104.7(12) 1_655 4
La1 O2 O4 59.5(9) 4_545 4
Ga4 O2 O4 62.6(9) . 4
Ga3 O2 O4 58.9(8) . 4
Ga4 O2 O4 110.6(12) 4_645 4
O7 O2 O4 134.7(15) 2_656 4
O3 O2 O4 82.5(10) 2_666 4
O4 O2 O4 71.4(13) 4_655 4
Ga2 O2 O4 40.4(8) 1_455 4
O6 O2 O4 130.3(13) 2_655 4
O7 O2 O4 84.9(12) 2_556 4
O1 O2 O4 41.5(8) 1_565 4
La1 O2 O4 109.7(10) 2 4
O6 O2 O4 84.2(10) 2 4
Ga2 O2 O4 62.6(9) 4_655 4
O4 O2 O4 150.9(14) 2_655 4
Ga1 O2 O4 124.1(12) 1_665 4
Ta O2 O4 124.1(12) 1_665 4
O7 O2 O4 88.6(12) 1_564 4
Ga4 O2 O4 110.7(11) 3_554 4
O3 O2 O4 31.3(8) 2_566 4
O6 O2 O4 83.0(11) 4_645 4
Ga3 O2 O2 55.5(12) 1_655 1_655
Ga2 O2 O2 58.0(12) . 1_655
La2 O2 O2 125.0(9) . 1_655
O6 O2 O2 98.1(8) . 1_655
La1 O2 O2 124.2(9) . 1_655
O3 O2 O2 88.7(11) 3_554 1_655
O5 O2 O2 93.2(10) 1_554 1_655
O1 O2 O2 146.8(14) 4 1_655
O5 O2 O2 36.9(13) 2_656 1_655
O4 O2 O2 81.5(11) . 1_655
O2 O2 O2 48.7(15) 2_655 1_655
O1 O2 O2 28.1(12) 4_655 1_655
O5 O2 O2 147.3(12) 2_556 1_655
Ta O2 O2 114.8(6) 1_565 1_655
Ga1 O2 O2 114.8(6) 1_565 1_655
O1 O2 O2 99.5(6) 3_554 1_655
O2 O2 O2 139.5(13) 2 1_655
Ga2 O2 O2 72.4(5) 2_655 1_655
Ga4 O2 O2 74.1(5) 4_655 1_655
O7 O2 O2 92.2(8) 1_554 1_655
La2 O2 O2 29.8(6) 1_655 1_655
La1 O2 O2 30.7(6) 1_655 1_655
La1 O2 O2 110.1(5) 4_545 1_655
Ga4 O2 O2 75.5(5) . 1_655
Ga3 O2 O2 158.3(6) . 1_655
Ga4 O2 O2 75.3(5) 4_645 1_655
O7 O2 O2 58.7(9) 2_656 1_655
O3 O2 O2 61.3(4) 2_666 1_655
O4 O2 O2 63.4(9) 4_655 1_655
Ga2 O2 O2 158.9(6) 1_455 1_655
O6 O2 O2 57.4(6) 2_655 1_655
O7 O2 O2 125.6(8) 2_556 1_655
O1 O2 O2 97.7(5) 1_565 1_655
La1 O2 O2 108.0(4) 2 1_655
O6 O2 O2 121.8(6) 2 1_655
Ga2 O2 O2 75.1(4) 4_655 1_655
O4 O2 O2 70.3(7) 2_655 1_655
Ga1 O2 O2 40.9(5) 1_665 1_655
Ta O2 O2 40.9(5) 1_665 1_655
O7 O2 O2 91.9(7) 1_564 1_655
Ga4 O2 O2 77.4(4) 3_554 1_655
O3 O2 O2 127.6(3) 2_566 1_655
O6 O2 O2 58.8(5) 4_645 1_655
O4 O2 O2 134.8(8) 4 1_655
Ga3 O2 O2 124.5(12) 1_655 1_455
Ga2 O2 O2 122.0(12) . 1_455
La2 O2 O2 55.0(9) . 1_455
O6 O2 O2 81.9(8) . 1_455
La1 O2 O2 55.8(9) . 1_455
O3 O2 O2 91.3(11) 3_554 1_455
O5 O2 O2 86.8(11) 1_554 1_455
O1 O2 O2 33.2(14) 4 1_455
O5 O2 O2 143.1(13) 2_656 1_455
O4 O2 O2 98.5(11) . 1_455
O2 O2 O2 131.3(15) 2_655 1_455
O1 O2 O2 151.9(12) 4_655 1_455
O5 O2 O2 32.7(12) 2_556 1_455
Ta O2 O2 65.2(6) 1_565 1_455
Ga1 O2 O2 65.2(6) 1_565 1_455
O1 O2 O2 80.5(6) 3_554 1_455
O2 O2 O2 40.5(13) 2 1_455
Ga2 O2 O2 107.6(5) 2_655 1_455
Ga4 O2 O2 105.9(5) 4_655 1_455
O7 O2 O2 87.8(8) 1_554 1_455
La2 O2 O2 150.2(6) 1_655 1_455
La1 O2 O2 149.3(6) 1_655 1_455
La1 O2 O2 69.9(5) 4_545 1_455
Ga4 O2 O2 104.5(5) . 1_455
Ga3 O2 O2 21.7(6) . 1_455
Ga4 O2 O2 104.7(5) 4_645 1_455
O7 O2 O2 121.3(9) 2_656 1_455
O3 O2 O2 118.7(4) 2_666 1_455
O4 O2 O2 116.6(9) 4_655 1_455
Ga2 O2 O2 21.1(6) 1_455 1_455
O6 O2 O2 122.6(6) 2_655 1_455
O7 O2 O2 54.4(8) 2_556 1_455
O1 O2 O2 82.3(5) 1_565 1_455
La1 O2 O2 72.0(4) 2 1_455
O6 O2 O2 58.2(6) 2 1_455
Ga2 O2 O2 104.9(4) 4_655 1_455
O4 O2 O2 109.7(7) 2_655 1_455
Ga1 O2 O2 139.1(5) 1_665 1_455
Ta O2 O2 139.1(5) 1_665 1_455
O7 O2 O2 88.1(7) 1_564 1_455
Ga4 O2 O2 102.6(4) 3_554 1_455
O3 O2 O2 52.4(3) 2_566 1_455
O6 O2 O2 121.2(5) 4_645 1_455
O4 O2 O2 45.2(8) 4 1_455
O2 O2 O2 179.999(8) 1_655 1_455
Ga3 O2 O7 34.1(12) 1_655 2_666
Ga2 O2 O7 113.1(17) . 2_666
La2 O2 O7 138.1(18) . 2_666
O6 O2 O7 41.1(10) . 2_666
La1 O2 O7 90.3(14) . 2_666
O3 O2 O7 112.7(14) 3_554 2_666
O5 O2 O7 50.3(13) 1_554 2_666
O1 O2 O7 142.0(19) 4 2_666
O5 O2 O7 26.1(14) 2_656 2_666
O4 O2 O7 142.0(15) . 2_666
O2 O2 O7 63.5(8) 2_655 2_666
O1 O2 O7 86.2(13) 4_655 2_666
O5 O2 O7 85.3(16) 2_556 2_666
Ta O2 O7 53.5(9) 1_565 2_666
Ga1 O2 O7 53.5(9) 1_565 2_666
O1 O2 O7 97.8(14) 3_554 2_666
O2 O2 O7 103.4(12) 2 2_666
Ga2 O2 O7 86.6(11) 2_655 2_666
Ga4 O2 O7 20.1(7) 4_655 2_666
O7 O2 O7 138.2(10) 1_554 2_666
La2 O2 O7 83.5(9) 1_655 2_666
La1 O2 O7 56.1(9) 1_655 2_666
La1 O2 O7 150.7(15) 4_545 2_666
Ga4 O2 O7 95.7(12) . 2_666
Ga3 O2 O7 100.3(11) . 2_666
Ga4 O2 O7 137.1(10) 4_645 2_666
O7 O2 O7 116.0(13) 2_656 2_666
O3 O2 O7 36.4(9) 2_666 2_666
O4 O2 O7 71.8(14) 4_655 2_666
Ga2 O2 O7 134.7(12) 1_455 2_666
O6 O2 O7 29.8(8) 2_655 2_666
O7 O2 O7 156.4(19) 2_556 2_666
O1 O2 O7 68.6(12) 1_565 2_666
La1 O2 O7 76.0(10) 2 2_666
O6 O2 O7 67.7(10) 2 2_666
Ga2 O2 O7 58.4(9) 4_655 2_666
O4 O2 O7 101.5(12) 2_655 2_666
Ga1 O2 O7 23.1(7) 1_665 2_666
Ta O2 O7 23.1(7) 1_665 2_666
O7 O2 O7 30.4(13) 1_564 2_666
Ga4 O2 O7 27.3(7) 3_554 2_666
O3 O2 O7 75.9(9) 2_566 2_666
O6 O2 O7 97.3(11) 4_645 2_666
O4 O2 O7 104.1(12) 4 2_666
O2 O2 O7 62.3(8) 1_655 2_666
O2 O2 O7 117.7(8) 1_455 2_666
Ga3 O2 Ga4 86.9(15) 1_655 3_544
Ga2 O2 Ga4 73.6(15) . 3_544
La2 O2 Ga4 46.9(8) . 3_544
O6 O2 Ga4 154.8(16) . 3_544
La1 O2 Ga4 149.2(14) . 3_544
O3 O2 Ga4 108.9(14) 3_554 3_544
O5 O2 Ga4 93.1(18) 1_554 3_544
O1 O2 Ga4 94.9(16) 4 3_544
O5 O2 Ga4 107.3(14) 2_656 3_544
O4 O2 Ga4 57.5(13) . 3_544
O2 O2 Ga4 56.8(7) 2_655 3_544
O1 O2 Ga4 75.1(12) 4_655 3_544
O5 O2 Ga4 126.1(15) 2_556 3_544
Ta O2 Ga4 124.5(12) 1_565 3_544
Ga1 O2 Ga4 124.5(12) 1_565 3_544
O1 O2 Ga4 45.0(9) 3_554 3_544
O2 O2 Ga4 78.5(9) 2 3_544
Ga2 O2 Ga4 37.4(5) 2_655 3_544
Ga4 O2 Ga4 140.3(10) 4_655 3_544
O7 O2 Ga4 18.2(7) 1_554 3_544
La2 O2 Ga4 48.4(5) 1_655 3_544
La1 O2 Ga4 106.3(8) 1_655 3_544
La1 O2 Ga4 82.4(8) 4_545 3_544
Ga4 O2 Ga4 116.5(10) . 3_544
Ga3 O2 Ga4 102.7(9) . 3_544
Ga4 O2 Ga4 38.1(4) 4_645 3_544
O7 O2 Ga4 26.8(8) 2_656 3_544
O3 O2 Ga4 139.1(7) 2_666 3_544
O4 O2 Ga4 127.9(13) 4_655 3_544
Ga2 O2 Ga4 96.8(9) 1_455 3_544
O6 O2 Ga4 91.6(8) 2_655 3_544
O7 O2 Ga4 51.1(8) 2_556 3_544
O1 O2 Ga4 165.0(13) 1_565 3_544
La1 O2 Ga4 76.1(7) 2 3_544
O6 O2 Ga4 104.4(10) 2 3_544
Ga2 O2 Ga4 149.1(9) 4_655 3_544
O4 O2 Ga4 19.5(6) 2_655 3_544
Ga1 O2 Ga4 101.0(7) 1_665 3_544
Ta O2 Ga4 101.0(7) 1_665 3_544
O7 O2 Ga4 125.9(12) 1_564 3_544
Ga4 O2 Ga4 105.9(9) 3_554 3_544
O3 O2 Ga4 154.0(7) 2_566 3_544
O6 O2 Ga4 98.0(9) 4_645 3_544
O4 O2 Ga4 134.9(11) 4 3_544
O2 O2 Ga4 78.1(4) 1_655 3_544
O2 O2 Ga4 101.9(4) 1_455 3_544
O7 O2 Ga4 120.3(11) 2_666 3_544
Ga3 O2 O4 67.1(15) 1_655 1_565
Ga2 O2 O4 113.6(19) . 1_565
La2 O2 O4 143.6(14) . 1_565
O6 O2 O4 14.2(8) . 1_565
La1 O2 O4 56.6(11) . 1_565
O3 O2 O4 90.2(12) 3_554 1_565
O5 O2 O4 68.0(17) 1_554 1_565
O1 O2 O4 109.9(16) 4 1_565
O5 O2 O4 50.3(13) 2_656 1_565
O4 O2 O4 139(2) . 1_565
O2 O2 O4 97.2(8) 2_655 1_565
O1 O2 O4 98.7(15) 4_655 1_565
O5 O2 O4 64.1(12) 2_556 1_565
Ta O2 O4 47.0(8) 1_565 1_565
Ga1 O2 O4 47.0(8) 1_565 1_565
O1 O2 O4 120.6(15) 3_554 1_565
O2 O2 O4 103.0(7) 2 1_565
Ga2 O2 O4 118.3(13) 2_655 1_565
Ga4 O2 O4 13.8(6) 4_655 1_565
O7 O2 O4 171.1(15) 1_554 1_565
La2 O2 O4 112.4(10) 1_655 1_565
La1 O2 O4 63.5(9) 1_655 1_565
La1 O2 O4 122.4(13) 4_545 1_565
Ga4 O2 O4 77.4(11) . 1_565
Ga3 O2 O4 86.0(9) . 1_565
Ga4 O2 O4 152.6(12) 4_645 1_565
O7 O2 O4 143.6(12) 2_656 1_565
O3 O2 O4 27.7(8) 2_666 1_565
O4 O2 O4 57.6(12) 4_655 1_565
Ga2 O2 O4 105.8(10) 1_455 1_565
O6 O2 O4 62.5(10) 2_655 1_565
O7 O2 O4 149.4(11) 2_556 1_565
O1 O2 O4 36.8(10) 1_565 1_565
La1 O2 O4 90.7(11) 2 1_565
O6 O2 O4 68.2(9) 2 1_565
Ga2 O2 O4 36.3(8) 4_655 1_565
O4 O2 O4 134.8(11) 2_655 1_565
Ga1 O2 O4 54.2(8) 1_665 1_565
Ta O2 O4 54.2(8) 1_665 1_565
O7 O2 O4 34.4(11) 1_564 1_565
Ga4 O2 O4 50.5(9) 3_554 1_565
O3 O2 O4 44.9(6) 2_566 1_565
O6 O2 O4 89.8(11) 4_645 1_565
O4 O2 O4 70.6(10) 4 1_565
O2 O2 O4 84.9(6) 1_655 1_565
O2 O2 O4 95.1(6) 1_455 1_565
O7 O2 O4 33.7(9) 2_666 1_565
Ga4 O2 O4 153.9(11) 3_544 1_565
Ga3 O2 O4 99.4(17) 1_655 2
Ga2 O2 O4 112.7(18) . 2
La2 O2 O4 13.1(9) . 2
O6 O2 O4 120.1(14) . 2
La1 O2 O4 110.3(11) . 2
O3 O2 O4 121.2(15) 3_554 2
O5 O2 O4 75.1(16) 1_554 2
O1 O2 O4 65.7(16) 4 2
O5 O2 O4 137.0(18) 2_656 2
O4 O2 O4 84.5(17) . 2
O2 O2 O4 83.9(15) 2_655 2
O1 O2 O4 124.9(16) 4_655 2
O5 O2 O4 75.8(13) 2_556 2
Ta O2 O4 86.5(10) 1_565 2
Ga1 O2 O4 86.5(10) 1_565 2
O1 O2 O4 32.3(9) 3_554 2
O2 O2 O4 30.6(8) 2 2
Ga2 O2 O4 56.1(8) 2_655 2
Ga4 O2 O4 133.8(12) 4_655 2
O7 O2 O4 43.3(10) 1_554 2
La2 O2 O4 96.5(10) 1_655 2
La1 O2 O4 155.8(11) 1_655 2
La1 O2 O4 83.1(9) 4_545 2
Ga4 O2 O4 138.7(11) . 2
Ga3 O2 O4 52.3(7) . 2
Ga4 O2 O4 74.0(9) 4_645 2
O7 O2 O4 75.8(12) 2_656 2
O3 O2 O4 159.3(15) 2_666 2
O4 O2 O4 162.6(17) 4_655 2
Ga2 O2 O4 59.6(8) 1_455 2
O6 O2 O4 101.8(11) 2_655 2
O7 O2 O4 31.2(11) 2_556 2
O1 O2 O4 136.8(10) 1_565 2
La1 O2 O4 49.3(7) 2 2
O6 O2 O4 65.7(8) 2 2
Ga2 O2 O4 159.4(10) 4_655 2
O4 O2 O4 55.0(8) 2_655 2
Ga1 O2 O4 124.6(11) 1_665 2
Ta O2 O4 124.6(11) 1_665 2
O7 O2 O4 103.3(12) 1_564 2
Ga4 O2 O4 97.9(10) 3_554 2
O3 O2 O4 104.0(8) 2_566 2
O6 O2 O4 135.0(11) 4_645 2
O4 O2 O4 98.3(9) 4 2
O2 O2 O4 125.3(7) 1_655 2
O2 O2 O4 54.7(7) 1_455 2
O7 O2 O4 125.2(13) 2_666 2
Ga4 O2 O4 50.4(7) 3_544 2
O4 O2 O4 133.4(11) 1_565 2
Ga3 O2 La1 102.5(12) 1_655 4_645
Ga2 O2 La1 10.7(8) . 4_645
La2 O2 La1 106.4(14) . 4_645
O6 O2 La1 123.0(14) . 4_645
La1 O2 La1 105.6(13) . 4_645
O3 O2 La1 50.5(11) 3_554 4_645
O5 O2 La1 139.5(14) 1_554 4_645
O1 O2 La1 99.5(16) 4 4_645
O5 O2 La1 78.5(13) 2_656 4_645
O4 O2 La1 38.0(10) . 4_645
O2 O2 La1 86.0(11) 2_655 4_645
O1 O2 La1 19.3(10) 4_655 4_645
O5 O2 La1 151.4(16) 2_556 4_645
Ta O2 La1 155.7(12) 1_565 4_645
Ga1 O2 La1 155.7(12) 1_565 4_645
O1 O2 La1 116.2(11) 3_554 4_645
O2 O2 La1 147.3(6) 2 4_645
Ga2 O2 La1 95.5(8) 2_655 4_645
Ga4 O2 La1 106.3(8) 4_655 4_645
O7 O2 La1 74.0(11) 1_554 4_645
La2 O2 La1 49.3(4) 1_655 4_645
La1 O2 La1 49.3(4) 1_655 4_645
La1 O2 La1 62.7(6) 4_545 4_645
Ga4 O2 La1 47.3(5) . 4_645
Ga3 O2 La1 154.0(11) . 4_645
Ga4 O2 La1 43.0(4) 4_645 4_645
O7 O2 La1 46.2(9) 2_656 4_645
O3 O2 La1 82.4(9) 2_666 4_645
O4 O2 La1 55.6(10) 4_655 4_645
Ga2 O2 La1 111.6(10) 1_455 4_645
O6 O2 La1 104.7(7) 2_655 4_645
O7 O2 La1 94.1(11) 2_556 4_645
O1 O2 La1 93.9(9) 1_565 4_645
La1 O2 La1 143.5(10) 2 4_645
O6 O2 La1 168.9(10) 2 4_645
Ga2 O2 La1 77.9(7) 4_655 4_645
O4 O2 La1 80.9(9) 2_655 4_645
Ga1 O2 La1 86.6(5) 1_665 4_645
Ta O2 La1 86.6(5) 1_665 4_645
O7 O2 La1 134.1(10) 1_564 4_645
Ga4 O2 La1 124.4(7) 3_554 4_645
O3 O2 La1 126.0(12) 2_566 4_645
O6 O2 La1 26.3(4) 4_645 4_645
O4 O2 La1 105.7(11) 4 4_645
O2 O2 La1 47.3(4) 1_655 4_645
O2 O2 La1 132.7(4) 1_455 4_645
O7 O2 La1 104.1(10) 2_666 4_645
Ga4 O2 La1 72.6(6) 3_544 4_645
O4 O2 La1 109.6(10) 1_565 4_645
O4 O2 La1 116.9(10) 2 4_645
Ga3 O2 Ga2 95.1(16) 1_655 2
Ga2 O2 Ga2 129.9(19) . 2
La2 O2 Ga2 29.0(6) . 2
O6 O2 Ga2 101.8(12) . 2
La1 O2 Ga2 98.6(9) . 2
O3 O2 Ga2 127.2(14) 3_554 2
O5 O2 Ga2 63.6(13) 1_554 2
O1 O2 Ga2 65.2(14) 4 2
O5 O2 Ga2 132.4(18) 2_656 2
O4 O2 Ga2 100.7(14) . 2
O2 O2 Ga2 88.7(17) 2_655 2
O1 O2 Ga2 142.5(16) 4_655 2
O5 O2 Ga2 58.8(11) 2_556 2
Ta O2 Ga2 68.7(7) 1_565 2
Ga1 O2 Ga2 68.7(7) 1_565 2
O1 O2 Ga2 36.6(5) 3_554 2
O2 O2 Ga2 12.3(6) 2 2
Ga2 O2 Ga2 63.7(7) 2_655 2
Ga4 O2 Ga2 117.4(11) 4_655 2
O7 O2 Ga2 61.6(10) 1_554 2
La2 O2 Ga2 110.2(10) 1_655 2
La1 O2 Ga2 164.0(11) 1_655 2
La1 O2 Ga2 91.9(7) 4_545 2
Ga4 O2 Ga2 144.2(9) . 2
Ga3 O2 Ga2 35.7(4) . 2
Ga4 O2 Ga2 92.0(8) 4_645 2
O7 O2 Ga2 93.6(12) 2_656 2
O3 O2 Ga2 142.3(13) 2_666 2
O4 O2 Ga2 160.5(12) 4_655 2
Ga2 O2 Ga2 55.8(5) 1_455 2
O6 O2 Ga2 96.2(9) 2_655 2
O7 O2 Ga2 44.3(9) 2_556 2
O1 O2 Ga2 122.2(8) 1_565 2
La1 O2 Ga2 38.9(4) 2 2
O6 O2 Ga2 48.6(5) 2 2
Ga2 O2 Ga2 143.5(9) 4_655 2
O4 O2 Ga2 68.1(8) 2_655 2
Ga1 O2 Ga2 120.0(10) 1_665 2
Ta O2 Ga2 120.0(10) 1_665 2
O7 O2 Ga2 87.3(10) 1_564 2
Ga4 O2 Ga2 86.5(8) 3_554 2
O3 O2 Ga2 87.9(7) 2_566 2
O6 O2 Ga2 149.5(11) 4_645 2
O4 O2 Ga2 89.1(9) 4 2
O2 O2 Ga2 136.1(4) 1_655 2
O2 O2 Ga2 43.9(4) 1_455 2
O7 O2 Ga2 113.2(12) 2_666 2
Ga4 O2 Ga2 67.4(6) 3_544 2
O4 O2 Ga2 115.3(10) 1_565 2
O4 O2 Ga2 18.3(6) 2 2
La1 O2 Ga2 135.0(10) 4_645 2
Ga3 O2 Ga1 119.1(18) 1_655 .
Ga2 O2 Ga1 72.4(15) . .
La2 O2 Ga1 28.7(7) . .
O6 O2 Ga1 156.2(12) . .
La1 O2 Ga1 115.2(12) . .
O3 O2 Ga1 89.4(13) 3_554 .
O5 O2 Ga1 111.4(18) 1_554 .
O1 O2 Ga1 61.1(14) 4 .
O5 O2 Ga1 139.7(15) 2_656 .
O4 O2 Ga1 44.4(12) . .
O2 O2 Ga1 90.3(8) 2_655 .
O1 O2 Ga1 90.3(13) 4_655 .
O5 O2 Ga1 106.0(13) 2_556 .
Ta O2 Ga1 126.3(10) 1_565 .
Ga1 O2 Ga1 126.3(10) 1_565 .
O1 O2 Ga1 59.2(10) 3_554 .
O2 O2 Ga1 69.8(5) 2 .
Ga2 O2 Ga1 66.7(7) 2_655 .
Ga4 O2 Ga1 172.3(12) 4_655 .
O7 O2 Ga1 15.8(7) 1_554 .
La2 O2 Ga1 77.8(8) 1_655 .
La1 O2 Ga1 125.5(10) 1_655 .
La1 O2 Ga1 53.9(5) 4_545 .
Ga4 O2 Ga1 104.1(10) . .
Ga3 O2 Ga1 84.6(7) . .
Ga4 O2 Ga1 35.1(4) 4_645 .
O7 O2 Ga1 46.6(9) 2_656 .
O3 O2 Ga1 160.0(13) 2_666 .
O4 O2 Ga1 126.1(14) 4_655 .
Ga2 O2 Ga1 64.4(6) 1_455 .
O6 O2 Ga1 123.5(10) 2_655 .
O7 O2 Ga1 20.4(7) 2_556 .
O1 O2 Ga1 138.2(11) 1_565 .
La1 O2 Ga1 86.8(8) 2 .
O6 O2 Ga1 106.0(9) 2 .
Ga2 O2 Ga1 145.1(11) 4_655 .
O4 O2 Ga1 52.0(7) 2_655 .
Ga1 O2 Ga1 134.9(9) 1_665 .
Ta O2 Ga1 134.9(9) 1_665 .
O7 O2 Ga1 143.1(12) 1_564 .
Ga4 O2 Ga1 131.6(10) 3_554 .
O3 O2 Ga1 125.1(6) 2_566 .
O6 O2 Ga1 94.9(9) 4_645 .
O4 O2 Ga1 100.9(9) 4 .
O2 O2 Ga1 105.2(4) 1_655 .
O2 O2 Ga1 74.8(4) 1_455 .
O7 O2 Ga1 153.2(13) 2_666 .
Ga4 O2 Ga1 34.0(3) 3_544 .
O4 O2 Ga1 169.8(9) 1_565 .
O4 O2 Ga1 40.4(6) 2 .
La1 O2 Ga1 77.7(7) 4_645 .
Ga2 O2 Ga1 57.6(5) 2 .
Ga3 O2 Ta 119.1(18) 1_655 .
Ga2 O2 Ta 72.4(15) . .
La2 O2 Ta 28.7(7) . .
O6 O2 Ta 156.2(12) . .
La1 O2 Ta 115.2(12) . .
O3 O2 Ta 89.4(13) 3_554 .
O5 O2 Ta 111.4(18) 1_554 .
O1 O2 Ta 61.1(14) 4 .
O5 O2 Ta 139.7(15) 2_656 .
O4 O2 Ta 44.4(12) . .
O2 O2 Ta 90.3(8) 2_655 .
O1 O2 Ta 90.3(13) 4_655 .
O5 O2 Ta 106.0(13) 2_556 .
Ta O2 Ta 126.3(10) 1_565 .
Ga1 O2 Ta 126.3(10) 1_565 .
O1 O2 Ta 59.2(10) 3_554 .
O2 O2 Ta 69.8(5) 2 .
Ga2 O2 Ta 66.7(7) 2_655 .
Ga4 O2 Ta 172.3(12) 4_655 .
O7 O2 Ta 15.8(7) 1_554 .
La2 O2 Ta 77.8(8) 1_655 .
La1 O2 Ta 125.5(10) 1_655 .
La1 O2 Ta 53.9(5) 4_545 .
Ga4 O2 Ta 104.1(10) . .
Ga3 O2 Ta 84.6(7) . .
Ga4 O2 Ta 35.1(4) 4_645 .
O7 O2 Ta 46.6(9) 2_656 .
O3 O2 Ta 160.0(13) 2_666 .
O4 O2 Ta 126.1(14) 4_655 .
Ga2 O2 Ta 64.4(6) 1_455 .
O6 O2 Ta 123.5(10) 2_655 .
O7 O2 Ta 20.4(7) 2_556 .
O1 O2 Ta 138.2(11) 1_565 .
La1 O2 Ta 86.8(8) 2 .
O6 O2 Ta 106.0(9) 2 .
Ga2 O2 Ta 145.1(11) 4_655 .
O4 O2 Ta 52.0(7) 2_655 .
Ga1 O2 Ta 134.9(9) 1_665 .
Ta O2 Ta 134.9(9) 1_665 .
O7 O2 Ta 143.1(12) 1_564 .
Ga4 O2 Ta 131.6(10) 3_554 .
O3 O2 Ta 125.1(6) 2_566 .
O6 O2 Ta 94.9(9) 4_645 .
O4 O2 Ta 100.9(9) 4 .
O2 O2 Ta 105.2(4) 1_655 .
O2 O2 Ta 74.8(4) 1_455 .
O7 O2 Ta 153.2(13) 2_666 .
Ga4 O2 Ta 34.0(3) 3_544 .
O4 O2 Ta 169.8(9) 1_565 .
O4 O2 Ta 40.4(6) 2 .
La1 O2 Ta 77.7(7) 4_645 .
Ga2 O2 Ta 57.6(5) 2 .
Ga1 O2 Ta 0.00(5) . .
Ga3 O2 Ga4 95.2(15) 1_655 4
Ga2 O2 Ga4 139.9(19) . 4
La2 O2 Ga4 94.5(10) . 4
O6 O2 Ga4 37.7(7) . 4
La1 O2 Ga4 40.7(7) . 4
O3 O2 Ga4 97.2(11) 3_554 4
O5 O2 Ga4 66.4(12) 1_554 4
O1 O2 Ga4 68.6(12) 4 4
O5 O2 Ga4 99.2(15) 2_656 4
O4 O2 Ga4 134.8(14) . 4
O2 O2 Ga4 121.5(12) 2_655 4
O1 O2 Ga4 146.5(17) 4_655 4
O5 O2 Ga4 13.0(10) 2_556 4
Ta O2 Ga4 31.1(4) 1_565 4
Ga1 O2 Ga4 31.1(4) 1_565 4
O1 O2 Ga4 97.8(10) 3_554 4
O2 O2 Ga4 59.9(6) 2 4
Ga2 O2 Ga4 118.6(11) 2_655 4
Ga4 O2 Ga4 61.7(6) 4_655 4
O7 O2 Ga4 129.7(11) 1_554 4
La2 O2 Ga4 156.6(11) 1_655 4
La1 O2 Ga4 113.4(10) 1_655 4
La1 O2 Ga4 100.8(7) 4_545 4
Ga4 O2 Ga4 98.2(8) . 4
Ga3 O2 Ga4 36.3(4) . 4
Ga4 O2 Ga4 147.7(9) 4_645 4
O7 O2 Ga4 164.1(13) 2_656 4
O3 O2 Ga4 77.6(6) 2_666 4
O4 O2 Ga4 93.2(12) 4_655 4
Ga2 O2 Ga4 59.7(5) 1_455 4
O6 O2 Ga4 91.2(9) 2_655 4
O7 O2 Ga4 98.3(9) 2_556 4
O1 O2 Ga4 53.1(6) 1_565 4
La1 O2 Ga4 70.6(6) 2 4
O6 O2 Ga4 41.8(5) 2 4
Ga2 O2 Ga4 72.6(6) 4_655 4
O4 O2 Ga4 133.5(11) 2_655 4
Ga1 O2 Ga4 98.0(8) 1_665 4
Ta O2 Ga4 98.0(8) 1_665 4
O7 O2 Ga4 49.0(8) 1_564 4
Ga4 O2 Ga4 69.5(6) 3_554 4
O3 O2 Ga4 19.5(5) 2_566 4
O6 O2 Ga4 119.3(10) 4_645 4
O4 O2 Ga4 44.3(8) 4 4
O2 O2 Ga4 135.7(4) 1_655 4
O2 O2 Ga4 44.3(4) 1_455 4
O7 O2 Ga4 75.1(9) 2_666 4
Ga4 O2 Ga4 138.4(9) 3_544 4
O4 O2 Ga4 51.4(6) 1_565 4
O4 O2 Ga4 88.5(8) 2 4
La1 O2 Ga4 145.5(10) 4_645 4
Ga2 O2 Ga4 71.0(5) 2 4
Ga1 O2 Ga4 118.6(6) . 4
Ta O2 Ga4 118.6(6) . 4
Ga3 O2 La1 19.3(10) 1_655 2_655
Ga2 O2 La1 103.1(13) . 2_655
La2 O2 La1 97.4(12) . 2_655
O6 O2 La1 90.3(12) . 2_655
La1 O2 La1 142.0(15) . 2_655
O3 O2 La1 139.4(14) 3_554 2_655
O5 O2 La1 46.9(11) 1_554 2_655
O1 O2 La1 154.5(19) 4 2_655
O5 O2 La1 48.8(13) 2_656 2_655
O4 O2 La1 113.1(14) . 2_655
O2 O2 La1 11.6(5) 2_655 2_655
O1 O2 La1 76.2(11) 4_655 2_655
O5 O2 La1 113.4(15) 2_556 2_655
Ta O2 La1 80.2(8) 1_565 2_655
Ga1 O2 La1 80.2(8) 1_565 2_655
O1 O2 La1 56.7(7) 3_554 2_655
O2 O2 La1 89.8(15) 2 2_655
Ga2 O2 La1 35.7(4) 2_655 2_655
Ga4 O2 La1 72.7(6) 4_655 2_655
O7 O2 La1 85.6(10) 1_554 2_655
La2 O2 La1 46.3(4) 1_655 2_655
La1 O2 La1 73.8(5) 1_655 2_655
La1 O2 La1 146.6(10) 4_545 2_655
Ga4 O2 La1 124.9(7) . 2_655
Ga3 O2 La1 109.1(10) . 2_655
Ga4 O2 La1 95.6(7) 4_645 2_655
O7 O2 La1 71.5(9) 2_656 2_655
O3 O2 La1 82.1(9) 2_666 2_655
O4 O2 La1 106.5(11) 4_655 2_655
Ga2 O2 La1 146.0(11) 1_455 2_655
O6 O2 La1 24.1(4) 2_655 2_655
O7 O2 La1 112.3(12) 2_556 2_655
O1 O2 La1 120.7(10) 1_565 2_655
La1 O2 La1 57.3(5) 2 2_655
O6 O2 La1 75.9(7) 2 2_655
Ga2 O2 La1 105.2(7) 4_655 2_655
O4 O2 La1 48.9(7) 2_655 2_655
Ga1 O2 La1 37.6(3) 1_665 2_655
Ta O2 La1 37.6(3) 1_665 2_655
O7 O2 La1 65.3(8) 1_564 2_655
Ga4 O2 La1 43.2(4) 3_554 2_655
O3 O2 La1 122.5(12) 2_566 2_655
O6 O2 La1 109.5(7) 4_645 2_655
O4 O2 La1 153.8(12) 4 2_655
O2 O2 La1 50.7(4) 1_655 2_655
O2 O2 La1 129.3(4) 1_455 2_655
O7 O2 La1 52.6(8) 2_666 2_655
Ga4 O2 La1 67.8(5) 3_544 2_655
O4 O2 La1 86.1(9) 1_565 2_655
O4 O2 La1 88.9(9) 2 2_655
La1 O2 La1 93.1(5) 4_645 2_655
Ga2 O2 La1 90.2(8) 2 2_655
Ga1 O2 La1 100.8(8) . 2_655
Ta O2 La1 100.8(8) . 2_655
Ga4 O2 La1 111.3(9) 4 2_655
Ga3 O2 O1 42.2(12) 1_655 3_654
Ga2 O2 O1 81.1(13) . 3_654
La2 O2 O1 91.4(12) . 3_654
O6 O2 O1 112.0(13) . 3_654
La1 O2 O1 159.9(14) . 3_654
O3 O2 O1 122.2(15) 3_554 3_654
O5 O2 O1 69.9(14) 1_554 3_654
O1 O2 O1 145(2) 4 3_654
O5 O2 O1 57.7(13) 2_656 3_654
O4 O2 O1 88.7(13) . 3_654
O2 O2 O1 14.3(10) 2_655 3_654
O1 O2 O1 58.3(15) 4_655 3_654
O5 O2 O1 136.0(16) 2_556 3_654
Ta O2 O1 104.5(11) 1_565 3_654
Ga1 O2 O1 104.5(11) 1_565 3_654
O1 O2 O1 59.7(8) 3_554 3_654
O2 O2 O1 100.7(16) 2 3_654
Ga2 O2 O1 32.7(5) 2_655 3_654
Ga4 O2 O1 90.8(9) 4_655 3_654
O7 O2 O1 68.3(9) 1_554 3_654
La2 O2 O1 23.1(6) 1_655 3_654
La1 O2 O1 69.6(7) 1_655 3_654
La1 O2 O1 122.5(10) 4_545 3_654
Ga4 O2 O1 113.2(8) . 3_654
Ga3 O2 O1 125.3(11) . 3_654
Ga4 O2 O1 71.8(7) 4_645 3_654
O7 O2 O1 47.6(10) 2_656 3_654
O3 O2 O1 91.7(8) 2_666 3_654
O4 O2 O1 103.1(11) 4_655 3_654
Ga2 O2 O1 145.6(11) 1_455 3_654
O6 O2 O1 46.8(7) 2_655 3_654
O7 O2 O1 100.8(12) 2_556 3_654
O1 O2 O1 132.6(11) 1_565 3_654
La1 O2 O1 73.6(8) 2 3_654
O6 O2 O1 97.6(10) 2 3_654
Ga2 O2 O1 111.5(8) 4_655 3_654
O4 O2 O1 34.9(8) 2_655 3_654
Ga1 O2 O1 50.7(6) 1_665 3_654
Ta O2 O1 50.7(6) 1_665 3_654
O7 O2 O1 89.2(11) 1_564 3_654
Ga4 O2 O1 67.4(7) 3_554 3_654
O3 O2 O1 146.1(12) 2_566 3_654
O6 O2 O1 93.5(8) 4_645 3_654
O4 O2 O1 174.0(12) 4 3_654
O2 O2 O1 39.7(6) 1_655 3_654
O2 O2 O1 140.3(6) 1_455 3_654
O7 O2 O1 71.5(10) 2_666 3_654
Ga4 O2 O1 50.3(6) 3_544 3_654
O4 O2 O1 104.6(11) 1_565 3_654
O4 O2 O1 87.6(9) 2 3_654
La1 O2 O1 72.1(6) 4_645 3_654
Ga2 O2 O1 96.3(8) 2 3_654
Ga1 O2 O1 84.2(8) . 3_654
Ta O2 O1 84.2(8) . 3_654
Ga4 O2 O1 135.6(10) 4 3_654
La1 O2 O1 24.4(6) 2_655 3_654
Ga3 O2 O4 151.9(19) 1_655 1_455
Ga2 O2 O4 89.1(15) . 1_455
La2 O2 O4 45.8(9) . 1_455
O6 O2 O4 110.7(12) . 1_455
La1 O2 O4 66.6(10) . 1_455
O3 O2 O4 70.3(13) 3_554 1_455
O5 O2 O4 116.7(14) 1_554 1_455
O1 O2 O4 12.4(14) 4 1_455
O5 O2 O4 168(2) 2_656 1_455
O4 O2 O4 63.9(11) . 1_455
O2 O2 O4 136.0(15) 2_655 1_455
O1 O2 O4 118.7(15) 4_655 1_455
O5 O2 O4 66.0(13) 2_556 1_455
Ta O2 O4 99.8(9) 1_565 1_455
Ga1 O2 O4 99.8(9) 1_565 1_455
O1 O2 O4 86.8(11) 3_554 1_455
O2 O2 O4 61.7(10) 2 1_455
Ga2 O2 O4 108.2(11) 2_655 1_455
Ga4 O2 O4 134.4(11) 4_655 1_455
O7 O2 O4 65.3(10) 1_554 1_455
La2 O2 O4 125.4(11) 1_655 1_455
La1 O2 O4 138.6(13) 1_655 1_455
La1 O2 O4 38.1(7) 4_545 1_455
Ga4 O2 O4 87.6(10) . 1_455
Ga3 O2 O4 54.6(8) . 1_455
Ga4 O2 O4 72.0(8) 4_645 1_455
O7 O2 O4 92.8(13) 2_656 1_455
O3 O2 O4 133.6(12) 2_666 1_455
O4 O2 O4 109.1(12) 4_655 1_455
Ga2 O2 O4 16.1(6) 1_455 1_455
O6 O2 O4 152.5(12) 2_655 1_455
O7 O2 O4 32.8(9) 2_556 1_455
O1 O2 O4 93.0(10) 1_565 1_455
La1 O2 O4 95.0(10) 2 1_455
O6 O2 O4 90.8(9) 2 1_455
Ga2 O2 O4 111.2(11) 4_655 1_455
O4 O2 O4 99.1(12) 2_655 1_455
Ga1 O2 O4 173.6(11) 1_665 1_455
Ta O2 O4 173.6(11) 1_665 1_455
O7 O2 O4 122.5(12) 1_564 1_455
Ga4 O2 O4 136.1(10) 3_554 1_455
O3 O2 O4 76.3(8) 2_566 1_455
O6 O2 O4 96.1(10) 4_645 1_455
O4 O2 O4 52.2(8) 4 1_455
O2 O2 O4 145.5(7) 1_655 1_455
O2 O2 O4 34.5(7) 1_455 1_455
O7 O2 O4 150.8(11) 2_666 1_455
Ga4 O2 O4 83.1(9) 3_544 1_455
O4 O2 O4 121.0(12) 1_565 1_455
O4 O2 O4 54.5(12) 2 1_455
La1 O2 O4 99.4(10) 4_645 1_455
Ga2 O2 O4 56.8(8) 2 1_455
Ga1 O2 O4 49.6(7) . 1_455
Ta O2 O4 49.6(7) . 1_455
Ga4 O2 O4 75.7(7) 4 1_455
La1 O2 O4 143.2(11) 2_655 1_455
O1 O2 O4 133.3(11) 3_654 1_455
Ga3 O2 O4 82.7(12) 1_655 1_655
Ga2 O2 O4 31.1(10) . 1_655
La2 O2 O4 107.5(13) . 1_655
O6 O2 O4 122.2(12) . 1_655
La1 O2 O4 123.1(15) . 1_655
O3 O2 O4 70.7(14) 3_554 1_655
O5 O2 O4 118.8(14) 1_554 1_655
O1 O2 O4 118.4(17) 4 1_655
O5 O2 O4 65.5(13) 2_656 1_655
O4 O2 O4 51.8(8) . 1_655
O2 O2 O4 65.2(12) 2_655 1_655
O1 O2 O4 10.8(12) 4_655 1_655
O5 O2 O4 169.1(17) 2_556 1_655
Ta O2 O4 144.5(11) 1_565 1_655
Ga1 O2 O4 144.5(11) 1_565 1_655
O1 O2 O4 102.3(11) 3_554 1_655
O2 O2 O4 142.5(13) 2 1_655
Ga2 O2 O4 78.0(8) 2_655 1_655
Ga4 O2 O4 100.1(8) 4_655 1_655
O7 O2 O4 72.2(11) 1_554 1_655
La2 O2 O4 29.2(7) 1_655 1_655
La1 O2 O4 44.7(6) 1_655 1_655
La1 O2 O4 81.8(9) 4_545 1_655
Ga4 O2 O4 64.3(8) . 1_655
Ga3 O2 O4 165.9(12) . 1_655
Ga4 O2 O4 47.7(6) 4_645 1_655
O7 O2 O4 38.5(9) 2_656 1_655
O3 O2 O4 80.8(8) 2_666 1_655
O4 O2 O4 64.8(11) 4_655 1_655
Ga2 O2 O4 130.0(12) 1_455 1_655
O6 O2 O4 85.4(8) 2_655 1_655
O7 O2 O4 101.0(11) 2_556 1_655
O1 O2 O4 105.1(10) 1_565 1_655
La1 O2 O4 124.6(10) 2 1_655
O6 O2 O4 148.1(11) 2 1_655
Ga2 O2 O4 84.8(8) 4_655 1_655
O4 O2 O4 66.6(12) 2_655 1_655
Ga1 O2 O4 70.6(7) 1_665 1_655
Ta O2 O4 70.6(7) 1_665 1_655
O7 O2 O4 121.5(10) 1_564 1_655
Ga4 O2 O4 106.5(8) 3_554 1_655
O3 O2 O4 139.6(11) 2_566 1_655
O6 O2 O4 43.1(8) 4_645 1_655
O4 O2 O4 125.7(11) 4 1_655
O2 O2 O4 29.7(7) 1_655 1_655
O2 O2 O4 150.3(7) 1_455 1_655
O7 O2 O4 91.5(10) 2_666 1_655
Ga4 O2 O4 64.4(7) 3_544 1_655
O4 O2 O4 108.1(10) 1_565 1_655
O4 O2 O4 114.3(12) 2 1_655
La1 O2 O4 21.0(6) 4_645 1_655
Ga2 O2 O4 131.7(10) 2 1_655
Ga1 O2 O4 81.4(8) . 1_655
Ta O2 O4 81.4(8) . 1_655
Ga4 O2 O4 157.2(10) 4 1_655
La1 O2 O4 72.2(7) 2_655 1_655
O1 O2 O4 51.5(8) 3_654 1_655
O4 O2 O4 115.7(13) 1_455 1_655
Ga3 O2 La1 89.0(16) 1_655 4
Ga2 O2 La1 113.0(18) . 4
La2 O2 La1 130.4(11) . 4
O6 O2 La1 19.2(7) . 4
La1 O2 La1 33.9(7) . 4
O3 O2 La1 77.7(8) 3_554 4
O5 O2 La1 80.4(16) 1_554 4
O1 O2 La1 86.9(14) 4 4
O5 O2 La1 72.2(14) 2_656 4
O4 O2 La1 129.0(17) . 4
O2 O2 La1 119.7(4) 2_655 4
O1 O2 La1 109.7(15) 4_655 4
O5 O2 La1 49.6(11) 2_556 4
Ta O2 La1 48.8(6) 1_565 4
Ga1 O2 La1 48.8(6) 1_565 4
O1 O2 La1 128.3(12) 3_554 4
O2 O2 La1 96.2(6) 2 4
Ga2 O2 La1 136.7(12) 2_655 4
Ga4 O2 La1 36.9(4) 4_655 4
O7 O2 La1 163.2(10) 1_554 4
La2 O2 La1 133.1(9) 1_655 4
La1 O2 La1 77.1(7) 1_655 4
La1 O2 La1 102.7(8) 4_545 4
Ga4 O2 La1 70.3(7) . 4
Ga3 O2 La1 73.1(6) . 4
Ga4 O2 La1 148.5(11) 4_645 4
O7 O2 La1 158.7(13) 2_656 4
O3 O2 La1 42.6(4) 2_666 4
O4 O2 La1 58.0(10) 4_655 4
Ga2 O2 La1 83.6(7) 1_455 4
O6 O2 La1 84.2(8) 2_655 4
O7 O2 La1 128.9(10) 2_556 4
O1 O2 La1 21.7(7) 1_565 4
La1 O2 La1 97.1(8) 2 4
O6 O2 La1 69.0(7) 2 4
Ga2 O2 La1 36.2(4) 4_655 4
O4 O2 La1 155.2(12) 2_655 4
Ga1 O2 La1 77.2(7) 1_665 4
Ta O2 La1 77.2(7) 1_665 4
O7 O2 La1 48.0(8) 1_564 4
Ga4 O2 La1 68.6(6) 3_554 4
O3 O2 La1 23.8(3) 2_566 4
O6 O2 La1 88.4(8) 4_645 4
O4 O2 La1 47.6(8) 4 4
O2 O2 La1 103.9(3) 1_655 4
O2 O2 La1 76.1(3) 1_455 4
O7 O2 La1 56.5(8) 2_666 4
Ga4 O2 La1 173.3(10) 3_544 4
O4 O2 La1 23.1(6) 1_565 4
O4 O2 La1 125.3(9) 2 4
La1 O2 La1 113.5(8) 4_645 4
Ga2 O2 La1 107.8(7) 2 4
Ga1 O2 La1 147.8(7) . 4
Ta O2 La1 147.8(7) . 4
Ga4 O2 La1 36.9(3) 4 4
La1 O2 La1 108.3(8) 2_655 4
O1 O2 La1 127.7(9) 3_654 4
O4 O2 La1 98.2(8) 1_455 4
O4 O2 La1 120.4(9) 1_655 4
Ga3 O2 La1 80.3(15) 1_655 3_544
Ga2 O2 La1 109.7(18) . 3_544
La2 O2 La1 30.4(7) . 3_544
O6 O2 La1 123.8(14) . 3_544
La1 O2 La1 131.8(11) . 3_544
O3 O2 La1 135.2(14) 3_554 3_544
O5 O2 La1 65.7(16) 1_554 3_544
O1 O2 La1 87.7(16) 4 3_544
O5 O2 La1 116.0(16) 2_656 3_544
O4 O2 La1 87.5(15) . 3_544
O2 O2 La1 61.3(13) 2_655 3_544
O1 O2 La1 110.4(14) 4_655 3_544
O5 O2 La1 91.2(13) 2_556 3_544
Ta O2 La1 89.4(9) 1_565 3_544
Ga1 O2 La1 89.4(9) 1_565 3_544
O1 O2 La1 13.5(8) 3_554 3_544
O2 O2 La1 42.9(9) 2 3_544
Ga2 O2 La1 33.4(4) 2_655 3_544
Ga4 O2 La1 126.5(11) 4_655 3_544
O7 O2 La1 39.6(9) 1_554 3_544
La2 O2 La1 76.6(7) 1_655 3_544
La1 O2 La1 134.4(9) 1_655 3_544
La1 O2 La1 98.0(8) 4_545 3_544
Ga4 O2 La1 149.5(11) . 3_544
Ga3 O2 La1 69.0(6) . 3_544
Ga4 O2 La1 71.2(7) 4_645 3_544
O7 O2 La1 63.7(10) 2_656 3_544
O3 O2 La1 147.2(13) 2_666 3_544
O4 O2 La1 164.5(13) 4_655 3_544
Ga2 O2 La1 82.3(7) 1_455 3_544
O6 O2 La1 83.5(8) 2_655 3_544
O7 O2 La1 47.2(9) 2_556 3_544
O1 O2 La1 155.2(9) 1_565 3_544
La1 O2 La1 42.6(4) 2 3_544
O6 O2 La1 68.3(7) 2 3_544
Ga2 O2 La1 169.1(11) 4_655 3_544
O4 O2 La1 34.5(6) 2_655 3_544
Ga1 O2 La1 104.2(8) 1_665 3_544
Ta O2 La1 104.2(8) 1_665 3_544
O7 O2 La1 98.8(11) 1_564 3_544
Ga4 O2 La1 86.0(7) 3_554 3_544
O3 O2 La1 120.7(9) 2_566 3_544
O6 O2 La1 134.5(10) 4_645 3_544
O4 O2 La1 120.7(9) 4 3_544
O2 O2 La1 103.8(3) 1_655 3_544
O2 O2 La1 76.2(3) 1_455 3_544
O7 O2 La1 111.2(11) 2_666 3_544
Ga4 O2 La1 37.0(3) 3_544 3_544
O4 O2 La1 133.1(12) 1_565 3_544
O4 O2 La1 22.7(6) 2 3_544
La1 O2 La1 109.6(8) 4_645 3_544
Ga2 O2 La1 33.6(3) 2 3_544
Ga1 O2 La1 45.9(4) . 3_544
Ta O2 La1 45.9(4) . 3_544
Ga4 O2 La1 102.3(7) 4 3_544
La1 O2 La1 67.2(5) 2_655 3_544
O1 O2 La1 65.1(6) 3_654 3_544
O4 O2 La1 76.0(8) 1_455 3_544
O4 O2 La1 99.7(8) 1_655 3_544
La1 O2 La1 136.8(8) 4 3_544
Ga3 O2 O4 39.0(13) 1_655 3_554
Ga2 O2 O4 130.6(17) . 3_554
La2 O2 O4 72.4(12) . 3_554
O6 O2 O4 88.1(13) . 3_554
La1 O2 O4 129.7(14) . 3_554
O3 O2 O4 173.3(15) 3_554 3_554
O5 O2 O4 26.4(15) 1_554 3_554
O1 O2 O4 122.0(18) 4 3_554
O5 O2 O4 77.0(16) 2_656 3_554
O4 O2 O4 124.3(18) . 3_554
O2 O2 O4 38.0(13) 2_655 3_554
O1 O2 O4 109.1(15) 4_655 3_554
O5 O2 O4 85.7(14) 2_556 3_554
Ta O2 O4 61.3(9) 1_565 3_554
Ga1 O2 O4 61.3(9) 1_565 3_554
O1 O2 O4 30.8(10) 3_554 3_554
O2 O2 O4 55.1(13) 2 3_554
Ga2 O2 O4 31.2(7) 2_655 3_554
Ga4 O2 O4 83.0(10) 4_655 3_554
O7 O2 O4 79.1(11) 1_554 3_554
La2 O2 O4 73.6(8) 1_655 3_554
La1 O2 O4 107.2(9) 1_655 3_554
La1 O2 O4 142.2(12) 4_545 3_554
Ga4 O2 O4 158.9(10) . 3_554
Ga3 O2 O4 75.4(8) . 3_554
Ga4 O2 O4 104.6(10) 4_645 3_554
O7 O2 O4 85.3(12) 2_656 3_554
O3 O2 O4 103.3(13) 2_666 3_554
O4 O2 O4 136.6(14) 4_655 3_554
Ga2 O2 O4 111.7(10) 1_455 3_554
O6 O2 O4 41.1(7) 2_655 3_554
O7 O2 O4 90.5(12) 2_556 3_554
O1 O2 O4 127.5(13) 1_565 3_554
La1 O2 O4 22.9(5) 2 3_554
O6 O2 O4 47.7(8) 2 3_554
Ga2 O2 O4 125.2(11) 4_655 3_554
O4 O2 O4 49.7(6) 2_655 3_554
Ga1 O2 O4 64.4(8) 1_665 3_554
Ta O2 O4 64.4(8) 1_665 3_554
O7 O2 O4 59.3(10) 1_564 3_554
Ga4 O2 O4 42.3(7) 3_554 3_554
O3 O2 O4 107.1(12) 2_566 3_554
O6 O2 O4 143.8(9) 4_645 3_554
O4 O2 O4 131.5(11) 4 3_554
O2 O2 O4 85.3(6) 1_655 3_554
O2 O2 O4 94.7(6) 1_455 3_554
O7 O2 O4 67.0(10) 2_666 3_554
Ga4 O2 O4 66.9(8) 3_544 3_554
O4 O2 O4 92.3(12) 1_565 3_554
O4 O2 O4 60.7(8) 2 3_554
La1 O2 O4 122.8(8) 4_645 3_554
Ga2 O2 O4 56.9(7) 2 3_554
Ga1 O2 O4 89.2(9) . 3_554
Ta O2 O4 89.2(9) . 3_554
Ga4 O2 O4 89.2(8) 4 3_554
La1 O2 O4 34.8(6) 2_655 3_554
O1 O2 O4 51.1(8) 3_654 3_554
O4 O2 O4 113.4(12) 1_455 3_554
O4 O2 O4 102.6(10) 1_655 3_554
La1 O2 O4 106.7(9) 4 3_554
La1 O2 O4 44.2(6) 3_544 3_554
Ga3 O2 O1 147.1(16) 1_655 .
Ga2 O2 O1 38.9(10) . .
La2 O2 O1 70.9(12) . .
O6 O2 O1 135.0(14) . .
La1 O2 O1 85.5(12) . .
O3 O2 O1 42.0(10) 3_554 .
O5 O2 O1 158.8(19) 1_554 .
O1 O2 O1 52.0(12) 4 .
O5 O2 O1 126.7(15) 2_656 .
O4 O2 O1 17.3(11) . .
O2 O2 O1 119.0(7) 2_655 .
O1 O2 O1 68.4(12) 4_655 .
O5 O2 O1 112.3(14) 2_556 .
Ta O2 O1 147.7(9) 1_565 .
Ga1 O2 O1 147.7(9) 1_565 .
O1 O2 O1 106.7(14) 3_554 .
O2 O2 O1 106.6(8) 2 .
Ga2 O2 O1 107.4(11) 2_655 .
Ga4 O2 O1 139.9(12) 4_655 .
O7 O2 O1 56.6(11) 1_554 .
La2 O2 O1 85.7(8) 1_655 .
La1 O2 O1 94.2(8) 1_655 .
La1 O2 O1 16.8(4) 4_545 .
Ga4 O2 O1 56.8(7) . .
Ga3 O2 O1 104.9(8) . .
Ga4 O2 O1 35.3(6) 4_645 .
O7 O2 O1 59.0(10) 2_656 .
O3 O2 O1 116.0(13) 2_666 .
O4 O2 O1 79.9(13) 4_655 .
Ga2 O2 O1 63.5(6) 1_455 .
O6 O2 O1 150.9(9) 2_655 .
O7 O2 O1 53.3(10) 2_556 .
O1 O2 O1 96.3(12) 1_565 .
La1 O2 O1 133.2(10) 2 .
O6 O2 O1 140.7(8) 2 .
Ga2 O2 O1 97.5(9) 4_655 .
O4 O2 O1 88.9(10) 2_655 .
Ga1 O2 O1 135.7(8) 1_665 .
Ta O2 O1 135.7(8) 1_665 .
O7 O2 O1 163.6(12) 1_564 .
Ga4 O2 O1 172.8(8) 3_554 .
O3 O2 O1 106.9(11) 2_566 .
O6 O2 O1 52.4(7) 4_645 .
O4 O2 O1 75.7(10) 4 .
O2 O2 O1 95.8(4) 1_655 .
O2 O2 O1 84.2(4) 1_455 .
O7 O2 O1 149.8(12) 2_666 .
Ga4 O2 O1 70.0(8) 3_544 .
O4 O2 O1 132.0(13) 1_565 .
O4 O2 O1 84.0(8) 2 .
La1 O2 O1 49.1(4) 4_645 .
Ga2 O2 O1 97.1(8) 2 .
Ga1 O2 O1 47.6(6) . .
Ta O2 O1 47.6(6) . .
Ga4 O2 O1 117.6(7) 4 .
La1 O2 O1 130.3(8) 2_655 .
O1 O2 O1 105.9(9) 3_654 .
O4 O2 O1 50.3(7) 1_455 .
O4 O2 O1 66.5(7) 1_655 .
La1 O2 O1 115.8(9) 4 .
La1 O2 O1 93.5(8) 3_544 .
O4 O2 O1 135.7(10) 3_554 .
Ga3 O2 O1 73.0(14) 1_655 1_665
Ga2 O2 O1 66.5(14) . 1_665
La2 O2 O1 166.8(15) . 1_665
O6 O2 O1 63.6(10) . 1_665
La1 O2 O1 79.0(10) . 1_665
O3 O2 O1 65.3(10) 3_554 1_665
O5 O2 O1 100.8(16) 1_554 1_665
O1 O2 O1 123.3(16) 4 1_665
O5 O2 O1 35.0(14) 2_656 1_665
O4 O2 O1 95.9(14) . 1_665
O2 O2 O1 86.7(13) 2_655 1_665
O1 O2 O1 49.6(9) 4_655 1_665
O5 O2 O1 110.8(14) 2_556 1_665
Ta O2 O1 95.3(10) 1_565 1_665
Ga1 O2 O1 95.3(10) 1_565 1_665
O1 O2 O1 138.8(12) 3_554 1_665
O2 O2 O1 151.7(6) 2 1_665
Ga2 O2 O1 114.3(8) 2_655 1_665
Ga4 O2 O1 46.1(7) 4_655 1_665
O7 O2 O1 131.9(12) 1_554 1_665
La2 O2 O1 74.9(7) 1_655 1_665
La1 O2 O1 15.9(5) 1_655 1_665
La1 O2 O1 102.6(10) 4_545 1_665
Ga4 O2 O1 47.6(6) . 1_665
Ga3 O2 O1 134.1(10) . 1_665
Ga4 O2 O1 103.4(9) 4_645 1_665
O7 O2 O1 98.0(11) 2_656 1_665
O3 O2 O1 21.9(6) 2_666 1_665
O4 O2 O1 24.8(9) 4_655 1_665
Ga2 O2 O1 129.9(10) 1_455 1_665
O6 O2 O1 71.0(8) 2_655 1_665
O7 O2 O1 152.3(13) 2_556 1_665
O1 O2 O1 52.1(6) 1_565 1_665
La1 O2 O1 126.3(10) 2 1_665
O6 O2 O1 114.9(10) 2 1_665
Ga2 O2 O1 29.5(4) 4_655 1_665
O4 O2 O1 115.8(9) 2_655 1_665
Ga1 O2 O1 47.6(6) 1_665 1_665
Ta O2 O1 47.6(6) 1_665 1_665
O7 O2 O1 76.1(10) 1_564 1_665
Ga4 O2 O1 77.8(8) 3_554 1_665
O3 O2 O1 83.8(6) 2_566 1_665
O6 O2 O1 46.9(7) 4_645 1_665
O4 O2 O1 91.2(10) 4 1_665
O2 O2 O1 45.6(5) 1_655 1_665
O2 O2 O1 134.4(5) 1_455 1_665
O7 O2 O1 50.7(10) 2_666 1_665
Ga4 O2 O1 122.2(7) 3_544 1_665
O4 O2 O1 49.6(8) 1_565 1_665
O4 O2 O1 170.4(10) 2 1_665
La1 O2 O1 60.6(6) 4_645 1_665
Ga2 O2 O1 163.3(11) 2 1_665
Ga1 O2 O1 138.3(9) . 1_665
Ta O2 O1 138.3(9) . 1_665
Ga4 O2 O1 97.9(8) 4 1_665
La1 O2 O1 82.1(7) 2_655 1_665
O1 O2 O1 82.8(5) 3_654 1_665
O4 O2 O1 134.0(12) 1_455 1_665
O4 O2 O1 59.7(8) 1_655 1_665
La1 O2 O1 61.4(6) 4 1_665
La1 O2 O1 147.7(8) 3_544 1_665
O4 O2 O1 112.0(10) 3_554 1_665
O1 O2 O1 99.2(9) . 1_665
Ga3 O2 O4 23.9(11) 1_655 2_665
Ga2 O2 O4 132.5(14) . 2_665
La2 O2 O4 112.4(15) . 2_665
O6 O2 O4 50.2(11) . 2_665
La1 O2 O4 101.2(14) . 2_665
O3 O2 O4 137.8(13) 3_554 2_665
O5 O2 O4 24.8(12) 1_554 2_665
O1 O2 O4 137.3(16) 4 2_665
O5 O2 O4 45.8(14) 2_656 2_665
O4 O2 O4 153.9(11) . 2_665
O2 O2 O4 53.3(7) 2_655 2_665
O1 O2 O4 102.8(12) 4_655 2_665
O5 O2 O4 77.0(14) 2_556 2_665
Ta O2 O4 41.6(7) 1_565 2_665
Ga1 O2 O4 41.6(7) 1_565 2_665
O1 O2 O4 73.4(12) 3_554 2_665
O2 O2 O4 79.9(10) 2 2_665
Ga2 O2 O4 68.3(9) 2_655 2_665
Ga4 O2 O4 40.1(7) 4_655 2_665
O7 O2 O4 120.7(13) 1_554 2_665
La2 O2 O4 85.3(8) 1_655 2_665
La1 O2 O4 79.1(8) 1_655 2_665
La1 O2 O4 171.5(11) 4_545 2_665
Ga4 O2 O4 121.3(10) . 2_665
Ga3 O2 O4 83.9(9) . 2_665
Ga4 O2 O4 137.3(10) 4_645 2_665
O7 O2 O4 113.2(11) 2_656 2_665
O3 O2 O4 61.7(11) 2_666 2_665
O4 O2 O4 97.5(12) 4_655 2_665
Ga2 O2 O4 125.7(10) 1_455 2_665
O6 O2 O4 19.9(6) 2_655 2_665
O7 O2 O4 130.7(13) 2_556 2_665
O1 O2 O4 87.1(11) 1_565 2_665
La1 O2 O4 50.4(7) 2 2_665
O6 O2 O4 47.6(7) 2 2_665
Ga2 O2 O4 82.3(9) 4_655 2_665
O4 O2 O4 86.1(10) 2_655 2_665
Ga1 O2 O4 35.8(5) 1_665 2_665
Ta O2 O4 35.8(5) 1_665 2_665
O7 O2 O4 23.5(8) 1_564 2_665
Ga4 O2 O4 2.3(4) 3_554 2_665
O3 O2 O4 80.8(10) 2_566 2_665
O6 O2 O4 121.9(9) 4_645 2_665
O4 O2 O4 112.0(13) 4 2_665
O2 O2 O4 75.1(5) 1_655 2_665
O2 O2 O4 104.9(5) 1_455 2_665
O7 O2 O4 25.7(9) 2_666 2_665
Ga4 O2 O4 105.5(9) 3_544 2_665
O4 O2 O4 50.4(13) 1_565 2_665
O4 O2 O4 99.5(11) 2 2_665
La1 O2 O4 122.1(7) 4_645 2_665
Ga2 O2 O4 88.4(9) 2 2_665
Ga1 O2 O4 132.2(10) . 2_665
Ta O2 O4 132.2(10) . 2_665
Ga4 O2 O4 71.3(7) 4 2_665
La1 O2 O4 41.8(6) 2_655 2_665
O1 O2 O4 65.8(8) 3_654 2_665
O4 O2 O4 138.4(9) 1_455 2_665
O4 O2 O4 104.3(7) 1_655 2_665
La1 O2 O4 69.2(8) 4 2_665
La1 O2 O4 86.9(8) 3_544 2_665
O4 O2 O4 43.0(7) 3_554 2_665
O1 O2 O4 170.7(8) . 2_665
O1 O2 O4 76.0(8) 1_665 2_665
Ga3 O2 O2 125.7(16) 1_655 4_645
Ga2 O2 O2 12.8(6) . 4_645
La2 O2 O2 97.2(9) . 4_645
O6 O2 O2 123.7(17) . 4_645
La1 O2 O2 88.9(15) . 4_645
O3 O2 O2 32.5(12) 3_554 4_645
O5 O2 O2 162.6(16) 1_554 4_645
O1 O2 O2 76.6(15) 4 4_645
O5 O2 O2 97.7(16) 2_656 4_645
O4 O2 O2 25.7(11) . 4_645
O2 O2 O2 107.7(12) 2_655 4_645
O1 O2 O2 42.1(12) 4_655 4_645
O5 O2 O2 130.5(17) 2_556 4_645
Ta O2 O2 156.4(14) 1_565 4_645
Ga1 O2 O2 156.4(14) 1_565 4_645
O1 O2 O2 123.3(11) 3_554 4_645
O2 O2 O2 135.5(8) 2 4_645
Ga2 O2 O2 110.7(8) 2_655 4_645
Ga4 O2 O2 116.3(12) 4_655 4_645
O7 O2 O2 72.7(9) 1_554 4_645
La2 O2 O2 70.4(6) 1_655 4_645
La1 O2 O2 65.1(9) 1_655 4_645
La1 O2 O2 40.2(4) 4_545 4_645
Ga4 O2 O2 37.9(9) . 4_645
Ga3 O2 O2 131.4(10) . 4_645
Ga4 O2 O2 41.43(18) 4_645 4_645
O7 O2 O2 56.6(8) 2_656 4_645
O3 O2 O2 90.9(14) 2_666 4_645
O4 O2 O2 56.4(13) 4_655 4_645
Ga2 O2 O2 88.8(9) 1_455 4_645
O6 O2 O2 127.6(10) 2_655 4_645
O7 O2 O2 80.9(8) 2_556 4_645
O1 O2 O2 86.2(12) 1_565 4_645
La1 O2 O2 154.7(10) 2 4_645
O6 O2 O2 167.9(11) 2 4_645
Ga2 O2 O2 77.8(11) 4_655 4_645
O4 O2 O2 93.0(8) 2_655 4_645
Ga1 O2 O2 107.6(9) 1_665 4_645
Ta O2 O2 107.6(9) 1_665 4_645
O7 O2 O2 146.8(12) 1_564 4_645
Ga4 O2 O2 145.6(9) 3_554 4_645
O3 O2 O2 111.5(15) 2_566 4_645
O6 O2 O2 25.1(7) 4_645 4_645
O4 O2 O2 85.4(12) 4 4_645
O2 O2 O2 70.2(6) 1_655 4_645
O2 O2 O2 109.8(6) 1_455 4_645
O7 O2 O2 121.1(12) 2_666 4_645
Ga4 O2 O2 78.8(4) 3_544 4_645
O4 O2 O2 113.9(13) 1_565 4_645
O4 O2 O2 109.9(7) 2 4_645
La1 O2 O2 23.3(4) 4_645 4_645
Ga2 O2 O2 125.1(7) 2 4_645
Ga1 O2 O2 69.99(19) . 4_645
Ta O2 O2 69.99(19) . 4_645
Ga4 O2 O2 129.2(11) 4 4_645
La1 O2 O2 115.8(8) 2_655 4_645
O1 O2 O2 93.4(8) 3_654 4_645
O4 O2 O2 77.9(9) 1_455 4_645
O4 O2 O2 43.9(7) 1_655 4_645
La1 O2 O2 107.9(11) 4 4_645
La1 O2 O2 112.3(5) 3_544 4_645
O4 O2 O2 141.4(10) 3_554 4_645
O1 O2 O2 29.1(4) . 4_645
O1 O2 O2 71.5(9) 1_665 4_645
O4 O2 O2 143.4(9) 2_665 4_645
Ga3 O2 O2 86.4(12) 1_655 4_655
Ga2 O2 O2 78.0(19) . 4_655
La2 O2 O2 161.7(16) . 4_655
O6 O2 O2 47.7(7) . 4_655
La1 O2 O2 54.7(9) . 4_655
O3 O2 O2 58.0(10) 3_554 4_655
O5 O2 O2 101.9(14) 1_554 4_655
O1 O2 O2 103.9(19) 4 4_655
O5 O2 O2 51.9(12) 2_656 4_655
O4 O2 O2 103.3(17) . 4_655
O2 O2 O2 107.7(12) 2_655 4_655
O1 O2 O2 70.4(15) 4_655 4_655
O5 O2 O2 88.5(12) 2_556 4_655
Ta O2 O2 82.5(5) 1_565 4_655
Ga1 O2 O2 82.5(5) 1_565 4_655
O1 O2 O2 153.1(13) 3_554 4_655
O2 O2 O2 135.5(8) 2 4_655
Ga2 O2 O2 135.7(10) 2_655 4_655
Ga4 O2 O2 40.7(2) 4_655 4_655
O7 O2 O2 149.4(14) 1_554 4_655
La2 O2 O2 99.4(9) 1_655 4_655
La1 O2 O2 40.1(6) 1_655 4_655
La1 O2 O2 95.5(12) 4_545 4_655
Ga4 O2 O2 42.5(9) . 4_655
Ga3 O2 O2 111.9(8) . 4_655
Ga4 O2 O2 117.4(11) 4_645 4_655
O7 O2 O2 119.3(13) 2_656 4_655
O3 O2 O2 19.3(6) 2_666 4_655
O4 O2 O2 21.4(11) 4_655 4_655
Ga2 O2 O2 107.7(11) 1_455 4_655
O6 O2 O2 83.0(6) 2_655 4_655
O7 O2 O2 146.2(15) 2_556 4_655
O1 O2 O2 27.5(3) 1_565 4_655
La1 O2 O2 126.4(7) 2 4_655
O6 O2 O2 103.9(6) 2 4_655
Ga2 O2 O2 5.1(2) 4_655 4_655
O4 O2 O2 140.3(11) 2_655 4_655
Ga1 O2 O2 63.1(5) 1_665 4_655
Ta O2 O2 63.1(5) 1_665 4_655
O7 O2 O2 69.8(8) 1_564 4_655
Ga4 O2 O2 80.8(4) 3_554 4_655
O3 O2 O2 60.0(6) 2_566 4_655
O6 O2 O2 53.7(9) 4_645 4_655
O4 O2 O2 67.7(10) 4 4_655
O2 O2 O2 70.2(6) 1_655 4_655
O2 O2 O2 109.8(6) 1_455 4_655
O7 O2 O2 55.2(7) 2_666 4_655
Ga4 O2 O2 145.4(9) 3_544 4_655
O4 O2 O2 36.2(7) 1_565 4_655
O4 O2 O2 164.0(10) 2 4_655
La1 O2 O2 75.8(9) 4_645 4_655
Ga2 O2 O2 147.1(8) 2 4_655
Ga1 O2 O2 146.6(11) . 4_655
Ta O2 O2 146.6(11) . 4_655
Ga4 O2 O2 76.1(5) 4 4_655
La1 O2 O2 100.6(7) 2_655 4_655
O1 O2 O2 106.3(9) 3_654 4_655
O4 O2 O2 116.0(13) 1_455 4_655
O4 O2 O2 81.1(9) 1_655 4_655
La1 O2 O2 39.3(3) 4 4_655
La1 O2 O2 166.4(10) 3_544 4_655
O4 O2 O2 122.3(9) 3_554 4_655
O1 O2 O2 99.2(11) . 4_655
O1 O2 O2 24.6(5) 1_665 4_655
O4 O2 O2 79.8(7) 2_665 4_655
O2 O2 O2 77.7(11) 4_645 4_655
Ga3 O2 O1 102.4(15) 1_655 3_454
Ga2 O2 O1 131.3(17) . 3_454
La2 O2 O1 33.3(8) . 3_454
O6 O2 O1 96.3(11) . 3_454
La1 O2 O1 87.8(10) . 3_454
O3 O2 O1 119.3(14) 3_554 3_454
O5 O2 O1 67.9(13) 1_554 3_454
O1 O2 O1 56.6(17) 4 3_454
O5 O2 O1 137.6(17) 2_656 3_454
O4 O2 O1 101.6(14) . 3_454
O2 O2 O1 99.1(17) 2_655 3_454
O1 O2 O1 150.4(17) 4_655 3_454
O5 O2 O1 49.9(12) 2_556 3_454
Ta O2 O1 65.6(8) 1_565 3_454
Ga1 O2 O1 65.6(8) 1_565 3_454
O1 O2 O1 47.5(5) 3_554 3_454
O2 O2 O1 12.1(8) 2 3_454
Ga2 O2 O1 74.6(7) 2_655 3_454
Ga4 O2 O1 115.0(10) 4_655 3_454
O7 O2 O1 68.1(10) 1_554 3_454
La2 O2 O1 120.8(10) 1_655 3_454
La1 O2 O1 171.0(11) 1_655 3_454
La1 O2 O1 86.9(8) 4_545 3_454
Ga4 O2 O1 135.3(9) . 3_454
Ga3 O2 O1 26.4(6) . 3_454
Ga4 O2 O1 96.4(8) 4_645 3_454
O7 O2 O1 101.6(12) 2_656 3_454
O3 O2 O1 138.1(10) 2_666 3_454
O4 O2 O1 149.6(12) 4_655 3_454
Ga2 O2 O1 46.3(6) 1_455 3_454
O6 O2 O1 102.7(9) 2_655 3_454
O7 O2 O1 44.7(9) 2_556 3_454
O1 O2 O1 112.1(8) 1_565 3_454
La1 O2 O1 45.3(5) 2 3_454
O6 O2 O1 47.6(6) 2 3_454
Ga2 O2 O1 134.1(9) 4_655 3_454
O4 O2 O1 78.7(8) 2_655 3_454
Ga1 O2 O1 126.1(10) 1_665 3_454
Ta O2 O1 126.1(10) 1_665 3_454
O7 O2 O1 86.5(10) 1_564 3_454
Ga4 O2 O1 89.8(8) 3_554 3_454
O3 O2 O1 78.3(7) 2_566 3_454
O6 O2 O1 145.6(10) 4_645 3_454
O4 O2 O1 78.2(10) 4 3_454
O2 O2 O1 146.9(5) 1_655 3_454
O2 O2 O1 33.1(5) 1_455 3_454
O7 O2 O1 115.0(11) 2_666 3_454
Ga4 O2 O1 76.3(7) 3_544 3_454
O4 O2 O1 110.3(9) 1_565 3_454
O4 O2 O1 25.9(7) 2 3_454
La1 O2 O1 138.6(9) 4_645 3_454
Ga2 O2 O1 10.9(4) 2 3_454
Ga1 O2 O1 61.3(6) . 3_454
Ta O2 O1 61.3(6) . 3_454
Ga4 O2 O1 62.6(6) 4 3_454
La1 O2 O1 99.8(8) 2_655 3_454
O1 O2 O1 107.2(10) 3_654 3_454
O4 O2 O1 49.8(9) 1_455 3_454
O4 O2 O1 140.1(10) 1_655 3_454
La1 O2 O1 99.4(7) 4 3_454
La1 O2 O1 44.2(5) 3_544 3_454
O4 O2 O1 65.5(7) 3_554 3_454
O1 O2 O1 94.8(7) . 3_454
O1 O2 O1 159.9(11) 1_665 3_454
O4 O2 O1 91.9(9) 2_665 3_454
O2 O2 O1 123.8(8) 4_645 3_454
O2 O2 O1 138.2(8) 4_655 3_454
Ga3 O2 O4 63.9(13) 1_655 2_565
Ga2 O2 O4 172.1(19) . 2_565
La2 O2 O4 87.0(12) . 2_565
O6 O2 O4 46.7(10) . 2_565
La1 O2 O4 77.5(11) . 2_565
O3 O2 O4 134.0(13) 3_554 2_565
O5 O2 O4 29.6(11) 1_554 2_565
O1 O2 O4 95.0(15) 4 2_565
O5 O2 O4 85.6(15) 2_656 2_565
O4 O2 O4 157.7(13) . 2_565
O2 O2 O4 85.1(13) 2_655 2_565
O1 O2 O4 145.2(13) 4_655 2_565
O5 O2 O4 37.2(13) 2_556 2_565
Ta O2 O4 12.0(7) 1_565 2_565
Ga1 O2 O4 12.0(7) 1_565 2_565
O1 O2 O4 67.9(11) 3_554 2_565
O2 O2 O4 46.1(6) 2 2_565
Ga2 O2 O4 82.7(9) 2_655 2_565
Ga4 O2 O4 59.5(7) 4_655 2_565
O7 O2 O4 116.2(12) 1_554 2_565
La2 O2 O4 122.3(10) 1_655 2_565
La1 O2 O4 115.4(9) 1_655 2_565
La1 O2 O4 131.7(8) 4_545 2_565
Ga4 O2 O4 130.6(10) . 2_565
Ga3 O2 O4 41.6(6) . 2_565
Ga4 O2 O4 148.3(11) 4_645 2_565
O7 O2 O4 136.5(14) 2_656 2_565
O3 O2 O4 84.4(10) 2_666 2_565
O4 O2 O4 115.7(15) 4_655 2_565
Ga2 O2 O4 83.2(7) 1_455 2_565
O6 O2 O4 61.1(7) 2_655 2_565
O7 O2 O4 100.9(12) 2_556 2_565
O1 O2 O4 81.9(10) 1_565 2_565
La1 O2 O4 36.9(7) 2 2_565
O6 O2 O4 9.6(7) 2 2_565
Ga2 O2 O4 93.3(9) 4_655 2_565
O4 O2 O4 100.0(12) 2_655 2_565
Ga1 O2 O4 77.7(7) 1_665 2_565
Ta O2 O4 77.7(7) 1_665 2_565
O7 O2 O4 30.3(9) 1_564 2_565
Ga4 O2 O4 40.3(5) 3_554 2_565
O3 O2 O4 55.0(9) 2_566 2_565
O6 O2 O4 147.9(11) 4_645 2_565
O4 O2 O4 81.4(9) 4 2_565
O2 O2 O4 117.7(5) 1_655 2_565
O2 O2 O4 62.3(5) 1_455 2_565
O7 O2 O4 60.0(8) 2_666 2_565
Ga4 O2 O4 112.9(9) 3_544 2_565
O4 O2 O4 58.6(12) 1_565 2_565
O4 O2 O4 75.3(8) 2 2_565
La1 O2 O4 164.1(8) 4_645 2_565
Ga2 O2 O4 58.0(7) 2 2_565
Ga1 O2 O4 115.5(8) . 2_565
Ta O2 O4 115.5(8) . 2_565
Ga4 O2 O4 37.3(6) 4 2_565
La1 O2 O4 76.2(7) 2_655 2_565
O1 O2 O4 99.4(9) 3_654 2_565
O4 O2 O4 96.2(7) 1_455 2_565
O4 O2 O4 146.5(8) 1_655 2_565
La1 O2 O4 60.5(7) 4 2_565
La1 O2 O4 77.4(7) 3_544 2_565
O4 O2 O4 52.2(8) 3_554 2_565
O1 O2 O4 146.4(7) . 2_565
O1 O2 O4 105.6(8) 1_665 2_565
O4 O2 O4 42.6(4) 2_665 2_565
O2 O2 O4 166.4(11) 4_645 2_565
O2 O2 O4 94.3(6) 4_655 2_565
O1 O2 O4 56.2(7) 3_454 2_565
Ga3 O2 O2 170.7(16) 1_655 4_545
Ga2 O2 O2 57.8(11) . 4_545
La2 O2 O2 71.7(7) . 4_545
O6 O2 O2 115.2(14) . 4_545
La1 O2 O2 63.6(13) . 4_545
O3 O2 O2 37.8(11) 3_554 4_545
O5 O2 O2 150.8(16) 1_554 4_545
O1 O2 O2 31.2(12) 4 4_545
O5 O2 O2 137.3(19) 2_656 4_545
O4 O2 O2 41.2(10) . 4_545
O2 O2 O2 142.2(5) 2_655 4_545
O1 O2 O2 87.5(14) 4_655 4_545
O5 O2 O2 89.1(14) 2_556 4_545
Ta O2 O2 124.1(10) 1_565 4_545
Ga1 O2 O2 124.1(10) 1_565 4_545
O1 O2 O2 113.7(11) 3_554 4_545
O2 O2 O2 96.2(10) 2 4_545
Ga2 O2 O2 124.6(8) 2_655 4_545
Ga4 O2 O2 129.2(12) 4_655 4_545
O7 O2 O2 71.7(8) 1_554 4_545
La2 O2 O2 109.6(8) 1_655 4_545
La1 O2 O2 104.4(12) 1_655 4_545
La1 O2 O2 7.2(4) 4_545 4_545
Ga4 O2 O2 55.5(9) . 4_545
Ga3 O2 O2 86.0(8) . 4_545
Ga4 O2 O2 58.2(3) 4_645 4_545
O7 O2 O2 82.3(8) 2_656 4_545
O3 O2 O2 112.2(16) 2_666 4_545
O4 O2 O2 79.0(14) 4_655 4_545
Ga2 O2 O2 43.4(6) 1_455 4_545
O6 O2 O2 172.8(12) 2_655 4_545
O7 O2 O2 53.6(7) 2_556 4_545
O1 O2 O2 80.5(12) 1_565 4_545
La1 O2 O2 129.2(10) 2 4_545
O6 O2 O2 122.5(10) 2 4_545
Ga2 O2 O2 89.5(11) 4_655 4_545
O4 O2 O2 107.8(8) 2_655 4_545
Ga1 O2 O2 149.6(13) 1_665 4_545
Ta O2 O2 149.6(13) 1_665 4_545
O7 O2 O2 140.9(10) 1_564 4_545
Ga4 O2 O2 162.9(8) 3_554 4_545
O3 O2 O2 83.7(11) 2_566 4_545
O6 O2 O2 61.6(8) 4_645 4_545
O4 O2 O2 52.4(10) 4 4_545
O2 O2 O2 115.6(6) 1_655 4_545
O2 O2 O2 64.4(6) 1_455 4_545
O7 O2 O2 147.8(15) 2_666 4_545
Ga4 O2 O2 88.3(3) 3_544 4_545
O4 O2 O2 117.1(13) 1_565 4_545
O4 O2 O2 83.6(8) 2 4_545
La1 O2 O2 68.5(6) 4_645 4_545
Ga2 O2 O2 90.4(7) 2 4_545
Ga1 O2 O2 58.20(19) . 4_545
Ta O2 O2 58.20(19) . 4_545
Ga4 O2 O2 93.6(8) 4 4_545
La1 O2 O2 153.8(7) 2_655 4_545
O1 O2 O2 129.7(8) 3_654 4_545
O4 O2 O2 34.5(7) 1_455 4_545
O4 O2 O2 88.1(9) 1_655 4_545
La1 O2 O2 96.5(9) 4 4_545
La1 O2 O2 100.5(6) 3_544 4_545
O4 O2 O2 144.1(11) 3_554 4_545
O1 O2 O2 24.0(4) . 4_545
O1 O2 O2 103.0(11) 1_665 4_545
O4 O2 O2 164.4(9) 2_665 4_545
O2 O2 O2 45.4(5) 4_645 4_545
O2 O2 O2 93.0(13) 4_655 4_545
O1 O2 O2 84.2(8) 3_454 4_545
O4 O2 O2 125.4(8) 2_565 4_545
Ga3 O2 O2 111.7(13) 1_655 4
Ga2 O2 O2 102(2) . 4
La2 O2 O2 118.4(12) . 4
O6 O2 O2 41.3(7) . 4
La1 O2 O2 11.8(9) . 4
O3 O2 O2 60.6(10) 3_554 4
O5 O2 O2 99.0(14) 1_554 4
O1 O2 O2 66.2(16) 4 4
O5 O2 O2 90.8(14) 2_656 4
O4 O2 O2 109.4(18) . 4
O2 O2 O2 142.2(5) 2_655 4
O1 O2 O2 110.3(18) 4_655 4
O5 O2 O2 48.5(11) 2_556 4
Ta O2 O2 63.7(4) 1_565 4
Ga1 O2 O2 63.7(4) 1_565 4
O1 O2 O2 136.9(13) 3_554 4
O2 O2 O2 96.2(10) 2 4
Ga2 O2 O2 156.2(12) 2_655 4
Ga4 O2 O2 58.8(3) 4_655 4
O7 O2 O2 142.7(11) 1_554 4
La2 O2 O2 144.5(12) 1_655 4
La1 O2 O2 85.3(9) 1_655 4
La1 O2 O2 80.3(10) 4_545 4
Ga4 O2 O2 58.9(9) . 4
Ga3 O2 O2 69.7(7) . 4
Ga4 O2 O2 129.2(12) 4_645 4
O7 O2 O2 149.6(16) 2_656 4
O3 O2 O2 57.3(6) 2_666 4
O4 O2 O2 56.4(11) 4_655 4
Ga2 O2 O2 65.5(8) 1_455 4
O6 O2 O2 106.9(6) 2_655 4
O7 O2 O2 110.8(11) 2_556 4
O1 O2 O2 17.9(3) 1_565 4
La1 O2 O2 109.6(8) 2 4
O6 O2 O2 80.3(7) 2 4
Ga2 O2 O2 40.5(4) 4_655 4
O4 O2 O2 172.7(13) 2_655 4
Ga1 O2 O2 98.0(6) 1_665 4
Ta O2 O2 98.0(6) 1_665 4
O7 O2 O2 69.2(7) 1_564 4
Ga4 O2 O2 90.7(4) 3_554 4
O3 O2 O2 19.9(5) 2_566 4
O6 O2 O2 79.9(11) 4_645 4
O4 O2 O2 26.2(9) 4 4
O2 O2 O2 115.6(6) 1_655 4
O2 O2 O2 64.4(6) 1_455 4
O7 O2 O2 78.8(7) 2_666 4
Ga4 O2 O2 160.9(8) 3_544 4
O4 O2 O2 45.1(7) 1_565 4
O4 O2 O2 118.9(10) 2 4
La1 O2 O2 106.1(11) 4_645 4
Ga2 O2 O2 105.0(8) 2 4
Ga1 O2 O2 127.0(8) . 4
Ta O2 O2 127.0(8) . 4
Ga4 O2 O2 39.4(3) 4 4
La1 O2 O2 130.9(6) 2_655 4
O1 O2 O2 148.4(9) 3_654 4
O4 O2 O2 78.3(9) 1_455 4
O4 O2 O2 120.7(12) 1_655 4
La1 O2 O2 22.7(3) 4 4
La1 O2 O2 138.6(9) 3_544 4
O4 O2 O2 125.0(9) 3_554 4
O1 O2 O2 94.4(10) . 4
O1 O2 O2 70.0(7) 1_665 4
O4 O2 O2 91.4(6) 2_665 4
O2 O2 O2 93.0(13) 4_645 4
O2 O2 O2 45.4(5) 4_655 4
O1 O2 O2 94.6(9) 3_454 4
O4 O2 O2 73.7(7) 2_565 4
O2 O2 O2 73.9(9) 4_545 4
Ga3 O2 O1 54.6(12) 1_655 2_565
Ga2 O2 O1 158.5(18) . 2_565
La2 O2 O1 71.5(11) . 2_565
O6 O2 O1 70.2(12) . 2_565
La1 O2 O1 102.3(12) . 2_565
O3 O2 O1 158.4(13) 3_554 2_565
O5 O2 O1 18.4(11) 1_554 2_565
O1 O2 O1 102.9(14) 4 2_565
O5 O2 O1 88.2(15) 2_656 2_565
O4 O2 O1 141.1(17) . 2_565
O2 O2 O1 65.3(14) 2_655 2_565
O1 O2 O1 135.6(15) 4_655 2_565
O5 O2 O1 57.5(12) 2_556 2_565
Ta O2 O1 37.2(7) 1_565 2_565
Ga1 O2 O1 37.2(7) 1_565 2_565
O1 O2 O1 42.7(6) 3_554 2_565
O2 O2 O1 37.4(9) 2 2_565
Ga2 O2 O1 57.2(8) 2_655 2_565
Ga4 O2 O1 75.9(8) 4_655 2_565
O7 O2 O1 93.5(12) 1_554 2_565
La2 O2 O1 101.8(9) 1_655 2_565
La1 O2 O1 121.6(9) 1_655 2_565
La1 O2 O1 136.3(8) 4_545 2_565
Ga4 O2 O1 156.1(11) . 2_565
Ga3 O2 O1 49.8(5) . 2_565
Ga4 O2 O1 124.6(10) 4_645 2_565
O7 O2 O1 110.5(13) 2_656 2_565
O3 O2 O1 101.0(12) 2_666 2_565
O4 O2 O1 136.5(13) 4_655 2_565
Ga2 O2 O1 91.0(7) 1_455 2_565
O6 O2 O1 54.1(6) 2_655 2_565
O7 O2 O1 89.0(11) 2_556 2_565
O1 O2 O1 107.6(12) 1_565 2_565
La1 O2 O1 11.4(5) 2 2_565
O6 O2 O1 19.8(5) 2 2_565
Ga2 O2 O1 115.9(10) 4_655 2_565
O4 O2 O1 74.0(10) 2_655 2_565
Ga1 O2 O1 76.7(7) 1_665 2_565
Ta O2 O1 76.7(7) 1_665 2_565
O7 O2 O1 45.8(9) 1_564 2_565
Ga4 O2 O1 41.0(5) 3_554 2_565
O3 O2 O1 80.4(10) 2_566 2_565
O6 O2 O1 164.8(9) 4_645 2_565
O4 O2 O1 103.3(10) 4 2_565
O2 O2 O1 109.0(3) 1_655 2_565
O2 O2 O1 71.0(3) 1_455 2_565
O7 O2 O1 67.9(10) 2_666 2_565
Ga4 O2 O1 87.3(8) 3_544 2_565
O4 O2 O1 79.6(10) 1_565 2_565
O4 O2 O1 58.5(8) 2 2_565
La1 O2 O1 151.0(8) 4_645 2_565
Ga2 O2 O1 45.5(5) 2 2_565
Ga1 O2 O1 97.3(8) . 2_565
Ta O2 O1 97.3(8) . 2_565
Ga4 O2 O1 61.6(6) 4 2_565
La1 O2 O1 59.4(5) 2_655 2_565
O1 O2 O1 79.0(6) 3_654 2_565
O4 O2 O1 98.6(9) 1_455 2_565
O4 O2 O1 130.5(9) 1_655 2_565
La1 O2 O1 86.0(7) 4 2_565
La1 O2 O1 53.8(6) 3_544 2_565
O4 O2 O1 28.2(6) 3_554 2_565
O1 O2 O1 142.2(9) . 2_565
O1 O2 O1 118.5(10) 1_665 2_565
O4 O2 O1 43.0(7) 2_665 2_565
O2 O2 O1 166.0(10) 4_645 2_565
O2 O2 O1 115.6(7) 4_655 2_565
O1 O2 O1 49.5(4) 3_454 2_565
O4 O2 O1 26.1(7) 2_565 2_565
O2 O2 O1 133.1(9) 4_545 2_565
O2 O2 O1 99.6(7) 4 2_565
Ga3 O2 O1 15.4(11) 1_655 2_665
Ga2 O2 O1 122.1(13) . 2_665
La2 O2 O1 95.5(13) . 2_665
O6 O2 O1 76.7(12) . 2_665
La1 O2 O1 127.2(14) . 2_665
O3 O2 O1 152.9(14) 3_554 2_665
O5 O2 O1 27.7(11) 1_554 2_665
O1 O2 O1 144.0(19) 4 2_665
O5 O2 O1 53.4(14) 2_656 2_665
O4 O2 O1 130.9(14) . 2_665
O2 O2 O1 29.1(8) 2_655 2_665
O1 O2 O1 94.2(11) 4_655 2_665
O5 O2 O1 94.1(14) 2_556 2_665
Ta O2 O1 61.3(8) 1_565 2_665
Ga1 O2 O1 61.3(8) 1_565 2_665
O1 O2 O1 53.1(7) 3_554 2_665
O2 O2 O1 76.3(13) 2 2_665
Ga2 O2 O1 42.1(7) 2_655 2_665
Ga4 O2 O1 64.4(7) 4_655 2_665
O7 O2 O1 94.9(10) 1_554 2_665
La2 O2 O1 65.5(6) 1_655 2_665
La1 O2 O1 84.5(7) 1_655 2_665
La1 O2 O1 161.3(11) 4_545 2_665
Ga4 O2 O1 135.6(8) . 2_665
Ga3 O2 O1 91.6(8) . 2_665
Ga4 O2 O1 112.0(8) 4_645 2_665
O7 O2 O1 88.5(11) 2_656 2_665
O3 O2 O1 81.2(10) 2_666 2_665
O4 O2 O1 113.0(11) 4_655 2_665
Ga2 O2 O1 132.5(9) 1_455 2_665
O6 O2 O1 17.7(5) 2_655 2_665
O7 O2 O1 113.2(13) 2_556 2_665
O1 O2 O1 112.9(13) 1_565 2_665
La1 O2 O1 42.5(5) 2 2_665
O6 O2 O1 57.0(6) 2 2_665
Ga2 O2 O1 104.1(8) 4_655 2_665
O4 O2 O1 59.6(9) 2_655 2_665
Ga1 O2 O1 40.8(5) 1_665 2_665
Ta O2 O1 40.8(5) 1_665 2_665
O7 O2 O1 49.0(9) 1_564 2_665
Ga4 O2 O1 27.2(5) 3_554 2_665
O3 O2 O1 105.5(11) 2_566 2_665
O6 O2 O1 125.1(7) 4_645 2_665
O4 O2 O1 136.2(11) 4 2_665
O2 O2 O1 67.1(4) 1_655 2_665
O2 O2 O1 112.9(4) 1_455 2_665
O7 O2 O1 45.9(9) 2_666 2_665
Ga4 O2 O1 79.0(7) 3_544 2_665
O4 O2 O1 76.2(10) 1_565 2_665
O4 O2 O1 84.2(9) 2 2_665
La1 O2 O1 112.0(6) 4_645 2_665
Ga2 O2 O1 79.9(7) 2 2_665
Ga1 O2 O1 108.1(8) . 2_665
Ta O2 O1 108.1(8) . 2_665
Ga4 O2 O1 92.4(7) 4 2_665
La1 O2 O1 19.3(3) 2_655 2_665
O1 O2 O1 43.2(4) 3_654 2_665
O4 O2 O1 136.7(11) 1_455 2_665
O4 O2 O1 91.1(8) 1_655 2_665
La1 O2 O1 95.8(7) 4 2_665
La1 O2 O1 66.0(6) 3_544 2_665
O4 O2 O1 23.6(6) 3_554 2_665
O1 O2 O1 147.3(9) . 2_665
O1 O2 O1 88.4(9) 1_665 2_665
O4 O2 O1 26.6(7) 2_665 2_665
O2 O2 O1 134.9(8) 4_645 2_665
O2 O2 O1 100.5(7) 4_655 2_665
O1 O2 O1 87.6(6) 3_454 2_665
O4 O2 O1 56.9(6) 2_565 2_665
O2 O2 O1 166.2(10) 4_545 2_665
O2 O2 O1 117.9(6) 4 2_665
O1 O2 O1 41.9(5) 2_565 2_665
Ga3 O2 O4 96.4(16) 1_655 1_465
Ga2 O2 O4 133.3(19) . 1_465
La2 O2 O4 101.5(10) . 1_465
O6 O2 O4 33.0(8) . 1_465
La1 O2 O4 34.6(9) . 1_465
O3 O2 O4 91.1(11) 3_554 1_465
O5 O2 O4 71.0(14) 1_554 1_465
O1 O2 O4 69.9(13) 4 1_465
O5 O2 O4 95.2(15) 2_656 1_465
O4 O2 O4 133.0(18) . 1_465
O2 O2 O4 124.8(11) 2_655 1_465
O1 O2 O4 138.6(16) 4_655 1_465
O5 O2 O4 20.3(10) 2_556 1_465
Ta O2 O4 34.9(7) 1_565 1_465
Ga1 O2 O4 34.9(7) 1_565 1_465
O1 O2 O4 105.6(11) 3_554 1_465
O2 O2 O4 67.9(8) 2 1_465
Ga2 O2 O4 125.3(12) 2_655 1_465
Ga4 O2 O4 57.3(7) 4_655 1_465
O7 O2 O4 136.3(11) 1_554 1_465
La2 O2 O4 156.1(11) 1_655 1_465
La1 O2 O4 106.3(10) 1_655 1_465
La1 O2 O4 99.2(9) 4_545 1_465
Ga4 O2 O4 90.8(9) . 1_465
Ga3 O2 O4 43.7(6) . 1_465
Ga4 O2 O4 149.0(10) 4_645 1_465
O7 O2 O4 170.5(13) 2_656 1_465
O3 O2 O4 70.9(7) 2_666 1_465
O4 O2 O4 85.1(13) 4_655 1_465
Ga2 O2 O4 62.3(7) 1_455 1_465
O6 O2 O4 92.1(10) 2_655 1_465
O7 O2 O4 103.6(10) 2_556 1_465
O1 O2 O4 45.1(8) 1_565 1_465
La1 O2 O4 77.7(8) 2 1_465
O6 O2 O4 48.5(8) 2 1_465
Ga2 O2 O4 64.7(7) 4_655 1_465
O4 O2 O4 141.1(10) 2_655 1_465
Ga1 O2 O4 95.7(9) 1_665 1_465
Ta O2 O4 95.7(9) 1_665 1_465
O7 O2 O4 49.4(9) 1_564 1_465
Ga4 O2 O4 70.9(8) 3_554 1_465
O3 O2 O4 12.2(8) 2_566 1_465
O6 O2 O4 111.7(10) 4_645 1_465
O4 O2 O4 40.6(9) 4 1_465
O2 O2 O4 130.8(5) 1_655 1_465
O2 O2 O4 49.2(5) 1_455 1_465
O7 O2 O4 72.6(10) 2_666 1_465
Ga4 O2 O4 146.2(9) 3_544 1_465
O4 O2 O4 45.8(5) 1_565 1_465
O4 O2 O4 96.1(7) 2 1_465
La1 O2 O4 138.0(10) 4_645 1_465
Ga2 O2 O4 78.9(7) 2 1_465
Ga1 O2 O4 124.0(7) . 1_465
Ta O2 O4 124.0(7) . 1_465
Ga4 O2 O4 8.0(5) 4 1_465
La1 O2 O4 113.9(9) 2_655 1_465
O1 O2 O4 138.2(11) 3_654 1_465
O4 O2 O4 78.3(7) 1_455 1_465
O4 O2 O4 149.4(12) 1_655 1_465
La1 O2 O4 29.3(5) 4 1_465
La1 O2 O4 110.3(8) 3_544 1_465
O4 O2 O4 95.1(10) 3_554 1_465
O1 O2 O4 115.8(9) . 1_465
O1 O2 O4 90.6(8) 1_665 1_465
O4 O2 O4 72.6(11) 2_665 1_465
O2 O2 O4 123.5(12) 4_645 1_465
O2 O2 O4 68.3(6) 4_655 1_465
O1 O2 O4 70.2(7) 3_454 1_465
O4 O2 O4 43.0(11) 2_565 1_465
O2 O2 O4 92.0(9) 4_545 1_465
O2 O2 O4 32.0(6) 4 1_465
O1 O2 O4 68.2(8) 2_565 1_465
O1 O2 O4 95.7(9) 2_665 1_465
Ga3 O2 O1 122.2(16) 1_655 1_465
Ga2 O2 O1 113.0(16) . 1_465
La2 O2 O1 93.0(9) . 1_465
O6 O2 O1 54.2(8) . 1_465
La1 O2 O1 18.3(7) . 1_465
O3 O2 O1 70.5(11) 3_554 1_465
O5 O2 O1 95.0(14) 1_554 1_465
O1 O2 O1 46.8(10) 4 1_465
O5 O2 O1 113.4(15) 2_656 1_465
O4 O2 O1 107.2(15) . 1_465
O2 O2 O1 150.2(11) 2_655 1_465
O1 O2 O1 131.4(14) 4_655 1_465
O5 O2 O1 30.5(12) 2_556 1_465
Ta O2 O1 59.8(7) 1_565 1_465
Ga1 O2 O1 59.8(7) 1_565 1_465
O1 O2 O1 115.4(9) 3_554 1_465
O2 O2 O1 73.2(11) 2 1_465
Ga2 O2 O1 141.4(10) 2_655 1_465
Ga4 O2 O1 77.1(7) 4_655 1_465
O7 O2 O1 122.0(10) 1_554 1_465
La2 O2 O1 168.9(11) 1_655 1_465
La1 O2 O1 110.9(9) 1_655 1_465
La1 O2 O1 73.3(7) 4_545 1_465
Ga4 O2 O1 76.0(7) . 1_465
Ga3 O2 O1 46.7(6) . 1_465
Ga4 O2 O1 123.7(9) 4_645 1_465
O7 O2 O1 147.7(12) 2_656 1_465
O3 O2 O1 81.9(6) 2_666 1_465
O4 O2 O1 80.3(11) 4_655 1_465
Ga2 O2 O1 42.4(6) 1_455 1_465
O6 O2 O1 117.8(10) 2_655 1_465
O7 O2 O1 87.9(9) 2_556 1_465
O1 O2 O1 43.6(4) 1_565 1_465
La1 O2 O1 95.0(7) 2 1_465
O6 O2 O1 68.5(7) 2 1_465
Ga2 O2 O1 66.2(6) 4_655 1_465
O4 O2 O1 148.2(9) 2_655 1_465
Ga1 O2 O1 117.6(9) 1_665 1_465
Ta O2 O1 117.6(9) 1_665 1_465
O7 O2 O1 75.1(8) 1_564 1_465
Ga4 O2 O1 96.8(8) 3_554 1_465
O3 O2 O1 19.4(6) 2_566 1_465
O6 O2 O1 97.1(8) 4_645 1_465
O4 O2 O1 15.8(8) 4 1_465
O2 O2 O1 141.3(5) 1_655 1_465
O2 O2 O1 38.7(5) 1_455 1_465
O7 O2 O1 95.3(10) 2_666 1_465
Ga4 O2 O1 138.8(8) 3_544 1_465
O4 O2 O1 63.7(7) 1_565 1_465
O4 O2 O1 93.3(8) 2 1_465
La1 O2 O1 121.0(9) 4_645 1_465
Ga2 O2 O1 80.5(5) 2 1_465
Ga1 O2 O1 106.7(7) . 1_465
Ta O2 O1 106.7(7) . 1_465
Ga4 O2 O1 28.7(5) 4 1_465
La1 O2 O1 139.7(9) 2_655 1_465
O1 O2 O1 164.1(12) 3_654 1_465
O4 O2 O1 57.3(8) 1_455 1_465
O4 O2 O1 140.2(10) 1_655 1_465
La1 O2 O1 41.2(4) 4 1_465
La1 O2 O1 113.9(6) 3_544 1_465
O4 O2 O1 116.1(9) 3_554 1_465
O1 O2 O1 90.0(7) . 1_465
O1 O2 O1 95.7(9) 1_665 1_465
O4 O2 O1 98.4(9) 2_665 1_465
O2 O2 O1 101.2(10) 4_645 1_465
O2 O2 O1 71.1(7) 4_655 1_465
O1 O2 O1 69.7(4) 3_454 1_465
O4 O2 O1 65.6(7) 2_565 1_465
O2 O2 O1 66.1(8) 4_545 1_465
O2 O2 O1 25.7(5) 4 1_465
O1 O2 O1 87.9(8) 2_565 1_465
O1 O2 O1 121.1(9) 2_665 1_465
O4 O2 O1 25.9(7) 1_465 1_465
Ga3 O2 O4 49.9(13) 1_655 1_665
Ga2 O2 O4 85.9(14) . 1_665
La2 O2 O4 159.7(15) . 1_665
O6 O2 O4 54.4(9) . 1_665
La1 O2 O4 89.3(11) . 1_665
O3 O2 O4 89.3(12) 3_554 1_665
O5 O2 O4 77.0(14) 1_554 1_665
O1 O2 O4 142.0(18) 4 1_665
O5 O2 O4 13.7(13) 2_656 1_665
O4 O2 O4 115.5(14) . 1_665
O2 O2 O4 69.6(10) 2_655 1_665
O1 O2 O4 61.6(12) 4_655 1_665
O5 O2 O4 104.6(13) 2_556 1_665
Ta O2 O4 78.6(8) 1_565 1_665
Ga1 O2 O4 78.6(8) 1_565 1_665
O1 O2 O4 117.6(12) 3_554 1_665
O2 O2 O4 131.2(10) 2 1_665
Ga2 O2 O4 97.5(8) 2_655 1_665
Ga4 O2 O4 31.0(5) 4_655 1_665
O7 O2 O4 135.5(11) 1_554 1_665
La2 O2 O4 72.1(7) 1_655 1_665
La1 O2 O4 28.7(6) 1_655 1_665
La1 O2 O4 126.8(11) 4_545 1_665
Ga4 O2 O4 71.5(8) . 1_665
Ga3 O2 O4 124.3(10) . 1_665
Ga4 O2 O4 116.8(8) 4_645 1_665
O7 O2 O4 102.6(10) 2_656 1_665
O3 O2 O4 21.1(6) 2_666 1_665
O4 O2 O4 48.1(12) 4_655 1_665
Ga2 O2 O4 143.5(10) 1_455 1_665
O6 O2 O4 47.4(7) 2_655 1_665
O7 O2 O4 169.5(11) 2_556 1_665
O1 O2 O4 62.0(7) 1_565 1_665
La1 O2 O4 102.3(9) 2 1_665
O6 O2 O4 95.1(8) 2 1_665
Ga2 O2 O4 43.1(6) 4_655 1_665
O4 O2 O4 105.6(7) 2_655 1_665
Ga1 O2 O4 25.1(6) 1_665 1_665
Ta O2 O4 25.1(6) 1_665 1_665
O7 O2 O4 56.5(8) 1_564 1_665
Ga4 O2 O4 54.1(6) 3_554 1_665
O3 O2 O4 84.8(6) 2_566 1_665
O6 O2 O4 69.9(8) 4_645 1_665
O4 O2 O4 103.5(11) 4 1_665
O2 O2 O4 43.9(5) 1_655 1_665
O2 O2 O4 136.1(5) 1_455 1_665
O7 O2 O4 27.7(9) 2_666 1_665
Ga4 O2 O4 119.3(7) 3_544 1_665
O4 O2 O4 41.0(5) 1_565 1_665
O4 O2 O4 149.2(9) 2 1_665
La1 O2 O4 77.7(7) 4_645 1_665
Ga2 O2 O4 140.6(10) 2 1_665
Ga1 O2 O4 149.1(7) . 1_665
Ta O2 O4 149.1(7) . 1_665
Ga4 O2 O4 92.1(7) 4 1_665
La1 O2 O4 62.3(6) 2_655 1_665
O1 O2 O4 70.7(8) 3_654 1_665
O4 O2 O4 154.3(14) 1_455 1_665
O4 O2 O4 69.1(6) 1_655 1_665
La1 O2 O4 61.2(5) 4 1_665
La1 O2 O4 129.3(8) 3_544 1_665
O4 O2 O4 88.5(9) 3_554 1_665
O1 O2 O4 122.1(9) . 1_665
O1 O2 O4 24.2(7) 1_665 1_665
O4 O2 O4 52.2(10) 2_665 1_665
O2 O2 O4 93.4(9) 4_645 1_665
O2 O2 O4 38.3(6) 4_655 1_665
O1 O2 O4 142.6(9) 3_454 1_665
O4 O2 O4 86.8(9) 2_565 1_665
O2 O2 O4 127.0(12) 4_545 1_665
O2 O2 O4 78.1(6) 4 1_665
O1 O2 O4 95.1(8) 2_565 1_665
O1 O2 O4 65.0(7) 2_665 1_665
O4 O2 O4 86.9(8) 1_465 1_665
O1 O2 O4 101.9(7) 1_465 1_665
Ga3 O2 O1 77.4(15) 1_655 4_565
Ga2 O2 O1 130.7(19) . 4_565
La2 O2 O1 121.0(12) . 4_565
O6 O2 O1 9.7(7) . 4_565
La1 O2 O1 46.3(10) . 4_565
O3 O2 O1 95.8(10) 3_554 4_565
O5 O2 O1 62.5(15) 1_554 4_565
O1 O2 O1 92.3(13) 4 4_565
O5 O2 O1 71.7(13) 2_656 4_565
O4 O2 O1 146.5(17) . 4_565
O2 O2 O1 108.1(6) 2_655 4_565
O1 O2 O1 121.6(15) 4_655 4_565
O5 O2 O1 40.7(11) 2_556 4_565
Ta O2 O1 30.5(7) 1_565 4_565
Ga1 O2 O1 30.5(7) 1_565 4_565
O1 O2 O1 110.1(12) 3_554 4_565
O2 O2 O1 82.1(5) 2 4_565
Ga2 O2 O1 119.7(11) 2_655 4_565
Ga4 O2 O1 33.9(4) 4_655 4_565
O7 O2 O1 155.8(12) 1_554 4_565
La2 O2 O1 133.1(9) 1_655 4_565
La1 O2 O1 86.7(8) 1_655 4_565
La1 O2 O1 116.6(9) 4_545 4_565
Ga4 O2 O1 88.6(9) . 4_565
Ga3 O2 O1 62.7(6) . 4_565
Ga4 O2 O1 166.4(11) 4_645 4_565
O7 O2 O1 165.6(11) 2_656 4_565
O3 O2 O1 50.6(5) 2_666 4_565
O4 O2 O1 74.4(12) 4_655 4_565
Ga2 O2 O1 85.6(7) 1_455 4_565
O6 O2 O1 72.8(8) 2_655 4_565
O7 O2 O1 126.4(9) 2_556 4_565
O1 O2 O1 40.1(10) 1_565 4_565
La1 O2 O1 78.8(8) 2 4_565
O6 O2 O1 51.3(7) 2 4_565
Ga2 O2 O1 51.9(6) 4_655 4_565
O4 O2 O1 138.5(12) 2_655 4_565
Ga1 O2 O1 72.6(6) 1_665 4_565
Ta O2 O1 72.6(6) 1_665 4_565
O7 O2 O1 32.0(9) 1_564 4_565
Ga4 O2 O1 54.0(6) 3_554 4_565
O3 O2 O1 26.8(5) 2_566 4_565
O6 O2 O1 105.9(9) 4_645 4_565
O4 O2 O1 57.5(9) 4 4_565
O2 O2 O1 107.8(3) 1_655 4_565
O2 O2 O1 72.2(3) 1_455 4_565
O7 O2 O1 49.7(8) 2_666 4_565
Ga4 O2 O1 154.8(11) 3_544 4_565
O4 O2 O1 23.4(5) 1_565 4_565
O4 O2 O1 112.5(9) 2 4_565
La1 O2 O1 129.7(9) 4_645 4_565
Ga2 O2 O1 94.3(7) 2 4_565
Ga1 O2 O1 146.7(6) . 4_565
Ta O2 O1 146.7(6) . 4_565
Ga4 O2 O1 28.1(3) 4 4_565
La1 O2 O1 96.4(7) 2_655 4_565
O1 O2 O1 119.4(9) 3_654 4_565
O4 O2 O1 101.6(8) 1_455 4_565
O4 O2 O1 131.3(8) 1_655 4_565
La1 O2 O1 18.4(4) 4 4_565
La1 O2 O1 119.6(8) 3_544 4_565
O4 O2 O1 88.9(9) 3_554 4_565
O1 O2 O1 131.6(7) . 4_565
O1 O2 O1 72.0(7) 1_665 4_565
O4 O2 O1 55.0(7) 2_665 4_565
O2 O2 O1 126.3(11) 4_645 4_565
O2 O2 O1 53.9(4) 4_655 4_565
O1 O2 O1 87.8(7) 3_454 4_565
O4 O2 O1 42.4(7) 2_565 4_565
O2 O2 O1 109.7(8) 4_545 4_565
O2 O2 O1 37.3(4) 4 4_565
O1 O2 O1 67.6(6) 2_565 4_565
O1 O2 O1 81.0(7) 2_665 4_565
O4 O2 O1 23.5(5) 1_465 4_565
O1 O2 O1 46.0(5) 1_465 4_565
O4 O2 O1 64.1(5) 1_665 4_565
Ga3 O2 O1 54.0(13) 1_655 4_665
Ga2 O2 O1 106.6(16) . 4_665
La2 O2 O1 152.1(15) . 4_665
O6 O2 O1 29.5(7) . 4_665
La1 O2 O1 72.4(11) . 4_665
O3 O2 O1 94.8(10) 3_554 4_665
O5 O2 O1 65.5(15) 1_554 4_665
O1 O2 O1 126.5(17) 4 4_665
O5 O2 O1 33.2(12) 2_656 4_665
O4 O2 O1 135.8(15) . 4_665
O2 O2 O1 82.3(6) 2_655 4_665
O1 O2 O1 85.8(11) 4_655 4_665
O5 O2 O1 79.5(12) 2_556 4_665
Ta O2 O1 55.7(7) 1_565 4_665
Ga1 O2 O1 55.7(7) 1_565 4_665
O1 O2 O1 116.5(12) 3_554 4_665
O2 O2 O1 111.7(6) 2 4_665
Ga2 O2 O1 106.5(9) 2_655 4_665
Ga4 O2 O1 6.3(4) 4_655 4_665
O7 O2 O1 156.5(10) 1_554 4_665
La2 O2 O1 95.2(7) 1_655 4_665
La1 O2 O1 51.1(6) 1_655 4_665
La1 O2 O1 131.7(11) 4_545 4_665
Ga4 O2 O1 79.0(8) . 4_665
Ga3 O2 O1 99.7(8) . 4_665
Ga4 O2 O1 141.5(8) 4_645 4_665
O7 O2 O1 127.0(10) 2_656 4_665
O3 O2 O1 20.0(7) 2_666 4_665
O4 O2 O1 55.9(11) 4_655 4_665
Ga2 O2 O1 123.0(9) 1_455 4_665
O6 O2 O1 49.7(7) 2_655 4_665
O7 O2 O1 165.1(11) 2_556 4_665
O1 O2 O1 48.8(9) 1_565 4_665
La1 O2 O1 90.9(8) 2 4_665
O6 O2 O1 74.8(7) 2 4_665
Ga2 O2 O1 39.3(6) 4_655 4_665
O4 O2 O1 120.6(9) 2_655 4_665
Ga1 O2 O1 37.5(5) 1_665 4_665
Ta O2 O1 37.5(5) 1_665 4_665
O7 O2 O1 36.2(9) 1_564 4_665
Ga4 O2 O1 44.0(6) 3_554 4_665
O3 O2 O1 62.1(5) 2_566 4_665
O6 O2 O1 85.7(8) 4_645 4_665
O4 O2 O1 86.7(10) 4 4_665
O2 O2 O1 68.6(3) 1_655 4_665
O2 O2 O1 111.4(3) 1_455 4_665
O7 O2 O1 20.0(8) 2_666 4_665
Ga4 O2 O1 138.4(7) 3_544 4_665
O4 O2 O1 17.2(6) 1_565 4_665
O4 O2 O1 139.3(10) 2 4_665
La1 O2 O1 100.1(7) 4_645 4_665
Ga2 O2 O1 123.4(9) 2 4_665
Ga1 O2 O1 172.4(7) . 4_665
Ta O2 O1 172.4(7) . 4_665
Ga4 O2 O1 67.2(5) 4 4_665
La1 O2 O1 71.9(6) 2_655 4_665
O1 O2 O1 88.2(7) 3_654 4_665
O4 O2 O1 138.0(9) 1_455 4_665
O4 O2 O1 94.0(7) 1_655 4_665
La1 O2 O1 39.8(4) 4 4_665
La1 O2 O1 129.9(9) 3_544 4_665
O4 O2 O1 85.8(8) 3_554 4_665
O1 O2 O1 135.7(8) . 4_665
O1 O2 O1 40.0(6) 1_665 4_665
O4 O2 O1 43.0(7) 2_665 4_665
O2 O2 O1 110.8(10) 4_645 4_665
O2 O2 O1 36.8(5) 4_655 4_665
O1 O2 O1 121.3(9) 3_454 4_665
O4 O2 O1 65.6(6) 2_565 4_665
O2 O2 O1 128.0(11) 4_545 4_665
O2 O2 O1 60.6(4) 4 4_665
O1 O2 O1 81.0(7) 2_565 4_665
O1 O2 O1 65.8(5) 2_665 4_665
O4 O2 O1 62.4(6) 1_465 4_665
O1 O2 O1 80.8(7) 1_465 4_665
O4 O2 O1 25.1(4) 1_665 4_665
O1 O2 O1 39.2(3) 4_565 4_665
Ga3 O2 O1 135.9(16) 1_655 4_455
Ga2 O2 O1 110.6(15) . 4_455
La2 O2 O1 54.5(8) . 4_455
O6 O2 O1 88.5(9) . 4_455
La1 O2 O1 53.8(8) . 4_455
O3 O2 O1 81.3(12) 3_554 4_455
O5 O2 O1 98.2(12) 1_554 4_455
O1 O2 O1 21.7(9) 4 4_455
O5 O2 O1 150.7(16) 2_656 4_455
O4 O2 O1 87.9(12) . 4_455
O2 O2 O1 139.0(19) 2_655 4_455
O1 O2 O1 140.4(18) 4_655 4_455
O5 O2 O1 41.7(12) 2_556 4_455
Ta O2 O1 75.8(7) 1_565 4_455
Ga1 O2 O1 75.8(7) 1_565 4_455
O1 O2 O1 86.5(10) 3_554 4_455
O2 O2 O1 49.3(11) 2 4_455
Ga2 O2 O1 112.8(9) 2_655 4_455
Ga4 O2 O1 112.7(8) 4_655 4_455
O7 O2 O1 83.8(10) 1_554 4_455
La2 O2 O1 147.0(11) 1_655 4_455
La1 O2 O1 144.9(11) 1_655 4_455
La1 O2 O1 58.5(6) 4_545 4_455
Ga4 O2 O1 95.7(8) . 4_455
Ga3 O2 O1 33.1(5) . 4_455
Ga4 O2 O1 96.0(8) 4_645 4_455
O7 O2 O1 115.2(12) 2_656 4_455
O3 O2 O1 120.9(8) 2_666 4_455
O4 O2 O1 111.0(12) 4_655 4_455
Ga2 O2 O1 9.6(5) 1_455 4_455
O6 O2 O1 134.1(10) 2_655 4_455
O7 O2 O1 49.5(8) 2_556 4_455
O1 O2 O1 81.4(6) 1_565 4_455
La1 O2 O1 82.2(7) 2 4_455
O6 O2 O1 69.7(7) 2 4_455
Ga2 O2 O1 103.3(8) 4_655 4_455
O4 O2 O1 111.1(10) 2_655 4_455
Ga1 O2 O1 149.3(10) 1_665 4_455
Ta O2 O1 149.3(10) 1_665 4_455
O7 O2 O1 98.3(9) 1_564 4_455
Ga4 O2 O1 113.9(8) 3_554 4_455
O3 O2 O1 56.0(5) 2_566 4_455
O6 O2 O1 110.8(9) 4_645 4_455
O4 O2 O1 41.0(8) 4 4_455
O2 O2 O1 168.5(6) 1_655 4_455
O2 O2 O1 11.5(6) 1_455 4_455
O7 O2 O1 126.9(11) 2_666 4_455
Ga4 O2 O1 99.8(7) 3_544 4_455
O4 O2 O1 100.6(8) 1_565 4_455
O4 O2 O1 57.3(8) 2 4_455
La1 O2 O1 121.2(9) 4_645 4_455
Ga2 O2 O1 50.3(5) 2 4_455
Ga1 O2 O1 69.3(6) . 4_455
Ta O2 O1 69.3(6) . 4_455
Ga4 O2 O1 52.0(5) 4 4_455
La1 O2 O1 139.1(9) 2_655 4_455
O1 O2 O1 144.9(9) 3_654 4_455
O4 O2 O1 24.3(8) 1_455 4_455
O4 O2 O1 139.5(10) 1_655 4_455
La1 O2 O1 79.5(5) 4 4_455
La1 O2 O1 79.8(6) 3_544 4_455
O4 O2 O1 104.3(9) 3_554 4_455
O1 O2 O1 73.0(6) . 4_455
O1 O2 O1 132.3(8) 1_665 4_455
O4 O2 O1 116.1(9) 2_665 4_455
O2 O2 O1 98.3(9) 4_645 4_455
O2 O2 O1 108.4(9) 4_655 4_455
O1 O2 O1 40.0(9) 3_454 4_455
O4 O2 O1 73.5(7) 2_565 4_455
O2 O2 O1 52.9(7) 4_545 4_455
O2 O2 O1 64.0(7) 4 4_455
O1 O2 O1 82.0(5) 2_565 4_455
O1 O2 O1 123.8(9) 2_665 4_455
O4 O2 O1 55.5(6) 1_465 4_455
O1 O2 O1 39.0(4) 1_465 4_455
O4 O2 O1 140.7(8) 1_665 4_455
O1 O2 O1 79.0(4) 4_565 4_455
O1 O2 O1 117.6(7) 4_665 4_455
Ga3 O2 O1 107.6(13) 1_655 1_655
Ga2 O2 O1 9.1(12) . 1_655
La2 O2 O1 96.9(12) . 1_655
O6 O2 O1 132.0(13) . 1_655
La1 O2 O1 108.3(13) . 1_655
O3 O2 O1 51.8(11) 3_554 1_655
O5 O2 O1 142.5(14) 1_554 1_655
O1 O2 O1 93.6(15) 4 1_655
O5 O2 O1 87.0(14) 2_656 1_655
O4 O2 O1 29.0(10) . 1_655
O2 O2 O1 87.2(11) 2_655 1_655
O1 O2 O1 26.9(9) 4_655 1_655
O5 O2 O1 150.9(15) 2_556 1_655
Ta O2 O1 165.3(11) 1_565 1_655
Ga1 O2 O1 165.3(11) 1_565 1_655
O1 O2 O1 110.1(12) 3_554 1_655
O2 O2 O1 137.9(5) 2 1_655
Ga2 O2 O1 92.3(9) 2_655 1_655
Ga4 O2 O1 115.9(8) 4_655 1_655
O7 O2 O1 65.1(11) 1_554 1_655
La2 O2 O1 49.9(6) 1_655 1_655
La1 O2 O1 58.8(6) 1_655 1_655
La1 O2 O1 56.9(6) 4_545 1_655
Ga4 O2 O1 52.2(6) . 1_655
Ga3 O2 O1 146.4(10) . 1_655
Ga4 O2 O1 33.7(5) 4_645 1_655
O7 O2 O1 40.0(10) 2_656 1_655
O3 O2 O1 91.9(9) 2_666 1_655
O4 O2 O1 63.7(12) 4_655 1_655
Ga2 O2 O1 105.3(9) 1_455 1_655
O6 O2 O1 110.3(7) 2_655 1_655
O7 O2 O1 84.6(10) 2_556 1_655
O1 O2 O1 100.4(10) 1_565 1_655
La1 O2 O1 139.8(9) 2 1_655
O6 O2 O1 169.0(10) 2 1_655
Ga2 O2 O1 86.2(7) 4_655 1_655
O4 O2 O1 76.0(9) 2_655 1_655
Ga1 O2 O1 94.2(6) 1_665 1_655
Ta O2 O1 94.2(6) 1_665 1_655
O7 O2 O1 143.3(10) 1_564 1_655
Ga4 O2 O1 131.2(7) 3_554 1_655
O3 O2 O1 130.2(12) 2_566 1_655
O6 O2 O1 32.6(6) 4_645 1_655
O4 O2 O1 105.8(11) 4 1_655
O2 O2 O1 53.9(4) 1_655 1_655
O2 O2 O1 126.1(4) 1_455 1_655
O7 O2 O1 112.9(9) 2_666 1_655
Ga4 O2 O1 65.5(6) 3_544 1_655
O4 O2 O1 118.9(10) 1_565 1_655
O4 O2 O1 107.7(9) 2 1_655
La1 O2 O1 9.6(4) 4_645 1_655
Ga2 O2 O1 125.7(9) 2 1_655
Ga1 O2 O1 68.2(6) . 1_655
Ta O2 O1 68.2(6) . 1_655
Ga4 O2 O1 149.0(9) 4 1_655
La1 O2 O1 95.7(6) 2_655 1_655
O1 O2 O1 72.9(5) 3_654 1_655
O4 O2 O1 92.0(9) 1_455 1_655
O4 O2 O1 24.9(6) 1_655 1_655
La1 O2 O1 121.0(8) 4 1_655
La1 O2 O1 102.1(7) 3_544 1_655
O4 O2 O1 121.7(8) 3_554 1_655
O1 O2 O1 41.9(4) . 1_655
O1 O2 O1 70.1(5) 1_665 1_655
O4 O2 O1 129.0(7) 2_665 1_655
O2 O2 O1 20.5(5) 4_645 1_655
O2 O2 O1 84.4(8) 4_655 1_655
O1 O2 O1 129.1(10) 3_454 1_655
O4 O2 O1 171.4(8) 2_565 1_655
O2 O2 O1 63.2(5) 4_545 1_655
O2 O2 O1 110.7(10) 4 1_655
O1 O2 O1 149.4(7) 2_565 1_655
O1 O2 O1 115.0(6) 2_665 1_655
O4 O2 O1 142.4(10) 1_465 1_655
O1 O2 O1 121.6(10) 1_465 1_655
O4 O2 O1 87.0(7) 1_665 1_655
O1 O2 O1 138.1(7) 4_565 1_655
O1 O2 O1 109.6(5) 4_665 1_655
O1 O2 O1 114.9(8) 4_455 1_655
Ga2 O3 Ga4 117.6(14) 3_545 3_545
Ga2 O3 La1 102.8(16) 3_545 3_545
Ga4 O3 La1 112.9(15) 3_545 3_545
Ga2 O3 La1 95.8(13) 3_545 2_546
Ga4 O3 La1 119.5(17) 3_545 2_546
La1 O3 La1 105.7(9) 3_545 2_546
Ga2 O3 O2 43.4(15) 3_545 3_545
Ga4 O3 O2 136.5(15) 3_545 3_545
La1 O3 O2 59.6(9) 3_545 3_545
La1 O3 O2 102.9(17) 2_546 3_545
Ga2 O3 O4 44.9(16) 3_545 3_545
Ga4 O3 O4 122.9(19) 3_545 3_545
La1 O3 O4 123.6(19) 3_545 3_545
La1 O3 O4 53.3(14) 2_546 3_545
O2 O3 O4 74(2) 3_545 3_545
Ga2 O3 O1 86.4(17) 3_545 2_556
Ga4 O3 O1 155.8(18) 3_545 2_556
La1 O3 O1 54.1(13) 3_545 2_556
La1 O3 O1 56.4(11) 2_546 2_556
O2 O3 O1 59.1(16) 3_545 2_556
O4 O3 O1 75.7(17) 3_545 2_556
Ga2 O3 O4 92.6(17) 3_545 2_656
Ga4 O3 O4 43.6(16) 3_545 2_656
La1 O3 O4 86.7(15) 3_545 2_656
La1 O3 O4 163(2) 2_546 2_656
O2 O3 O4 93.4(17) 3_545 2_656
O4 O3 O4 128.9(11) 3_545 2_656
O1 O3 O4 139(2) 2_556 2_656
Ga2 O3 O1 30.1(10) 3_545 2_656
Ga4 O3 O1 87.6(13) 3_545 2_656
La1 O3 O1 116.8(16) 3_545 2_656
La1 O3 O1 114.3(14) 2_546 2_656
O2 O3 O1 65.0(16) 3_545 2_656
O4 O3 O1 61.6(16) 3_545 2_656
O1 O3 O1 116(2) 2_556 2_656
O4 O3 O1 68.2(16) 2_656 2_656
Ga2 O3 O1 120.3(17) 3_545 3
Ga4 O3 O1 70.9(11) 3_545 3
La1 O3 O1 42.3(8) 3_545 3
La1 O3 O1 133.4(9) 2_546 3
O2 O3 O1 87.7(12) 3_545 3
O4 O3 O1 162(2) 3_545 3
O1 O3 O1 95.0(14) 2_556 3
O4 O3 O1 51.1(13) 2_656 3
O1 O3 O1 111.3(14) 2_656 3
Ga2 O3 O4 132.7(18) 3_545 2_556
Ga4 O3 O4 103.0(14) 3_545 2_556
La1 O3 O4 35.1(9) 3_545 2_556
La1 O3 O4 83.4(11) 2_546 2_556
O2 O3 O4 90.5(15) 3_545 2_556
O4 O3 O4 127.3(14) 3_545 2_556
O1 O3 O4 54.0(15) 2_556 2_556
O4 O3 O4 101.6(19) 2_656 2_556
O1 O3 O4 151.8(16) 2_656 2_556
O1 O3 O4 50.8(8) 3 2_556
Ga2 O3 O2 85.6(13) 3_545 2_646
Ga4 O3 O2 66.3(13) 3_545 2_646
La1 O3 O2 170.3(11) 3_545 2_646
La1 O3 O2 68.1(8) 2_546 2_646
O2 O3 O2 128.2(17) 3_545 2_646
O4 O3 O2 59.4(16) 3_545 2_646
O1 O3 O2 122.5(14) 2_556 2_646
O4 O3 O2 98.0(16) 2_656 2_646
O1 O3 O2 73.0(12) 2_656 2_646
O1 O3 O2 136.8(15) 3 2_646
O4 O3 O2 135.2(12) 2_556 2_646
Ga4 O4 Ga2 124(3) 4_645 .
Ga4 O4 La1 128(3) 4_645 4_545
Ga2 O4 La1 107(2) . 4_545
Ga4 O4 O6 43.0(13) 4_645 1_545
Ga2 O4 O6 154(3) . 1_545
La1 O4 O6 86.0(18) 4_545 1_545
Ga4 O4 O7 50(2) 4_645 1_554
Ga2 O4 O7 102(3) . 1_554
La1 O4 O7 112.7(18) 4_545 1_554
O6 O4 O7 52.0(15) 1_545 1_554
Ga4 O4 O7 33.8(18) 4_645 2_656
Ga2 O4 O7 90(2) . 2_656
La1 O4 O7 159(3) 4_545 2_656
O6 O4 O7 73.5(17) 1_545 2_656
O7 O4 O7 50(2) 1_554 2_656
Ga4 O4 La2 94(2) 4_645 .
Ga2 O4 La2 74(2) . .
La1 O4 La2 88.9(14) 4_545 .
O6 O4 La2 83.8(16) 1_545 .
O7 O4 La2 44.1(14) 1_554 .
O7 O4 La2 83.8(19) 2_656 .
Ga4 O4 O3 167(3) 4_645 3_554
Ga2 O4 O3 45.0(14) . 3_554
La1 O4 O3 64.8(15) 4_545 3_554
O6 O4 O3 150(2) 1_545 3_554
O7 O4 O3 132(3) 1_554 3_554
O7 O4 O3 135(3) 2_656 3_554
La2 O4 O3 88.9(17) . 3_554
Ga4 O4 O3 48.6(16) 4_645 2_656
Ga2 O4 O3 122(2) . 2_656
La1 O4 O3 113(3) 4_545 2_656
O6 O4 O3 69.3(16) 1_545 2_656
O7 O4 O3 99(2) 1_554 2_656
O7 O4 O3 64.7(19) 2_656 2_656
La2 O4 O3 143(2) . 2_656
O3 O4 O3 127(2) 3_554 2_656
Ga4 O4 O2 121(3) 4_645 .
Ga2 O4 O2 30.1(13) . .
La1 O4 O2 96.7(18) 4_545 .
O6 O4 O2 128(2) 1_545 .
O7 O4 O2 80(2) 1_554 .
O7 O4 O2 92(2) 2_656 .
La2 O4 O2 44.8(12) . .
O3 O4 O2 54.3(17) 3_554 .
O3 O4 O2 147(2) 2_656 .
Ga4 O4 O1 134(3) 4_645 4
Ga2 O4 O1 72(2) . 4
La1 O4 O1 50.8(11) 4_545 4
O6 O4 O1 101.8(17) 1_545 4
O7 O4 O1 85.4(19) 1_554 4
O7 O4 O1 128(3) 2_656 4
La2 O4 O1 44.4(13) . 4
O3 O4 O1 55.1(14) 3_554 4
O3 O4 O1 163(3) 2_656 4
O2 O4 O1 49.3(14) . 4
Ga4 O4 O1 99(2) 4_645 4_655
Ga2 O4 O1 34.9(12) . 4_655
La1 O4 O1 132(2) 4_545 4_655
O6 O4 O1 142(2) 1_545 4_655
O7 O4 O1 105(2) 1_554 4_655
O7 O4 O1 68.8(19) 2_656 4_655
La2 O4 O1 99(2) . 4_655
O3 O4 O1 68.3(17) 3_554 4_655
O3 O4 O1 87.8(17) 2_656 4_655
O2 O4 O1 61.5(17) . 4_655
O1 O4 O1 107(2) 4 4_655
Ga4 O4 O7 80.4(19) 4_645 2_556
Ga2 O4 O7 111(2) . 2_556
La1 O4 O7 71.3(15) 4_545 2_556
O6 O4 O7 51.2(13) 1_545 2_556
O7 O4 O7 41.6(15) 1_554 2_556
O7 O4 O7 91(2) 2_656 2_556
La2 O4 O7 37.4(10) . 2_556
O3 O4 O7 109.3(19) 3_554 2_556
O3 O4 O7 120(2) 2_656 2_556
O2 O4 O7 80.8(17) . 2_556
O1 O4 O7 54.2(13) 4 2_556
O1 O4 O7 135(2) 4_655 2_556
Ga4 O4 Ga1 52.1(14) 4_645 .
Ga2 O4 Ga1 128(3) . .
La1 O4 Ga1 89.2(14) 4_545 .
O6 O4 Ga1 27.4(8) 1_545 .
O7 O4 Ga1 29.6(11) 1_554 .
O7 O4 Ga1 70.2(16) 2_656 .
La2 O4 Ga1 56.6(9) . .
O3 O4 Ga1 138.1(17) 3_554 .
O3 O4 Ga1 92.8(17) 2_656 .
O2 O4 Ga1 100.9(18) . .
O1 O4 Ga1 82.9(14) 4 .
O1 O4 Ga1 134(2) 4_655 .
O7 O4 Ga1 28.8(9) 2_556 .
Ga4 O4 Ta 52.1(14) 4_645 .
Ga2 O4 Ta 128(3) . .
La1 O4 Ta 89.2(14) 4_545 .
O6 O4 Ta 27.4(8) 1_545 .
O7 O4 Ta 29.6(11) 1_554 .
O7 O4 Ta 70.2(16) 2_656 .
La2 O4 Ta 56.6(9) . .
O3 O4 Ta 138.1(17) 3_554 .
O3 O4 Ta 92.8(17) 2_656 .
O2 O4 Ta 100.9(18) . .
O1 O4 Ta 82.9(14) 4 .
O1 O4 Ta 134(2) 4_655 .
O7 O4 Ta 28.8(9) 2_556 .
Ga1 O4 Ta 0.00(17) . .
Ga4 O4 O1 88(3) 4_645 .
Ga2 O4 O1 144(3) . .
La1 O4 O1 48.9(13) 4_545 .
O6 O4 O1 60.3(18) 1_545 .
O7 O4 O1 111(2) 1_554 .
O7 O4 O1 121(2) 2_656 .
La2 O4 O1 122.7(16) . .
O3 O4 O1 101(2) 3_554 .
O3 O4 O1 65.3(16) 2_656 .
O2 O4 O1 146(2) . .
O1 O4 O1 98.1(15) 4 .
O1 O4 O1 137(2) 4_655 .
O7 O4 O1 87.4(16) 2_556 .
Ga1 O4 O1 82.4(16) . .
Ta O4 O1 82.4(16) . .
Ga4 O4 Ga2 74(2) 4_645 4_645
Ga2 O4 Ga2 134(3) . 4_645
La1 O4 Ga2 78.2(18) 4_545 4_645
O6 O4 Ga2 69.7(16) 1_545 4_645
O7 O4 Ga2 118(2) 1_554 4_645
O7 O4 Ga2 99(2) 2_656 4_645
La2 O4 Ga2 151.1(18) . 4_645
O3 O4 Ga2 108(2) 3_554 4_645
O3 O4 Ga2 35.2(10) 2_656 4_645
O2 O4 Ga2 161(2) . 4_645
O1 O4 Ga2 129(2) 4 4_645
O1 O4 Ga2 108.7(19) 4_655 4_645
O7 O4 Ga2 113.7(17) 2_556 4_645
Ga1 O4 Ga2 97.0(14) . 4_645
Ta O4 Ga2 97.0(14) . 4_645
O1 O4 Ga2 32.8(8) . 4_645
Ga4 O4 O3 93(2) 4_645 2_556
Ga2 O4 O3 135(2) . 2_556
La1 O4 O3 37.6(10) 4_545 2_556
O6 O4 O3 49.7(11) 1_545 2_556
O7 O4 O3 80.3(15) 1_554 2_556
O7 O4 O3 121(2) 2_656 2_556
La2 O4 O3 77.6(11) . 2_556
O3 O4 O3 100.4(15) 3_554 2_556
O3 O4 O3 101.6(19) 2_656 2_556
O2 O4 O3 110.4(16) . 2_556
O1 O4 O3 63.0(11) 4 2_556
O1 O4 O3 168(2) 4_655 2_556
O7 O4 O3 44.4(11) 2_556 2_556
Ga1 O4 O3 53.0(9) . 2_556
Ta O4 O3 53.0(9) . 2_556
O1 O4 O3 45.1(11) . 2_556
Ga2 O4 O3 76.5(13) 4_645 2_556
Ga4 O4 La1 83.4(17) 4_645 4_645
Ga2 O4 La1 77.8(16) . 4_645
La1 O4 La1 120(2) 4_545 4_645
O6 O4 La1 115.5(18) 1_545 4_645
O7 O4 La1 124.6(18) 1_554 4_645
O7 O4 La1 74.7(17) 2_656 4_645
La2 O4 La1 144.5(19) . 4_645
O3 O4 La1 86.6(16) 3_554 4_645
O3 O4 La1 46.5(11) 2_656 4_645
O2 O4 La1 107.3(16) . 4_645
O1 O4 La1 141(2) 4 4_645
O1 O4 La1 46.9(11) 4_655 4_645
O7 O4 La1 163.9(19) 2_556 4_645
Ga1 O4 La1 135.3(15) . 4_645
Ta O4 La1 135.3(15) . 4_645
O1 O4 La1 92.7(16) . 4_645
Ga2 O4 La1 61.9(10) 4_645 4_645
O3 O4 La1 138(2) 2_556 4_645
Ga4 O4 Ga4 38.2(17) 4_645 3_544
Ga2 O4 Ga4 98(2) . 3_544
La1 O4 Ga4 131.7(18) 4_545 3_544
O6 O4 Ga4 58.0(12) 1_545 3_544
O7 O4 Ga4 19.8(10) 1_554 3_544
O7 O4 Ga4 30.2(13) 2_656 3_544
La2 O4 Ga4 58.7(10) . 3_544
O3 O4 Ga4 139(2) 3_554 3_544
O3 O4 Ga4 85.0(16) 2_656 3_544
O2 O4 Ga4 84.6(17) . 3_544
O1 O4 Ga4 102.5(18) 4 3_544
O1 O4 Ga4 90.7(18) 4_655 3_544
O7 O4 Ga4 61.3(10) 2_556 3_544
Ga1 O4 Ga4 43.9(6) . 3_544
Ta O4 Ga4 43.9(6) . 3_544
O1 O4 Ga4 118(2) . 3_544
Ga2 O4 Ga4 112.2(15) 4_645 3_544
O3 O4 Ga4 96.9(13) 2_556 3_544
La1 O4 Ga4 104.9(13) 4_645 3_544
Ga4 O4 O5 136(3) 4_645 3_544
Ga2 O4 O5 90(2) . 3_544
La1 O4 O5 44.1(13) 4_545 3_544
O6 O4 O5 114(2) 1_545 3_544
O7 O4 O5 156.7(19) 1_554 3_544
O7 O4 O5 151(3) 2_656 3_544
La2 O4 O5 123.6(18) . 3_544
O3 O4 O5 48.3(15) 3_554 3_544
O3 O4 O5 91(2) 2_656 3_544
O2 O4 O5 102.0(18) . 3_544
O1 O4 O5 79.2(17) 4 3_544
O1 O4 O5 96.1(19) 4_655 3_544
O7 O4 O5 115.4(19) 2_556 3_544
Ga1 O4 O5 129.7(18) . 3_544
Ta O4 O5 129.7(18) . 3_544
O1 O4 O5 54.6(18) . 3_544
Ga2 O4 O5 61.9(16) 4_645 3_544
O3 O4 O5 77.1(15) 2_556 3_544
La1 O4 O5 77.3(15) 4_645 3_544
Ga4 O4 O5 172.2(19) 3_544 3_544
Ga4 O4 O5 12.7(16) 4_645 2_646
Ga2 O4 O5 128(2) . 2_646
La1 O4 O5 125(2) 4_545 2_646
O6 O4 O5 45.7(11) 1_545 2_646
O7 O4 O5 62.9(14) 1_554 2_646
O7 O4 O5 40.8(12) 2_656 2_646
La2 O4 O5 106.9(17) . 2_646
O3 O4 O5 160.9(18) 3_554 2_646
O3 O4 O5 36.1(13) 2_656 2_646
O2 O4 O5 132(2) . 2_646
O1 O4 O5 144.0(18) 4 2_646
O1 O4 O5 98.0(15) 4_655 2_646
O7 O4 O5 89.8(15) 2_556 2_646
Ga1 O4 O5 61.1(10) . 2_646
Ta O4 O5 61.1(10) . 2_646
O1 O4 O5 79.8(18) . 2_646
Ga2 O4 O5 62.4(12) 4_645 2_646
O3 O4 O5 93.5(14) 2_556 2_646
La1 O4 O5 74.3(9) 4_645 2_646
Ga4 O4 O5 50.7(11) 3_544 2_646
O5 O4 O5 124(2) 3_544 2_646
Ga4 O4 La2 67.9(18) 4_645 1_655
Ga2 O4 La2 56.4(15) . 1_655
La1 O4 La2 163(2) 4_545 1_655
O6 O4 La2 107.7(17) 1_545 1_655
O7 O4 La2 70.6(16) 1_554 1_655
O7 O4 La2 34.6(13) 2_656 1_655
La2 O4 La2 82.4(14) . 1_655
O3 O4 La2 100.0(18) 3_554 1_655
O3 O4 La2 82.1(14) 2_656 1_655
O2 O4 La2 66.7(13) . 1_655
O1 O4 La2 114(2) 4 1_655
O1 O4 La2 36.4(13) 4_655 1_655
O7 O4 La2 108.8(16) 2_556 1_655
Ga1 O4 La2 98.2(14) . 1_655
Ta O4 La2 98.2(14) . 1_655
O1 O4 La2 147.3(18) . 1_655
Ga2 O4 La2 115.9(13) 4_645 1_655
O3 O4 La2 150.9(17) 2_556 1_655
La1 O4 La2 63.9(8) 4_645 1_655
Ga4 O4 La2 54.4(8) 3_544 1_655
O5 O4 La2 131.9(16) 3_544 1_655
O5 O4 La2 72.3(11) 2_646 1_655
Ga4 O4 O6 121(2) 4_645 4_645
Ga2 O4 O6 61.6(15) . 4_645
La1 O4 O6 91.1(19) 4_545 4_645
O6 O4 O6 142(2) 1_545 4_645
O7 O4 O6 155(2) 1_554 4_645
O7 O4 O6 108.3(19) 2_656 4_645
La2 O4 O6 133.7(17) . 4_645
O3 O4 O6 50.3(13) 3_554 4_645
O3 O4 O6 77.6(17) 2_656 4_645
O2 O4 O6 89.4(15) . 4_645
O1 O4 O6 105.2(17) 4 4_645
O1 O4 O6 50.3(13) 4_655 4_645
O7 O4 O6 158.5(18) 2_556 4_645
Ga1 O4 O6 169.6(18) . 4_645
Ta O4 O6 169.6(18) . 4_645
O1 O4 O6 90.1(18) . 4_645
Ga2 O4 O6 73.0(13) 4_645 4_645
O3 O4 O6 124.7(18) 2_556 4_645
La1 O4 O6 37.6(7) 4_645 4_645
Ga4 O4 O6 137.2(14) 3_544 4_645
O5 O4 O6 48.0(11) 3_544 4_645
O5 O4 O6 110.7(12) 2_646 4_645
La2 O4 O6 84.3(10) 1_655 4_645
Ga4 O4 Ga4 91.3(18) 4_645 4_545
Ga2 O4 Ga4 120(2) . 4_545
La1 O4 Ga4 50.0(9) 4_545 4_545
O6 O4 Ga4 51.8(10) 1_545 4_545
O7 O4 Ga4 62.8(11) 1_554 4_545
O7 O4 Ga4 110.7(19) 2_656 4_545
La2 O4 Ga4 54.8(7) . 4_545
O3 O4 Ga4 100.9(14) 3_554 4_545
O3 O4 Ga4 117.1(17) 2_656 4_545
O2 O4 Ga4 91.9(13) . 4_545
O1 O4 Ga4 50.7(10) 4 4_545
O1 O4 Ga4 153(2) 4_655 4_545
O7 O4 Ga4 22.6(8) 2_556 4_545
Ga1 O4 Ga4 41.3(5) . 4_545
Ta O4 Ga4 41.3(5) . 4_545
O1 O4 Ga4 67.9(11) . 4_545
Ga2 O4 Ga4 98.2(13) 4_645 4_545
O3 O4 Ga4 22.9(6) 2_556 4_545
La1 O4 Ga4 160.1(19) 4_645 4_545
Ga4 O4 Ga4 81.7(9) 3_544 4_545
O5 O4 Ga4 93.8(14) 3_544 4_545
O5 O4 Ga4 97.1(12) 2_646 4_545
La2 O4 Ga4 131.4(15) 1_655 4_545
O6 O4 Ga4 140.9(16) 4_645 4_545
Ga4 O4 Ga4 148(2) 4_645 .
Ga2 O4 Ga4 52.4(15) . .
La1 O4 Ga4 72.5(14) 4_545 .
O6 O4 Ga4 153(2) 1_545 .
O7 O4 Ga4 153(2) 1_554 .
O7 O4 Ga4 128.6(19) 2_656 .
La2 O4 Ga4 111.8(15) . .
O3 O4 Ga4 23.6(10) 3_554 .
O3 O4 Ga4 103.3(19) 2_656 .
O2 O4 Ga4 72.4(14) . .
O1 O4 Ga4 77.9(14) 4 .
O1 O4 Ga4 60.6(14) 4_655 .
O7 O4 Ga4 131.4(16) 2_556 .
Ga1 O4 Ga4 159.3(14) . .
Ta O4 Ga4 159.3(14) . .
O1 O4 Ga4 92.5(18) . .
Ga2 O4 Ga4 89.1(15) 4_645 .
O3 O4 Ga4 110.0(15) 2_556 .
La1 O4 Ga4 64.7(9) 4_645 .
Ga4 O4 Ga4 149.2(16) 3_544 .
O5 O4 Ga4 38.5(10) 3_544 .
O5 O4 Ga4 137.9(14) 2_646 .
La2 O4 Ga4 96.9(11) 1_655 .
O6 O4 Ga4 27.3(6) 4_645 .
Ga4 O4 Ga4 118.3(12) 4_545 .
Ga4 O4 O4 52(2) 4_645 2_655
Ga2 O4 O4 80(2) . 2_655
La1 O4 O4 140(2) 4_545 2_655
O6 O4 O4 76.1(16) 1_545 2_655
O7 O4 O4 30.2(15) 1_554 2_655
O7 O4 O4 30.3(14) 2_656 2_655
La2 O4 O4 53.7(11) . 2_655
O3 O4 O4 121.7(17) 3_554 2_655
O3 O4 O4 94.2(17) 2_656 2_655
O2 O4 O4 68.8(14) . 2_655
O1 O4 O4 97.4(19) 4 2_655
O1 O4 O4 75.2(17) 4_655 2_655
O7 O4 O4 69.2(13) 2_556 2_655
Ga1 O4 O4 59.0(11) . 2_655
Ta O4 O4 59.0(11) . 2_655
O1 O4 O4 135.9(16) . 2_655
Ga2 O4 O4 126.1(12) 4_645 2_655
O3 O4 O4 110.5(16) 2_556 2_655
La1 O4 O4 100.2(15) 4_645 2_655
Ga4 O4 O4 18.3(8) 3_544 2_655
O5 O4 O4 169.5(14) 3_544 2_655
O5 O4 O4 63.9(12) 2_646 2_655
La2 O4 O4 40.6(7) 1_655 2_655
O6 O4 O4 124.8(15) 4_645 2_655
Ga4 O4 O4 91.6(14) 4_545 2_655
Ga4 O4 O4 131.2(11) . 2_655
Ga4 O4 La1 154(3) 4_645 .
Ga2 O4 La1 43.8(12) . .
La1 O4 La1 65.4(12) 4_545 .
O6 O4 La1 133.9(16) 1_545 .
O7 O4 La1 105.2(18) 1_554 .
O7 O4 La1 126(2) 2_656 .
La2 O4 La1 61.4(9) . .
O3 O4 La1 27.7(10) 3_554 .
O3 O4 La1 154(2) 2_656 .
O2 O4 La1 34.3(10) . .
O1 O4 La1 32.0(10) 4 .
O1 O4 La1 77.4(15) 4_655 .
O7 O4 La1 84.5(14) 2_556 .
Ga1 O4 La1 112.6(12) . .
Ta O4 La1 112.6(12) . .
O1 O4 La1 112.7(17) . .
Ga2 O4 La1 131.7(18) 4_645 .
O3 O4 La1 91.4(10) 2_556 .
La1 O4 La1 110.2(13) 4_645 .
Ga4 O4 La1 115.6(14) 3_544 .
O5 O4 La1 69.8(13) 3_544 .
O5 O4 La1 166.0(19) 2_646 .
La2 O4 La1 97.3(12) 1_655 .
O6 O4 La1 76.8(10) 4_645 .
Ga4 O4 La1 82.5(8) 4_545 .
Ga4 O4 La1 51.1(7) . .
O4 O4 La1 102.1(10) 2_655 .
Ga4 O4 O2 93(2) 4_645 4_645
Ga2 O4 O2 105(2) . 4_645
La1 O4 O2 82.5(19) 4_545 4_645
O6 O4 O2 99(2) 1_545 4_645
O7 O4 O2 143(2) 1_554 4_645
O7 O4 O2 105(2) 2_656 4_645
La2 O4 O2 170.8(18) . 4_645
O3 O4 O2 84.5(17) 3_554 4_645
O3 O4 O2 45.2(11) 2_656 4_645
O2 O4 O2 133(2) . 4_645
O1 O4 O2 127(2) 4 4_645
O1 O4 O2 84.4(17) 4_655 4_645
O7 O4 O2 140.1(19) 2_556 4_645
Ga1 O4 O2 126.1(17) . 4_645
Ta O4 O2 126.1(17) . 4_645
O1 O4 O2 52.8(13) . 4_645
Ga2 O4 O2 29.2(9) 4_645 4_645
O3 O4 O2 97.3(16) 2_556 4_645
La1 O4 O2 41.6(9) 4_645 4_645
Ga4 O4 O2 130.0(14) 3_544 4_645
O5 O4 O2 47.3(13) 3_544 4_645
O5 O4 O2 80.8(13) 2_646 4_645
La2 O4 O2 105.0(12) 1_655 4_645
O6 O4 O2 43.8(11) 4_645 4_645
Ga4 O4 O2 120.2(16) 4_545 4_645
Ga4 O4 O2 62.5(12) . 4_645
O4 O4 O2 135.5(15) 2_655 4_645
La1 O4 O2 111.6(15) . 4_645
Ga4 O4 Ga3 107(3) 4_645 1_655
Ga2 O4 Ga3 27.1(14) . 1_655
La1 O4 Ga3 115.0(18) 4_545 1_655
O6 O4 Ga3 127(2) 1_545 1_655
O7 O4 Ga3 75.1(18) 1_554 1_655
O7 O4 Ga3 75.2(17) 2_656 1_655
La2 O4 Ga3 51.1(9) . 1_655
O3 O4 Ga3 65.8(15) 3_554 1_655
O3 O4 Ga3 129.7(17) 2_656 1_655
O2 O4 Ga3 18.4(8) . 1_655
O1 O4 Ga3 67.0(15) 4 1_655
O1 O4 Ga3 48.7(14) 4_655 1_655
O7 O4 Ga3 88.5(14) 2_556 1_655
Ga1 O4 Ga3 101.2(14) . 1_655
Ta O4 Ga3 101.2(14) . 1_655
O1 O4 Ga3 163.8(18) . 1_655
Ga2 O4 Ga3 157.4(14) 4_645 1_655
O3 O4 Ga3 125.4(14) 2_556 1_655
La1 O4 Ga3 95.5(12) 4_645 1_655
Ga4 O4 Ga3 73.6(10) 3_544 1_655
O5 O4 Ga3 113.9(16) 3_544 1_655
O5 O4 Ga3 115.9(16) 2_646 1_655
La2 O4 Ga3 48.3(7) 1_655 1_655
O6 O4 Ga3 88.0(11) 4_645 1_655
Ga4 O4 Ga3 104.3(11) 4_545 1_655
Ga4 O4 Ga3 78.6(10) . 1_655
O4 O4 Ga3 55.9(7) 2_655 1_655
La1 O4 Ga3 51.3(7) . 1_655
O2 O4 Ga3 130.5(15) 4_645 1_655
Ga4 O4 La1 62.3(17) 4_645 1_545
Ga2 O4 La1 171(2) . 1_545
La1 O4 La1 65.8(13) 4_545 1_545
O6 O4 La1 26.0(9) 1_545 1_545
O7 O4 La1 76.8(15) 1_554 1_545
O7 O4 La1 95.8(17) 2_656 1_545
La2 O4 La1 99.3(12) . 1_545
O3 O4 La1 130(2) 3_554 1_545
O3 O4 La1 66.9(13) 2_656 1_545
O2 O4 La1 142.1(16) . 1_545
O1 O4 La1 98.8(13) 4 1_545
O1 O4 La1 154.4(19) 4_655 1_545
O7 O4 La1 62.1(11) 2_556 1_545
Ga1 O4 La1 48.7(6) . 1_545
Ta O4 La1 48.7(6) . 1_545
O1 O4 La1 34.6(12) . 1_545
Ga2 O4 La1 51.8(9) 4_645 1_545
O3 O4 La1 36.2(7) 2_556 1_545
La1 O4 La1 110.5(15) 4_645 1_545
Ga4 O4 La1 84.0(10) 3_544 1_545
O5 O4 La1 88.3(16) 3_544 1_545
O5 O4 La1 59.5(10) 2_646 1_545
La2 O4 La1 130.3(13) 1_655 1_545
O6 O4 La1 122.5(17) 4_645 1_545
Ga4 O4 La1 50.8(6) 4_545 1_545
Ga4 O4 La1 126.7(16) . 1_545
O4 O4 La1 102.1(10) 2_655 1_545
La1 O4 La1 127.3(11) . 1_545
O2 O4 La1 80.1(13) 4_645 1_545
Ga3 O4 La1 149.3(14) 1_655 1_545
Ga4 O4 O5 63.3(16) 4_645 2_546
Ga2 O4 O5 144(2) . 2_546
La1 O4 O5 69.2(13) 4_545 2_546
O6 O4 O5 22.0(10) 1_545 2_546
O7 O4 O5 53.1(12) 1_554 2_546
O7 O4 O5 89.7(18) 2_656 2_546
La2 O4 O5 70.4(11) . 2_546
O3 O4 O5 129.5(15) 3_554 2_546
O3 O4 O5 89.4(15) 2_656 2_546
O2 O4 O5 114.4(17) . 2_546
O1 O4 O5 80.2(13) 4 2_546
O1 O4 O5 157(2) 4_655 2_546
O7 O4 O5 33.6(9) 2_556 2_546
Ga1 O4 O5 23.6(8) . 2_546
Ta O4 O5 23.6(8) . 2_546
O1 O4 O5 60.0(14) . 2_546
Ga2 O4 O5 80.8(13) 4_645 2_546
O3 O4 O5 31.6(9) 2_556 2_546
La1 O4 O5 135.9(16) 4_645 2_546
Ga4 O4 O5 66.7(10) 3_544 2_546
O5 O4 O5 106.5(17) 3_544 2_546
O5 O4 O5 67.5(10) 2_646 2_546
La2 O4 O5 120.9(15) 1_655 2_546
O6 O4 O5 150.0(19) 4_645 2_546
Ga4 O4 O5 29.8(6) 4_545 2_546
Ga4 O4 O5 141.6(14) . 2_546
O4 O4 O5 82.6(13) 2_655 2_546
La1 O4 O5 112.2(10) . 2_546
O2 O4 O5 109.1(16) 4_645 2_546
Ga3 O4 O5 120.4(14) 1_655 2_546
La1 O4 O5 29.1(8) 1_545 2_546
Ga4 O4 O5 30.8(12) 4_645 1_544
Ga2 O4 O5 127(3) . 1_544
La1 O4 O5 109.1(17) 4_545 1_544
O6 O4 O5 28.6(10) 1_545 1_544
O7 O4 O5 26.9(14) 1_554 1_544
O7 O4 O5 49.8(13) 2_656 1_544
La2 O4 O5 68.4(12) . 1_544
O3 O4 O5 157(2) 3_554 1_544
O3 O4 O5 76.1(16) 2_656 1_544
O2 O4 O5 107(2) . 1_544
O1 O4 O5 103.1(17) 4 1_544
O1 O4 O5 118(2) 4_655 1_544
O7 O4 O5 49.7(10) 2_556 1_544
Ga1 O4 O5 22.1(5) . 1_544
Ta O4 O5 22.1(5) . 1_544
O1 O4 O5 88.6(17) . 1_544
Ga2 O4 O5 91.3(14) 4_645 1_544
O3 O4 O5 71.6(11) 2_556 1_544
La1 O4 O5 114.1(14) 4_645 1_544
Ga4 O4 O5 29.5(7) 3_544 1_544
O5 O4 O5 143(2) 3_544 1_544
O5 O4 O5 41.3(12) 2_646 1_544
La2 O4 O5 81.6(12) 1_655 1_544
O6 O4 O5 151.6(16) 4_645 1_544
Ga4 O4 O5 63.2(9) 4_545 1_544
Ga4 O4 O5 178.4(16) . 1_544
O4 O4 O5 47.6(10) 2_655 1_544
La1 O4 O5 129.4(15) . 1_544
O2 O4 O5 117.5(16) 4_645 1_544
Ga3 O4 O5 100.6(14) 1_655 1_544
La1 O4 O5 54.5(8) 1_545 1_544
O5 O4 O5 40.0(11) 2_546 1_544
Ga4 O4 Ga2 126(2) 4_645 1_455
Ga2 O4 Ga2 85.1(16) . 1_455
La1 O4 Ga2 43.1(9) 4_545 1_455
O6 O4 Ga2 90.0(13) 1_545 1_455
O7 O4 Ga2 82.2(13) 1_554 1_455
O7 O4 Ga2 130(2) 2_656 1_455
La2 O4 Ga2 46.7(6) . 1_455
O3 O4 Ga2 64.6(11) 3_554 1_455
O3 O4 Ga2 151.2(19) 2_656 1_455
O2 O4 Ga2 61.5(10) . 1_455
O1 O4 Ga2 13.1(8) 4 1_455
O1 O4 Ga2 120.0(19) 4_655 1_455
O7 O4 Ga2 45.6(10) 2_556 1_455
Ga1 O4 Ga2 73.9(8) . 1_455
Ta O4 Ga2 73.9(8) . 1_455
O1 O4 Ga2 87.4(12) . 1_455
Ga2 O4 Ga2 119.7(15) 4_645 1_455
O3 O4 Ga2 50.0(7) 2_556 1_455
La1 O4 Ga2 150.5(16) 4_645 1_455
Ga4 O4 Ga2 101.1(11) 3_544 1_455
O5 O4 Ga2 78.9(13) 3_544 1_455
O5 O4 Ga2 134.3(13) 2_646 1_455
La2 O4 Ga2 124.4(15) 1_655 1_455
O6 O4 Ga2 112.9(13) 4_645 1_455
Ga4 O4 Ga2 38.3(4) 4_545 1_455
Ga4 O4 Ga2 85.8(10) . 1_455
O4 O4 Ga2 100.2(14) 2_655 1_455
La1 O4 Ga2 44.3(5) . 1_455
O2 O4 Ga2 124.2(15) 4_645 1_455
Ga3 O4 Ga2 78.6(9) 1_655 1_455
La1 O4 Ga2 85.7(8) 1_545 1_455
O5 O4 Ga2 68.1(8) 2_546 1_455
O5 O4 Ga2 95.4(11) 1_544 1_455
Ga4 O4 Ta 23.8(11) 4_645 1_655
Ga2 O4 Ta 102(2) . 1_655
La1 O4 Ta 151(2) 4_545 1_655
O6 O4 Ta 66.8(11) 1_545 1_655
O7 O4 Ta 59.4(13) 1_554 1_655
O7 O4 Ta 17.1(13) 2_656 1_655
La2 O4 Ta 98.6(14) . 1_655
O3 O4 Ta 143.1(18) 3_554 1_655
O3 O4 Ta 48.0(12) 2_656 1_655
O2 O4 Ta 108.7(18) . 1_655
O1 O4 Ta 143(2) 4 1_655
O1 O4 Ta 74.9(14) 4_655 1_655
O7 O4 Ta 97.8(14) 2_556 1_655
Ga1 O4 Ta 72.0(9) . 1_655
Ta O4 Ta 72.0(9) . 1_655
O1 O4 Ta 104.9(17) . 1_655
Ga2 O4 Ta 81.8(11) 4_645 1_655
O3 O4 Ta 116.5(14) 2_556 1_655
La1 O4 Ta 66.5(8) 4_645 1_655
Ga4 O4 Ta 40.9(5) 3_544 1_655
O5 O4 Ta 137.8(19) 3_544 1_655
O5 O4 Ta 26.1(8) 2_646 1_655
La2 O4 Ta 46.2(6) 1_655 1_655
O6 O4 Ta 103.5(11) 4_645 1_655
Ga4 O4 Ta 113.0(12) 4_545 1_655
Ga4 O4 Ta 128.7(12) . 1_655
O4 O4 Ta 46.3(8) 2_655 1_655
La1 O4 Ta 142.4(15) . 1_655
O2 O4 Ta 90.5(11) 4_645 1_655
Ga3 O4 Ta 91.2(11) 1_655 1_655
La1 O4 Ta 85.0(10) 1_545 1_655
O5 O4 Ta 86.6(10) 2_546 1_655
O5 O4 Ta 49.9(8) 1_544 1_655
Ga2 O4 Ta 141.6(14) 1_455 1_655
Ga4 O4 Ga1 23.8(11) 4_645 1_655
Ga2 O4 Ga1 102(2) . 1_655
La1 O4 Ga1 151(2) 4_545 1_655
O6 O4 Ga1 66.8(11) 1_545 1_655
O7 O4 Ga1 59.4(13) 1_554 1_655
O7 O4 Ga1 17.1(13) 2_656 1_655
La2 O4 Ga1 98.6(14) . 1_655
O3 O4 Ga1 143.1(18) 3_554 1_655
O3 O4 Ga1 48.0(12) 2_656 1_655
O2 O4 Ga1 108.7(18) . 1_655
O1 O4 Ga1 143(2) 4 1_655
O1 O4 Ga1 74.9(14) 4_655 1_655
O7 O4 Ga1 97.8(14) 2_556 1_655
Ga1 O4 Ga1 72.0(9) . 1_655
Ta O4 Ga1 72.0(9) . 1_655
O1 O4 Ga1 104.9(17) . 1_655
Ga2 O4 Ga1 81.8(11) 4_645 1_655
O3 O4 Ga1 116.5(14) 2_556 1_655
La1 O4 Ga1 66.5(8) 4_645 1_655
Ga4 O4 Ga1 40.9(5) 3_544 1_655
O5 O4 Ga1 137.8(19) 3_544 1_655
O5 O4 Ga1 26.1(8) 2_646 1_655
La2 O4 Ga1 46.2(6) 1_655 1_655
O6 O4 Ga1 103.5(11) 4_645 1_655
Ga4 O4 Ga1 113.0(12) 4_545 1_655
Ga4 O4 Ga1 128.7(12) . 1_655
O4 O4 Ga1 46.3(8) 2_655 1_655
La1 O4 Ga1 142.4(15) . 1_655
O2 O4 Ga1 90.5(11) 4_645 1_655
Ga3 O4 Ga1 91.2(11) 1_655 1_655
La1 O4 Ga1 85.0(10) 1_545 1_655
O5 O4 Ga1 86.6(10) 2_546 1_655
O5 O4 Ga1 49.9(8) 1_544 1_655
Ga2 O4 Ga1 141.6(14) 1_455 1_655
Ta O4 Ga1 0.00(15) 1_655 1_655
Ga4 O4 O6 151(3) 4_645 4_545
Ga2 O4 O6 84.6(18) . 4_545
La1 O4 O6 22.9(9) 4_545 4_545
O6 O4 O6 108.5(15) 1_545 4_545
O7 O4 O6 123.8(15) 1_554 4_545
O7 O4 O6 171(2) 2_656 4_545
La2 O4 O6 87.4(10) . 4_545
O3 O4 O6 42.0(11) 3_554 4_545
O3 O4 O6 125(2) 2_656 4_545
O2 O4 O6 79.6(13) . 4_545
O1 O4 O6 43.3(11) 4 4_545
O1 O4 O6 109.9(18) 4_655 4_545
O7 O4 O6 83.4(12) 2_556 4_545
Ga1 O4 O6 107.2(11) . 4_545
Ta O4 O6 107.2(11) . 4_545
O1 O4 O6 66.9(14) . 4_545
Ga2 O4 O6 90.2(15) 4_645 4_545
O3 O4 O6 59.1(9) 2_556 4_545
La1 O4 O6 111.5(16) 4_645 4_545
Ga4 O4 O6 143.2(13) 3_544 4_545
O5 O4 O6 36.7(9) 3_544 4_545
O5 O4 O6 146.2(18) 2_646 4_545
La2 O4 O6 141.0(15) 1_655 4_545
O6 O4 O6 75.9(12) 4_645 4_545
Ga4 O4 O6 66.0(7) 4_545 4_545
Ga4 O4 O6 52.7(8) . 4_545
O4 O4 O6 140.7(15) 2_655 4_545
La1 O4 O6 45.8(6) . 4_545
O2 O4 O6 83.4(14) 4_645 4_545
Ga3 O4 O6 97.0(11) 1_655 4_545
La1 O4 O6 88.5(11) 1_545 4_545
O5 O4 O6 90.1(10) 2_546 4_545
O5 O4 O6 128.8(13) 1_544 4_545
Ga2 O4 O6 42.3(5) 1_455 4_545
Ta O4 O6 171.7(17) 1_655 4_545
Ga1 O4 O6 171.7(17) 1_655 4_545
Ga4 O4 O2 85(2) 4_645 2_655
Ga2 O4 O2 43.5(17) . 2_655
La1 O4 O2 135.3(19) 4_545 2_655
O6 O4 O2 111.9(19) 1_545 2_655
O7 O4 O2 61.5(17) 1_554 2_655
O7 O4 O2 52.8(16) 2_656 2_655
La2 O4 O2 55.1(10) . 2_655
O3 O4 O2 87(2) 3_554 2_655
O3 O4 O2 111.5(17) 2_656 2_655
O2 O4 O2 39.6(13) . 2_655
O1 O4 O2 84.8(18) 4 2_655
O1 O4 O2 47.6(15) 4_655 2_655
O7 O4 O2 88.3(14) 2_556 2_655
Ga1 O4 O2 90.7(13) . 2_655
Ta O4 O2 90.7(13) . 2_655
O1 O4 O2 172(2) . 2_655
Ga2 O4 O2 145.9(14) 4_645 2_655
O3 O4 O2 132.1(16) 2_556 2_655
La1 O4 O2 89.5(12) 4_645 2_655
Ga4 O4 O2 54.5(9) 3_544 2_655
O5 O4 O2 133.3(17) 3_544 2_655
O5 O4 O2 93.6(14) 2_646 2_655
La2 O4 O2 30.0(6) 1_655 2_655
O6 O4 O2 96.3(13) 4_645 2_655
Ga4 O4 O2 109.1(13) 4_545 2_655
Ga4 O4 O2 95.4(13) . 2_655
O4 O4 O2 36.2(8) 2_655 2_655
La1 O4 O2 73.5(10) . 2_655
O2 O4 O2 130.6(15) 4_645 2_655
Ga3 O4 O2 22.3(6) 1_655 2_655
La1 O4 O2 137.7(15) 1_545 2_655
O5 O4 O2 113.6(15) 2_546 2_655
O5 O4 O2 83.5(13) 1_544 2_655
Ga2 O4 O2 94.4(11) 1_455 2_655
Ta O4 O2 69.1(9) 1_655 2_655
Ga1 O4 O2 69.1(9) 1_655 2_655
O6 O4 O2 119.2(13) 4_545 2_655
Ga4 O4 O1 81(2) 4_645 3_554
Ga2 O4 O1 68(2) . 3_554
La1 O4 O1 111.7(17) 4_545 3_554
O6 O4 O1 86.9(17) 1_545 3_554
O7 O4 O1 36.3(15) 1_554 3_554
O7 O4 O1 62.9(16) 2_656 3_554
La2 O4 O1 22.8(6) . 3_554
O3 O4 O1 97(2) 3_554 3_554
O3 O4 O1 127(2) 2_656 3_554
O2 O4 O1 44.1(14) . 3_554
O1 O4 O1 64.8(17) 4 3_554
O1 O4 O1 82.7(19) 4_655 3_554
O7 O4 O1 52.9(11) 2_556 3_554
Ga1 O4 O1 60.7(10) . 3_554
Ta O4 O1 60.7(10) . 3_554
O1 O4 O1 140.0(17) . 3_554
Ga2 O4 O1 154.2(18) 4_645 3_554
O3 O4 O1 96.8(12) 2_556 3_554
La1 O4 O1 123.7(15) 4_645 3_554
Ga4 O4 O1 43.1(8) 3_544 3_554
O5 O4 O1 141.7(19) 3_544 3_554
O5 O4 O1 93.8(15) 2_646 3_554
La2 O4 O1 60.1(8) 1_655 3_554
O6 O4 O1 128.4(16) 4_645 3_554
Ga4 O4 O1 74.0(9) 4_545 3_554
Ga4 O4 O1 116.4(15) . 3_554
O4 O4 O1 32.8(8) 2_655 3_554
La1 O4 O1 72.6(11) . 3_554
O2 O4 O1 165.2(14) 4_645 3_554
Ga3 O4 O1 40.5(8) 1_655 3_554
La1 O4 O1 109.1(12) 1_545 3_554
O5 O4 O1 81.0(12) 2_546 3_554
O5 O4 O1 63.2(12) 1_544 3_554
Ga2 O4 O1 69.1(9) 1_455 3_554
Ta O4 O1 79.1(10) 1_655 3_554
Ga1 O4 O1 79.1(10) 1_655 3_554
O6 O4 O1 107.9(12) 4_545 3_554
O2 O4 O1 35.4(7) 2_655 3_554
Ga4 O4 Ga3 14.7(11) 4_645 1_645
Ga2 O4 Ga3 135(2) . 1_645
La1 O4 Ga3 114.0(17) 4_545 1_645
O6 O4 Ga3 28.4(8) 1_545 1_645
O7 O4 Ga3 46.3(14) 1_554 1_645
O7 O4 Ga3 46.3(14) 2_656 1_645
La2 O4 Ga3 89.4(12) . 1_645
O3 O4 Ga3 178.0(17) 3_554 1_645
O3 O4 Ga3 55.0(13) 2_656 1_645
O2 O4 Ga3 125(2) . 1_645
O1 O4 Ga3 122.8(16) 4 1_645
O1 O4 Ga3 113.2(17) 4_655 1_645
O7 O4 Ga3 68.7(11) 2_556 1_645
Ga1 O4 Ga3 39.9(5) . 1_645
Ta O4 Ga3 39.9(5) . 1_645
O1 O4 Ga3 79.0(16) . 1_645
Ga2 O4 Ga3 72.9(10) 4_645 1_645
O3 O4 Ga3 78.1(10) 2_556 1_645
La1 O4 Ga3 95.5(11) 4_645 1_645
Ga4 O4 Ga3 40.7(5) 3_544 1_645
O5 O4 Ga3 132.1(19) 3_544 1_645
O5 O4 Ga3 21.2(7) 2_646 1_645
La2 O4 Ga3 80.9(9) 1_655 1_645
O6 O4 Ga3 131.7(13) 4_645 1_645
Ga4 O4 Ga3 77.2(8) 4_545 1_645
Ga4 O4 Ga3 158.3(14) . 1_645
O4 O4 Ga3 58.0(8) 2_655 1_645
La1 O4 Ga3 150.6(14) . 1_645
O2 O4 Ga3 97.0(13) 4_645 1_645
Ga3 O4 Ga3 113.9(13) 1_655 1_645
La1 O4 Ga3 49.6(6) 1_545 1_645
O5 O4 Ga3 48.7(7) 2_546 1_645
O5 O4 Ga3 21.2(6) 1_544 1_645
Ga2 O4 Ga3 113.4(10) 1_455 1_645
Ta O4 Ga3 38.5(4) 1_655 1_645
Ga1 O4 Ga3 38.5(4) 1_655 1_645
O6 O4 Ga3 136.7(13) 4_545 1_645
O2 O4 Ga3 93.2(12) 2_655 1_645
O1 O4 Ga3 81.4(11) 3_554 1_645
Ga4 O4 Ga2 73(2) 4_645 2_655
Ga2 O4 Ga2 62.2(19) . 2_655
La1 O4 Ga2 131.1(18) 4_545 2_655
O6 O4 Ga2 92.2(16) 1_545 2_655
O7 O4 Ga2 40.9(14) 1_554 2_655
O7 O4 Ga2 47.0(15) 2_656 2_655
La2 O4 Ga2 42.5(8) . 2_655
O3 O4 Ga2 101.9(19) 3_554 2_655
O3 O4 Ga2 111.6(18) 2_656 2_655
O2 O4 Ga2 48.6(13) . 2_655
O1 O4 Ga2 82.2(17) 4 2_655
O1 O4 Ga2 67.4(17) 4_655 2_655
O7 O4 Ga2 70.0(11) 2_556 2_655
Ga1 O4 Ga2 70.0(10) . 2_655
Ta O4 Ga2 70.0(10) . 2_655
O1 O4 Ga2 152.1(19) . 2_655
Ga2 O4 Ga2 145.6(15) 4_645 2_655
O3 O4 Ga2 114.4(13) 2_556 2_655
La1 O4 Ga2 104.4(13) 4_645 2_655
Ga4 O4 Ga2 37.0(6) 3_544 2_655
O5 O4 Ga2 150.2(18) 3_544 2_655
O5 O4 Ga2 83.9(13) 2_646 2_655
La2 O4 Ga2 40.6(6) 1_655 2_655
O6 O4 Ga2 116.9(13) 4_645 2_655
Ga4 O4 Ga2 92.2(10) 4_545 2_655
Ga4 O4 Ga2 114.6(13) . 2_655
O4 O4 Ga2 20.2(6) 2_655 2_655
La1 O4 Ga2 82.1(10) . 2_655
O2 O4 Ga2 145.5(13) 4_645 2_655
Ga3 O4 Ga2 36.6(5) 1_655 2_655
La1 O4 Ga2 117.6(12) 1_545 2_655
O5 O4 Ga2 93.0(12) 2_546 2_655
O5 O4 Ga2 64.5(11) 1_544 2_655
Ga2 O4 Ga2 88.1(10) 1_455 2_655
Ta O4 Ga2 64.0(8) 1_655 2_655
Ga1 O4 Ga2 64.0(8) 1_655 2_655
O6 O4 Ga2 123.8(12) 4_545 2_655
O2 O4 Ga2 20.7(6) 2_655 2_655
O1 O4 Ga2 19.7(3) 3_554 2_655
Ga3 O4 Ga2 77.7(9) 1_645 2_655
Ga4 O4 O6 23.3(16) 4_645 2_645
Ga2 O4 O6 103(2) . 2_645
La1 O4 O6 142.5(18) 4_545 2_645
O6 O4 O6 57.9(12) 1_545 2_645
O7 O4 O6 37.7(11) 1_554 2_645
O7 O4 O6 16.4(13) 2_656 2_645
La2 O4 O6 78.0(12) . 2_645
O3 O4 O6 148(2) 3_554 2_645
O3 O4 O6 66.4(14) 2_656 2_645
O2 O4 O6 98.1(18) . 2_645
O1 O4 O6 121.9(19) 4 2_645
O1 O4 O6 85.0(16) 4_655 2_645
O7 O4 O6 77.3(12) 2_556 2_645
Ga1 O4 O6 54.1(7) . 2_645
Ta O4 O6 54.1(7) . 2_645
O1 O4 O6 110.8(18) . 2_645
Ga2 O4 O6 96.6(12) 4_645 2_645
O3 O4 O6 104.9(12) 2_556 2_645
La1 O4 O6 87.6(10) 4_645 2_645
Ga4 O4 O6 19.4(4) 3_544 2_645
O5 O4 O6 158(2) 3_544 2_645
O5 O4 O6 34.3(10) 2_646 2_645
La2 O4 O6 49.7(7) 1_655 2_645
O6 O4 O6 123.3(12) 4_645 2_645
Ga4 O4 O6 95.2(10) 4_545 2_645
Ga4 O4 O6 145.0(13) . 2_645
O4 O4 O6 29.6(7) 2_655 2_645
La1 O4 O6 131.7(15) . 2_645
O2 O4 O6 110.9(12) 4_645 2_645
Ga3 O4 O6 83.5(11) 1_655 2_645
La1 O4 O6 81.7(9) 1_545 2_645
O5 O4 O6 73.3(10) 2_546 2_645
O5 O4 O6 33.4(7) 1_544 2_645
Ga2 O4 O6 119.9(12) 1_455 2_645
Ta O4 O6 21.8(4) 1_655 2_645
Ga1 O4 O6 21.8(4) 1_655 2_645
O6 O4 O6 160.7(13) 4_545 2_645
O2 O4 O6 61.7(10) 2_655 2_645
O1 O4 O6 60.7(9) 3_554 2_645
Ga3 O4 O6 32.4(4) 1_645 2_645
Ga2 O4 O6 49.6(7) 2_655 2_645
Ga4 O4 O2 116(2) 4_645 4_545
Ga2 O4 O2 120(2) . 4_545
La1 O4 O2 15.9(11) 4_545 4_545
O6 O4 O2 77.0(15) 1_545 4_545
O7 O4 O2 114.6(17) 1_554 4_545
O7 O4 O2 149(2) 2_656 4_545
La2 O4 O2 100.8(12) . 4_545
O3 O4 O2 75.9(15) 3_554 4_545
O3 O4 O2 97.5(19) 2_656 4_545
O2 O4 O2 112.6(15) . 4_545
O1 O4 O2 66.2(13) 4 4_545
O1 O4 O2 138(2) 4_655 4_545
O7 O4 O2 76.0(12) 2_556 4_545
Ga1 O4 O2 87.1(11) . 4_545
Ta O4 O2 87.1(11) . 4_545
O1 O4 O2 33.0(10) . 4_545
Ga2 O4 O2 63.0(12) 4_645 4_545
O3 O4 O2 34.3(7) 2_556 4_545
La1 O4 O2 112.1(17) 4_645 4_545
Ga4 O4 O2 130.9(13) 3_544 4_545
O5 O4 O2 42.8(12) 3_544 4_545
O5 O4 O2 110.4(16) 2_646 4_545
La2 O4 O2 174.7(16) 1_655 4_545
O6 O4 O2 90.4(14) 4_645 4_545
Ga4 O4 O2 53.4(8) 4_545 4_545
Ga4 O4 O2 78.0(12) . 4_545
O4 O4 O2 144.6(16) 2_655 4_545
La1 O4 O2 80.7(10) . 4_545
O2 O4 O2 71.4(13) 4_645 4_545
Ga3 O4 O2 130.9(12) 1_655 4_545
La1 O4 O2 53.7(9) 1_545 4_545
O5 O4 O2 64.3(11) 2_546 4_545
O5 O4 O2 103.5(13) 1_544 4_545
Ga2 O4 O2 57.2(8) 1_455 4_545
Ta O4 O2 136.5(14) 1_655 4_545
Ga1 O4 O2 136.5(14) 1_655 4_545
O6 O4 O2 35.9(8) 4_545 4_545
O2 O4 O2 150.9(14) 2_655 4_545
O1 O4 O2 123.4(12) 3_554 4_545
Ga3 O4 O2 103.2(12) 1_645 4_545
Ga2 O4 O2 143.1(12) 2_655 4_545
O6 O4 O2 134.9(13) 2_645 4_545
Ga4 O4 Ga3 117(3) 4_645 3_645
Ga2 O4 Ga3 96(2) . 3_645
La1 O4 Ga3 61.9(14) 4_545 3_645
O6 O4 Ga3 110(2) 1_545 3_645
O7 O4 Ga3 162(2) 1_554 3_645
O7 O4 Ga3 130(2) 2_656 3_645
La2 O4 Ga3 145.8(15) . 3_645
O3 O4 Ga3 63.5(16) 3_554 3_645
O3 O4 Ga3 69.8(16) 2_656 3_645
O2 O4 Ga3 117.1(17) . 3_645
O1 O4 Ga3 101.5(16) 4 3_645
O1 O4 Ga3 89.4(17) 4_655 3_645
O7 O4 Ga3 131.0(15) 2_556 3_645
Ga1 O4 Ga3 133.5(16) . 3_645
Ta O4 Ga3 133.5(16) . 3_645
O1 O4 Ga3 51.2(13) . 3_645
Ga2 O4 Ga3 44.7(9) 4_645 3_645
O3 O4 Ga3 87.5(13) 2_556 3_645
La1 O4 Ga3 58.4(9) 4_645 3_645
Ga4 O4 Ga3 154.9(14) 3_544 3_645
O5 O4 Ga3 22.2(10) 3_544 3_645
O5 O4 Ga3 104.5(14) 2_646 3_645
La2 O4 Ga3 120.2(11) 1_655 3_645
O6 O4 Ga3 39.4(8) 4_645 3_645
Ga4 O4 Ga3 108.4(12) 4_545 3_645
Ga4 O4 Ga3 45.3(7) . 3_645
O4 O4 Ga3 158.4(16) 2_655 3_645
La1 O4 Ga3 88.9(11) . 3_645
O2 O4 Ga3 25.1(8) 4_645 3_645
Ga3 O4 Ga3 123.4(12) 1_655 3_645
La1 O4 Ga3 85.2(12) 1_545 3_645
O5 O4 Ga3 110.7(14) 2_546 3_645
O5 O4 Ga3 135.3(16) 1_544 3_645
Ga2 O4 Ga3 100.6(11) 1_455 3_645
Ta O4 Ga3 115.5(12) 1_655 3_645
Ga1 O4 Ga3 115.5(12) 1_655 3_645
O6 O4 Ga3 58.7(9) 4_545 3_645
O2 O4 Ga3 135.6(13) 2_655 3_645
O1 O4 Ga3 161.0(16) 3_554 3_645
Ga3 O4 Ga3 117.6(13) 1_645 3_645
Ga2 O4 Ga3 156.3(12) 2_655 3_645
O6 O4 Ga3 136.0(12) 2_645 3_645
O2 O4 Ga3 55.0(9) 4_545 3_645
Ga4 O4 O4 111.3(15) 4_645 1_455
Ga2 O4 O4 106.2(15) . 1_455
La1 O4 O4 36.0(14) 4_545 1_455
O6 O4 O4 71.0(11) 1_545 1_455
O7 O4 O4 78.1(12) 1_554 1_455
O7 O4 O4 127.9(16) 2_656 1_455
La2 O4 O4 55.7(9) . 1_455
O3 O4 O4 80.9(12) 3_554 1_455
O3 O4 O4 130.7(13) 2_656 1_455
O2 O4 O4 81.5(11) . 1_455
O1 O4 O4 34.2(13) 4 1_455
O1 O4 O4 141.1(14) 4_655 1_455
O7 O4 O4 36.6(11) 2_556 1_455
Ga1 O4 O4 60.7(7) . 1_455
Ta O4 O4 60.7(7) . 1_455
O1 O4 O4 70.2(10) . 1_455
Ga2 O4 O4 103.0(9) 4_645 1_455
O3 O4 O4 29.1(10) 2_556 1_455
La1 O4 O4 156.3(11) 4_645 1_455
Ga4 O4 O4 97.8(6) 3_544 1_455
O5 O4 O4 79.3(12) 3_544 1_455
O5 O4 O4 116.7(8) 2_646 1_455
La2 O4 O4 138.2(8) 1_655 1_455
O6 O4 O4 123.2(9) 4_645 1_455
Ga4 O4 O4 20.0(7) 4_545 1_455
Ga4 O4 O4 98.7(7) . 1_455
O4 O4 O4 103.6(10) 2_655 1_455
La1 O4 O4 64.6(6) . 1_455
O2 O4 O4 116.6(9) 4_645 1_455
Ga3 O4 O4 97.6(6) 1_655 1_455
La1 O4 O4 64.5(6) 1_545 1_455
O5 O4 O4 49.1(7) 2_546 1_455
O5 O4 O4 82.8(8) 1_544 1_455
Ga2 O4 O4 21.1(7) 1_455 1_455
Ta O4 O4 132.6(6) 1_655 1_455
Ga1 O4 O4 132.6(6) 1_655 1_455
O6 O4 O4 47.3(7) 4_545 1_455
O2 O4 O4 109.7(7) 2_655 1_455
O1 O4 O4 78.2(6) 3_554 1_455
Ga3 O4 O4 97.2(5) 1_645 1_455
Ga2 O4 O4 97.9(5) 2_655 1_455
O6 O4 O4 113.5(6) 2_645 1_455
O2 O4 O4 45.2(8) 4_545 1_455
Ga3 O4 O4 97.9(6) 3_645 1_455
Ga4 O4 O4 68.6(16) 4_645 1_655
Ga2 O4 O4 73.8(15) . 1_655
La1 O4 O4 144.0(14) 4_545 1_655
O6 O4 O4 109.0(11) 1_545 1_655
O7 O4 O4 101.9(12) 1_554 1_655
O7 O4 O4 52.1(16) 2_656 1_655
La2 O4 O4 124.3(9) . 1_655
O3 O4 O4 99.1(12) 3_554 1_655
O3 O4 O4 49.3(13) 2_656 1_655
O2 O4 O4 98.5(10) . 1_655
O1 O4 O4 145.8(13) 4 1_655
O1 O4 O4 38.9(14) 4_655 1_655
O7 O4 O4 143.4(11) 2_556 1_655
Ga1 O4 O4 119.3(7) . 1_655
Ta O4 O4 119.3(7) . 1_655
O1 O4 O4 109.8(10) . 1_655
Ga2 O4 O4 77.0(9) 4_645 1_655
O3 O4 O4 150.9(10) 2_556 1_655
La1 O4 O4 23.7(11) 4_645 1_655
Ga4 O4 O4 82.2(6) 3_544 1_655
O5 O4 O4 100.7(12) 3_544 1_655
O5 O4 O4 63.3(8) 2_646 1_655
La2 O4 O4 41.8(8) 1_655 1_655
O6 O4 O4 56.8(9) 4_645 1_655
Ga4 O4 O4 160.0(7) 4_545 1_655
Ga4 O4 O4 81.3(7) . 1_655
O4 O4 O4 76.4(10) 2_655 1_655
La1 O4 O4 115.4(6) . 1_655
O2 O4 O4 63.4(9) 4_645 1_655
Ga3 O4 O4 82.4(6) 1_655 1_655
La1 O4 O4 115.5(6) 1_545 1_655
O5 O4 O4 130.9(7) 2_546 1_655
O5 O4 O4 97.2(8) 1_544 1_655
Ga2 O4 O4 158.9(7) 1_455 1_655
Ta O4 O4 47.3(6) 1_655 1_655
Ga1 O4 O4 47.3(6) 1_655 1_655
O6 O4 O4 132.7(7) 4_545 1_655
O2 O4 O4 70.3(7) 2_655 1_655
O1 O4 O4 101.8(6) 3_554 1_655
Ga3 O4 O4 82.8(5) 1_645 1_655
Ga2 O4 O4 82.1(5) 2_655 1_655
O6 O4 O4 66.5(6) 2_645 1_655
O2 O4 O4 134.8(8) 4_545 1_655
Ga3 O4 O4 82.1(6) 3_645 1_655
O4 O4 O4 180.00(3) 1_455 1_655
Ga4 O4 O4 78(2) 4_645 2
Ga2 O4 O4 94(2) . 2
La1 O4 O4 88.9(14) 4_545 2
O6 O4 O4 62.9(14) 1_545 2
O7 O4 O4 29.1(12) 1_554 2
O7 O4 O4 77.3(19) 2_656 2
La2 O4 O4 21.0(10) . 2
O3 O4 O4 107.8(14) 3_554 2
O3 O4 O4 125.3(18) 2_656 2
O2 O4 O4 65.5(13) . 2
O1 O4 O4 56.5(12) 4 2
O1 O4 O4 114(2) 4_655 2
O7 O4 O4 21.6(9) 2_556 2
Ga1 O4 O4 35.7(9) . 2
Ta O4 O4 35.7(9) . 2
O1 O4 O4 108.6(13) . 2
Ga2 O4 O4 131.5(10) 4_645 2
O3 O4 O4 65.9(10) 2_556 2
La1 O4 O4 151(2) 4_645 2
Ga4 O4 O4 47.8(9) 3_544 2
O5 O4 O4 131.3(18) 3_544 2
O5 O4 O4 89.8(13) 2_646 2
La2 O4 O4 88.2(14) 1_655 2
O6 O4 O4 154.7(10) 4_645 2
Ga4 O4 O4 43.6(6) 4_545 2
Ga4 O4 O4 131.3(9) . 2
O4 O4 O4 50.7(11) 2_655 2
La1 O4 O4 80.2(7) . 2
O2 O4 O4 160.3(13) 4_645 2
Ga3 O4 O4 69.2(9) 1_655 2
La1 O4 O4 80.2(7) 1_545 2
O5 O4 O4 51.2(9) 2_546 2
O5 O4 O4 49.2(10) 1_544 2
Ga2 O4 O4 53.3(7) 1_455 2
Ta O4 O4 88.4(13) 1_655 2
Ga1 O4 O4 88.4(13) 1_655 2
O6 O4 O4 95.5(11) 4_545 2
O2 O4 O4 66.8(11) 2_655 2
O1 O4 O4 31.5(7) 3_554 2
Ga3 O4 O4 70.4(9) 1_645 2
Ga2 O4 O4 48.6(8) 2_655 2
O6 O4 O4 66.6(11) 2_645 2
O2 O4 O4 96.2(12) 4_545 2
Ga3 O4 O4 150.8(15) 3_645 2
O4 O4 O4 52.9(10) 1_455 2
O4 O4 O4 127.1(10) 1_655 2
Ga4 O4 O2 33.6(15) 4_645 1_545
Ga2 O4 O2 156(3) . 1_545
La1 O4 O2 94.3(16) 4_545 1_545
O6 O4 O2 15.1(9) 1_545 1_545
O7 O4 O2 59.2(15) 1_554 1_545
O7 O4 O2 67.0(16) 2_656 1_545
La2 O4 O2 96.6(13) . 1_545
O3 O4 O2 158(2) 3_554 1_545
O3 O4 O2 54.3(12) 2_656 1_545
O2 O4 O2 139(2) . 1_545
O1 O4 O2 116.8(15) 4 1_545
O1 O4 O2 130.8(17) 4_655 1_545
O7 O4 O2 66.0(12) 2_556 1_545
Ga1 O4 O2 40.2(7) . 1_545
Ta O4 O2 40.2(7) . 1_545
O1 O4 O2 58.6(15) . 1_545
Ga2 O4 O2 59.3(11) 4_645 1_545
O3 O4 O2 60.8(9) 2_556 1_545
La1 O4 O2 100.4(12) 4_645 1_545
Ga4 O4 O2 59.4(9) 3_544 1_545
O5 O4 O2 112.9(19) 3_544 1_545
O5 O4 O2 32.8(8) 2_646 1_545
La2 O4 O2 101.4(12) 1_655 1_545
O6 O4 O2 129.5(15) 4_645 1_545
Ga4 O4 O2 66.4(8) 4_545 1_545
Ga4 O4 O2 148.0(17) . 1_545
O4 O4 O2 77.5(9) 2_655 1_545
La1 O4 O2 148.8(11) . 1_545
O2 O4 O2 87.3(15) 4_645 1_545
Ga3 O4 O2 132.8(15) 1_655 1_545
La1 O4 O2 28.8(6) 1_545 1_545
O5 O4 O2 36.6(7) 2_546 1_545
O5 O4 O2 32.6(8) 1_544 1_545
Ga2 O4 O2 104.6(10) 1_455 1_545
Ta O4 O2 56.7(7) 1_655 1_545
Ga1 O4 O2 56.7(7) 1_655 1_545
O6 O4 O2 117.2(13) 4_545 1_545
O2 O4 O2 113.5(12) 2_655 1_545
O1 O4 O2 95.5(13) 3_554 1_545
Ga3 O4 O2 21.0(5) 1_645 1_545
Ga2 O4 O2 96.2(11) 2_655 1_545
O6 O4 O2 53.4(8) 2_645 1_545
O2 O4 O2 82.5(12) 4_545 1_545
Ga3 O4 O2 102.7(13) 3_645 1_545
O4 O4 O2 84.9(6) 1_455 1_545
O4 O4 O2 95.1(6) 1_655 1_545
O4 O4 O2 75.7(8) 2 1_545
Ga4 O4 O2 104(2) 4_645 2
Ga2 O4 O2 67.3(17) . 2
La1 O4 O2 84.9(14) 4_545 2
O6 O4 O2 92.3(16) 1_545 2
O7 O4 O2 53.6(15) 1_554 2
O7 O4 O2 90.6(19) 2_656 2
La2 O4 O2 9.6(7) . 2
O3 O4 O2 79.3(17) 3_554 2
O3 O4 O2 152(2) 2_656 2
O2 O4 O2 37.3(11) . 2
O1 O4 O2 37.1(13) 4 2
O1 O4 O2 95.3(19) 4_655 2
O7 O4 O2 43.6(12) 2_556 2
Ga1 O4 O2 65.5(10) . 2
Ta O4 O2 65.5(10) . 2
O1 O4 O2 124.3(13) . 2
Ga2 O4 O2 155.9(14) 4_645 2
O3 O4 O2 79.6(10) 2_556 2
La1 O4 O2 142.1(16) 4_645 2
Ga4 O4 O2 67.3(10) 3_544 2
O5 O4 O2 115.7(16) 3_544 2
O5 O4 O2 116.4(15) 2_646 2
La2 O4 O2 84.1(11) 1_655 2
O6 O4 O2 124.9(14) 4_645 2
Ga4 O4 O2 57.8(8) 4_545 2
Ga4 O4 O2 102.2(12) . 2
O4 O4 O2 60.3(10) 2_655 2
La1 O4 O2 51.7(8) . 2
O2 O4 O2 162.6(17) 4_645 2
Ga3 O4 O2 46.6(7) 1_655 2
La1 O4 O2 105.5(10) 1_545 2
O5 O4 O2 77.2(11) 2_546 2
O5 O4 O2 78.0(12) 1_544 2
Ga2 O4 O2 41.9(6) 1_455 2
Ta O4 O2 106.3(12) 1_655 2
Ga1 O4 O2 106.3(12) 1_655 2
O6 O4 O2 80.3(9) 4_545 2
O2 O4 O2 55.0(8) 2_655 2
O1 O4 O2 27.8(6) 3_554 2
Ga3 O4 O2 99.0(11) 1_645 2
Ga2 O4 O2 46.3(7) 2_655 2
O6 O4 O2 86.3(11) 2_645 2
O2 O4 O2 98.3(9) 4_545 2
Ga3 O4 O2 137.6(12) 3_645 2
O4 O4 O2 54.7(7) 1_455 2
O4 O4 O2 125.3(7) 1_655 2
O4 O4 O2 30.0(7) 2 2
O2 O4 O2 105.6(10) 1_545 2
Ga4 O4 O4 142(3) 4_645 4_655
Ga2 O4 O4 30.9(7) . 4_655
La1 O4 O4 88(2) 4_545 4_655
O6 O4 O4 174(3) 1_545 4_655
O7 O4 O4 133(3) 1_554 4_655
O7 O4 O4 112(2) 2_656 4_655
La2 O4 O4 98.2(14) . 4_655
O3 O4 O4 25.1(7) 3_554 4_655
O3 O4 O4 111(2) 2_656 4_655
O2 O4 O4 54.6(10) . 4_655
O1 O4 O4 76.1(14) 4 4_655
O1 O4 O4 43.9(13) 4_655 4_655
O7 O4 O4 128.6(18) 2_556 4_655
Ga1 O4 O4 154.8(19) . 4_655
Ta O4 O4 154.8(19) . 4_655
O1 O4 O4 114(3) . 4_655
Ga2 O4 O4 107(2) 4_645 4_655
O3 O4 O4 125.1(19) 2_556 4_655
La1 O4 O4 65.7(14) 4_645 4_655
Ga4 O4 O4 128(2) 3_544 4_655
O5 O4 O4 60.0(16) 3_544 4_655
O5 O4 O4 137.8(16) 2_646 4_655
La2 O4 O4 78.2(14) 1_655 4_655
O6 O4 O4 35.6(12) 4_645 4_655
Ga4 O4 O4 125.1(15) 4_545 4_655
Ga4 O4 O4 21.7(9) . 4_655
O4 O4 O4 109.6(16) 2_655 4_655
La1 O4 O4 44.5(6) . 4_655
O2 O4 O4 78.4(19) 4_645 4_655
Ga3 O4 O4 57.7(9) 1_655 4_655
La1 O4 O4 148(2) 1_545 4_655
O5 O4 O4 154.5(16) 2_546 4_655
O5 O4 O4 157(2) 1_544 4_655
Ga2 O4 O4 87.4(11) 1_455 4_655
Ta O4 O4 118.2(17) 1_655 4_655
Ga1 O4 O4 118.2(17) 1_655 4_655
O6 O4 O4 66.1(13) 4_545 4_655
O2 O4 O4 73.7(14) 2_655 4_655
O1 O4 O4 97.1(16) 3_554 4_655
Ga3 O4 O4 156.6(18) 1_645 4_655
Ga2 O4 O4 93.1(15) 2_655 4_655
O6 O4 O4 128.0(18) 2_645 4_655
O2 O4 O4 97.0(18) 4_545 4_655
Ga3 O4 O4 65.7(16) 3_645 4_655
O4 O4 O4 105.4(11) 1_455 4_655
O4 O4 O4 74.6(11) 1_655 4_655
O4 O4 O4 119.2(13) 2 4_655
O2 O4 O4 165.0(19) 1_545 4_655
O2 O4 O4 89.3(12) 2 4_655
Ga4 O4 O4 57.3(13) 4_645 4_645
Ga2 O4 O4 144(3) . 4_645
La1 O4 O4 89(2) 4_545 4_645
O6 O4 O4 56.3(8) 1_545 4_645
O7 O4 O4 101.6(18) 1_554 4_645
O7 O4 O4 84.3(19) 2_656 4_645
La2 O4 O4 140.1(18) . 4_645
O3 O4 O4 125(3) 3_554 4_645
O3 O4 O4 26.0(9) 2_656 4_645
O2 O4 O4 173(2) . 4_645
O1 O4 O4 137(2) 4 4_645
O1 O4 O4 112(2) 4_655 4_645
O7 O4 O4 105.2(15) 2_556 4_645
Ga1 O4 O4 83.5(10) . 4_645
Ta O4 O4 83.5(10) . 4_645
O1 O4 O4 39.9(12) . 4_645
Ga2 O4 O4 17.2(10) 4_645 4_645
O3 O4 O4 76.6(13) 2_556 4_645
La1 O4 O4 66.0(15) 4_645 4_645
Ga4 O4 O4 95.1(14) 3_544 4_645
O5 O4 O4 79(2) 3_544 4_645
O5 O4 O4 45.7(12) 2_646 4_645
La2 O4 O4 107.5(16) 1_655 4_645
O6 O4 O4 86(2) 4_645 4_645
Ga4 O4 O4 95.0(12) 4_545 4_645
Ga4 O4 O4 105(2) . 4_645
O4 O4 O4 109.6(15) 2_655 4_645
La1 O4 O4 148(2) . 4_645
O2 O4 O4 43.4(16) 4_645 4_645
Ga3 O4 O4 155.6(18) 1_655 4_645
La1 O4 O4 44.5(6) 1_545 4_645
O5 O4 O4 71.6(10) 2_546 4_645
O5 O4 O4 74.9(11) 1_544 4_645
Ga2 O4 O4 125.3(16) 1_455 4_645
Ta O4 O4 67.3(11) 1_655 4_645
Ga1 O4 O4 67.3(11) 1_655 4_645
O6 O4 O4 104(2) 4_545 4_645
O2 O4 O4 135.7(18) 2_655 4_645
O1 O4 O4 137.2(19) 3_554 4_645
Ga3 O4 O4 55.8(9) 1_645 4_645
Ga2 O4 O4 129.6(18) 2_655 4_645
O6 O4 O4 80.0(12) 2_645 4_645
O2 O4 O4 72.9(16) 4_545 4_645
Ga3 O4 O4 61.8(17) 3_645 4_645
O4 O4 O4 105.4(11) 1_455 4_645
O4 O4 O4 74.6(11) 1_655 4_645
O4 O4 O4 119.2(13) 2 4_645
O2 O4 O4 44.0(9) 1_545 4_645
O2 O4 O4 148.4(16) 2 4_645
O4 O4 O4 122(3) 4_655 4_645
Ga4 O4 Ga2 101(2) 4_645 4_545
Ga2 O4 Ga2 133(2) . 4_545
La1 O4 Ga2 27.3(9) 4_545 4_545
O6 O4 Ga2 59.0(11) 1_545 4_545
O7 O4 Ga2 94.9(14) 1_554 4_545
O7 O4 Ga2 132.4(18) 2_656 4_545
La2 O4 Ga2 89.3(9) . 4_545
O3 O4 Ga2 92.1(16) 3_554 4_545
O3 O4 Ga2 97.6(16) 2_656 4_545
O2 O4 Ga2 115.1(13) . 4_545
O1 O4 Ga2 65.9(11) 4 4_545
O1 O4 Ga2 158(2) 4_655 4_545
O7 O4 Ga2 58.5(10) 2_556 4_545
Ga1 O4 Ga2 66.9(7) . 4_545
Ta O4 Ga2 66.9(7) . 4_545
O1 O4 Ga2 34.8(7) . 4_545
Ga2 O4 Ga2 67.5(10) 4_645 4_545
O3 O4 Ga2 14.6(6) 2_556 4_545
La1 O4 Ga2 126.0(17) 4_645 4_545
Ga4 O4 Ga2 110.7(11) 3_544 4_545
O5 O4 Ga2 62.9(12) 3_544 4_545
O5 O4 Ga2 98.6(13) 2_646 4_545
La2 O4 Ga2 165.1(14) 1_655 4_545
O6 O4 Ga2 110.2(15) 4_645 4_545
Ga4 O4 Ga2 36.3(4) 4_545 4_545
Ga4 O4 Ga2 97.6(12) . 4_545
O4 O4 Ga2 125.0(13) 2_655 4_545
La1 O4 Ga2 89.4(8) . 4_545
O2 O4 Ga2 84.6(13) 4_645 4_545
Ga3 O4 Ga2 132.4(11) 1_655 4_545
La1 O4 Ga2 39.1(4) 1_545 4_545
O5 O4 Ga2 44.3(7) 2_546 4_545
O5 O4 Ga2 83.9(10) 1_544 4_545
Ga2 O4 Ga2 53.8(5) 1_455 4_545
Ta O4 Ga2 123.9(12) 1_655 4_545
Ga1 O4 Ga2 123.9(12) 1_655 4_545
O6 O4 Ga2 50.1(7) 4_545 4_545
O2 O4 Ga2 144.3(12) 2_655 4_545
O1 O4 Ga2 110.0(9) 3_554 4_545
Ga3 O4 Ga2 86.7(9) 1_645 4_545
Ga2 O4 Ga2 128.4(11) 2_655 4_545
O6 O4 Ga2 116.5(10) 2_645 4_545
O2 O4 Ga2 20.1(6) 4_545 4_545
Ga3 O4 Ga2 73.0(9) 3_645 4_545
O4 O4 Ga2 35.5(6) 1_455 4_545
O4 O4 Ga2 144.5(6) 1_655 4_545
O4 O4 Ga2 79.8(8) 2 4_545
O2 O4 Ga2 67.2(8) 1_545 4_545
O2 O4 Ga2 89.7(8) 2 4_545
O4 O4 Ga2 115.3(18) 4_655 4_545
O4 O4 Ga2 71.6(12) 4_645 4_545
Ga4 O4 La1 115(2) 4_645 1_655
Ga2 O4 La1 24.8(11) . 1_655
La1 O4 La1 115.7(18) 4_545 1_655
O6 O4 La1 158.1(17) 1_545 1_655
O7 O4 La1 116(2) 1_554 1_655
O7 O4 La1 85.0(16) 2_656 1_655
La2 O4 La1 97.8(14) . 1_655
O3 O4 La1 51.7(12) 3_554 1_655
O3 O4 La1 98.4(14) 2_656 1_655
O2 O4 La1 54.7(11) . 1_655
O1 O4 La1 94.2(15) 4 1_655
O1 O4 La1 16.6(10) 4_655 1_655
O7 O4 La1 135.1(17) 2_556 1_655
Ga1 O4 La1 145.1(17) . 1_655
Ta O4 La1 145.1(17) . 1_655
O1 O4 La1 132.2(19) . 1_655
Ga2 O4 La1 111.1(13) 4_645 1_655
O3 O4 La1 152.0(14) 2_556 1_655
La1 O4 La1 53.1(7) 4_645 1_655
Ga4 O4 La1 104.2(12) 3_544 1_655
O5 O4 La1 83.1(13) 3_544 1_655
O5 O4 La1 114.0(10) 2_646 1_655
La2 O4 La1 51.4(6) 1_655 1_655
O6 O4 La1 42.2(6) 4_645 1_655
Ga4 O4 La1 144.4(13) 4_545 1_655
Ga4 O4 La1 45.7(6) . 1_655
O4 O4 La1 87.2(9) 2_655 1_655
La1 O4 La1 63.1(7) . 1_655
O2 O4 La1 83.1(12) 4_645 1_655
Ga3 O4 La1 47.3(6) 1_655 1_655
La1 O4 La1 162.9(14) 1_545 1_655
O5 O4 La1 167.6(16) 2_546 1_655
O5 O4 La1 132.8(15) 1_544 1_655
Ga2 O4 La1 107.1(11) 1_455 1_655
Ta O4 La1 91.5(9) 1_655 1_655
Ga1 O4 La1 91.5(9) 1_655 1_655
O6 O4 La1 93.3(10) 4_545 1_655
O2 O4 La1 54.5(8) 2_655 1_655
O1 O4 La1 86.6(11) 3_554 1_655
Ga3 O4 La1 129.8(11) 1_645 1_655
Ga2 O4 La1 75.2(8) 2_655 1_655
O6 O4 La1 100.9(10) 2_645 1_655
O2 O4 La1 123.6(13) 4_545 1_655
Ga3 O4 La1 81.2(9) 3_645 1_655
O4 O4 La1 127.7(6) 1_455 1_655
O4 O4 La1 52.3(6) 1_655 1_655
O4 O4 La1 116.5(10) 2 1_655
O2 O4 La1 146.7(11) 1_545 1_655
O2 O4 La1 91.6(10) 2 1_655
O4 O4 La1 27.4(8) 4_655 1_655
O4 O4 La1 118.9(16) 4_645 1_655
Ga2 O4 La1 142.6(12) 4_545 1_655
Ga4 O4 La1 40.0(15) 4_645 1_645
Ga2 O4 La1 126.0(18) . 1_645
La1 O4 La1 116(2) 4_545 1_645
O6 O4 La1 62.3(12) 1_545 1_645
O7 O4 La1 90.2(16) 1_554 1_645
O7 O4 La1 58.7(15) 2_656 1_645
La2 O4 La1 134.3(15) . 1_645
O3 O4 La1 135.6(19) 3_554 1_645
O3 O4 La1 8.8(11) 2_656 1_645
O2 O4 La1 146.8(17) . 1_645
O1 O4 La1 162.0(18) 4 1_645
O1 O4 La1 91.1(14) 4_655 1_645
O7 O4 La1 112.6(15) 2_556 1_645
Ga1 O4 La1 84.6(10) . 1_645
Ta O4 La1 84.6(10) . 1_645
O1 O4 La1 67.4(13) . 1_645
Ga2 O4 La1 40.2(6) 4_645 1_645
O3 O4 La1 99.1(13) 2_556 1_645
La1 O4 La1 53.2(7) 4_645 1_645
Ga4 O4 La1 76.9(8) 3_544 1_645
O5 O4 La1 99.0(18) 3_544 1_645
O5 O4 La1 27.4(8) 2_646 1_645
La2 O4 La1 80.1(8) 1_655 1_645
O6 O4 La1 85.9(11) 4_645 1_645
Ga4 O4 La1 112.1(11) 4_545 1_645
Ga4 O4 La1 112.0(12) . 1_645
O4 O4 La1 87.2(9) 2_655 1_645
La1 O4 La1 162.7(13) . 1_645
O2 O4 La1 53.6(9) 4_645 1_645
Ga3 O4 La1 128.5(11) 1_655 1_645
La1 O4 La1 63.3(7) 1_545 1_645
O5 O4 La1 83.2(10) 2_546 1_645
O5 O4 La1 67.4(9) 1_544 1_645
Ga2 O4 La1 148.9(12) 1_455 1_645
Ta O4 La1 41.6(4) 1_655 1_645
Ga1 O4 La1 41.6(4) 1_655 1_645
O6 O4 La1 130.4(15) 4_545 1_645
O2 O4 La1 108.3(10) 2_655 1_645
O1 O4 La1 119.3(13) 3_554 1_645
Ga3 O4 La1 46.3(5) 1_645 1_645
Ga2 O4 La1 105.6(10) 2_655 1_645
O6 O4 La1 58.6(6) 2_645 1_645
O2 O4 La1 100.3(12) 4_545 1_645
Ga3 O4 La1 78.0(9) 3_645 1_645
O4 O4 La1 127.8(6) 1_455 1_645
O4 O4 La1 52.2(6) 1_655 1_645
O4 O4 La1 116.6(10) 2 1_645
O2 O4 La1 47.2(6) 1_545 1_645
O2 O4 La1 143.7(13) 2 1_645
O4 O4 La1 118.7(16) 4_655 1_645
O4 O4 La1 27.5(8) 4_645 1_645
Ga2 O4 La1 97.3(10) 4_545 1_645
La1 O4 La1 103.4(8) 1_655 1_645
Ga4 O4 Ga1 149(3) 4_645 3
Ga2 O4 Ga1 83.2(19) . 3
La1 O4 Ga1 35.8(10) 4_545 3
O6 O4 Ga1 117.4(18) 1_545 3
O7 O4 Ga1 145.7(14) 1_554 3
O7 O4 Ga1 164(2) 2_656 3
La2 O4 Ga1 108.1(12) . 3
O3 O4 Ga1 38.6(13) 3_554 3
O3 O4 Ga1 107(2) 2_656 3
O2 O4 Ga1 89.5(14) . 3
O1 O4 Ga1 63.8(13) 4 3
O1 O4 Ga1 98.3(16) 4_655 3
O7 O4 Ga1 104.6(13) 2_556 3
Ga1 O4 Ga1 125.0(12) . 3
Ta O4 Ga1 125.0(12) . 3
O1 O4 Ga1 62.3(14) . 3
Ga2 O4 Ga1 75.9(13) 4_645 3
O3 O4 Ga1 72.6(10) 2_556 3
La1 O4 Ga1 89.7(12) 4_645 3
Ga4 O4 Ga1 165.4(12) 3_544 3
O5 O4 Ga1 15.5(9) 3_544 3
O5 O4 Ga1 138.1(17) 2_646 3
La2 O4 Ga1 134.4(13) 1_655 3
O6 O4 Ga1 55.9(9) 4_645 3
Ga4 O4 Ga1 85.1(8) 4_545 3
Ga4 O4 Ga1 37.6(6) . 3
O4 O4 Ga1 158.0(10) 2_655 3
La1 O4 Ga1 55.9(6) . 3
O2 O4 Ga1 62.8(11) 4_645 3
Ga3 O4 Ga1 103.8(10) 1_655 3
La1 O4 Ga1 92.7(11) 1_545 3
O5 O4 Ga1 104.1(11) 2_546 3
O5 O4 Ga1 143.9(13) 1_544 3
Ga2 O4 Ga1 64.4(6) 1_455 3
Ta O4 Ga1 153.2(13) 1_655 3
Ga1 O4 Ga1 153.2(13) 1_655 3
O6 O4 Ga1 22.1(5) 4_545 3
O2 O4 Ga1 125.4(12) 2_655 3
O1 O4 Ga1 126.4(13) 3_554 3
Ga3 O4 Ga1 141.2(14) 1_645 3
Ga2 O4 Ga1 138.0(12) 2_655 3
O6 O4 Ga1 172.4(14) 2_645 3
O2 O4 Ga1 40.6(8) 4_545 3
Ga3 O4 Ga1 37.7(5) 3_645 3
O4 O4 Ga1 68.0(5) 1_455 3
O4 O4 Ga1 112.0(5) 1_655 3
O4 O4 Ga1 117.6(11) 2 3
O2 O4 Ga1 120.3(13) 1_545 3
O2 O4 Ga1 100.1(9) 2 3
O4 O4 Ga1 56.6(13) 4_655 3
O4 O4 Ga1 92(2) 4_645 3
Ga2 O4 Ga1 60.0(7) 4_545 3
La1 O4 Ga1 83.0(8) 1_655 3
La1 O4 Ga1 114.2(13) 1_645 3
Ga4 O4 Ta 149(3) 4_645 3
Ga2 O4 Ta 83.2(19) . 3
La1 O4 Ta 35.8(10) 4_545 3
O6 O4 Ta 117.4(18) 1_545 3
O7 O4 Ta 145.7(14) 1_554 3
O7 O4 Ta 164(2) 2_656 3
La2 O4 Ta 108.1(12) . 3
O3 O4 Ta 38.6(13) 3_554 3
O3 O4 Ta 107(2) 2_656 3
O2 O4 Ta 89.5(14) . 3
O1 O4 Ta 63.8(13) 4 3
O1 O4 Ta 98.3(16) 4_655 3
O7 O4 Ta 104.6(13) 2_556 3
Ga1 O4 Ta 125.0(12) . 3
Ta O4 Ta 125.0(12) . 3
O1 O4 Ta 62.3(14) . 3
Ga2 O4 Ta 75.9(13) 4_645 3
O3 O4 Ta 72.6(10) 2_556 3
La1 O4 Ta 89.7(12) 4_645 3
Ga4 O4 Ta 165.4(12) 3_544 3
O5 O4 Ta 15.5(9) 3_544 3
O5 O4 Ta 138.1(17) 2_646 3
La2 O4 Ta 134.4(13) 1_655 3
O6 O4 Ta 55.9(9) 4_645 3
Ga4 O4 Ta 85.1(8) 4_545 3
Ga4 O4 Ta 37.6(6) . 3
O4 O4 Ta 158.0(10) 2_655 3
La1 O4 Ta 55.9(6) . 3
O2 O4 Ta 62.8(11) 4_645 3
Ga3 O4 Ta 103.8(10) 1_655 3
La1 O4 Ta 92.7(11) 1_545 3
O5 O4 Ta 104.1(11) 2_546 3
O5 O4 Ta 143.9(13) 1_544 3
Ga2 O4 Ta 64.4(6) 1_455 3
Ta O4 Ta 153.2(13) 1_655 3
Ga1 O4 Ta 153.2(13) 1_655 3
O6 O4 Ta 22.1(5) 4_545 3
O2 O4 Ta 125.4(12) 2_655 3
O1 O4 Ta 126.4(13) 3_554 3
Ga3 O4 Ta 141.2(14) 1_645 3
Ga2 O4 Ta 138.0(12) 2_655 3
O6 O4 Ta 172.4(14) 2_645 3
O2 O4 Ta 40.6(8) 4_545 3
Ga3 O4 Ta 37.7(5) 3_645 3
O4 O4 Ta 68.0(5) 1_455 3
O4 O4 Ta 112.0(5) 1_655 3
O4 O4 Ta 117.6(11) 2 3
O2 O4 Ta 120.3(13) 1_545 3
O2 O4 Ta 100.1(9) 2 3
O4 O4 Ta 56.6(13) 4_655 3
O4 O4 Ta 92(2) 4_645 3
Ga2 O4 Ta 60.0(7) 4_545 3
La1 O4 Ta 83.0(8) 1_655 3
La1 O4 Ta 114.2(13) 1_645 3
Ga1 O4 Ta 0.00(15) 3 3
Ga4 O4 O1 66.9(19) 4_645 1_655
Ga2 O4 O1 103.9(18) . 1_655
La1 O4 O1 113(2) 4_545 1_655
O6 O4 O1 90.6(17) 1_545 1_655
O7 O4 O1 116.3(18) 1_554 1_655
O7 O4 O1 72.8(18) 2_656 1_655
La2 O4 O1 156.6(17) . 1_655
O3 O4 O1 106.4(18) 3_554 1_655
O3 O4 O1 21.6(12) 2_656 1_655
O2 O4 O1 132.9(16) . 1_655
O1 O4 O1 158.2(19) 4 1_655
O1 O4 O1 71.5(12) 4_655 1_655
O7 O4 O1 141.8(18) 2_556 1_655
Ga1 O4 O1 114.3(15) . 1_655
Ta O4 O1 114.3(15) . 1_655
O1 O4 O1 72.5(14) . 1_655
Ga2 O4 O1 39.8(8) 4_645 1_655
O3 O4 O1 115.6(16) 2_556 1_655
La1 O4 O1 26.2(7) 4_645 1_655
Ga4 O4 O1 99.2(12) 3_544 1_655
O5 O4 O1 79.3(16) 3_544 1_655
O5 O4 O1 55.3(11) 2_646 1_655
La2 O4 O1 77.7(9) 1_655 1_655
O6 O4 O1 56.3(10) 4_645 1_655
Ga4 O4 O1 135.3(15) 4_545 1_655
Ga4 O4 O1 82.8(11) . 1_655
O4 O4 O1 102.9(13) 2_655 1_655
La1 O4 O1 133.1(14) . 1_655
O2 O4 O1 32.6(9) 4_645 1_655
Ga3 O4 O1 119.0(11) 1_655 1_655
La1 O4 O1 84.6(12) 1_545 1_655
O5 O4 O1 109.9(14) 2_546 1_655
O5 O4 O1 96.4(14) 1_544 1_655
Ga2 O4 O1 156.4(16) 1_455 1_655
Ta O4 O1 58.6(9) 1_655 1_655
Ga1 O4 O1 58.6(9) 1_655 1_655
O6 O4 O1 115.8(15) 4_545 1_655
O2 O4 O1 107.2(11) 2_655 1_655
O1 O4 O1 134.5(14) 3_554 1_655
Ga3 O4 O1 75.6(11) 1_645 1_655
Ga2 O4 O1 115.5(11) 2_655 1_655
O6 O4 O1 79.9(11) 2_645 1_655
O2 O4 O1 100.1(13) 4_545 1_655
Ga3 O4 O1 57.1(9) 3_645 1_655
O4 O4 O1 142.7(8) 1_455 1_655
O4 O4 O1 37.3(8) 1_655 1_655
O4 O4 O1 144.8(14) 2 1_655
O2 O4 O1 75.8(11) 1_545 1_655
O2 O4 O1 161.6(14) 2 1_655
O4 O4 O1 89.6(16) 4_655 1_655
O4 O4 O1 40.2(12) 4_645 1_655
Ga2 O4 O1 107.3(13) 4_545 1_655
La1 O4 O1 79.2(9) 1_655 1_655
La1 O4 O1 29.6(7) 1_645 1_655
Ga1 O4 O1 94.6(12) 3 1_655
Ta O4 O1 94.6(12) 3 1_655
Ga4 O4 Ga4 75.1(17) 4_645 3_444
Ga2 O4 Ga4 109(2) . 3_444
La1 O4 Ga4 79.1(13) 4_545 3_444
O6 O4 Ga4 50.4(11) 1_545 3_444
O7 O4 Ga4 33.9(10) 1_554 3_444
O7 O4 Ga4 83.7(17) 2_656 3_444
La2 O4 Ga4 34.6(6) . 3_444
O3 O4 Ga4 113.6(15) 3_554 3_444
O3 O4 Ga4 117.9(17) 2_656 3_444
O2 O4 Ga4 79.3(14) . 3_444
O1 O4 Ga4 58.7(12) 4 3_444
O1 O4 Ga4 130(2) 4_655 3_444
O7 O4 Ga4 7.8(8) 2_556 3_444
Ga1 O4 Ga4 25.2(4) . 3_444
Ta O4 Ga4 25.2(4) . 3_444
O1 O4 Ga4 92.9(13) . 3_444
Ga2 O4 Ga4 116.7(13) 4_645 3_444
O3 O4 Ga4 51.3(8) 2_556 3_444
La1 O4 Ga4 157.5(15) 4_645 3_444
Ga4 O4 Ga4 53.6(6) 3_544 3_444
O5 O4 Ga4 123.2(15) 3_544 3_444
O5 O4 Ga4 85.3(11) 2_646 3_444
La2 O4 Ga4 101.3(12) 1_655 3_444
O6 O4 Ga4 163.9(13) 4_645 3_444
Ga4 O4 Ga4 30.2(4) 4_545 3_444
Ga4 O4 Ga4 136.6(11) . 3_444
O4 O4 Ga4 61.5(10) 2_655 3_444
La1 O4 Ga4 87.5(8) . 3_444
O2 O4 Ga4 144.8(15) 4_645 3_444
Ga3 O4 Ga4 84.7(9) 1_655 3_444
La1 O4 Ga4 64.9(6) 1_545 3_444
O5 O4 Ga4 35.9(8) 2_546 3_444
O5 O4 Ga4 44.4(7) 1_544 3_444
Ga2 O4 Ga4 51.5(5) 1_455 3_444
Ta O4 Ga4 91.0(9) 1_655 3_444
Ga1 O4 Ga4 91.0(9) 1_655 3_444
O6 O4 Ga4 90.7(8) 4_545 3_444
O2 O4 Ga4 82.2(10) 2_655 3_444
O1 O4 Ga4 47.1(6) 3_554 3_444
Ga3 O4 Ga4 64.4(6) 1_645 3_444
Ga2 O4 Ga4 63.2(7) 2_655 3_444
O6 O4 Ga4 70.1(7) 2_645 3_444
O2 O4 Ga4 83.6(9) 4_545 3_444
Ga3 O4 Ga4 138.5(11) 3_645 3_444
O4 O4 Ga4 44.2(5) 1_455 3_444
O4 O4 Ga4 135.8(5) 1_655 3_444
O4 O4 Ga4 15.8(5) 2 3_444
O2 O4 Ga4 64.6(7) 1_545 3_444
O2 O4 Ga4 42.2(6) 2 3_444
O4 O4 Ga4 130.4(14) 4_655 3_444
O4 O4 Ga4 106.2(12) 4_645 3_444
Ga2 O4 Ga4 65.7(6) 4_545 3_444
La1 O4 Ga4 132.0(12) 1_655 3_444
La1 O4 Ga4 109.8(9) 1_645 3_444
Ga1 O4 Ga4 112.2(8) 3 3_444
Ta O4 Ga4 112.2(8) 3 3_444
O1 O4 Ga4 139.4(14) 1_655 3_444
Ga4 O4 O2 88.1(19) 4_645 1_655
Ga2 O4 O2 41.4(13) . 1_655
La1 O4 O2 143.3(19) 4_545 1_655
O6 O4 O2 130.6(17) 1_545 1_655
O7 O4 O2 95.3(18) 1_554 1_655
O7 O4 O2 57.5(15) 2_656 1_655
La2 O4 O2 96.0(14) . 1_655
O3 O4 O2 79.0(16) 3_554 1_655
O3 O4 O2 83.7(14) 2_656 1_655
O2 O4 O2 63.9(11) . 1_655
O1 O4 O2 112.2(18) 4 1_655
O1 O4 O2 11.3(13) 4_655 1_655
O7 O4 O2 129.6(17) 2_556 1_655
Ga1 O4 O2 123.6(15) . 1_655
Ta O4 O2 123.6(15) . 1_655
O1 O4 O2 141.3(16) . 1_655
Ga2 O4 O2 109.8(12) 4_645 1_655
O3 O4 O2 173.6(16) 2_556 1_655
La1 O4 O2 48.6(8) 4_645 1_655
Ga4 O4 O2 79.8(11) 3_544 1_655
O5 O4 O2 106.7(14) 3_544 1_655
O5 O4 O2 88.6(11) 2_646 1_655
La2 O4 O2 25.4(6) 1_655 1_655
O6 O4 O2 59.8(9) 4_645 1_655
Ga4 O4 O2 150.7(15) 4_545 1_655
Ga4 O4 O2 71.9(9) . 1_655
O4 O4 O2 65.1(10) 2_655 1_655
La1 O4 O2 85.2(10) . 1_655
O2 O4 O2 89.0(11) 4_645 1_655
Ga3 O4 O2 48.4(7) 1_655 1_655
La1 O4 O2 147.5(12) 1_545 1_655
O5 O4 O2 146.2(15) 2_546 1_655
O5 O4 O2 106.5(13) 1_544 1_655
Ga2 O4 O2 125.0(13) 1_455 1_655
Ta O4 O2 64.4(8) 1_655 1_655
Ga1 O4 O2 64.4(8) 1_655 1_655
O6 O4 O2 120.8(12) 4_545 1_655
O2 O4 O2 41.6(10) 2_655 1_655
O1 O4 O2 77.0(10) 3_554 1_655
Ga3 O4 O2 102.4(10) 1_645 1_655
Ga2 O4 O2 59.8(8) 2_655 1_655
O6 O4 O2 73.7(9) 2_645 1_655
O2 O4 O2 149.3(14) 4_545 1_655
Ga3 O4 O2 97.8(10) 3_645 1_655
O4 O4 O2 145.5(7) 1_455 1_655
O4 O4 O2 34.5(7) 1_655 1_655
O4 O4 O2 108.1(14) 2 1_655
O2 O4 O2 121.0(12) 1_545 1_655
O2 O4 O2 94.0(12) 2 1_655
O4 O4 O2 55.0(12) 4_655 1_655
O4 O4 O2 109.1(15) 4_645 1_655
Ga2 O4 O2 169.5(14) 4_545 1_655
La1 O4 O2 27.6(6) 1_655 1_655
La1 O4 O2 85.6(8) 1_645 1_655
Ga1 O4 O2 109.6(11) 3 1_655
Ta O4 O2 109.6(11) 3 1_655
O1 O4 O2 70.5(8) 1_655 1_655
Ga4 O4 O2 123.0(13) 3_444 1_655
Ga4 O4 La2 100(2) 4_645 3_545
Ga2 O4 La2 132(2) . 3_545
La1 O4 La2 42.0(12) 4_545 3_545
O6 O4 La2 72.5(15) 1_545 3_545
O7 O4 La2 122.5(18) 1_554 3_545
O7 O4 La2 131(2) 2_656 3_545
La2 O4 La2 125.3(12) . 3_545
O3 O4 La2 88.5(18) 3_554 3_545
O3 O4 La2 71.2(15) 2_656 3_545
O2 O4 La2 136.5(16) . 3_545
O1 O4 La2 92.8(15) 4 3_545
O1 O4 La2 130(2) 4_655 3_545
O7 O4 La2 93.6(12) 2_556 3_545
Ga1 O4 La2 93.1(11) . 3_545
Ta O4 La2 93.1(11) . 3_545
O1 O4 La2 12.6(11) . 3_545
Ga2 O4 La2 36.2(7) 4_645 3_545
O3 O4 La2 49.4(9) 2_556 3_545
La1 O4 La2 89.8(13) 4_645 3_545
Ga4 O4 La2 130.2(12) 3_544 3_545
O5 O4 La2 42.1(12) 3_544 3_545
O5 O4 La2 90.8(14) 2_646 3_545
La2 O4 La2 151.4(12) 1_655 3_545
O6 O4 La2 80.3(12) 4_645 3_545
Ga4 O4 La2 72.2(8) 4_545 3_545
Ga4 O4 La2 80.1(11) . 3_545
O4 O4 La2 148.4(7) 2_655 3_545
La1 O4 La2 102.4(10) . 3_545
O2 O4 La2 48.3(9) 4_645 3_545
Ga3 O4 La2 153.3(12) 1_655 3_545
La1 O4 La2 46.6(6) 1_545 3_545
O5 O4 La2 69.9(10) 2_546 3_545
O5 O4 La2 101.0(11) 1_544 3_545
Ga2 O4 La2 83.9(8) 1_455 3_545
Ta O4 La2 114.8(12) 1_655 3_545
Ga1 O4 La2 114.8(12) 1_655 3_545
O6 O4 La2 56.9(8) 4_545 3_545
O2 O4 La2 175.3(13) 2_655 3_545
O1 O4 La2 146.1(10) 3_554 3_545
Ga3 O4 La2 91.5(10) 1_645 3_545
Ga2 O4 La2 162.7(11) 2_655 3_545
O6 O4 La2 122.9(11) 2_645 3_545
O2 O4 La2 26.8(6) 4_545 3_545
Ga3 O4 La2 40.9(6) 3_645 3_545
O4 O4 La2 69.9(5) 1_455 3_545
O4 O4 La2 110.1(5) 1_655 3_545
O4 O4 La2 115.2(10) 2 3_545
O2 O4 La2 71.2(9) 1_545 3_545
O2 O4 La2 124.4(9) 2 3_545
O4 O4 La2 101.8(19) 4_655 3_545
O4 O4 La2 47.8(13) 4_645 3_545
Ga2 O4 La2 36.3(4) 4_545 3_545
La1 O4 La2 121.8(12) 1_655 3_545
La1 O4 La2 74.9(9) 1_645 3_545
Ga1 O4 La2 50.0(6) 3 3_545
Ta O4 La2 50.0(6) 3 3_545
O1 O4 La2 73.8(10) 1_655 3_545
Ga4 O4 La2 100.1(8) 3_444 3_545
O2 O4 La2 136.7(12) 1_655 3_545
Ga4 O4 O4 159(3) 4_645 4
Ga2 O4 O4 64.4(10) . 4
La1 O4 O4 43.9(15) 4_545 4
O6 O4 O4 120.0(17) 1_545 4
O7 O4 O4 110.8(19) 1_554 4
O7 O4 O4 146(2) 2_656 4
La2 O4 O4 68.1(10) . 4
O3 O4 O4 32.1(8) 3_554 4
O3 O4 O4 148(3) 2_656 4
O2 O4 O4 54.4(8) . 4
O1 O4 O4 25.6(10) 4 4
O1 O4 O4 96.0(12) 4_655 4
O7 O4 O4 78.3(16) 2_556 4
Ga1 O4 O4 106.7(14) . 4
Ta O4 O4 106.7(14) . 4
O1 O4 O4 91.7(19) . 4
Ga2 O4 O4 115(2) 4_645 4
O3 O4 O4 72.4(13) 2_556 4
La1 O4 O4 117.8(16) 4_645 4
Ga4 O4 O4 126.7(17) 3_544 4
O5 O4 O4 56.5(14) 3_544 4
O5 O4 O4 165.7(12) 2_646 4
La2 O4 O4 118.8(11) 1_655 4
O6 O4 O4 80.4(12) 4_645 4
Ga4 O4 O4 69.0(11) 4_545 4
Ga4 O4 O4 53.2(7) . 4
O4 O4 O4 117.8(16) 2_655 4
La1 O4 O4 21.5(3) . 4
O2 O4 O4 103.2(19) 4_645 4
Ga3 O4 O4 72.1(6) 1_655 4
La1 O4 O4 107.3(13) 1_545 4
O5 O4 O4 98.3(12) 2_546 4
O5 O4 O4 128.0(17) 1_544 4
Ga2 O4 O4 32.8(8) 1_455 4
Ta O4 O4 162.9(18) 1_655 4
Ga1 O4 O4 162.9(18) 1_655 4
O6 O4 O4 25.4(8) 4_545 4
O2 O4 O4 94.0(10) 2_655 4
O1 O4 O4 85.5(13) 3_554 4
Ga3 O4 O4 145.9(14) 1_645 4
Ga2 O4 O4 99.2(12) 2_655 4
O6 O4 O4 145.8(18) 2_645 4
O2 O4 O4 59.2(12) 4_545 4
Ga3 O4 O4 78.2(14) 3_645 4
O4 O4 O4 49.2(8) 1_455 4
O4 O4 O4 130.8(8) 1_655 4
O4 O4 O4 82.1(11) 2 4
O2 O4 O4 133.0(12) 1_545 4
O2 O4 O4 59.5(10) 2 4
O4 O4 O4 56.3(7) 4_655 4
O4 O4 O4 130(2) 4_645 4
Ga2 O4 O4 68.5(10) 4_545 4
La1 O4 O4 80.2(5) 1_655 4
La1 O4 O4 155.0(19) 1_645 4
Ga1 O4 O4 41.0(9) 3 4
Ta O4 O4 41.0(9) 3 4
O1 O4 O4 133.0(19) 1_655 4
Ga4 O4 O4 83.7(11) 3_444 4
O2 O4 O4 105.1(8) 1_655 4
La2 O4 O4 82.2(13) 3_545 4
Ga4 O4 O4 83.7(14) 4_645 4_545
Ga2 O4 O4 151(2) . 4_545
La1 O4 O4 44.3(16) 4_545 4_545
O6 O4 O4 44.2(7) 1_545 4_545
O7 O4 O4 88.8(15) 1_554 4_545
O7 O4 O4 116.8(17) 2_656 4_545
La2 O4 O4 96.7(14) . 4_545
O3 O4 O4 109(2) 3_554 4_545
O3 O4 O4 81.7(12) 2_656 4_545
O2 O4 O4 130.7(17) . 4_545
O1 O4 O4 82.2(16) 4 4_545
O1 O4 O4 164(3) 4_655 4_545
O7 O4 O4 60.8(13) 2_556 4_545
Ga1 O4 O4 59.3(7) . 4_545
Ta O4 O4 59.3(7) . 4_545
O1 O4 O4 26.6(8) . 4_545
Ga2 O4 O4 56.2(8) 4_645 4_545
O3 O4 O4 20.6(8) 2_556 4_545
La1 O4 O4 118.1(17) 4_645 4_545
Ga4 O4 O4 100.7(12) 3_544 4_545
O5 O4 O4 71.9(18) 3_544 4_545
O5 O4 O4 80.7(9) 2_646 4_545
La2 O4 O4 151.4(14) 1_655 4_545
O6 O4 O4 115(2) 4_645 4_545
Ga4 O4 O4 42.1(8) 4_545 4_545
Ga4 O4 O4 109.7(19) . 4_545
O4 O4 O4 117.8(16) 2_655 4_545
La1 O4 O4 107.4(13) . 4_545
O2 O4 O4 79.4(15) 4_645 4_545
Ga3 O4 O4 146.0(14) 1_655 4_545
La1 O4 O4 21.4(4) 1_545 4_545
O5 O4 O4 35.7(9) 2_546 4_545
O5 O4 O4 71.7(9) 1_544 4_545
Ga2 O4 O4 69.5(11) 1_455 4_545
Ta O4 O4 106.4(8) 1_655 4_545
Ga1 O4 O4 106.4(8) 1_655 4_545
O6 O4 O4 67.1(14) 4_545 4_545
O2 O4 O4 148.4(18) 2_655 4_545
O1 O4 O4 113.5(15) 3_554 4_545
Ga3 O4 O4 70.5(5) 1_645 4_545
Ga2 O4 O4 128.2(16) 2_655 4_545
O6 O4 O4 102.0(9) 2_645 4_545
O2 O4 O4 32.9(12) 4_545 4_545
Ga3 O4 O4 75.4(15) 3_645 4_545
O4 O4 O4 49.2(8) 1_455 4_545
O4 O4 O4 130.8(8) 1_655 4_545
O4 O4 O4 82.1(11) 2 4_545
O2 O4 O4 50.1(5) 1_545 4_545
O2 O4 O4 99.8(13) 2 4_545
O4 O4 O4 130(2) 4_655 4_545
O4 O4 O4 56.3(7) 4_645 4_545
Ga2 O4 O4 18.0(8) 4_545 4_545
La1 O4 O4 155.0(19) 1_655 4_545
La1 O4 O4 80.3(6) 1_645 4_545
Ga1 O4 O4 73.2(14) 3 4_545
Ta O4 O4 73.2(14) 3 4_545
O1 O4 O4 95.0(12) 1_655 4_545
Ga4 O4 O4 66.5(10) 3_444 4_545
O2 O4 O4 165.3(13) 1_655 4_545
La2 O4 O4 34.5(9) 3_545 4_545
O4 O4 O4 86.5(14) 4 4_545
Ga4 O4 O2 123(2) 4_645 1_455
Ga2 O4 O2 77.8(16) . 1_455
La1 O4 O2 54.3(12) 4_545 1_455
O6 O4 O2 93.0(14) 1_545 1_455
O7 O4 O2 75.6(14) 1_554 1_455
O7 O4 O2 120(2) 2_656 1_455
La2 O4 O2 36.6(7) . 1_455
O3 O4 O2 65.3(13) 3_554 1_455
O3 O4 O2 160.0(18) 2_656 1_455
O2 O4 O2 51.8(8) . 1_455
O1 O4 O2 10.3(11) 4 1_455
O1 O4 O2 112.3(18) 4_655 1_455
O7 O4 O2 44.1(12) 2_556 1_455
Ga1 O4 O2 72.9(9) . 1_455
Ta O4 O2 72.9(9) . 1_455
O1 O4 O2 98.3(12) . 1_455
Ga2 O4 O2 130.8(14) 4_645 1_455
O3 O4 O2 58.7(9) 2_556 1_455
La1 O4 O2 151.2(14) 4_645 1_455
Ga4 O4 O2 93.5(11) 3_544 1_455
O5 O4 O2 87.6(14) 3_544 1_455
O5 O4 O2 133.8(13) 2_646 1_455
La2 O4 O2 113.2(13) 1_655 1_455
O6 O4 O2 115.4(12) 4_645 1_455
Ga4 O4 O2 43.1(6) 4_545 1_455
Ga4 O4 O2 88.2(10) . 1_455
O4 O4 O2 90.3(12) 2_655 1_455
La1 O4 O2 41.0(6) . 1_455
O2 O4 O2 134.2(13) 4_645 1_455
Ga3 O4 O2 68.2(8) 1_655 1_455
La1 O4 O2 93.1(9) 1_545 1_455
O5 O4 O2 71.8(9) 2_546 1_455
O5 O4 O2 92.8(12) 1_544 1_455
Ga2 O4 O2 11.3(5) 1_455 1_455
Ta O4 O2 134.3(13) 1_655 1_455
Ga1 O4 O2 134.3(13) 1_655 1_455
O6 O4 O2 51.0(7) 4_545 1_455
O2 O4 O2 83.2(11) 2_655 1_455
O1 O4 O2 58.5(8) 3_554 1_455
Ga3 O4 O2 112.7(10) 1_645 1_455
Ga2 O4 O2 77.1(9) 2_655 1_455
O6 O4 O2 112.8(12) 2_645 1_455
O2 O4 O2 68.5(9) 4_545 1_455
Ga3 O4 O2 109.7(11) 3_645 1_455
O4 O4 O2 29.7(7) 1_455 1_455
O4 O4 O2 150.3(7) 1_655 1_455
O4 O4 O2 46.6(7) 2 1_455
O2 O4 O2 108.1(10) 1_545 1_455
O2 O4 O2 30.9(8) 2 1_455
O4 O4 O2 85.5(10) 4_655 1_455
O4 O4 O2 135.2(16) 4_645 1_455
Ga2 O4 O2 64.3(7) 4_545 1_455
La1 O4 O2 101.3(10) 1_655 1_455
La1 O4 O2 155.0(11) 1_645 1_455
Ga1 O4 O2 72.5(7) 3 1_455
Ta O4 O2 72.5(7) 3 1_455
O1 O4 O2 166.8(15) 1_655 1_455
Ga4 O4 O2 48.5(6) 3_444 1_455
O2 O4 O2 115.7(13) 1_655 1_455
La2 O4 O2 95.2(9) 3_545 1_455
O4 O4 O2 35.8(9) 4 1_455
O4 O4 O2 78.9(11) 4_545 1_455
Ga4 O4 La1 66(2) 4_645 3_544
Ga2 O4 La1 88(2) . 3_544
La1 O4 La1 109.4(15) 4_545 3_544
O6 O4 La1 66.2(14) 1_545 3_544
O7 O4 La1 16.5(13) 1_554 3_544
O7 O4 La1 57.8(15) 2_656 3_544
La2 O4 La1 28.9(6) . 3_544
O3 O4 La1 115.8(18) 3_554 3_544
O3 O4 La1 114.2(18) 2_656 3_544
O2 O4 La1 64.3(14) . 3_544
O1 O4 La1 72.5(15) 4 3_544
O1 O4 La1 98.6(19) 4_655 3_544
O7 O4 La1 40.1(9) 2_556 3_544
Ga1 O4 La1 40.5(7) . 3_544
Ta O4 La1 40.5(7) . 3_544
O1 O4 La1 122.2(16) . 3_544
Ga2 O4 La1 134.3(14) 4_645 3_544
O3 O4 La1 83.9(10) 2_556 3_544
La1 O4 La1 130.3(14) 4_645 3_544
Ga4 O4 La1 30.0(4) 3_544 3_544
O5 O4 La1 150.9(16) 3_544 3_544
O5 O4 La1 78.4(12) 2_646 3_544
La2 O4 La1 68.7(9) 1_655 3_544
O6 O4 La1 147.7(14) 4_645 3_544
Ga4 O4 La1 62.8(7) 4_545 3_544
Ga4 O4 La1 136.6(13) . 3_544
O4 O4 La1 30.2(8) 2_655 3_544
La1 O4 La1 89.0(10) . 3_544
O2 O4 La1 159.2(14) 4_645 3_544
Ga3 O4 La1 61.0(7) 1_655 3_544
La1 O4 La1 89.2(9) 1_545 3_544
O5 O4 La1 62.3(10) 2_546 3_544
O5 O4 La1 43.2(8) 1_544 3_544
Ga2 O4 La1 72.0(7) 1_455 3_544
Ta O4 La1 70.7(8) 1_655 3_544
Ga1 O4 La1 70.7(8) 1_655 3_544
O6 O4 La1 114.3(10) 4_545 3_544
O2 O4 La1 51.5(8) 2_655 3_544
O1 O4 La1 20.7(6) 3_554 3_544
Ga3 O4 La1 62.8(7) 1_645 3_544
Ga2 O4 La1 31.3(4) 2_655 3_544
O6 O4 La1 49.4(6) 2_645 3_544
O2 O4 La1 116.1(10) 4_545 3_544
Ga3 O4 La1 171.1(10) 3_645 3_544
O4 O4 La1 73.4(4) 1_455 3_544
O4 O4 La1 106.6(4) 1_655 3_544
O4 O4 La1 20.5(6) 2 3_544
O2 O4 La1 75.1(9) 1_545 3_544
O2 O4 La1 38.0(6) 2 3_544
O4 O4 La1 117.9(16) 4_655 3_544
O4 O4 La1 118.0(15) 4_645 3_544
Ga2 O4 La1 98.3(8) 4_545 3_544
La1 O4 La1 105.5(11) 1_655 3_544
La1 O4 La1 105.7(9) 1_645 3_544
Ga1 O4 La1 136.1(9) 3 3_544
Ta O4 La1 136.1(9) 3 3_544
O1 O4 La1 129.3(13) 1_655 3_544
Ga4 O4 La1 32.7(3) 3_444 3_544
O2 O4 La1 90.6(10) 1_655 3_544
La2 O4 La1 131.5(9) 3_545 3_544
O4 O4 La1 96.9(13) 4 3_544
O4 O4 La1 97.0(12) 4_545 3_544
O2 O4 La1 63.6(7) 1_455 3_544
Ga4 O4 O2 114(3) 4_645 3_545
Ga2 O4 O2 109(2) . 3_545
La1 O4 O2 50.3(13) 4_545 3_545
O6 O4 O2 96.7(18) 1_545 3_545
O7 O4 O2 147.9(19) 1_554 3_545
O7 O4 O2 136(2) 2_656 3_545
La2 O4 O2 138.8(13) . 3_545
O3 O4 O2 70.3(16) 3_554 3_545
O3 O4 O2 71.6(15) 2_656 3_545
O2 O4 O2 124.3(18) . 3_545
O1 O4 O2 96.2(16) 4 3_545
O1 O4 O2 105.0(18) 4_655 3_545
O7 O4 O2 116.1(14) 2_556 3_545
Ga1 O4 O2 118.6(13) . 3_545
Ta O4 O2 118.6(13) . 3_545
O1 O4 O2 36.7(13) . 3_545
Ga2 O4 O2 39.8(9) 4_645 3_545
O3 O4 O2 72.1(11) 2_556 3_545
La1 O4 O2 71.4(11) 4_645 3_545
Ga4 O4 O2 151.0(14) 3_544 3_545
O5 O4 O2 22.3(12) 3_544 3_545
O5 O4 O2 102.1(14) 2_646 3_545
La2 O4 O2 134.8(12) 1_655 3_545
O6 O4 O2 55.0(10) 4_645 3_545
Ga4 O4 O2 93.6(10) 4_545 3_545
Ga4 O4 O2 56.6(10) . 3_545
O4 O4 O2 165.6(10) 2_655 3_545
La1 O4 O2 91.9(11) . 3_545
O2 O4 O2 32.3(10) 4_645 3_545
Ga3 O4 O2 134.9(12) 1_655 3_545
La1 O4 O2 71.3(10) 1_545 3_545
O5 O4 O2 95.4(12) 2_546 3_545
O5 O4 O2 124.3(14) 1_544 3_545
Ga2 O4 O2 92.1(10) 1_455 3_545
Ta O4 O2 119.5(12) 1_655 3_545
Ga1 O4 O2 119.5(12) 1_655 3_545
O6 O4 O2 53.3(9) 4_545 3_545
O2 O4 O2 150.6(14) 2_655 3_545
O1 O4 O2 161.0(12) 3_554 3_545
Ga3 O4 O2 110.3(12) 1_645 3_545
Ga2 O4 O2 171.1(12) 2_655 3_545
O6 O4 O2 136.3(12) 2_645 3_545
O2 O4 O2 40.8(10) 4_545 3_545
Ga3 O4 O2 15.6(5) 3_645 3_545
O4 O4 O2 85.3(6) 1_455 3_545
O4 O4 O2 94.7(6) 1_655 3_545
O4 O4 O2 136.9(13) 2 3_545
O2 O4 O2 92.3(12) 1_545 3_545
O2 O4 O2 133.2(10) 2 3_545
O4 O4 O2 78.1(17) 4_655 3_545
O4 O4 O2 56.6(16) 4_645 3_545
Ga2 O4 O2 57.7(8) 4_545 3_545
La1 O4 O2 96.3(10) 1_655 3_545
La1 O4 O2 78.4(9) 1_645 3_545
Ga1 O4 O2 36.2(6) 3 3_545
Ta O4 O2 36.2(6) 3 3_545
O1 O4 O2 64.3(10) 1_655 3_545
Ga4 O4 O2 123.3(10) 3_444 3_545
O2 O4 O2 113.4(12) 1_655 3_545
La2 O4 O2 25.6(5) 3_545 3_545
O4 O4 O2 76.6(14) 4 3_545
O4 O4 O2 59.8(13) 4_545 3_545
O2 O4 O2 102.6(10) 1_455 3_545
La1 O4 O2 156.0(10) 3_544 3_545
Ga4 O4 O1 66(2) 4_645 3_654
Ga2 O4 O1 58.2(17) . 3_654
La1 O4 O1 158(2) 4_545 3_654
O6 O4 O1 102.0(16) 1_545 3_654
O7 O4 O1 60.4(15) 1_554 3_654
O7 O4 O1 32.4(14) 2_656 3_654
La2 O4 O1 71.8(11) . 3_654
O3 O4 O1 103.2(19) 3_554 3_654
O3 O4 O1 88.9(15) 2_656 3_654
O2 O4 O1 62.1(13) . 3_654
O1 O4 O1 107.1(19) 4 3_654
O1 O4 O1 45.2(17) 4_655 3_654
O7 O4 O1 97.6(13) 2_556 3_654
Ga1 O4 O1 89.0(12) . 3_654
Ta O4 O1 89.0(12) . 3_654
O1 O4 O1 152(2) . 3_654
Ga2 O4 O1 123.8(13) 4_645 3_654
O3 O4 O1 140.6(15) 2_556 3_654
La1 O4 O1 75.1(10) 4_645 3_654
Ga4 O4 O1 45.8(7) 3_544 3_654
O5 O4 O1 141.2(16) 3_544 3_654
O5 O4 O1 72.9(12) 2_646 3_654
La2 O4 O1 11.3(5) 1_655 3_654
O6 O4 O1 94.6(11) 4_645 3_654
Ga4 O4 O1 120.2(12) 4_545 3_654
Ga4 O4 O1 104.1(12) . 3_654
O4 O4 O1 30.2(8) 2_655 3_654
La1 O4 O1 95.1(12) . 3_654
O2 O4 O1 116.0(12) 4_645 3_654
Ga3 O4 O1 44.0(7) 1_655 3_654
La1 O4 O1 126.7(13) 1_545 3_654
O5 O4 O1 112.3(13) 2_546 3_654
O5 O4 O1 74.4(11) 1_544 3_654
Ga2 O4 O1 115.6(12) 1_455 3_654
Ta O4 O1 47.3(7) 1_655 3_654
Ga1 O4 O1 47.3(7) 1_655 3_654
O6 O4 O1 140.7(14) 4_545 3_654
O2 O4 O1 22.8(6) 2_655 3_654
O1 O4 O1 49.2(7) 3_554 3_654
Ga3 O4 O1 77.4(9) 1_645 3_654
Ga2 O4 O1 29.5(4) 2_655 3_654
O6 O4 O1 45.1(7) 2_645 3_654
O2 O4 O1 172.6(13) 4_545 3_654
Ga3 O4 O1 131.4(10) 3_645 3_654
O4 O4 O1 127.4(6) 1_455 3_654
O4 O4 O1 52.6(6) 1_655 3_654
O4 O4 O1 76.9(12) 2 3_654
O2 O4 O1 98.4(12) 1_545 3_654
O2 O4 O1 74.3(9) 2 3_654
O4 O4 O1 84.0(15) 4_655 3_654
O4 O4 O1 112.9(16) 4_645 3_654
Ga2 O4 O1 155.2(12) 4_545 3_654
La1 O4 O1 58.6(8) 1_655 3_654
La1 O4 O1 85.6(8) 1_645 3_654
Ga1 O4 O1 140.5(12) 3 3_654
Ta O4 O1 140.5(12) 3 3_654
O1 O4 O1 87.3(8) 1_655 3_654
Ga4 O4 O1 90.1(9) 3_444 3_654
O2 O4 O1 34.9(7) 1_655 3_654
La2 O4 O1 160.1(11) 3_545 3_654
O4 O4 O1 116.2(12) 4 3_654
O4 O4 O1 146.1(15) 4_545 3_654
O2 O4 O1 104.3(11) 1_455 3_654
La1 O4 O1 57.5(6) 3_544 3_654
O2 O4 O1 146.1(10) 3_545 3_654
Ga4 O4 O1 161(3) 4_645 1_565
Ga2 O4 O1 37.2(14) . 1_565
La1 O4 O1 70.2(14) 4_545 1_565
O6 O4 O1 151.1(15) 1_545 1_565
O7 O4 O1 122.1(19) 1_554 1_565
O7 O4 O1 127.3(19) 2_656 1_565
La2 O4 O1 79.6(10) . 1_565
O3 O4 O1 10.7(13) 3_554 1_565
O3 O4 O1 134.8(19) 2_656 1_565
O2 O4 O1 43.5(12) . 1_565
O1 O4 O1 50.4(12) 4 1_565
O1 O4 O1 65.2(14) 4_655 1_565
O7 O4 O1 103.9(14) 2_556 1_565
Ga1 O4 O1 132.2(12) . 1_565
Ta O4 O1 132.2(12) . 1_565
O1 O4 O1 110.4(19) . 1_565
Ga2 O4 O1 118.8(16) 4_645 1_565
O3 O4 O1 103.3(11) 2_556 1_565
La1 O4 O1 91.2(11) 4_645 1_565
Ga4 O4 O1 128.0(14) 3_544 1_565
O5 O4 O1 58.9(13) 3_544 1_565
O5 O4 O1 163.0(11) 2_646 1_565
La2 O4 O1 93.5(10) 1_655 1_565
O6 O4 O1 57.2(9) 4_645 1_565
Ga4 O4 O1 99.4(8) 4_545 1_565
Ga4 O4 O1 32.2(7) . 1_565
O4 O4 O1 111.3(8) 2_655 1_565
La1 O4 O1 19.6(4) . 1_565
O2 O4 O1 94.4(14) 4_645 1_565
Ga3 O4 O1 55.6(7) 1_655 1_565
La1 O4 O1 136.0(11) 1_545 1_565
O5 O4 O1 129.2(9) 2_546 1_565
O5 O4 O1 148.0(15) 1_544 1_565
Ga2 O4 O1 61.5(6) 1_455 1_565
Ta O4 O1 139.0(11) 1_655 1_565
Ga1 O4 O1 139.0(11) 1_655 1_565
O6 O4 O1 47.6(7) 4_545 1_565
O2 O4 O1 77.2(10) 2_655 1_565
O1 O4 O1 86.9(11) 3_554 1_565
Ga3 O4 O1 168.3(14) 1_645 1_565
Ga2 O4 O1 91.4(10) 2_655 1_565
O6 O4 O1 138.9(13) 2_645 1_565
O2 O4 O1 83.0(10) 4_545 1_565
Ga3 O4 O1 74.1(10) 3_645 1_565
O4 O4 O1 80.1(5) 1_455 1_565
O4 O4 O1 99.9(5) 1_655 1_565
O4 O4 O1 99.3(7) 2 1_565
O2 O4 O1 164.1(11) 1_545 1_565
O2 O4 O1 70.0(9) 2 1_565
O4 O4 O1 25.9(7) 4_655 1_565
O4 O4 O1 136(2) 4_645 1_565
Ga2 O4 O1 97.1(9) 4_545 1_565
La1 O4 O1 49.0(5) 1_655 1_565
La1 O4 O1 143.1(11) 1_645 1_565
Ga1 O4 O1 48.3(7) 3 1_565
Ta O4 O1 48.3(7) 3 1_565
O1 O4 O1 113.5(13) 1_655 1_565
Ga4 O4 O1 107.1(8) 3_444 1_565
O2 O4 O1 75.0(8) 1_655 1_565
La2 O4 O1 98.2(10) 3_545 1_565
O4 O4 O1 31.3(4) 4 1_565
O4 O4 O1 114.6(13) 4_545 1_565
O2 O4 O1 60.0(6) 1_455 1_565
La1 O4 O1 105.6(9) 3_544 1_565
O2 O4 O1 81.0(10) 3_545 1_565
O1 O4 O1 95.1(10) 3_654 1_565
Ga4 O4 O2 6.5(12) 4_645 2_645
Ga2 O4 O2 127(2) . 2_645
La1 O4 O2 123.1(17) 4_545 2_645
O6 O4 O2 37.4(10) 1_545 2_645
O7 O4 O2 45.9(14) 1_554 2_645
O7 O4 O2 37.4(14) 2_656 2_645
La2 O4 O2 89.9(12) . 2_645
O3 O4 O2 172(2) 3_554 2_645
O3 O4 O2 53.2(15) 2_656 2_645
O2 O4 O2 120.5(16) . 2_645
O1 O4 O2 127.6(16) 4 2_645
O1 O4 O2 104.1(16) 4_655 2_645
O7 O4 O2 74.1(12) 2_556 2_645
Ga1 O4 O2 45.7(7) . 2_645
Ta O4 O2 45.7(7) . 2_645
O1 O4 O2 86.3(17) . 2_645
Ga2 O4 O2 76.2(11) 4_645 2_645
O3 O4 O2 87.0(12) 2_556 2_645
La1 O4 O2 89.8(10) 4_645 2_645
Ga4 O4 O2 36.1(6) 3_544 2_645
O5 O4 O2 137.4(18) 3_544 2_645
O5 O4 O2 17.3(9) 2_646 2_645
La2 O4 O2 72.0(9) 1_655 2_645
O6 O4 O2 127.1(12) 4_645 2_645
Ga4 O4 O2 84.8(9) 4_545 2_645
Ga4 O4 O2 154.4(12) . 2_645
O4 O4 O2 52.1(7) 2_655 2_645
La1 O4 O2 150.8(14) . 2_645
O2 O4 O2 97.5(12) 4_645 2_645
Ga3 O4 O2 107.6(12) 1_655 2_645
La1 O4 O2 58.3(7) 1_545 2_645
O5 O4 O2 57.1(8) 2_546 2_645
O5 O4 O2 24.5(7) 1_544 2_645
Ga2 O4 O2 119.6(10) 1_455 2_645
Ta O4 O2 29.6(5) 1_655 2_645
Ga1 O4 O2 29.6(5) 1_655 2_645
O6 O4 O2 145.8(12) 4_545 2_645
O2 O4 O2 86.1(10) 2_655 2_645
O1 O4 O2 78.7(10) 3_554 2_645
Ga3 O4 O2 9.1(4) 1_645 2_645
Ga2 O4 O2 72.2(8) 2_655 2_645
O6 O4 O2 24.5(5) 2_645 2_645
O2 O4 O2 112.0(13) 4_545 2_645
Ga3 O4 O2 120.1(12) 3_645 2_645
O4 O4 O2 104.9(5) 1_455 2_645
O4 O4 O2 75.1(5) 1_655 2_645
O4 O4 O2 72.5(9) 2 2_645
O2 O4 O2 29.5(8) 1_545 2_645
O2 O4 O2 99.5(11) 2 2_645
O4 O4 O2 147.8(17) 4_655 2_645
O4 O4 O2 59.0(11) 4_645 2_645
Ga2 O4 O2 95.8(9) 4_545 2_645
La1 O4 O2 120.8(10) 1_655 2_645
La1 O4 O2 44.5(6) 1_645 2_645
Ga1 O4 O2 148.5(13) 3 2_645
Ta O4 O2 148.5(13) 3 2_645
O1 O4 O2 72.4(11) 1_655 2_645
Ga4 O4 O2 68.9(7) 3_444 2_645
O2 O4 O2 93.3(8) 1_655 2_645
La2 O4 O2 98.6(9) 3_545 2_645
O4 O4 O2 152.3(14) 4 2_645
O4 O4 O2 79.4(7) 4_545 2_645
O2 O4 O2 117.3(9) 1_455 2_645
La1 O4 O2 61.8(7) 3_544 2_645
O2 O4 O2 115.1(12) 3_545 2_645
O1 O4 O2 69.0(8) 3_654 2_645
O1 O4 O2 163.2(13) 1_565 2_645
Ga4 O4 O1 105(2) 4_645 1_455
Ga2 O4 O1 126.0(19) . 1_455
La1 O4 O1 25.1(10) 4_545 1_455
O6 O4 O1 61.8(12) 1_545 1_455
O7 O4 O1 91.0(13) 1_554 1_455
O7 O4 O1 133.8(18) 2_656 1_455
La2 O4 O1 80.6(10) . 1_455
O3 O4 O1 88.4(15) 3_554 1_455
O3 O4 O1 106.6(16) 2_656 1_455
O2 O4 O1 106.1(13) . 1_455
O1 O4 O1 57.0(10) 4 1_455
O1 O4 O1 156.7(19) 4_655 1_455
O7 O4 O1 52.1(11) 2_556 1_455
Ga1 O4 O1 64.9(8) . 1_455
Ta O4 O1 64.9(8) . 1_455
O1 O4 O1 44.0(7) . 1_455
Ga2 O4 O1 76.8(11) 4_645 1_455
O3 O4 O1 12.5(7) 2_556 1_455
La1 O4 O1 134.3(16) 4_645 1_455
Ga4 O4 O1 108.5(11) 3_544 1_455
O5 O4 O1 65.9(13) 3_544 1_455
O5 O4 O1 104.4(13) 2_646 1_455
La2 O4 O1 160.9(14) 1_655 1_455
O6 O4 O1 113.9(14) 4_645 1_455
Ga4 O4 O1 29.5(6) 4_545 1_455
Ga4 O4 O1 97.6(11) . 1_455
O4 O4 O1 120.7(14) 2_655 1_455
La1 O4 O1 82.2(8) . 1_455
O2 O4 O1 92.7(13) 4_645 1_455
Ga3 O4 O1 123.2(10) 1_655 1_455
La1 O4 O1 45.3(6) 1_545 1_455
O5 O4 O1 44.1(8) 2_546 1_455
O5 O4 O1 84.0(10) 1_544 1_455
Ga2 O4 O1 44.7(6) 1_455 1_455
Ta O4 O1 128.4(12) 1_655 1_455
Ga1 O4 O1 128.4(12) 1_655 1_455
O6 O4 O1 46.8(7) 4_545 1_455
O2 O4 O1 135.5(11) 2_655 1_455
O1 O4 O1 102.0(9) 3_554 1_455
Ga3 O4 O1 90.1(9) 1_645 1_455
Ga2 O4 O1 121.0(10) 2_655 1_455
O6 O4 O1 117.4(11) 2_645 1_455
O2 O4 O1 24.0(8) 4_545 1_455
Ga3 O4 O1 78.9(9) 3_645 1_455
O4 O4 O1 26.2(7) 1_455 1_455
O4 O4 O1 153.8(7) 1_655 1_455
O4 O4 O1 72.8(9) 2 1_455
O2 O4 O1 72.0(9) 1_545 1_455
O2 O4 O1 80.6(8) 2 1_455
O4 O4 O1 112.9(17) 4_655 1_455
O4 O4 O1 80.6(13) 4_645 1_455
Ga2 O4 O1 9.3(4) 4_545 1_455
La1 O4 O1 140.1(12) 1_655 1_455
La1 O4 O1 105.8(11) 1_645 1_455
Ga1 O4 O1 60.4(7) 3 1_455
Ta O4 O1 60.4(7) 3 1_455
O1 O4 O1 116.6(14) 1_655 1_455
Ga4 O4 O1 59.6(6) 3_444 1_455
O2 O4 O1 167.0(13) 1_655 1_455
La2 O4 O1 44.6(6) 3_545 1_455
O4 O4 O1 62.0(11) 4 1_455
O4 O4 O1 25.6(8) 4_545 1_455
O2 O4 O1 55.0(7) 1_455 1_455
La1 O4 O1 92.2(8) 3_544 1_455
O2 O4 O1 64.2(8) 3_545 1_455
O1 O4 O1 149.7(13) 3_654 1_455
O1 O4 O1 92.1(9) 1_565 1_455
O2 O4 O1 99.2(10) 2_645 1_455
Ga4 O4 O1 55.7(16) 4_645 4_545
Ga2 O4 O1 169(2) . 4_545
La1 O4 O1 72.2(14) 4_545 4_545
O6 O4 O1 17.5(11) 1_545 4_545
O7 O4 O1 68.6(16) 1_554 4_545
O7 O4 O1 88.5(16) 2_656 4_545
La2 O4 O1 94.2(10) . 4_545
O3 O4 O1 136.8(19) 3_554 4_545
O3 O4 O1 67.2(13) 2_656 4_545
O2 O4 O1 138.6(15) . 4_545
O1 O4 O1 99.9(12) 4 4_545
O1 O4 O1 152.0(18) 4_655 4_545
O7 O4 O1 57.8(11) 2_556 4_545
Ga1 O4 O1 41.2(7) . 4_545
Ta O4 O1 41.2(7) . 4_545
O1 O4 O1 43.0(17) . 4_545
Ga2 O4 O1 57.3(10) 4_645 4_545
O3 O4 O1 39.4(8) 2_556 4_545
La1 O4 O1 112.8(14) 4_645 4_545
Ga4 O4 O1 75.5(8) 3_544 4_545
O5 O4 O1 96.8(16) 3_544 4_545
O5 O4 O1 54.4(9) 2_646 4_545
La2 O4 O1 123.1(11) 1_655 4_545
O6 O4 O1 129.5(16) 4_645 4_545
Ga4 O4 O1 50.0(6) 4_545 4_545
Ga4 O4 O1 135.2(15) . 4_545
O4 O4 O1 93.6(9) 2_655 4_545
La1 O4 O1 130.4(9) . 4_545
O2 O4 O1 86.2(14) 4_645 4_545
Ga3 O4 O1 142.4(13) 1_655 4_545
La1 O4 O1 8.5(6) 1_545 4_545
O5 O4 O1 24.1(8) 2_546 4_545
O5 O4 O1 46.1(9) 1_544 4_545
Ga2 O4 O1 87.0(7) 1_455 4_545
Ta O4 O1 78.9(8) 1_655 4_545
Ga1 O4 O1 78.9(8) 1_655 4_545
O6 O4 O1 95.1(10) 4_545 4_545
O2 O4 O1 129.3(13) 2_655 4_545
O1 O4 O1 101.9(10) 3_554 4_545
Ga3 O4 O1 42.2(5) 1_645 4_545
Ga2 O4 O1 109.3(10) 2_655 4_545
O6 O4 O1 73.9(7) 2_645 4_545
O2 O4 O1 61.2(10) 4_545 4_545
Ga3 O4 O1 93.2(12) 3_645 4_545
O4 O4 O1 66.1(5) 1_455 4_545
O4 O4 O1 113.9(5) 1_655 4_545
O4 O4 O1 74.3(7) 2 4_545
O2 O4 O1 22.2(5) 1_545 4_545
O2 O4 O1 101.3(9) 2 4_545
O4 O4 O1 157(2) 4_655 4_545
O4 O4 O1 47.5(8) 4_645 4_545
Ga2 O4 O1 45.0(6) 4_545 4_545
La1 O4 O1 165.6(11) 1_655 4_545
La1 O4 O1 62.3(7) 1_645 4_545
Ga1 O4 O1 100.7(11) 3 4_545
Ta O4 O1 100.7(11) 3 4_545
O1 O4 O1 86.6(12) 1_655 4_545
Ga4 O4 O1 59.6(6) 3_444 4_545
O2 O4 O1 143.0(10) 1_655 4_545
La2 O4 O1 55.1(8) 3_545 4_545
O4 O4 O1 111.8(11) 4 4_545
O4 O4 O1 28.3(6) 4_545 4_545
O2 O4 O1 93.1(8) 1_455 4_545
La1 O4 O1 81.6(7) 3_544 4_545
O2 O4 O1 79.6(10) 3_545 4_545
O1 O4 O1 118.8(10) 3_654 4_545
O1 O4 O1 142.0(9) 1_565 4_545
O2 O4 O1 51.2(6) 2_645 4_545
O1 O4 O1 50.0(6) 1_455 4_545
Ga4 O4 O2 49.1(14) 4_645 2_545
Ga2 O4 O2 139(2) . 2_545
La1 O4 O2 86.2(14) 4_545 2_545
O6 O4 O2 17.1(11) 1_545 2_545
O7 O4 O2 38.5(14) 1_554 2_545
O7 O4 O2 72.7(15) 2_656 2_545
La2 O4 O2 66.7(9) . 2_545
O3 O4 O2 142.8(15) 3_554 2_545
O3 O4 O2 84.8(16) 2_656 2_545
O2 O4 O2 111.2(14) . 2_545
O1 O4 O2 88.8(13) 4 2_545
O1 O4 O2 140.3(19) 4_655 2_545
O7 O4 O2 35.5(11) 2_556 2_545
Ga1 O4 O2 10.5(6) . 2_545
Ta O4 O2 10.5(6) . 2_545
O1 O4 O2 72.8(15) . 2_545
Ga2 O4 O2 86.5(11) 4_645 2_545
O3 O4 O2 48.7(9) 2_556 2_545
La1 O4 O2 129.7(12) 4_645 2_545
Ga4 O4 O2 49.9(7) 3_544 2_545
O5 O4 O2 123.0(15) 3_544 2_545
O5 O4 O2 56.0(9) 2_646 2_545
La2 O4 O2 103.8(11) 1_655 2_545
O6 O4 O2 159.4(15) 4_645 2_545
Ga4 O4 O2 42.2(6) 4_545 2_545
Ga4 O4 O2 158.7(12) . 2_545
O4 O4 O2 66.5(9) 2_655 2_545
La1 O4 O2 119.9(9) . 2_545
O2 O4 O2 115.7(15) 4_645 2_545
Ga3 O4 O2 111.6(11) 1_655 2_545
La1 O4 O2 38.6(6) 1_545 2_545
O5 O4 O2 17.2(8) 2_546 2_545
O5 O4 O2 22.9(6) 1_544 2_545
Ga2 O4 O2 78.4(7) 1_455 2_545
Ta O4 O2 71.2(8) 1_655 2_545
Ga1 O4 O2 71.2(8) 1_655 2_545
O6 O4 O2 106.4(9) 4_545 2_545
O2 O4 O2 100.0(12) 2_655 2_545
O1 O4 O2 71.1(9) 3_554 2_545
Ga3 O4 O2 35.2(5) 1_645 2_545
Ga2 O4 O2 79.4(8) 2_655 2_545
O6 O4 O2 56.3(6) 2_645 2_545
O2 O4 O2 81.4(9) 4_545 2_545
Ga3 O4 O2 123.8(12) 3_645 2_545
O4 O4 O2 62.3(5) 1_455 2_545
O4 O4 O2 117.7(5) 1_655 2_545
O4 O4 O2 45.8(6) 2 2_545
O2 O4 O2 30.9(8) 1_545 2_545
O2 O4 O2 75.2(8) 2 2_545
O4 O4 O2 164.0(15) 4_655 2_545
O4 O4 O2 73.4(10) 4_645 2_545
Ga2 O4 O2 61.4(6) 4_545 2_545
La1 O4 O2 153.7(13) 1_655 2_545
La1 O4 O2 77.1(7) 1_645 2_545
Ga1 O4 O2 121.3(9) 3 2_545
Ta O4 O2 121.3(9) 3 2_545
O1 O4 O2 106.3(12) 1_655 2_545
Ga4 O4 O2 33.7(5) 3_444 2_545
O2 O4 O2 129.1(11) 1_655 2_545
La2 O4 O2 84.0(8) 3_545 2_545
O4 O4 O2 110.7(11) 4 2_545
O4 O4 O2 51.3(9) 4_545 2_545
O2 O4 O2 79.1(6) 1_455 2_545
La1 O4 O2 50.8(6) 3_544 2_545
O2 O4 O2 109.4(11) 3_545 2_545
O1 O4 O2 95.6(10) 3_654 2_545
O1 O4 O2 139.1(9) 1_565 2_545
O2 O4 O2 42.6(4) 2_645 2_545
O1 O4 O2 61.1(7) 1_455 2_545
O1 O4 O2 30.8(6) 4_545 2_545
Ga4 O4 O1 31.0(18) 4_645 4_645
Ga2 O4 O1 142.2(18) . 4_645
La1 O4 O1 107.9(19) 4_545 4_645
O6 O4 O1 43.3(11) 1_545 4_645
O7 O4 O1 77.6(16) 1_554 4_645
O7 O4 O1 60.2(15) 2_656 4_645
La2 O4 O1 120.5(13) . 4_645
O3 O4 O1 150(2) 3_554 4_645
O3 O4 O1 26.3(12) 2_656 4_645
O2 O4 O1 151.8(19) . 4_645
O1 O4 O1 144.1(16) 4 4_645
O1 O4 O1 108.0(13) 4_655 4_645
O7 O4 O1 93.9(14) 2_556 4_645
Ga1 O4 O1 66.7(8) . 4_645
Ta O4 O1 66.7(8) . 4_645
O1 O4 O1 60.7(16) . 4_645
Ga2 O4 O1 43.4(10) 4_645 4_645
O3 O4 O1 83.0(11) 2_556 4_645
La1 O4 O1 72.3(9) 4_645 4_645
Ga4 O4 O1 68.9(8) 3_544 4_645
O5 O4 O1 105.2(18) 3_544 4_645
O5 O4 O1 19.8(10) 2_646 4_645
La2 O4 O1 89.4(8) 1_655 4_645
O6 O4 O1 103.4(12) 4_645 4_645
Ga4 O4 O1 93.5(9) 4_545 4_645
Ga4 O4 O1 127.7(14) . 4_645
O4 O4 O1 83.4(8) 2_655 4_645
La1 O4 O1 173.3(14) . 4_645
O2 O4 O1 65.7(12) 4_645 4_645
Ga3 O4 O1 135.3(12) 1_655 4_645
La1 O4 O1 46.8(6) 1_545 4_645
O5 O4 O1 64.3(8) 2_546 4_645
O5 O4 O1 52.1(9) 1_544 4_645
Ga2 O4 O1 131.3(10) 1_455 4_645
Ta O4 O1 44.3(5) 1_655 4_645
Ga1 O4 O1 44.3(5) 1_655 4_645
O6 O4 O1 127.6(14) 4_545 4_645
O2 O4 O1 113.0(11) 2_655 4_645
O1 O4 O1 111.6(11) 3_554 4_645
Ga3 O4 O1 31.3(5) 1_645 4_645
Ga2 O4 O1 103.5(10) 2_655 4_645
O6 O4 O1 53.9(7) 2_645 4_645
O2 O4 O1 92.6(12) 4_545 4_645
Ga3 O4 O1 87.3(11) 3_645 4_645
O4 O4 O1 110.5(4) 1_455 4_645
O4 O4 O1 69.5(4) 1_655 4_645
O4 O4 O1 100.6(8) 2 4_645
O2 O4 O1 28.2(6) 1_545 4_645
O2 O4 O1 130.1(12) 2 4_645
O4 O4 O1 137.5(16) 4_655 4_645
O4 O4 O1 26.3(11) 4_645 4_645
Ga2 O4 O1 84.2(9) 4_545 4_645
La1 O4 O1 121.6(8) 1_655 4_645
La1 O4 O1 19.0(4) 1_645 4_645
Ga1 O4 O1 118.5(13) 3 4_645
Ta O4 O1 118.5(13) 3 4_645
O1 O4 O1 47.9(9) 1_655 4_645
Ga4 O4 O1 91.8(8) 3_444 4_645
O2 O4 O1 100.8(8) 1_655 4_645
La2 O4 O1 71.2(9) 3_545 4_645
O4 O4 O1 151.8(14) 4 4_645
O4 O4 O1 66.3(5) 4_545 4_645
O2 O4 O1 136.1(10) 1_455 4_645
La1 O4 O1 94.0(8) 3_544 4_645
O2 O4 O1 82.9(11) 3_545 4_645
O1 O4 O1 91.6(8) 3_654 4_645
O1 O4 O1 159.9(11) 1_565 4_645
O2 O4 O1 32.9(6) 2_645 4_645
O1 O4 O1 91.7(10) 1_455 4_645
O1 O4 O1 44.4(5) 4_545 4_645
O2 O4 O1 58.5(6) 2_545 4_645
Ga4 O4 O2 26.4(15) 4_645 1_645
Ga2 O4 O2 119.7(18) . 1_645
La1 O4 O2 129.8(19) 4_545 1_645
O6 O4 O2 60.0(11) 1_545 1_645
O7 O4 O2 76.1(14) 1_554 1_645
O7 O4 O2 42.3(15) 2_656 1_645
La2 O4 O2 119.5(14) . 1_645
O3 O4 O2 145.1(16) 3_554 1_645
O3 O4 O2 24.1(14) 2_656 1_645
O2 O4 O2 133.0(18) . 1_645
O1 O4 O2 159.7(17) 4 1_645
O1 O4 O2 86.3(14) 4_655 1_645
O7 O4 O2 105.6(13) 2_556 1_645
Ga1 O4 O2 76.8(9) . 1_645
Ta O4 O2 76.8(9) . 1_645
O1 O4 O2 81.3(14) . 1_645
Ga2 O4 O2 56.6(9) 4_645 1_645
O3 O4 O2 105.0(12) 2_556 1_645
La1 O4 O2 58.6(9) 4_645 1_645
Ga4 O4 O2 61.0(7) 3_544 1_645
O5 O4 O2 115.4(18) 3_544 1_645
O5 O4 O2 15.7(6) 2_646 1_645
La2 O4 O2 67.3(8) 1_655 1_645
O6 O4 O2 95.1(11) 4_645 1_645
Ga4 O4 O2 111.8(10) 4_545 1_645
Ga4 O4 O2 122.4(11) . 1_645
O4 O4 O2 70.5(9) 2_655 1_645
La1 O4 O2 163.5(12) . 1_645
O2 O4 O2 69.0(12) 4_645 1_645
Ga3 O4 O2 114.9(11) 1_655 1_645
La1 O4 O2 69.1(7) 1_545 1_645
O5 O4 O2 82.0(8) 2_546 1_645
O5 O4 O2 56.6(8) 1_544 1_645
Ga2 O4 O2 149.7(11) 1_455 1_645
Ta O4 O2 25.2(5) 1_655 1_645
Ga1 O4 O2 25.2(5) 1_655 1_645
O6 O4 O2 146.7(15) 4_545 1_645
O2 O4 O2 93.5(8) 2_655 1_645
O1 O4 O2 102.8(11) 3_554 1_645
Ga3 O4 O2 36.9(5) 1_645 1_645
Ga2 O4 O2 89.0(9) 2_655 1_645
O6 O4 O2 42.3(6) 2_645 1_645
O2 O4 O2 114.1(13) 4_545 1_645
Ga3 O4 O2 93.9(10) 3_645 1_645
O4 O4 O2 130.8(5) 1_455 1_645
O4 O4 O2 49.2(5) 1_655 1_645
O4 O4 O2 104.2(11) 2 1_645
O2 O4 O2 45.8(5) 1_545 1_645
O2 O4 O2 128.4(11) 2 1_645
O4 O4 O2 122.9(15) 4_655 1_645
O4 O4 O2 42.4(11) 4_645 1_645
Ga2 O4 O2 107.0(10) 4_545 1_645
La1 O4 O2 101.3(8) 1_655 1_645
La1 O4 O2 16.7(5) 1_645 1_645
Ga1 O4 O2 130.8(12) 3 1_645
Ta O4 O2 130.8(12) 3 1_645
O1 O4 O2 40.5(9) 1_655 1_645
Ga4 O4 O2 100.9(9) 3_444 1_645
O2 O4 O2 78.3(7) 1_655 1_645
La2 O4 O2 90.2(9) 3_545 1_645
O4 O4 O2 171.7(18) 4 1_645
O4 O4 O2 89.0(5) 4_545 1_645
O2 O4 O2 149.4(12) 1_455 1_645
La1 O4 O2 90.6(8) 3_544 1_645
O2 O4 O2 95.1(10) 3_545 1_645
O1 O4 O2 71.0(8) 3_654 1_645
O1 O4 O2 148.7(9) 1_565 1_645
O2 O4 O2 32.2(8) 2_645 1_645
O1 O4 O2 114.3(10) 1_455 1_645
O1 O4 O2 65.7(6) 4_545 1_645
O2 O4 O2 71.5(8) 2_545 1_645
O1 O4 O2 22.7(4) 4_645 1_645
Ga4 O4 O2 70.1(16) 4_645 1_445
Ga2 O4 O2 145(2) . 1_445
La1 O4 O2 61.3(12) 4_545 1_445
O6 O4 O2 27.6(9) 1_545 1_445
O7 O4 O2 60.5(13) 1_554 1_445
O7 O4 O2 97.6(16) 2_656 1_445
La2 O4 O2 73.1(9) . 1_445
O3 O4 O2 122.9(14) 3_554 1_445
O3 O4 O2 91.3(14) 2_656 1_445
O2 O4 O2 115.5(14) . 1_445
O1 O4 O2 76.6(12) 4 1_445
O1 O4 O2 165(2) 4_655 1_445
O7 O4 O2 35.6(11) 2_556 1_445
Ga1 O4 O2 31.3(6) . 1_445
Ta O4 O2 31.3(6) . 1_445
O1 O4 O2 54.1(12) . 1_445
Ga2 O4 O2 78.1(11) 4_645 1_445
O3 O4 O2 23.7(7) 2_556 1_445
La1 O4 O2 136.9(14) 4_645 1_445
Ga4 O4 O2 74.7(8) 3_544 1_445
O5 O4 O2 98.6(14) 3_544 1_445
O5 O4 O2 73.2(9) 2_646 1_445
La2 O4 O2 129.0(12) 1_655 1_445
O6 O4 O2 143.5(15) 4_645 1_445
Ga4 O4 O2 26.0(5) 4_545 1_445
Ga4 O4 O2 133.6(12) . 1_445
O4 O4 O2 90.2(10) 2_655 1_445
La1 O4 O2 108.2(8) . 1_445
O2 O4 O2 105.2(14) 4_645 1_445
Ga3 O4 O2 124.0(11) 1_655 1_445
La1 O4 O2 26.7(5) 1_545 1_445
O5 O4 O2 8.1(7) 2_546 1_445
O5 O4 O2 48.0(8) 1_544 1_445
Ga2 O4 O2 64.0(6) 1_455 1_445
Ta O4 O2 93.7(9) 1_655 1_445
Ga1 O4 O2 93.7(9) 1_655 1_445
O6 O4 O2 82.6(8) 4_545 1_445
O2 O4 O2 120.0(10) 2_655 1_445
O1 O4 O2 86.1(9) 3_554 1_445
Ga3 O4 O2 55.4(6) 1_645 1_445
Ga2 O4 O2 99.5(9) 2_655 1_445
O6 O4 O2 81.2(8) 2_645 1_445
O2 O4 O2 56.3(10) 4_545 1_445
Ga3 O4 O2 104.1(11) 3_645 1_445
O4 O4 O2 43.9(5) 1_455 1_445
O4 O4 O2 136.1(5) 1_655 1_445
O4 O4 O2 55.3(6) 2 1_445
O2 O4 O2 41.0(5) 1_545 1_445
O2 O4 O2 78.8(6) 2 1_445
O4 O4 O2 148.0(16) 4_655 1_445
O4 O4 O2 71.0(10) 4_645 1_445
Ga2 O4 O2 36.2(5) 4_545 1_445
La1 O4 O2 170.1(11) 1_655 1_445
La1 O4 O2 86.1(8) 1_645 1_445
Ga1 O4 O2 96.0(8) 3 1_445
Ta O4 O2 96.0(8) 3 1_445
O1 O4 O2 110.7(12) 1_655 1_445
Ga4 O4 O2 39.5(5) 3_444 1_445
O2 O4 O2 154.3(14) 1_655 1_445
La2 O4 O2 63.2(7) 3_545 1_445
O4 O4 O2 92.5(10) 4 1_445
O4 O4 O2 28.7(9) 4_545 1_445
O2 O4 O2 69.1(6) 1_455 1_445
La1 O4 O2 68.4(6) 3_544 1_445
O2 O4 O2 88.5(9) 3_545 1_445
O1 O4 O2 120.2(11) 3_654 1_445
O1 O4 O2 123.8(7) 1_565 1_445
O2 O4 O2 64.1(8) 2_645 1_445
O1 O4 O2 36.2(6) 1_455 1_445
O1 O4 O2 24.2(4) 4_545 1_445
O2 O4 O2 25.3(7) 2_545 1_445
O1 O4 O2 67.5(6) 4_645 1_445
O2 O4 O2 86.9(8) 1_645 1_445
Ga4 O4 O1 97(2) 4_645 3_454
Ga2 O4 O1 85.6(19) . 3_454
La1 O4 O1 74.7(14) 4_545 3_454
O6 O4 O1 76.1(13) 1_545 3_454
O7 O4 O1 48.6(12) 1_554 3_454
O7 O4 O1 94.9(18) 2_656 3_454
La2 O4 O1 15.9(6) . 3_454
O3 O4 O1 89.2(15) 3_554 3_454
O3 O4 O1 143.5(18) 2_656 3_454
O2 O4 O1 55.5(12) . 3_454
O1 O4 O1 36.8(14) 4 3_454
O1 O4 O1 113.9(19) 4_655 3_454
O7 O4 O1 25.5(11) 2_556 3_454
Ga1 O4 O1 50.9(7) . 3_454
Ta O4 O1 50.9(7) . 3_454
O1 O4 O1 107.0(11) . 3_454
Ga2 O4 O1 137.3(13) 4_645 3_454
O3 O4 O1 61.9(9) 2_556 3_454
La1 O4 O1 160.3(15) 4_645 3_454
Ga4 O4 O1 66.6(8) 3_544 3_454
O5 O4 O1 113.6(15) 3_544 3_454
O5 O4 O1 109.0(12) 2_646 3_454
La2 O4 O1 98.0(11) 1_655 3_454
O6 O4 O1 138.9(14) 4_645 3_454
Ga4 O4 O1 39.4(6) 4_545 3_454
Ga4 O4 O1 112.8(11) . 3_454
O4 O4 O1 66.0(10) 2_655 3_454
La1 O4 O1 62.2(8) . 3_454
O2 O4 O1 156.8(13) 4_645 3_454
Ga3 O4 O1 65.3(7) 1_655 3_454
La1 O4 O1 86.9(8) 1_545 3_454
O5 O4 O1 59.0(9) 2_546 3_454
O5 O4 O1 67.9(10) 1_544 3_454
Ga2 O4 O1 34.8(6) 1_455 3_454
Ta O4 O1 107.5(11) 1_655 3_454
Ga1 O4 O1 107.5(11) 1_655 3_454
O6 O4 O1 77.1(9) 4_545 3_454
O2 O4 O1 71.0(8) 2_655 3_454
O1 O4 O1 38.0(4) 3_554 3_454
Ga3 O4 O1 88.8(9) 1_645 3_454
Ga2 O4 O1 57.7(6) 2_655 3_454
O6 O4 O1 85.8(9) 2_645 3_454
O2 O4 O1 85.4(9) 4_545 3_454
Ga3 O4 O1 135.2(10) 3_645 3_454
O4 O4 O1 40.2(5) 1_455 3_454
O4 O4 O1 139.8(5) 1_655 3_454
O4 O4 O1 19.7(7) 2 3_454
O2 O4 O1 90.5(9) 1_545 3_454
O2 O4 O1 18.8(5) 2 3_454
O4 O4 O1 104.4(13) 4_655 3_454
O4 O4 O1 130.6(13) 4_645 3_454
Ga2 O4 O1 73.3(6) 4_545 3_454
La1 O4 O1 110.2(10) 1_655 3_454
La1 O4 O1 135.1(11) 1_645 3_454
Ga1 O4 O1 99.0(8) 3 3_454
Ta O4 O1 99.0(8) 3 3_454
O1 O4 O1 164.3(16) 1_655 3_454
Ga4 O4 O1 25.9(4) 3_444 3_454
O2 O4 O1 111.7(11) 1_655 3_454
La2 O4 O1 109.4(7) 3_545 3_454
O4 O4 O1 62.4(11) 4 3_454
O4 O4 O1 81.5(11) 4_545 3_454
O2 O4 O1 27.0(6) 1_455 3_454
La1 O4 O1 37.2(4) 3_544 3_454
O2 O4 O1 124.9(9) 3_545 3_454
O1 O4 O1 87.2(9) 3_654 3_454
O1 O4 O1 81.7(8) 1_565 3_454
O2 O4 O1 91.8(8) 2_645 3_454
O1 O4 O1 64.7(5) 1_455 3_454
O1 O4 O1 83.2(6) 4_545 3_454
O2 O4 O1 59.6(6) 2_545 3_454
O1 O4 O1 117.6(9) 4_645 3_454
O2 O4 O1 123.8(10) 1_645 3_454
O2 O4 O1 60.1(6) 1_445 3_454
Ga4 O4 O1 55.6(18) 4_645 2
Ga2 O4 O1 104(2) . 2
La1 O4 O1 104.6(14) 4_545 2
O6 O4 O1 49.9(13) 1_545 2
O7 O4 O1 8.2(10) 1_554 2
O7 O4 O1 58.1(15) 2_656 2
La2 O4 O1 40.0(8) . 2
O3 O4 O1 128.9(18) 3_554 2
O3 O4 O1 103.7(17) 2_656 2
O2 O4 O1 80.0(15) . 2
O1 O4 O1 78.9(13) 4 2
O1 O4 O1 112(2) 4_655 2
O7 O4 O1 33.4(9) 2_556 2
Ga1 O4 O1 24.6(7) . 2
Ta O4 O1 24.6(7) . 2
O1 O4 O1 106.9(18) . 2
Ga2 O4 O1 118.5(14) 4_645 2
O3 O4 O1 73.0(10) 2_556 2
La1 O4 O1 132.6(13) 4_645 2
Ga4 O4 O1 27.9(5) 3_544 2
O5 O4 O1 148.6(14) 3_544 2
O5 O4 O1 67.8(11) 2_646 2
La2 O4 O1 78.1(9) 1_655 2
O6 O4 O1 162.0(14) 4_645 2
Ga4 O4 O1 54.8(6) 4_545 2
Ga4 O4 O1 151.5(14) . 2
O4 O4 O1 37.5(9) 2_655 2
La1 O4 O1 101.3(10) . 2
O2 O4 O1 146.0(15) 4_645 2
Ga3 O4 O1 77.3(9) 1_655 2
La1 O4 O1 73.1(8) 1_545 2
O5 O4 O1 47.5(10) 2_546 2
O5 O4 O1 28.6(8) 1_544 2
Ga2 O4 O1 74.7(7) 1_455 2
Ta O4 O1 66.9(7) 1_655 2
Ga1 O4 O1 66.9(7) 1_655 2
O6 O4 O1 115.9(9) 4_545 2
O2 O4 O1 66.3(9) 2_655 2
O1 O4 O1 37.1(4) 3_554 2
Ga3 O4 O1 49.4(6) 1_645 2
Ga2 O4 O1 45.5(6) 2_655 2
O6 O4 O1 45.3(6) 2_645 2
O2 O4 O1 107.1(10) 4_545 2
Ga3 O4 O1 158.1(12) 3_645 2
O4 O4 O1 69.9(4) 1_455 2
O4 O4 O1 110.1(4) 1_655 2
O4 O4 O1 22.4(7) 2 2
O2 O4 O1 59.3(9) 1_545 2
O2 O4 O1 49.6(7) 2 2
O4 O4 O1 134.1(17) 4_655 2
O4 O4 O1 102.9(14) 4_645 2
Ga2 O4 O1 87.6(7) 4_545 2
La1 O4 O1 120.7(12) 1_655 2
La1 O4 O1 94.9(9) 1_645 2
Ga1 O4 O1 137.7(8) 3 2
Ta O4 O1 137.7(8) 3 2
O1 O4 O1 122.4(13) 1_655 2
Ga4 O4 O1 25.7(3) 3_444 2
O2 O4 O1 102.3(11) 1_655 2
La2 O4 O1 117.3(9) 3_545 2
O4 O4 O1 104.5(13) 4 2
O4 O4 O1 83.0(11) 4_545 2
O2 O4 O1 68.9(7) 1_455 2
La1 O4 O1 16.4(4) 3_544 2
O2 O4 O1 142.9(11) 3_545 2
O1 O4 O1 67.6(6) 3_654 2
O1 O4 O1 119.4(10) 1_565 2
O2 O4 O1 50.5(6) 2_645 2
O1 O4 O1 83.3(9) 1_455 2
O1 O4 O1 65.4(6) 4_545 2
O2 O4 O1 34.6(6) 2_545 2
O1 O4 O1 80.6(8) 4_645 2
O2 O4 O1 81.9(8) 1_645 2
O2 O4 O1 54.4(6) 1_445 2
O1 O4 O1 42.1(4) 3_454 2
Ga4 O4 O1 36.0(19) 4_645 2_655
Ga2 O4 O1 94(2) . 2_655
La1 O4 O1 141.0(16) 4_545 2_655
O6 O4 O1 63.5(13) 1_545 2_655
O7 O4 O1 29.1(11) 1_554 2_655
O7 O4 O1 21.0(14) 2_656 2_655
La2 O4 O1 65.3(10) . 2_655
O3 O4 O1 138(2) 3_554 2_655
O3 O4 O1 79.7(16) 2_656 2_655
O2 O4 O1 85.3(16) . 2_655
O1 O4 O1 109.7(18) 4 2_655
O1 O4 O1 82.8(16) 4_655 2_655
O7 O4 O1 70.6(11) 2_556 2_655
Ga1 O4 O1 52.4(8) . 2_655
Ta O4 O1 52.4(8) . 2_655
O1 O4 O1 121(2) . 2_655
Ga2 O4 O1 110.0(13) 4_645 2_655
O3 O4 O1 105.4(12) 2_556 2_655
La1 O4 O1 95.7(11) 4_645 2_655
Ga4 O4 O1 9.4(4) 3_544 2_655
O5 O4 O1 171.0(18) 3_544 2_655
O5 O4 O1 47.6(12) 2_646 2_655
La2 O4 O1 46.4(7) 1_655 2_655
O6 O4 O1 127.9(11) 4_645 2_655
Ga4 O4 O1 91.1(9) 4_545 2_655
Ga4 O4 O1 142.9(13) . 2_655
O4 O4 O1 16.5(6) 2_655 2_655
La1 O4 O1 118.4(13) . 2_655
O2 O4 O1 123.7(12) 4_645 2_655
Ga3 O4 O1 72.0(9) 1_655 2_655
La1 O4 O1 89.0(10) 1_545 2_655
O5 O4 O1 74.6(10) 2_546 2_655
O5 O4 O1 35.7(8) 1_544 2_655
Ga2 O4 O1 109.5(10) 1_455 2_655
Ta O4 O1 33.3(6) 1_655 2_655
Ga1 O4 O1 33.3(6) 1_655 2_655
O6 O4 O1 151.8(12) 4_545 2_655
O2 O4 O1 51.2(8) 2_655 2_655
O1 O4 O1 47.2(5) 3_554 2_655
Ga3 O4 O1 42.1(6) 1_645 2_655
Ga2 O4 O1 36.8(5) 2_655 2_655
O6 O4 O1 13.5(5) 2_645 2_655
O2 O4 O1 138.9(12) 4_545 2_655
Ga3 O4 O1 148.8(11) 3_645 2_655
O4 O4 O1 107.1(4) 1_455 2_655
O4 O4 O1 72.9(4) 1_655 2_655
O4 O4 O1 56.5(9) 2 2_655
O2 O4 O1 62.4(9) 1_545 2_655
O2 O4 O1 73.3(9) 2 2_655
O4 O4 O1 122.5(17) 4_655 2_655
O4 O4 O1 93.2(15) 4_645 2_655
Ga2 O4 O1 118.9(9) 4_545 2_655
La1 O4 O1 97.2(9) 1_655 2_655
La1 O4 O1 72.1(8) 1_645 2_655
Ga1 O4 O1 173.5(11) 3 2_655
Ta O4 O1 173.5(11) 3 2_655
O1 O4 O1 91.9(12) 1_655 2_655
Ga4 O4 O1 62.9(6) 3_444 2_655
O2 O4 O1 71.7(9) 1_655 2_655
La2 O4 O1 133.5(11) 3_545 2_655
O4 O4 O1 132.5(16) 4 2_655
O4 O4 O1 107.3(11) 4_545 2_655
O2 O4 O1 101.2(9) 1_455 2_655
La1 O4 O1 37.6(4) 3_544 2_655
O2 O4 O1 149.7(11) 3_545 2_655
O1 O4 O1 38.8(4) 3_654 2_655
O1 O4 O1 127.6(12) 1_565 2_655
O2 O4 O1 35.7(6) 2_645 2_655
O1 O4 O1 117.3(10) 1_455 2_655
O1 O4 O1 80.7(8) 4_545 2_655
O2 O4 O1 57.5(6) 2_545 2_655
O1 O4 O1 66.9(7) 4_645 2_655
O2 O4 O1 55.6(7) 1_645 2_655
O2 O4 O1 82.6(7) 1_445 2_655
O1 O4 O1 74.8(6) 3_454 2_655
O1 O4 O1 37.2(4) 2 2_655
Ga4 O4 O1 124.2(19) 4_645 1_665
Ga2 O4 O1 29.1(15) . 1_665
La1 O4 O1 105.3(17) 4_545 1_665
O6 O4 O1 166.5(15) 1_545 1_665
O7 O4 O1 127(2) 1_554 1_665
O7 O4 O1 95.7(16) 2_656 1_665
La2 O4 O1 103.3(13) . 1_665
O3 O4 O1 42.8(11) 3_554 1_665
O3 O4 O1 99.1(15) 2_656 1_665
O2 O4 O1 58.7(11) . 1_665
O1 O4 O1 91.1(16) 4 1_665
O1 O4 O1 26.9(14) 4_655 1_665
O7 O4 O1 139.0(16) 2_556 1_665
Ga1 O4 O1 155.6(15) . 1_665
Ta O4 O1 155.6(15) . 1_665
O1 O4 O1 122.0(19) . 1_665
Ga2 O4 O1 105.0(13) 4_645 1_665
O3 O4 O1 142.6(14) 2_556 1_665
La1 O4 O1 52.5(8) 4_645 1_665
Ga4 O4 O1 115.8(11) 3_544 1_665
O5 O4 O1 71.6(12) 3_544 1_665
O5 O4 O1 120.8(9) 2_646 1_665
La2 O4 O1 62.7(7) 1_655 1_665
O6 O4 O1 33.0(8) 4_645 1_665
Ga4 O4 O1 141.5(11) 4_545 1_665
Ga4 O4 O1 34.2(7) . 1_665
O4 O4 O1 98.7(9) 2_655 1_665
La1 O4 O1 59.1(7) . 1_665
O2 O4 O1 76.0(12) 4_645 1_665
Ga3 O4 O1 55.0(7) 1_655 1_665
La1 O4 O1 155.6(14) 1_545 1_665
O5 O4 O1 171.3(11) 2_546 1_665
O5 O4 O1 144.3(13) 1_544 1_665
Ga2 O4 O1 103.3(10) 1_455 1_665
Ta O4 O1 100.5(8) 1_655 1_665
Ga1 O4 O1 100.5(8) 1_655 1_665
O6 O4 O1 83.5(10) 4_545 1_665
O2 O4 O1 65.1(9) 2_655 1_665
O1 O4 O1 95.3(11) 3_554 1_665
Ga3 O4 O1 138.9(9) 1_645 1_665
Ga2 O4 O1 85.8(8) 2_655 1_665
O6 O4 O1 111.9(9) 2_645 1_665
O2 O4 O1 112.2(12) 4_545 1_665
Ga3 O4 O1 70.9(9) 3_645 1_665
O4 O4 O1 122.5(5) 1_455 1_665
O4 O4 O1 57.5(5) 1_655 1_665
O4 O4 O1 123.4(8) 2 1_665
O2 O4 O1 152.1(10) 1_545 1_665
O2 O4 O1 95.9(10) 2 1_665
O4 O4 O1 17.7(9) 4_655 1_665
O4 O4 O1 115.7(16) 4_645 1_665
Ga2 O4 O1 131.6(11) 4_545 1_665
La1 O4 O1 11.6(5) 1_655 1_665
La1 O4 O1 105.4(8) 1_645 1_665
Ga1 O4 O1 71.7(8) 3 1_665
Ta O4 O1 71.7(8) 3 1_665
O1 O4 O1 78.3(8) 1_655 1_665
Ga4 O4 O1 137.9(11) 3_444 1_665
O2 O4 O1 38.2(6) 1_655 1_665
La2 O4 O1 110.9(10) 3_545 1_665
O4 O4 O1 73.5(6) 4 1_665
O4 O4 O1 143.4(17) 4_545 1_665
O2 O4 O1 99.6(9) 1_455 1_665
La1 O4 O1 115.2(9) 3_544 1_665
O2 O4 O1 85.5(10) 3_545 1_665
O1 O4 O1 70.1(6) 3_654 1_665
O1 O4 O1 42.4(5) 1_565 1_665
O2 O4 O1 130.1(9) 2_645 1_665
O1 O4 O1 130.2(12) 1_455 1_665
O1 O4 O1 162.3(11) 4_545 1_665
O2 O4 O1 165.0(11) 2_545 1_665
O1 O4 O1 124.4(7) 4_645 1_665
O2 O4 O1 106.6(8) 1_645 1_665
O2 O4 O1 165.7(9) 1_445 1_665
O1 O4 O1 113.5(10) 3_454 1_665
O1 O4 O1 131.0(10) 2 1_665
O1 O4 O1 108.7(8) 2_655 1_665
Ga4 O4 O1 29.4(13) 4_645 3_544
Ga2 O4 O1 135(2) . 3_544
La1 O4 O1 104.6(15) 4_545 3_544
O6 O4 O1 20.7(11) 1_545 3_544
O7 O4 O1 35.3(14) 1_554 3_544
O7 O4 O1 54.4(14) 2_656 3_544
La2 O4 O1 75.3(10) . 3_544
O3 O4 O1 161.5(16) 3_554 3_544
O3 O4 O1 70.6(15) 2_656 3_544
O2 O4 O1 115.6(17) . 3_544
O1 O4 O1 106.3(13) 4 3_544
O1 O4 O1 123.2(16) 4_655 3_544
O7 O4 O1 52.2(10) 2_556 3_544
Ga1 O4 O1 23.4(5) . 3_544
Ta O4 O1 23.4(5) . 3_544
O1 O4 O1 80.2(15) . 3_544
Ga2 O4 O1 83.0(11) 4_645 3_544
O3 O4 O1 67.1(9) 2_556 3_544
La1 O4 O1 111.9(11) 4_645 3_544
Ga4 O4 O1 37.5(6) 3_544 3_544
O5 O4 O1 134.7(16) 3_544 3_544
O5 O4 O1 37.7(8) 2_646 3_544
La2 O4 O1 87.7(10) 1_655 3_544
O6 O4 O1 148.0(13) 4_645 3_544
Ga4 O4 O1 62.1(6) 4_545 3_544
Ga4 O4 O1 171.9(15) . 3_544
O4 O4 O1 55.8(7) 2_655 3_544
La1 O4 O1 135.1(11) . 3_544
O2 O4 O1 110.0(13) 4_645 3_544
Ga3 O4 O1 109.3(11) 1_655 3_544
La1 O4 O1 46.5(6) 1_545 3_544
O5 O4 O1 35.7(7) 2_546 3_544
O5 O4 O1 8.7(8) 1_544 3_544
Ga2 O4 O1 97.1(8) 1_455 3_544
Ta O4 O1 51.3(6) 1_655 3_544
Ga1 O4 O1 51.3(6) 1_655 3_544
O6 O4 O1 125.9(10) 4_545 3_544
O2 O4 O1 91.9(11) 2_655 3_544
O1 O4 O1 71.6(9) 3_554 3_544
Ga3 O4 O1 16.5(3) 1_645 3_544
Ga2 O4 O1 73.1(8) 2_655 3_544
O6 O4 O1 38.2(5) 2_645 3_544
O2 O4 O1 97.2(10) 4_545 3_544
Ga3 O4 O1 126.6(12) 3_645 3_544
O4 O4 O1 82.1(4) 1_455 3_544
O4 O4 O1 97.9(4) 1_655 3_544
O4 O4 O1 55.2(6) 2 3_544
O2 O4 O1 24.0(7) 1_545 3_544
O2 O4 O1 84.8(9) 2 3_544
O4 O4 O1 165.2(19) 4_655 3_544
O4 O4 O1 66.9(11) 4_645 3_544
Ga2 O4 O1 78.3(7) 4_545 3_544
La1 O4 O1 139.1(10) 1_655 3_544
La1 O4 O1 62.2(6) 1_645 3_544
Ga1 O4 O1 137.8(10) 3 3_544
Ta O4 O1 137.8(10) 3 3_544
O1 O4 O1 91.7(11) 1_655 3_544
Ga4 O4 O1 48.0(5) 3_444 3_544
O2 O4 O1 111.9(10) 1_655 3_544
La2 O4 O1 92.7(8) 3_545 3_544
O4 O4 O1 129.9(12) 4 3_544
O4 O4 O1 64.7(8) 4_545 3_544
O2 O4 O1 96.2(8) 1_455 3_544
La1 O4 O1 51.4(6) 3_544 3_544
O2 O4 O1 115.6(10) 3_545 3_544
O1 O4 O1 81.4(9) 3_654 3_544
O1 O4 O1 154.5(11) 1_565 3_544
O2 O4 O1 22.8(4) 2_645 3_544
O1 O4 O1 79.6(7) 1_455 3_544
O1 O4 O1 38.1(8) 4_545 3_544
O2 O4 O1 20.0(3) 2_545 3_544
O1 O4 O1 45.4(8) 4_645 3_544
O2 O4 O1 53.4(6) 1_645 3_544
O2 O4 O1 43.4(5) 1_445 3_544
O1 O4 O1 72.9(6) 3_454 3_544
O1 O4 O1 36.1(5) 2 3_544
O1 O4 O1 42.8(5) 2_655 3_544
O1 O4 O1 150.1(10) 1_665 3_544
Ga4 O4 O1 121.0(19) 4_645 4_455
Ga2 O4 O1 92.8(17) . 4_455
La1 O4 O1 39.5(11) 4_545 4_455
O6 O4 O1 83.1(11) 1_545 4_455
O7 O4 O1 80.6(13) 1_554 4_455
O7 O4 O1 129.8(19) 2_656 4_455
La2 O4 O1 49.4(8) . 4_455
O3 O4 O1 70.4(12) 3_554 4_455
O3 O4 O1 143.8(17) 2_656 4_455
O2 O4 O1 68.7(11) . 4_455
O1 O4 O1 20.8(7) 4 4_455
O1 O4 O1 127.6(19) 4_655 4_455
O7 O4 O1 41.5(10) 2_556 4_455
Ga1 O4 O1 68.9(7) . 4_455
Ta O4 O1 68.9(7) . 4_455
O1 O4 O1 81.1(10) . 4_455
Ga2 O4 O1 113.7(13) 4_645 4_455
O3 O4 O1 42.4(7) 2_556 4_455
La1 O4 O1 154.3(14) 4_645 4_455
Ga4 O4 O1 100.1(10) 3_544 4_455
O5 O4 O1 78.8(13) 3_544 4_455
O5 O4 O1 128.1(11) 2_646 4_455
La2 O4 O1 129.9(13) 1_655 4_455
O6 O4 O1 117.0(12) 4_645 4_455
Ga4 O4 O1 31.3(5) 4_545 4_455
Ga4 O4 O1 90.5(9) . 4_455
O4 O4 O1 101.6(13) 2_655 4_455
La1 O4 O1 51.6(6) . 4_455
O2 O4 O1 121.9(13) 4_645 4_455
Ga3 O4 O1 85.5(9) 1_655 4_455
La1 O4 O1 78.0(7) 1_545 4_455
O5 O4 O1 61.1(7) 2_546 4_455
O5 O4 O1 90.8(10) 1_544 4_455
Ga2 O4 O1 7.7(4) 1_455 4_455
Ta O4 O1 139.2(11) 1_655 4_455
Ga1 O4 O1 139.2(11) 1_655 4_455
O6 O4 O1 43.2(7) 4_545 4_455
O2 O4 O1 100.1(11) 2_655 4_455
O1 O4 O1 72.2(9) 3_554 4_455
Ga3 O4 O1 107.6(8) 1_645 4_455
Ga2 O4 O1 91.7(9) 2_655 4_455
O6 O4 O1 118.0(10) 2_645 4_455
O2 O4 O1 52.3(7) 4_545 4_455
Ga3 O4 O1 99.7(9) 3_645 4_455
O4 O4 O1 13.5(6) 1_455 4_455
O4 O4 O1 166.5(6) 1_655 4_455
O4 O4 O1 52.5(8) 2 4_455
O2 O4 O1 97.5(8) 1_545 4_455
O2 O4 O1 46.0(7) 2 4_455
O4 O4 O1 93.9(12) 4_655 4_455
O4 O4 O1 118.2(14) 4_645 4_455
Ga2 O4 O1 46.9(5) 4_545 4_455
La1 O4 O1 114.6(10) 1_655 4_455
La1 O4 O1 141.3(11) 1_645 4_455
Ga1 O4 O1 65.3(6) 3 4_455
Ta O4 O1 65.3(6) 3 4_455
O1 O4 O1 152.4(12) 1_655 4_455
Ga4 O4 O1 48.2(5) 3_444 4_455
O2 O4 O1 132.5(12) 1_655 4_455
La2 O4 O1 78.7(7) 3_545 4_455
O4 O4 O1 38.3(9) 4 4_455
O4 O4 O1 62.1(9) 4_545 4_455
O2 O4 O1 17.3(6) 1_455 4_455
La1 O4 O1 72.3(6) 3_544 4_455
O2 O4 O1 89.6(8) 3_545 4_455
O1 O4 O1 120.3(10) 3_654 4_455
O1 O4 O1 68.2(6) 1_565 4_455
O2 O4 O1 114.5(9) 2_645 4_455
O1 O4 O1 37.7(5) 1_455 4_455
O1 O4 O1 79.4(5) 4_545 4_455
O2 O4 O1 72.4(6) 2_545 4_455
O1 O4 O1 123.8(9) 4_645 4_455
O2 O4 O1 143.1(9) 1_645 4_455
O2 O4 O1 56.6(5) 1_445 4_455
O1 O4 O1 35.6(8) 3_454 4_455
O1 O4 O1 72.7(5) 2 4_455
O1 O4 O1 109.0(9) 2_655 4_455
O1 O4 O1 110.3(10) 1_665 4_455
O1 O4 O1 91.7(6) 3_544 4_455
Ga3 O5 Ta 109(3) 1_656 1_566
Ga3 O5 Ga1 109(3) 1_656 1_566
Ta O5 Ga1 0.0(3) 1_566 1_566
Ga3 O5 La1 139(3) 1_656 2_556
Ta O5 La1 104.0(16) 1_566 2_556
Ga1 O5 La1 104.0(16) 1_566 2_556
Ga3 O5 O2 39.6(13) 1_656 1_556
Ta O5 O2 86(2) 1_566 1_556
Ga1 O5 O2 86(2) 1_566 1_556
La1 O5 O2 122(2) 2_556 1_556
Ga3 O5 O2 40.0(16) 1_656 2_656
Ta O5 O2 149(3) 1_566 2_656
Ga1 O5 O2 149(3) 1_566 2_656
La1 O5 O2 104(2) 2_556 2_656
O2 O5 O2 68(2) 1_556 2_656
Ga3 O5 O1 88(2) 1_656 3
Ta O5 O1 128.7(18) 1_566 3
Ga1 O5 O1 128.7(18) 1_566 3
La1 O5 O1 51.4(14) 2_556 3
O2 O5 O1 77.5(19) 1_556 3
O2 O5 O1 63.9(15) 2_656 3
Ga3 O5 O2 112(2) 1_656 2_556
Ta O5 O2 77.9(14) 1_566 2_556
Ga1 O5 O2 77.9(14) 1_566 2_556
La1 O5 O2 52.0(12) 2_556 2_556
O2 O5 O2 76(2) 1_556 2_556
O2 O5 O2 110(2) 2_656 2_556
O1 O5 O2 51.1(12) 3 2_556
Ga3 O5 O4 113(2) 1_656 3
Ta O5 O4 138(2) 1_566 3
Ga1 O5 O4 138(2) 1_566 3
La1 O5 O4 43.5(13) 2_556 3
O2 O5 O4 131(2) 1_556 3
O2 O5 O4 72.9(18) 2_656 3
O1 O5 O4 59.1(16) 3 3
O2 O5 O4 91.4(18) 2_556 3
Ga3 O5 O4 104.2(17) 1_656 2_666
Ta O5 O4 91(2) 1_566 2_666
Ga1 O5 O4 91(2) 1_566 2_666
La1 O5 O4 99.7(17) 2_556 2_666
O2 O5 O4 138(2) 1_556 2_666
O2 O5 O4 96.9(15) 2_656 2_666
O1 O5 O4 133(2) 3 2_666
O2 O5 O4 144.0(16) 2_556 2_666
O4 O5 O4 74.3(12) 3 2_666
Ga3 O5 O1 162(3) 1_656 2_566
Ta O5 O1 88.7(15) 1_566 2_566
Ga1 O5 O1 88.7(15) 1_566 2_566
La1 O5 O1 31.5(10) 2_556 2_566
O2 O5 O1 149.1(19) 1_556 2_566
O2 O5 O1 122(2) 2_656 2_566
O1 O5 O1 82.3(14) 3 2_566
O2 O5 O1 73.3(13) 2_556 2_566
O4 O5 O1 49.3(13) 3 2_566
O4 O5 O1 72.4(12) 2_666 2_566
Ga3 O5 O4 155(3) 1_656 2_566
Ta O5 O4 50.2(14) 1_566 2_566
Ga1 O5 O4 50.2(14) 1_566 2_566
La1 O5 O4 65.7(11) 2_556 2_566
O2 O5 O4 133.3(17) 1_556 2_566
O2 O5 O4 158.3(19) 2_656 2_566
O1 O5 O4 114.9(14) 3 2_566
O2 O5 O4 79.3(10) 2_556 2_566
O4 O5 O4 87.8(14) 3 2_566
O4 O5 O4 67.5(10) 2_666 2_566
O1 O5 O4 40.2(10) 2_566 2_566
Ga4 O6 Ta 112.0(13) 4_655 1_565
Ga4 O6 Ga1 112.0(13) 4_655 1_565
Ta O6 Ga1 0.0(4) 1_565 1_565
Ga4 O6 La1 141.0(13) 4_655 .
Ta O6 La1 106.7(11) 1_565 .
Ga1 O6 La1 106.7(11) 1_565 .
Ga4 O6 O4 39.9(12) 4_655 1_565
Ta O6 O4 113.8(18) 1_565 1_565
Ga1 O6 O4 113.8(18) 1_565 1_565
La1 O6 O4 124.5(17) . 1_565
Ga4 O6 O2 116.4(12) 4_655 .
Ta O6 O2 89.8(14) 1_565 .
Ga1 O6 O2 89.8(14) 1_565 .
La1 O6 O2 58.6(11) . .
O4 O6 O2 150.7(16) 1_565 .
Ga4 O6 O1 92.9(12) 4_655 1_565
Ta O6 O1 143.1(11) 1_565 1_565
Ga1 O6 O1 143.1(11) 1_565 1_565
La1 O6 O1 56.2(10) . 1_565
O4 O6 O1 68.7(18) 1_565 1_565
O2 O6 O1 103.4(16) . 1_565
Ga4 O6 O1 150.8(11) 4_655 4
Ta O6 O1 86.6(10) 1_565 4
Ga1 O6 O1 86.6(10) 1_565 4
La1 O6 O1 27.2(9) . 4
O4 O6 O1 151.7(18) 1_565 4
O2 O6 O1 38.5(9) . 4
O1 O6 O1 83.2(12) 1_565 4
Ga4 O6 O4 79.9(11) 4_655 4_655
Ta O6 O4 157.0(15) 1_565 4_655
Ga1 O6 O4 157.0(15) 1_565 4_655
La1 O6 O4 62.2(10) . 4_655
O4 O6 O4 88.1(10) 1_565 4_655
O2 O6 O4 67.3(14) . 4_655
O1 O6 O4 49.8(12) 1_565 4_655
O1 O6 O4 75.6(11) 4 4_655
Ga4 O6 O2 82.9(10) 4_655 2_655
Ta O6 O2 78.5(9) 1_565 2_655
Ga1 O6 O2 78.5(9) 1_565 2_655
La1 O6 O2 101.0(9) . 2_655
O4 O6 O2 122.7(14) 1_565 2_655
O2 O6 O2 42.4(12) . 2_655
O1 O6 O2 133.3(12) 1_565 2_655
O1 O6 O2 79.1(9) 4 2_655
O4 O6 O2 83.9(12) 4_655 2_655
Ga4 O6 O4 142.3(14) 4_655 4
Ta O6 O4 101.2(11) 1_565 4
Ga1 O6 O4 101.2(11) 1_565 4
La1 O6 O4 22.7(8) . 4
O4 O6 O4 110.4(11) 1_565 4
O2 O6 O4 79.9(13) . 4
O1 O6 O4 49.5(11) 1_565 4
O1 O6 O4 43.5(10) 4 4
O4 O6 O4 75.9(12) 4_655 4
O2 O6 O4 122.1(12) 2_655 4
Ga4 O6 O2 138.5(13) 4_655 2
Ta O6 O2 39.7(9) 1_565 2
Ga1 O6 O2 39.7(9) 1_565 2
La1 O6 O2 73.6(9) . 2
O4 O6 O2 153.3(17) 1_565 2
O2 O6 O2 53.6(13) . 2
O1 O6 O2 128.0(12) 1_565 2
O1 O6 O2 48.8(9) 4 2
O4 O6 O2 118.6(13) 4_655 2
O2 O6 O2 64.4(7) 2_655 2
O4 O6 O2 79.0(11) 4 2
Ga4 O7 Ta 110(3) 3_545 1_556
Ga4 O7 Ga1 110(3) 3_545 1_556
Ta O7 Ga1 0.0(3) 1_556 1_556
Ga4 O7 La2 131(3) 3_545 1_556
Ta O7 La2 105(2) 1_556 1_556
Ga1 O7 La2 105(2) 1_556 1_556
Ga4 O7 O4 127(2) 3_545 1_556
Ta O7 O4 101(2) 1_556 1_556
Ga1 O7 O4 101(2) 1_556 1_556
La2 O7 O4 76.2(19) 1_556 1_556
Ga4 O7 O4 31.5(16) 3_545 2_656
Ta O7 O4 136(3) 1_556 2_656
Ga1 O7 O4 136(3) 1_556 2_656
La2 O7 O4 101(2) 1_556 2_656
O4 O7 O4 120(3) 1_556 2_656
Ga4 O7 O1 83(2) 3_545 3
Ta O7 O1 126(2) 1_556 3
Ga1 O7 O1 126(2) 1_556 3
La2 O7 O1 48.5(14) 1_556 3
O4 O7 O1 112(2) 1_556 3
O4 O7 O1 55.0(15) 2_656 3
Ga4 O7 O4 101(2) 3_545 2_556
Ta O7 O4 73(2) 1_556 2_556
Ga1 O7 O4 73(2) 1_556 2_556
La2 O7 O4 58.0(14) 1_556 2_556
O4 O7 O4 129.4(19) 1_556 2_556
O4 O7 O4 91(2) 2_656 2_556
O1 O7 O4 52.7(11) 3 2_556
Ga4 O7 O2 119(2) 3_545 1_556
Ta O7 O2 130(2) 1_556 1_556
Ga1 O7 O2 130(2) 1_556 1_556
La2 O7 O2 36.7(11) 1_556 1_556
O4 O7 O2 51.6(16) 1_556 1_556
O4 O7 O2 90.4(19) 2_656 1_556
O1 O7 O2 60.1(15) 3 1_556
O4 O7 O2 93.1(16) 2_556 1_556
Ga4 O7 O1 157(3) 3_545 4_556
Ta O7 O1 92.4(17) 1_556 4_556
Ga1 O7 O1 92.4(17) 1_556 4_556
La2 O7 O1 30.8(10) 1_556 4_556
O4 O7 O1 50.2(14) 1_556 4_556
O4 O7 O1 126(2) 2_656 4_556
O1 O7 O1 78(2) 3 4_556
O4 O7 O1 79.4(13) 2_556 4_556
O2 O7 O1 37.9(9) 1_556 4_556
Ga4 O7 O2 74.4(19) 3_545 2_656
Ta O7 O2 170(3) 1_556 2_656
Ga1 O7 O2 170(3) 1_556 2_656
La2 O7 O2 66.8(14) 1_556 2_656
O4 O7 O2 82.0(18) 1_556 2_656
O4 O7 O2 45.5(16) 2_656 2_656
O1 O7 O2 44.8(11) 3 2_656
O4 O7 O2 97.4(16) 2_556 2_656
O2 O7 O2 45.2(13) 1_556 2_656
O1 O7 O2 82.3(14) 4_556 2_656
Ga4 O7 O2 117(3) 3_545 2_556
Ta O7 O2 103.3(19) 1_556 2_556
Ga1 O7 O2 103.3(19) 1_556 2_556
La2 O7 O2 19.1(9) 1_556 2_556
O4 O7 O2 95.2(18) 1_556 2_556
O4 O7 O2 89.7(18) 2_656 2_556
O1 O7 O2 34.7(10) 3 2_556
O4 O7 O2 42.1(11) 2_556 2_556
O2 O7 O2 51.0(14) 1_556 2_556
O1 O7 O2 48.9(11) 4_556 2_556
O2 O7 O2 66.9(12) 2_656 2_556
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
La1 O6 2.36(3) .
La1 O5 2.37(5) 2_556
La1 O3 2.48(3) 3_554
La1 O4 2.34(5) 4
La1 O1 2.57(5) 1_565
La1 O1 2.41(5) 4
La1 O2 2.57(4) .
La1 O3 2.64(3) 2_566
La1 Ga2 3.357(7) 4
La1 Ga2 3.390(7) .
La1 Ta 3.470(5) 1_565
La1 Ga1 3.470(5) 1_565
La2 O7 2.42(6) 2_556
La2 O7 2.42(6) 1_554
La2 O1 2.52(5) 4
La2 O1 2.52(5) 3_554
La2 O2 2.51(5) .
La2 O2 2.51(5) 2
La2 O4 3.38(6) 2
La2 O4 3.38(6) .
La2 Ga2 3.378(8) .
La2 Ga2 3.378(8) 2
La2 Ga1 3.475(8) .
La2 Ta 3.475(8) .
Ga1 O5 2.03(5) 2_546
Ga1 O5 2.03(5) 1_544
Ga1 O6 1.96(2) 2_545
Ga1 O6 1.96(2) 1_545
Ga1 O7 1.95(6) 1_554
Ga1 O7 1.95(6) 2_556
Ga1 O4 3.89(6) 2
Ga1 O4 3.89(6) .
Ga1 O2 3.43(5) 2_545
Ga1 O2 3.43(5) 1_545
Ga1 La1 3.470(5) 2_545
Ga1 La1 3.470(5) 1_545
Ta O5 2.03(5) 2_546
Ta O5 2.03(5) 1_544
Ta O6 1.96(2) 2_545
Ta O6 1.96(2) 1_545
Ta O7 1.95(6) 1_554
Ta O7 1.95(6) 2_556
Ta Ga4 3.110(7) 3_544
Ta Ga4 3.110(7) 4_545
Ta Ga3 3.138(8) 1_545
Ta Ga3 3.138(8) 1_645
Ta Ga4 3.139(8) 4_645
Ta Ga4 3.139(8) 3_444
Ga2 O1 1.793(15) 4_655
Ga2 O3 1.82(3) 3_554
Ga2 O2 1.84(5) .
Ga2 O4 1.82(6) .
Ga2 O1 3.236(14) 4
Ga2 La1 3.357(7) 4_545
Ga2 La2 3.525(7) 1_655
Ga2 La1 3.516(7) 4_645
Ga2 La1 3.525(7) 1_655
Ga2 O4 3.15(7) 4_655
Ga3 O2 1.90(4) 2
Ga3 O2 1.90(4) 1_455
Ga3 O5 1.82(5) 2_556
Ga3 O5 1.82(5) 1_454
Ga3 Ta 3.138(8) 1_565
Ga3 Ta 3.138(8) 1_465
Ga3 O1 3.48(5) 3_454
Ga3 O1 3.48(5) 4
Ga3 O2 4.25(4) 2_455
Ga3 O2 4.25(4) .
Ga3 O4 4.63(6) 2
Ga3 O4 4.63(6) 1_455
Ga4 O4 1.72(6) 4_655
Ga4 O7 1.84(5) 3_554
Ga4 O6 1.83(3) 4_645
Ga4 O3 1.87(3) 3_554
Ga4 Ta 3.110(7) 3
Ga4 Ta 3.139(8) 3_655
Ga4 O1 3.63(5) 1_565
Ga4 O1 3.57(5) 4_655
Ga4 O4 4.36(6) 3
Ga4 O2 3.99(5) 4_645
Ga4 O2 4.23(5) .
Ga4 O2 4.32(5) 4_655
O1 Ga2 1.793(15) 4_645
O1 La1 2.57(5) 1_545
O1 La2 2.52(5) 3_545
O1 La1 2.41(5) 4_545
O1 O3 2.79(5) 2_556
O1 O2 2.70(5) 4_545
O1 O4 3.30(6) 4_545
O1 O7 3.36(8) 3_544
O1 O6 2.97(6) 1_545
O1 O3 3.12(4) 2_656
O1 O4 2.95(6) 4_645
O1 O2 3.13(5) 4_645
O1 O5 3.03(8) 3_544
O1 Ga2 3.236(14) 4_545
O1 Ga4 3.63(5) 1_545
O1 Ga3 3.48(5) 3_645
O1 Ga4 3.57(5) 4_645
O1 O4 3.19(8) .
O1 O3 3.79(6) 3_544
O1 O2 3.72(7) 3_545
O1 O7 4.28(8) 4_546
O1 O5 4.27(7) 2_546
O1 O6 4.26(5) 4_545
O1 O2 4.55(7) 1_545
O1 O3 4.46(6) 3_554
O1 Ga4 4.65(4) 1_445
O1 Ga4 4.56(4) 4_545
O1 Ga3 4.51(4) 3_545
O1 O4 5.27(8) 3_545
O1 Ta 4.78(5) 3_545
O1 Ga1 4.78(5) 3_545
O1 Ta 4.58(5) 3
O1 Ga1 4.58(5) 3
O1 O5 4.73(7) 2_646
O1 O6 4.64(5) 4_535
O1 La1 4.85(3) 1_645
O1 La2 4.83(3) 3_645
O1 O7 4.98(8) 2_556
O1 La1 4.78(3) 4_645
O1 O7 4.73(7) 4_646
O1 O6 4.97(5) 4_645
O1 Ga2 4.87(5) 3_545
O1 Ga2 4.96(5) 1_545
O1 O5 4.85(7) 4_546
O1 O1 4.88(11) 2_556
O1 O1 4.90(5) 4_545
O1 O1 4.90(5) 4
O1 O1 5.0240 1_455
O1 O1 5.02401(17) 1_655
O1 Ga4 5.29(5) 2_646
O1 Ga3 5.30(5) 1_645
O1 O4 4.96(7) 1_455
O1 O1 5.70(9) 2_656
O1 O1 5.72(5) 4_655
O1 O1 5.72(5) 4_645
O1 O2 5.74(5) 3_445
O1 La1 5.92(5) 4_535
O1 La1 5.80(5) 3_545
O1 O2 6.07(7) .
O1 O2 6.31(6) 1_445
O1 O4 6.49(7) 3_445
O1 O4 6.29(8) 1_545
O1 La2 6.31(2) 3_445
O1 La1 6.34(2) 1_445
O1 La1 6.27(2) 4_445
O1 O4 6.80(6) 1_655
O1 O4 6.72(8) 4
O1 O2 6.72(5) 3_645
O1 O4 6.56(8) 4_655
O1 O2 6.93(8) 2_545
O1 O2 7.11(7) 2_645
O1 O2 7.22(5) 1_645
O1 O2 7.40(6) 4_535
O1 O4 7.99(7) 3_645
O1 O4 7.93(8) 2
O2 Ga3 1.90(4) 1_655
O2 O6 2.82(5) .
O2 O3 2.67(5) 3_554
O2 O5 2.91(7) 1_554
O2 O1 2.70(5) 4
O2 O5 2.89(6) 2_656
O2 O4 3.17(8) .
O2 O2 3.26(8) 2_655
O2 O1 3.13(5) 4_655
O2 O5 3.22(6) 2_556
O2 Ta 3.43(5) 1_565
O2 Ga1 3.43(5) 1_565
O2 O1 3.72(7) 3_554
O2 O2 3.78(9) 2
O2 Ga2 3.89(5) 2_655
O2 Ga4 3.99(5) 4_655
O2 O7 3.99(8) 1_554
O2 La2 4.13(4) 1_655
O2 La1 4.16(4) 1_655
O2 La1 4.16(5) 4_545
O2 Ga4 4.32(5) 4_645
O2 O7 4.44(8) 2_656
O2 O3 4.35(3) 2_666
O2 O4 3.76(8) 4_655
O2 Ga2 4.34(4) 1_455
O2 O6 4.74(5) 2_655
O2 O7 4.67(8) 2_556
O2 O1 4.55(7) 1_565
O2 La1 4.62(5) 2
O2 O6 4.69(5) 2
O2 Ga2 4.58(5) 4_655
O2 O4 5.00(8) 2_655
O2 Ga1 4.75(4) 1_665
O2 Ta 4.75(4) 1_665
O2 O7 4.57(8) 1_564
O2 Ga4 4.86(5) 3_554
O2 O3 4.81(3) 2_566
O2 O6 4.93(5) 4_645
O2 O4 4.74(7) 4
O2 O2 5.0240(2) 1_655
O2 O2 5.02400(17) 1_455
O2 O7 4.97(8) 2_666
O2 Ga4 5.14(5) 3_544
O2 O4 5.30(7) 1_565
O2 O4 5.77(7) 2
O2 La1 5.31(4) 4_645
O2 Ga2 5.34(4) 2
O2 Ga4 5.49(4) 4
O2 La1 5.68(4) 2_655
O2 O1 5.74(5) 3_654
O2 O4 5.53(7) 1_455
O2 O4 6.32(6) 1_655
O2 La1 5.96(5) 4
O2 La1 6.04(5) 3_544
O2 O4 5.75(8) 3_554
O2 O1 6.31(6) 1_665
O2 O4 6.57(7) 2_665
O2 O2 6.36(7) 4_645
O2 O2 6.36(7) 4_655
O2 O1 6.72(5) 3_454
O2 O4 7.17(7) 2_565
O2 O2 6.64(7) 4_545
O2 O2 6.64(7) 4
O2 O1 6.93(8) 2_565
O2 O1 7.11(7) 2_665
O2 O4 6.98(6) 1_465
O2 O1 7.22(5) 1_465
O2 O4 7.62(7) 1_665
O2 O1 7.40(6) 4_565
O2 O1 7.57(6) 4_665
O2 O1 7.43(3) 4_455
O2 O1 7.48(6) 1_655
O3 Ga2 1.82(3) 3_545
O3 Ga4 1.87(3) 3_545
O3 La1 2.48(3) 3_545
O3 La1 2.64(3) 2_546
O3 O2 2.67(5) 3_545
O3 O4 2.58(6) 3_545
O3 O1 2.79(5) 2_556
O3 O4 2.49(6) 2_656
O3 O1 3.12(4) 2_656
O3 O1 3.79(6) 3
O3 O4 3.89(5) 2_556
O3 O2 4.35(3) 2_646
O4 Ga4 1.72(6) 4_645
O4 La1 2.34(5) 4_545
O4 O6 2.66(6) 1_545
O4 O7 3.00(9) 1_554
O4 O7 2.99(7) 2_656
O4 O3 2.58(6) 3_554
O4 O3 2.49(6) 2_656
O4 O1 3.30(6) 4
O4 O1 2.95(6) 4_655
O4 O7 3.97(8) 2_556
O4 Ga2 3.15(7) 4_645
O4 O3 3.89(5) 2_556
O4 La1 3.42(5) 4_645
O4 Ga4 4.36(6) 3_544
O4 O5 3.40(9) 3_544
O4 O5 4.11(7) 2_646
O4 La2 4.19(6) 1_655
O4 O6 3.81(6) 4_645
O4 Ga4 4.68(5) 4_545
O4 O4 5.18(13) 2_655
O4 O2 3.76(8) 4_645
O4 Ga3 4.63(6) 1_655
O4 La1 4.44(6) 1_545
O4 O5 4.86(6) 2_546
O4 O5 5.00(8) 1_544
O4 Ga2 4.84(5) 1_455
O4 Ta 4.61(5) 1_655
O4 Ga1 4.61(5) 1_655
O4 O6 4.33(6) 4_545
O4 O2 5.00(8) 2_655
O4 O1 5.27(8) 3_554
O4 Ga3 4.89(6) 1_645
O4 Ga2 5.18(7) 2_655
O4 O6 5.23(7) 2_645
O4 O2 4.74(7) 4_545
O4 Ga3 4.44(7) 3_645
O4 O4 5.02400(17) 1_455
O4 O4 5.0240(2) 1_655
O4 O4 6.31(12) 2
O4 O2 5.30(7) 1_545
O4 O2 5.77(7) 2
O4 O4 4.57(6) 4_655
O4 O4 4.57(6) 4_645
O4 Ga2 5.30(6) 4_545
O4 La1 5.09(5) 1_655
O4 La1 5.08(5) 1_645
O4 Ga1 5.09(6) 3
O4 Ta 5.09(6) 3
O4 O1 4.96(7) 1_655
O4 Ga4 6.19(6) 3_444
O4 O2 5.53(7) 1_655
O4 La2 5.54(7) 3_545
O4 O4 5.82(7) 4
O4 O4 5.82(7) 4_545
O4 O2 6.32(6) 1_455
O4 La1 6.69(6) 3_544
O4 O2 5.75(8) 3_545
O4 O1 6.49(7) 3_654
O4 O1 6.29(8) 1_565
O4 O2 6.57(7) 2_645
O4 O1 6.80(6) 1_455
O4 O1 6.72(8) 4_545
O4 O2 7.17(7) 2_545
O4 O1 6.56(8) 4_645
O4 O2 6.98(6) 1_645
O4 O2 7.62(7) 1_445
O4 O1 7.99(7) 3_454
O4 O1 7.93(8) 2
O4 O1 7.79(8) 2_655
O4 O1 7.34(7) 1_665
O4 O1 7.88(8) 3_544
O4 O1 7.97(5) 4_455
O5 Ga3 1.82(5) 1_656
O5 Ta 2.03(5) 1_566
O5 Ga1 2.03(5) 1_566
O5 La1 2.37(5) 2_556
O5 O2 2.91(7) 1_556
O5 O2 2.89(6) 2_656
O5 O1 3.03(8) 3
O5 O2 3.22(6) 2_556
O5 O4 3.40(9) 3
O5 O4 4.11(7) 2_666
O5 O1 4.27(7) 2_566
O5 O4 4.86(6) 2_566
O6 Ga4 1.83(3) 4_655
O6 Ta 1.96(2) 1_565
O6 Ga1 1.96(2) 1_565
O6 O4 2.66(6) 1_565
O6 O1 2.97(6) 1_565
O6 O1 4.26(5) 4
O6 O4 3.81(6) 4_655
O6 O2 4.74(5) 2_655
O6 O4 4.33(6) 4
O6 O2 4.69(5) 2
O7 Ga4 1.84(5) 3_545
O7 Ta 1.95(6) 1_556
O7 Ga1 1.95(6) 1_556
O7 La2 2.42(6) 1_556
O7 O4 3.00(9) 1_556
O7 O4 2.99(7) 2_656
O7 O1 3.36(8) 3
O7 O4 3.97(8) 2_556
O7 O2 3.99(8) 1_556
O7 O1 4.28(8) 4_556
O7 O2 4.44(8) 2_656
O7 O2 4.67(8) 2_556
loop_
_cod_related_suboptimal_struct
2103504
2103505
